Mao-Hong Yu Generalized Plasticity
Mao-Hong Yu Guo-Wei Ma Hong-Fu Qiang Yong-Qiang Zhang
Generalized Plasticity
With...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Mao-Hong Yu Generalized Plasticity

Mao-Hong Yu Guo-Wei Ma Hong-Fu Qiang Yong-Qiang Zhang

Generalized Plasticity

With 315 Figures

Professor Mao-Hong Yu Xian Jiaotong University School of Civil Engineering and Mechanics 710049 Xian, People’s Republic of China E-mail: [email protected]

Co-Authors Guo-Wei Ma Nanyang Technological University, Singapore

Hong-Fu Qiang Yi’an Hi-Tech Research Institute, China

Yong-Qiang Zhang National University of Singapore, Singapore

Library of Congress Control Number: 2005932191

ISBN-10 3-540-25127-8 Springer Berlin Heidelberg New York ISBN-13 978-3-540-25127-0 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specif ically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microf ilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to to prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media. springeronline.com © Springer-Verlag Berlin Heidelberg 2006 Printed in Germany The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specif ic statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Camera-ready by the Author and SPI, India Cover design: design & production GmbH, Heidelberg Printed on acid-free paper

SPIN 11009092

62/3141/SPI 5 4 3 2 1 0

Appreciate the beauty of the discover the truth of the universe.

universe;

Zhuang Zi (369 –286 B.C. China)

I have loved the principle of beauty in all things, and if I had had time I would have made myself remembered. Keats, John (1795 – 1821, UK)

A thing of beauty is a joy for ever. Keats, John (1795 – 1821, UK)

“Beauty is truth, truth is beauty,” — that is all ye know on earth, and all ye need to know. Keats, John (1795 – 1821, UK)

Preface

Generalized plasticity is a generalization of the unified strength theory to the theory of plasticity. It is the unification of metal plasticity for Tresca materials, Huber-von Mises materials, and twin-shear materials. It is also the unification of geomaterial plasticity for Mohr-Coulomb materials and generalized twin-shear materials. Moreover, it leads to unification of metal plasticity and plasticity of geomaterials, in general. It is a companion volume to Unified Strength Theory and Its Applications published by Springer in 2004. Generalized Plasticity is based on the lectures on the unified theory of materials and structures given by the author at the School of Civil Engineering and Mechanics, Xi’an Jiaotong University in Xi’an, China and at the Nanyang Technological University of Singapore in 1996. It is a course entitled “Generalized Plasticity” for Ph.D. students at Xi’an Jiaotong University since 1993. The main contents are the unified yield function (unified strength theory) of material, the unified slip line field theory for plane strain problem, unified characteristics field theory for plane stress problem, unified characteristics field theory for spatial axisymmetric problem, limit pressure and shakedown pressure of a pressure vessel, the plastic zone analysis at a crack tip under small-scale yielding and the unified fracture criterion. Several chapters in this book have been presented in conferences and published in various journals. They are: Unified Strength Theory (Yu, 1991, 1992, 1994, 2002, 2004); Unified Slip Line Field Theory for Plane Strain Problem (Yu, Yang, et al., 1997, 1999); Unified Characteristics Field Theory for Plane Stress Problem (Yu and Zhang, 1998, 1999; Zhang, Hao and Yu, et al., 2003); Unified Characteristics Field Theory for Spatial Axisymmetric Problem (Yu and Li, 2001); Unified Solution for Limit Pressure of a Pressure Vessel (Wang and Fan, 1998; Zhao et al., 1999); Unified Solution for Shakedown Pressure of a Pressure Vessel (Xu and Yu, 2004, 2005); Analysis of Plastic Zone at Crack Tip (Qiang et al., 1998, 2004); Unified Fracture Criterion (Yu, Fan, Che, Yoshimine, et al., 2003, 2004; Qiang and Yu, 2004). The beauty of the unified strength theory discussed in Chap. 5 is a part of a closing lecture delivered at the International Symposium on Developments in Plasticity and Fracture: Centenary of M.T. Huber Criterion, held at Cracow, Poland in 2004. The garden of the flowers of strength theory, the beauty of the Huber-von Mises criterion, and the beauty of the unified strength theory were discussed at the lecture. The analytical results of the generalized plasticity are a series of results. It is different from the conventional plasticity. As an example, a unified solution of bearing capacity of a plane strain structure by using the unified slip line field theory is shown in Fig. 1. The conventional solution of bearing capacity of a

VIII

Preface

structure is adapted only for one kind of material. It is shown in Fig. 1 at b = 0. This result is obtained by using the Mohr-Coulomb strength theory (inner bound or lower bound as shown in Fig. 2a), Fig. 2b is a special case for Į = 1 materials. It can also be obtained by using the unified strength theory with b = 0. The unified solution includes a series of solutions and encompasses the solution of the Mohr-Coulomb strength theory as a special case. It is also possible to obtain a series of new solutions for different values of parameter b and different ratios of tension and compression strength of material, i.e., Į = ıt/ıc 1.

Fig. 1 Limit loads of a plane strain structure.

(a) Į = ıt/ıc 1 materials

(b) Į = ıt/ıc = 1 materials

Fig. 2 Yield loci of the unified strength theory on the deviatoric plane.

Preface

IX

The unified strength theory and the unified slip line field theory for plane strain problem can be expressed in terms of another material parameter, such as friction angle ĳ, it is widely used in geomechanics and geotechnical engineering. The unified solutions for a plane strain problem in terms of the friction ĳ are shown in Fig. 3. The description of the unified solutions of plane strain problems can be seen in Chap. 9.

Fig. 3 Unified solutions of a plane strain problem in terms of the friction ĳ.

For the plane stress problems, the yield loci of the unified strength theory in plane stress state is shown in Fig. 4, and the unified solution of bearing capacity of a plane stress structure by using the unified characteristics line field theory is shown in Fig. 5. It can be seen that a series of new results are given whereas the Mohr-Coulomb theory and the Tresca criterion can give only one result. It is a special case of the unified solution by using the unified strength theory and the unified characteristics line theory with b = 0 and b = 0, Į = 1.

(a) Į = ıt/ıc 1 materials

(b) Į = ıt/ıc =1 materials

Fig. 4 Yield loci of the unified strength theory in plane stress state.

X

Preface

1.35

α = 0.2 α = 0.5 α = 0.8 α = 1.0

1.30 1.25 1.20

q

1.15 1.10 1.05 1.00 0.95

0.0

0.2

0.4

0.6

0.8

1.0

b

Fig. 5 Limit loads of a plane stress structure. The analytical results are clearly illustrated to show the effects of yield criterion on plastic limit behaviors for plane strain problems, plane stress problems, axisymmetric problems, other engineering structures, the shape and size of plastic zone at crack tip, discontinuous bifurcation, and angle of shear band. Generalized plasticity gives us a series of results, which can be adapted for different materials and structures. The contents of the book can be divided into five parts as follows: Part One. The unified strength theory, material parameters in the unified strength theory, yield surfaces, yield loci, reasonable choice of the yield criterion, and the beauty of the unified strength theory are described in Chaps. 4 and 5. Part Two. Plastic stress–strain relation and concrete plasticity, discussed in Chaps. 6 and 7. Part Three. Twin-shear slip field and the unified slip-line field theory for plane strain problems, twin-shear characteristics field and the unified characteristics line theory for plane stress problems, and unified characteristics line field theory for axisymmetric problems and high velocity penetration problem are explained in Chaps. 8–12. Part Four. The unified solution of plastic zone at crack tip under small-scale yielding is given. Based on the unified strength theory, a unified fracture criterion, a new closed form of plastic core region model, and variation for the angle of initial crack growth versus crack inclination under different loading conditions are obtained. They are described in Chaps. 13 and 14. Part Five. Chapter 15 is devoted to the unified solutions of limit loads and shakedown loads for pressure vessels. Stress state analysis and basic behaviors of materials under complex stress are discussed in Chaps. 2 and 3. The description of the stress state may be found in a number of books covering mechanics of materials, solid mechanics, and elasticity and plasticity. Only some basic formulae and figures as well as some new ideas are

Preface

XI

given here. Brief summaries, problems, and references and bibliography are given at the end of the chapters. I would like to express my gratitude for the support of the National Natural Science Foundation of China (Grants nos. 59779028, 59924033, and 50078046), the Ministry of Education of China, the China Academy of Launch Vehicle Technology, the Aircraft Strength Research Institute of China, the Department of Science and Technology of Xi’an Jiaotong University, as well as the School of Civil and Environmental Engineering, Nanyang Technological University, Singapore. I am indebted to many authors and colleagues, especially Dr Ma at Nangyang Technological University, Singapore, Prof. Qiang at Xi’an Hi-Tech Research Institute, and Dr Zhang at National University of Singapore for going through the manuscript of this book. I am also indebted to Dr Li YM, Dr Yang SY, Dr Zhao JH, Dr Wang F, Dr Li JC, Dr Song L, Dr Liu YH, Dr Fan W, Dr Zan YW, Dr Wei XY, Dr Xu SQ, Dr Yoshimine M, Dr Yang JH, Dr Zheng H, Dr Gao JP, Dr Liu FY, and Mr Liu JY and Ms Zeng WB for their research work at Xi’an Jiaotong University. Thanks are due to Ms He, Ms Lei, and others for their support during the course of writing this book. I would like to thank many professors from other universities and many research scientists and engineers from various institutions for their work in the research and application of the unified strength theory. I would also like to acknowledge the support from all other individuals and universities, research organizations, journals, and publishers. I would also like to express my sincere thanks to Dr Dieter Merkle, Editorial Director, Engineering and Editorial Department and International Engineering Department, Springer-Verlag, Germany, and his team for their excellent editorial work on this manuscript. The study of generalized plasticity based on the unified strength theory is just the beginning. A lot of research in generalized plasticity is still to be done. Mao-Hong Yu Spring 2005

Contents

Preface Notations 1

Introduction 1.1 1.2 1.3 1.4 1.5 1.6 1.7

2

Stress Space and Stress State 2.1 2.2 2.3 2.4 2.5 2.6 2.7

3

Linear Elasticity ................................................................................. Classical Plasticity ............................................................................. Concrete Plasticity ............................................................................. Soil Plasticity .................................................................................... Rock Plasticity ................................................................................... Generalized Plasticity ........................................................................ Generalized Plasticity Based on the Unified Strength Theory.......... References and Bibliography.............................................................

Elements ............................................................................................ Stress at a Point, Stress Invariants...................................................... Deviatoric Stress Tensor, Deviatoric Tensor Invariants..................... Stresses on the Oblique Plane ............................................................ Hexahedron, Octahedron, Dodecahedron .......................................... Stress Space ........................................................................................ Stress State Parameters....................................................................... Summary ............................................................................................ References ........................................................................................

Basic Characteristics of Yield of Materials under Complex Stress 3.1 3.2 3.3 3.4 3.5 3.6

Introduction ........................................................................................ Strength Difference Effect (SD effect) ............................................ Effect of Hydrostatic Stress ............................................................... Effect of Normal Stress...................................................................... Effect of Intermediate Principal Stress .............................................. Effect of Intermediate Principal Shear-Stress ...................................

1 1 2 5 6 7 8 8 10

15 15 15 16 17 21 22 27 31 31

33 33 33 35 37 38 43

XIV

Contents

3.7

Bounds of the Convex Strength Theories ........................................ Summary........................................................................................... References .......................................................................................

46 47 47

4 Unified Strength Theory and Its Material Parameters

50

4.1 4.2 4.3 4.4 4.5 4.6 4.7 4.8 4.9

Introduction ................................................................................... Mechanical Model of the Unified Strength Theory ....................... Unified Strength Theory ............................................................... Special Cases of the Unified Strength Theory ............................... Material Parameters of the Unified Strength Theory ..................... Other Material Parameters of the Unified Strength T heory ............ Yield Surfaces and Yield Loci........................................................ Yield Loci of the Unified Strength Theory in the π í Plane ........ Yield Surfaces of the Unified Strength Theory in Principal Stress Space .................................................................................... 4.10 Yield Loci of the Unified Strength Theory in Plane Stress State .. 4.11 Unified Strength Theory in Meridian Plane ................................... 4.12 Yield Surfaces of the Non-linear Unified Strength T heory ............. Summary ....................................................................................... Problems ............................................................................. References and Bibliography .........................................................

50 51 53 54 60 63 66 69 72 75 78 81 85 87 93

5 Reasonable Choice of a Yield Function 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9 5.10

Introduction ..................................................................................... Some Experimental Data of Metallic Materials............................. Reasonable Choice of a Yield Function for Non-SD Materials.... Experiments for Iron under σ – τ Stress State................................. Experiments for Concrete under Complex Stress ......................... Experiments for Rock under Complex Stress ............................... Experiments on Clay and Loess under Complex Stress ............... Experiments on Sand under Complex Stress ................................ Reasonable Choice of a Yield Function for SD-Materials ........... The Beauty of the Unified Strength Theory.................................. Summary............................................................................................. Problems ............................................................................................. References and Bibliography ..............................................................

6 Elasto-Plastic Costitutive Relations 6.1 6.2

95

Introduction ....................................................................................... Plastic Deformation in Uniaxial Stress State....................................

95 96 100 102 103 105 108 109 112 113 117 118 119

122 122 122

6.3 6.4 6.5 6.6 6.7 6.8 6.9 6.10 6.11 6.12

7

XV

Three-dimensional Elastic Stress-strain Relation ........................... Plastic Work Hardening and Strain Hardening................................ Plastic Flow Rule............................................................................. Drucker’s Postulate – Convexity of the Loading Surface ................. Incremental Constitutive Equations in Matrix Formulation........... Determination of Flow Vector for Different Yield Functions........ Singularity of Piecewise-Linear Yield Functions ............................ Process of the Plastic Flow Singularity........................................... Suggested Methods.......................................................................... Unified Process of the Corner Singularity ...................................... Summary .......................................................................................... Problems........................................................................................... References and Bibliography...........................................................

124 125 127 129 132 135 137 142 145 148 152 152 153

Concrete Plasticity 7.1 7.2 7.3 7.4 7.5 7.6 7.7

8

Contents

Introduction....................................................................................... Multi-Parameter Yield Criteria......................................................... Multi-Parameter Unified Yield Criterion......................................... Yield and Loading Functions ........................................................... Processing of Corner Singularity ..................................................... Strain Softening Phenomena and Material Damage ........................ Applcations ....................................................................................... Summary ........................................................................................... Problems............................................................................................ References and Bibliography............................................................

Twin- Shear Slip-Line Field for Plane Strain Problem 8.1 8.2 8.3 8.4 8.5 8.6

Introduction....................................................................................... Stress State in Plane Strain Problem ................................................ Twin-Shear Strength Theory of Plane Strain Problem .................... Twin-Shear Line Field Theory for Plane Strain Problem (Statically Admissible Field) ............................................................................ Twin-Shear Slip Line Field Theory for Plane Strain Problem (Kinematically Admissible Field) .................................................. Applications of the Twin-Shear Slip Line Field Theory for Plane Strain Problems ................................................................. Summary........................................................................................... Problems ........................................................................................... References and Bibliography ...........................................................

155 155 157 162 168 176 179 182 192 192 193

195 195 198 200 202 204 209 218 218 223

XVI

9

Contents

Unified Slip- Line Field Theory for Plane Strain Problem 9.1 9.2 9.3 9.4 9.5 9.6 9.7 9.8 9.9

Introduction ...................................................................................... 225 Unified Strength Theory in Plane Strain Condition......................... 226 Unified Slip Line Field Theory for Plane Strain Problem (Statically Admissible Field) ............................................................................ 230 Unified Slip Line Field Theory for Plane Strain Problem (Kinematically Admissible Field) ............................................................................ 233 Special Cases of the Unified Slip Line Field Theory ...................... 236 Applications of the Unified Slip Line Field Theory ........................ 240 Comparison of the Unified Slip Line Field Theory with Finite Element Method ............................................................................... 252 Comparison of the Unified Slip Line Field Theory with Experimental Results........................................................................ 256 Discontinuous Bifurcations of Elasto-Plastic Material For Plane Strain Problem .................................................................................. 257 Summary........................................................................................... 260 Problems ........................................................................................... 260 References and Bibliography ........................................................... 268

10 Twin-Shear Characteristics Field for Plane Stress Problem 10.1 Introduction ................................................................................... 10.2 Characteristics Method Based on the Tresca Criterion and the Huber-von Mises Criterion ....................................................... 10.3 Characteristics Method Based on the Twin-Shear Yield Criterion 10.4 Twin-Shear Characteristics Field for Plane Stress Problems (Velocity Field) ............................................................................. 10.5 Applications of the Twin-Shear Characteristics Method............... 10.6 Comparison of These Different Methods ....................................... Summary......................................................................................... Problems ......................................................................................... References and Bibliography .........................................................

11 Unified Characteristics Field Theory for Plane Stress Problem 11.1 11.2 11.3 11.4

225

Introduction.................................................................................... Unified Yield Function in Plane Stress State.................................. Characteristics Filed for Plane Stress Problems ........................... Applications of the Unified Characteristics Field for Plane Stress Problems.............................................................................

270 270 270 274 278 281 287 288 288 292

293 293 293 296 302

Contents

XVII

11.5 Discontinuous Bifurcations of Elasto-Plastic Material for Plane Stress ............................................................................... 11.6 Discontinuous Bifurcations of Non-associated Flow Elasto-Plastic Materials Based on Yu Unified Strength Theory... 11.7 Discussion and Experimental Verification .................................... Summary......................................................................................... Problems ......................................................................................... References and Bibliography .........................................................

310 317 319 320 320

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

322

12.1 Introduction.................................................................................... 12.2 The Unified Strength Theory......................................................... 12.3 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Stress Field) ........................................ 12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Velocity Field) .................................... 12.5 Applications of the Unified Characteristics Field Theory ............ 12.6 Penetration of High Velocity Rod to Target .................................. 12.7 Elastic-Damage-Plastic Analysis of the Target ................................ 12.8 Comparison and Verification ......................................................... Summary............................................................................................. Problems ............................................................................................. References and Bibliography .............................................................

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding 13.1 Introduction................................................................................... 13.2 Unified Strength Theory ............................................................... 13.3 Stress Field Around Crack-Tip ..................................................... 13.4 Shape and Size of Plastic Zone for Mode-I Crack Tip ................ 13.5 Shape and Size of Plastic Zone for Mode-II Crack Tip ............... 13.6 Plastic Zone for Mode-III Crack Tip............................................ 13.7 Shape and Size of Plastic Zone for Non-Conventional Materials 13.8 Effect of b’ Value ........................................................................ 13.9 Influence of SD Effect................................................................... 13.10 Influence of Poisson’s Ratio .......................................................... Summary ....................................................................................... Problems ....................................................................................... References and Bibliography .......................................................

308

322 324 324 329 331 334 338 343 346 347 348

351 351 352 355 357 361 365 365 368 369 370 371 372 374

’

XVIII

Contents

14 Unified Fracture Criteria for Mixed Mode Crack Initiation and Fatigue Crack Growth 14.1 14.2 14.3 14.4 14.5 14.6

375

Introduction ................................................................................. Main Idea of T-Criterion .............................................................. A Generalization for T-Criterion Using UST .............................. Significance of Parameters b, α and v .......................................... Crack Initiation Angle of the Generalized T-Criterion................ Application of the Unified Strength Theory in Establishing the Mixed Fracture Criterion........................................................ 14.7 Unified Fracture Criterion ............................................................ 14.8 Unified Fracture Criterion of Mixed Mode I – III ....................... 14.9 Unified Fracture Criterion of Mixed Mode II – III....................... Summary........................................................................................ Problems....................................................................................... References and Bibliography.......................................................

375 377 378 384 388 389 392 395 396 397 398 399

15 Limit Load and Shakedown Load of Pressures Vessel

401

15.1 Introduction ............................................................................ 15.2 Theorems of Limit Analysis of Structures............................... 15.3 Unified Solution of Limit Pressures for Thin-Walled Pressure Vessel............................................................................. 15.4 Unified Solution of Elastic Limit Pressure for Thick-Walled Cylinders ............................................................... 15.5 Unified Solution of Plastic Limit Pressure for Thick-Walled Cylinder................................................................. 15.6 Statical Shakedown Theorem (Melan Theorem) ....................... 15.7 Unified Solution of Shakedown Pressure for Thick-Walled Cylinder................................................................. 15.8 Effects of Yield Function on the Plastic Limit Pressure and Shakedown Pressure of Thick-Walled Cylinders ................. 15.9 Connection between Shakedown Theorem and Limit Load Theorem ............................................................. Summary ....................................................................................... Problems.......................................................................................... References and Bibliography..........................................................

401 402 403 406 416 423 425 430 434 435 436 437

Indexes Author Index ..................................................................................................... Subject Index.....................................................................................................

441 445

Notations

Stresses and Invariants σ1 , σ 2 , σ 3 σ13 , σ 12 , σ23

m σr , σθ , σz r

r

σr , σ z , σθ σ ij σ τ 13 τ 12 , τ 23 µσ µ τ µτ ′

r

θ τ 8 or τ oct σ 8 or σ oct

I1 , I2 , I3

σm

S1 , S2 , S3 J1 , J2 , J3 K I , K II , K III

major principal stress, intermediate principal stress and minor principal stress normal stresses acted on the orthogonal octahedron element intermediate principal stress state parameter radial stress, circumferential stress and axial stress in polar coordinates residual stresses of the cylinder in polar coordinates stress tensor normal stress maximum principal shear stress intermediate shear stress or minimum shear stress Lode stress parameter twin-shear parameter for stress state µτ = τ 12 / τ 23 , µτ ′ = τ 23 / τ 13 stress angle corresponding to the twin-shear parameter octahedral shear stress octahedral normal stress invariants of the stress tensor σ ij hydrostatic stress or mean stress deviatoric stresses invariants of the deviatoric stress tensor stress-intensity factors for mode-I, mode -II and mode-III

Strain and Flow Vector İ1, İ2, İ3 İe İp dİe dİp d ε ij e

principal strain elastic strain plastic strain elastic strain increment plastic strain increment elastic strain increment tensor

XX

Notations

d ε ij p İij

ε r , εθ εz ε r , εθ

Cijkl dλ {a1}, {a2}, {a3} C1, C2, C3 or C1′ , C2′, C3′

plastic strain increment tensor strain tensor radial and circumferential strain longitudinal strain radial and circumferential strain stiffness tensor proportional positive scalar factor flow vectors parameters defining the yield surface

Material Parameters σy σt σc α

m τ 0 or τ y

b β

C0 Ct Cuni

ϕ0 ϕt ϕuni

E G λ ν κ

K I c , K II c , KIII c

yield stress uniaxial tensile strength uniaxial compressive strength ratio of tensile strength to compressive strength compressive-tensile strength ratio of materials pure shear strength or shear yield strength of materials failure criterion parameter in the unified strength theory coefficient in the unified strength theory that represents the effect of the normal stress on failure cohesive strength twin-shear cohesion unified cohesion friction angle twin-shear friction angle unified friction angle elastic modulus (Young’s modulus) shear modulus Lame constant Poisson’s ratio hardening parameter of material stress-intensity factors of materials under mode-I, mode -II and mode-III

Miscellaneous f, f ′ F, F ′ ρ

u , v, w [σ ] p

yield criterion function yield criterion function or fracture criterion function density of the material displacements σ allowable tensile stress, [ σ ] = t n internal pressure subjected to the cylinder

Notations

pe pp p max r ri , re rp

elastic limit pressure plastic limit pressure shakedown pressure of the cylinder radial variable the internal and external radii of the cylinder plastic zone radius of the cylinder subjected to internal pressure p

XXI

1 Introduction

1.1 Linear Elasticity A structure deforms when it is subjected to external forces. The deformation is elastic if it is reversible, that is, if the deformation vanishes instantaneously as the external forces are removed. It is also assumed that the relationships of forcedisplacement and stress-strain are linear. Most engineering materials possess to a certain extent the property of linear-elasticity. The stress states of materials in structures are usually biaxial and triaxial, or in general multiaxial or polyaxial. It is very important to see how the stress combinations affect the strength of material and structure. Serious errors may be resulted if the uniaxial stress assumptions are extended directly to the multiaxial stress state. It will be assumed that the material of an elastic structure is homogeneous and continuously distributed over its volume so that the smallest element cut from the structure possesses the same specific physical properties as the structure. It will also be considered that the material of a structure is isotropic, i.e., the properties are the same in all directions. On the other hand, engineering materials are generally very complicated in compositions. The important material steel, for instance, consists of various kinds of crystals oriented in different directions. The material is very far from being homogeneous in microscope scale. The solutions in view of the theory of elasticity, however, based on the assumptions of homogeneity and isotropy can be applied to steel structures with very great accuracy on the macro-scale level. The explanation is that the crystals are very small; there are millions of them in one cubic inch of space. While the elastic properties of a single crystal may be very different in different directions, the crystals are ordinarily distributed at random and the elastic properties of larger pieces of metal represent averages of the properties of the crystals. Therefore, as long as the geometrical dimensions of a structure are very huge in comparison with the dimensions of a single crystal the assumption of homogeneity can be used with very high accuracy. And if the crystals are orientated randomly the material can be treated as isotropic (Timoshenko and Goodier 1970; Fung 1977). The assumptions of isotropy and homogeneity for materials are also used in plasticity. Discussions of the plasticity for heterogeneous and anisotropic materials are not in the scope of this book.

2

1 Introduction

1.2 Classical Plasticity The deformation of a material is plastic if it is irreversible. A brittle material such as glass, concrete, or rock under tension has only elastic deformation before it fails. On the other hand, metals, rocks and concrete under high confining pressure can undergo substantial plastic deformation before failure and therefore show ductile material properties. The " Theory of Plasticity " or " Plasticity " is a branch of solid mechanics regarding the plastic deformation and the limit load carrying capacity of materials and structures. It deals with the theories and methods of yield initiation of materials under complex stress state and calculation of stresses and strains in a deformed structure after part or the whole structure has yielded. It is necessary, as for elasticity, to establish equations of equilibrium and compatibility and to determine the experimental relations between stress and strain, besides , a condition of yield initiation is needed. It is called yield criterion or yield function. In 1864, Tresca presented two notes dealing with the experimental investigations on plastic flow of metals under great pressure to the French Academy. He first postulated a yield condition for the continuum problem. It is the well-known Tresca yield criterion. Saint-Venant (Barre de Saint-Venant 1797–1886) was the first to set up the fundamental equations of plasticity and to use them to solve several practical problems. The fundamental equations of plasticity are based on the following assumptions. 1. The volume of materials does not change during plastic deformation; 2. The directions of principal strains coincide with the directions of principal stresses; 3. The maximum shearing stress at each point is equal to a specific constant. It means that the Tresca criterion was used as a yield condition. Sometimes, it is referred as the maximum shear stress criterion or single-shear criterion. The yield surface of the Tresca criterion in stress space and its yield locus in deviatoric plane are shown in Fig. 1.1. The yield loci and the yield surfaces will be described in detail in Chapter 6.

Fig. 1.1 Yield surface of the Tresca criterion in stress space

1.2 Classical Plasticity

3

Using these hypotheses, Saint-Venant solved several problems such as torsion of circular shafts, pure bending of rectangular prismatic bars, and the plastic deformation of hollow circular cylinders under the internal pressure. In fact, SaintVenant initiated the study of a complete new field of solid mechanics. SaintVenant called the new subject "Plasticodynamics" . Now plasticity has been the object of considerable research. Prandtl (Ludwig Prandtl 1875–1953) made further progress in the field of plasticity. He solved the more complicated two-dimensional problem of a semiinfinite body under a uniform pressure p distributed over a strip of width. He obtained the limit pressure plimit of strip as follows

§ π · p lim it = σ s ¨1 + ¸ © 2¹ The first systematic treatment of plasticity was given by Nadai in 1931. Rapid progress in plasticity began with the appearance of the paper of Prandtl and the book of Nadai. After the Second World War, the subject of plasticity constitutes an important branch in the solid mechanics. Some books relating the plasticity were published near 1950 by Sokolovsky (1946), Freudental (1950), Hill (1950), Nadai (1950), Prager and Hodge (1951) et. al. After the Tresca yield criterion, the Huber-von Mises yield criterion was proposed by Huber in 1904 and von Mises in 1913. The yield surface of the HuberMises yield criterion in stress space and its yield locus in deviatoric plane are shown in Fig.1.2.

Fig. 1.2 Yield surface of the Huber-von Mises criterion in stress space

The classical plasticity is widely applied in mechanical engineering and metal forming. It is assumed by the Tresca criterion and the Huber-von Mises criterion that these materials have the same strength in both tension and compression and the ratio of shear yield stress Ĳy to the tensile yield stress ıy is Ĳy/ıy=0.5 based on the Tresca criterion or 0.577 on the Huber-von Mises criterion.

4

1 Introduction

In 1961, a new yield criterion was proposed by Haythorthwaite and Yu. It is introduced from the maximum deviatoric stress by Haythorthwaite and the twinshear stresses by Yu, and referred to respectively as the maximum deviatoric stress yield criterion and the twin-shear yield criterion. The yield surface of the twinshear yield criterion in stress space and its yield locus in ʌ plane are shown in Fig.1.3. The twin-shear yield criterion is adapted for those material have the same strength in tension and compression and the ratio of the shear yield stress Ĳy to the tensile yield stress ıy is Ĳy/ıy = 0.667. The mathematical expression of the twinshear yield criterion is linear. It is convenient for analytical solution of limit analysis of structure.

Fig. 1.3 Yield surface of the Twin-shear criterion in stress space

The yield loci in deviatoric plane and meridian plane of the three yield criteria are shown in Fig.1.4.

Fig. 1.4 Yield loci of the three yield criteria

1.3 Concrete Plasticity

5

Classical plasticity is widely used for metallic materials. However, classical plasticity models are not able to predict basic failure phenomena of rocks, soils, concrete, polymers and other materials. Applications in concrete structural engineering, geotechnical engineering, mining and petroleum engineering, nuclear power plant, underground excavation, structure safety problems under earthquake, and solid mechanics problems at meso/micro scales call for more realistic and more accurate solutions. Now developments in plasticity theory is an active field of mechanics. The concrete plasticity, soil plasticity, rock plasticity and computational plasticity etc. are developed.

1.3 Concrete Plasticity Concrete as a structural material has been used widely in many major constructions such as tall buildings, bridge, dam, offshore platforms, reactor vessels, nuclear containment structures, etc. Plastic analysis of these structures has become increasingly important. Concrete is a composite material, consisting of coarse aggregate and a continuous matrix, which itself comprises a mixture of cement paste and smaller sand particles. Its physical behavior is quite complex. In engineering application, only the mechanical behavior instead of the composition of the material is concerned, which is developed on the basis of a homogeneous continuum. Also, the material is assumed to be initially isotropic. In recent years, a good progress has been achieved in the area of constitutive modeling of concrete materials. Various predictive models with two-parameter, three-parameter and multi-parameter have been proposed and used for analysis of concrete structures. The models are based on the principles of continuum mechanics, neglecting the microstructure effect of the concrete materials. To this end, nonlinear elasticity and plasticity are found adequate in characterizing the macroscopic stress-strain behavior of concrete. The theory of concrete plasticity, i.e. the basic concepts and applications of plasticity modeling to concrete materials were presented by Chen (1982) and Nielsen (1984, 1999). Systematical descriptions on the " Plasticity in Reinforced Concrete" and " Limit Analysis and Concrete Plasticity" were given. The Mohr-Coulomb strength theory and some multi-parameter criteria are widely used in concrete plasticity. The yield locus of the Mohr-Coulomb strength theory in deviatoric plane is shown in Fig.1.5. The solid line is the yield locus of the generalized twin-shear criterion (Yu et al. 1985).

6

1 Introduction

Fig. 1.5 Two bounds of the convex yield criteria

1.4 Soil Plasticity Soils are complex materials consisting of solid, air and water. It exhibits a wide range of behavior depending on classification, stress history, void ratio, density and characteristics of the disturbing force. The plastic behavior of soils was studied by Roscoe, Schofield and Thurairajah (1963), Roscoe (1968), Roscoe and Burland (1968), Schofield and Wroth (1968) et al in Cambridge University. Soil Plasticity was presented by Roscoe (1968), Schofield and Wroth (1968), Chen (1975) and Salencon (1977) in 60’s and 70’s of the last century and continued by Chen and Baladi (1985). The soil plasticity was also implemented into computational code by Zienkiewicz and Pande (1977), Zienkiewicz and Humpheson (1977), Zienkiewicz and Mroz (1984), Desai (1984), Vermeer and de Borst (1984), de Boer R (1988) and others. Over the last 30 years, significant advances in this area have led to the development of several constitutive models, which may efficiently represent the behavior of soils subjected to complex stress. Now, the soil plasticity is still one of the most active research areas. The Mohr-Coulomb strength theory (Mohr 1900) and the Drucker-Prager (1952) criterion are widely used in soil plasticity. The yield loci in deviatoric plane and meridian plane of the Drucker-Prager criteria and the Mohr-Coulomb criterion are shown in Figs.1.6 and 1.7. Two bounds of failure criteria are shown in Fig.1.8. Systematical descriptions on the soil mechanics and applications were given by Chen (1975), Salencon (1977) and Chen and Baladi (1985), Zeng, Shen and Gong (2002). Soil plasticity based on the Critical State Soil Mechanics were described by Schofield and Wroth (1968), Atkingson & Bransby (1978), Atkingson (1981) and Wood (1990).

1.5 Rock Plasticity

7

Fig. 1.6 Some varieties of the Drucker-Prager criteria

Fig. 1.7 Yield loci of the Drucker-Prager criteria

Fig. 1.8 Yield loci of the two bounds (single-shear and twin-shear criteria)

1.5 Rock Plasticity The plastic behavior of rock was not generally known until 60’s of the last century when the rigid test equipment was produced. The first congress of international society of rock mechanics was hold in Lisbon in 1966. The flow behavior of rocks were studied by Broms (1966), Goodman, Taylor and Brekke (1968) and others. The bearing capacity of rock and concrete block was studied by Chen and Drucker (1969). Non-associated plasticity for soils, concrete and rock were studied by Vermeer and de Borst (1984) et al.

8

1 Introduction

The Mohr-Coulomb strength theory and the Hoek-Browm (1980) criterion are widely used in rock plasticity. “Finite Element Code for Soil and Rock Plasticity” was presented by Vermeer (1991, 1998). The concept of plastic zone of rock is widely used for rock mechanics and engineering.

1.6 Generalized Plasticity The theory of plasticity was originally developed for the description of the behavior of metallic materials. From the microscopic point of view, the deformational mechanisms of metal are quite different from those of concrete, rock and soils. The former is due to the arrangement of dislocations of polycrystals, while the later is due to the initiation and nucleation of microcracks at the aggregate-mortar interface as well as through the mortar, air or cracks. However, if we do not limit our interpretations of the behavior "plastic" and "yielding" in the usual sense, the classical theory of plasticity can be extended to approximate the concrete, rock and soils behavior under various circumstances (Chen 1978). In other words, the theory of plasticity, when not interpreted too narrowly, provides a very flexible mathematical model that can be used to describe a wide variety of behaviors of concrete, rock and soils. The continuum theory of plasticity was given by Khan et al. (1995). The generalized stress-strain behaviour of wet clay was studied by Roscoe and Burland (1968). The generalized cap model for geological materials was studied by Sandler, DiMaggio and Baladi (1976). The term of Generalized Plasticity was introduced by Zienkiewicz and Mroz (1984), Pastor and Zienkiewicz (1986), and by Pastor, Zienkiewicz and Chan (1990). The word of ‘generalized’ means the extension of plastic conception for metallic materials to geomaterials. Now, generalized plasticity is widely studied and applied in literature and engineering.

1.7 Generalized Plasticity Based on the Unified Strength Theory Great effort has been devoted to the formulation of yield criteria for various materials during the past 100 years (Yu 2002). Most yield criteria are suitable for only a certain type of materials. The plasticity theory for metallic materials is mainly based on the Tresca yield criterion and the Huber-Mises yield criterion. The plasticity theory of soils is mainly based on the Drucker-Prager criterion; and the plasticity theory for concrete and rock is mainly based on the Mohr-Coulomb criterion. What is the relationship among various yield criteria and different “Plasticity”? Many scientists have devoted considerable effort to this topic. Based on a unified mechanical model that takes into account the effects of all the stress components on the failure of materials, a new unified strength theory that has a unified mathematical expression was proposed by Yu in 1991. The Mohr– Coulomb strength theory, the twin-shear stress theory, and many other new criteria

1.7 Generalized Plasticity based on the Unified Strength Theory

9

can be deduced from the unified strength theory. A relationship among most of the prevailing failure criteria and yield criteria is established The unified strength theory contains two families of yield criteria for metal materials and geomaterials. The first family is the convex yield criteria. A series of convex yield criteria can be deduced from the unified strength theory by giving a certain value to material parameter b (0 0, σ

2

= σ 3 < 0, uniaxial tension, equal biaxial compression stress state.

′

If µ τ = µ τ = 0.5 (stress angle equals θ = 30 o ), the corresponding stress states are as follows: 1. σ

2

2. σ

2

1 (σ 1 + σ 3 ) = 0 , pure shear stress state; 2 = (σ 1 + σ 3 ) / 2 > 0, biaxial tension and uniaxial compression stress state;

3. σ

2

= (σ 1 + σ 3 ) / 2 < 0, uniaxial tension and biaxial compression stress state.

=

If µ τ = 0 ( µ τ ′ = 1 , stress angle equals θ = 60 o ), then the corresponding stress states are as follows:

2.7 Stress State Parameters

29

1. σ 1 = σ 2 = 0, σ 3 < 0, uniaxial compression stress state; 2. σ 1 = σ 2 > 0, σ 3 = 0, equal biaxial tension stress state; 3. σ 1 = σ 2 > 0, σ 3 < 0, equal biaxial tension and uniaxial compression stress state. According to the twin-shear stress parameters and the magnitude of the two smaller principal shear stresses, the stress state can be divided into three kinds of conditions as follows: 1. Extended tension stress state, that is, τ 12 > τ 23 , 0≤ µτ ′ < 0.5 von Mises

Mild steel

Solid bars

0.45–0.49

Tresca

Tubes

–

von Mises

Tubes

–

Tubes

–

von Mises von Mises von Mises near twin shear

Review work

–

No one agreed

Tubes

–

Tresca, von Mises

Tubes

–

von Mises

Tubes

–

von Mises

Tubes

–

von Mises

Tubes

0.54

von Mises

Tubes

–

> von Mises

Tubes Tubes Tubes

– – –

von Mises > von Mises von Mises

Lode 1926 Ros & Eichinger 1926 Taylor & Quinney 1931 Marin 1936

Iron, mild steel, nickle, copper Mild steel Aluminum, copper, Mild steel Mild steel

Morrison Mild steel 1940, 1948 Davis 1945 Copper, Davis and Parker medium carbon 1948 steel Osgood 1947 Aluminum alloy Cunningham et al. Magnesium alloy 1947 Bishop and Hill 1951 Polycrystals Fikri and Johnson Mild steel 1955 Marin and Hu 1956 Mild steel Naghdi et al. 1958 Aluminum alloy Hu and Bratt 1958 Aluminum alloy

5.2 Some Experimental Data of Metallic Materials

99

Table 5.1. (Continue) Researchers

Materials

Ivey 1961 Aluminum alloy Bertsch and Findley 1962 Aluminum alloy

Specimen

Ĳ s /ı s

Tubes Tubes

o.66 –

Suitable Criterion

Twin shear von Mises

Mair and Pugh 1964

Copper

Tubes

–

Miastkowski 1965

Brass

–

–

von Mises Twin shear von Mises

Rogan 1969

Steel

tubes

0.5

Tresca

–

von Mises

0.64

near Twin shear between Tresca and von Mises

Low Pisarenko et al. 1969 Copper, Cr-steel temperature Dawson 1970 Polycrystals – Phillips et al. Elevated Aluminum 1970, 1972 temperature Deneshi et al. 1976

Aluminum, Copper

Winstone 1984

Nickel alloy

Ellyin 1989 Wu and Yeh 1991 Ellyin 1993 Ishikawa 1997

Titanium Aluminum stainless steel Titanium Stainless steel

Low temperature Elevated temperature Tubes Tubes Tubes Tubes

0.53 0.6

> von Mises

0.7

Twin shear

0.66

Twin shear

0.58 0.66–0.7 0.62–0.7 0.6–0.63

von Mises Twin shear – > von Mises

The unified strength theory under σ − τ combined stress can be expressed as 2+b b σ 2 + 4τ 2 + σ = σs , 2 + 2b 2 + 2b b 2+b f = σ 2 + 4τ 2 − σ = σs , 2 + 2b 2 + 2b f =

when σ ≥ 0

(5-1a)

when σ ≥ 0

(5-1b)

The corresponding yield loci are shown in Fig. 5.4.

Fig. 5.4 Yield loci of the unified yield criterion under σ − τ combined stress state

100

5 Reasonable Choice of a Yield Function

It is seen that: 1. The unified yield criterion almost encompasses various yield criteria of materials under (σ −τ ) combined stresses. 2. The yield loci are convex when the parameter b varies from 0 to 1. It should be noted that the yield loci in the three–dimensional stress state and the plane stress state will be nonconvex when b >1 or b < 0. The nonconvex yield surfaces have been discussed in Chap. 3. 3. The differences between various yield functions are obvious under simple shear stress. The ratios of pure shear yield stress τ s to tensile yield stress σ s of some typical yield criteria are shown as follows: single-shear yield criterion (Tresca yield criterion): τ s = 0.5σ s; Huber-von Mises yield criterion: τ s=0.577σ s; twin-shear yield criterion: τ s = 0.667σ s; maximum tensile strain theory: τ s=0.769σ s (ν=0.3); maximum normal stress theory: τ y =1.0σ y. After the comparison of the shear yield strength and tensile yield strength among the 30 materials, Kishkin and Ratner (see Onksov 1963) divided the metals into four kinds according to the ratio of the shear yield strength to tensile yield strength τ s /σs as follows: 1. τ s /σ s ≅ 0.50 (0.48̢0.53, five materials), which agrees with the single-shear yield criterion (Tresca yield criterion) or with the unified yield criterion when b=0. 2. τ s /σ s ≅ 0.58 (0.54̢0.62, nine materials), which agrees with the Huber-von Mises yield criterion, or with the unified yield criterion when b =1+ 1/(1+ 3 ) or b=1/2. 3. τ s /σ s ≅ 0.68 (0.67̢0.71, eight materials), which agrees with the twin-shear yield criterion, or with the unified yield criterion when b = 1 . 4. τ s /σ s < 0.40 (0.31̢0.41, eight materials), which gives a nonconvex result that does not agree with existing criteria. This kind of result is not indicated by any theoretical criterion, but matches the unified yield criterion when b=̢1/3.

With regard to the ratio of shear strength to tensile strength of metals, the values in some manuals are 0.52~0.63 (carbon steel) and 0.65~0.78 (alloy steel). Generally, the ratio of shear yield stress τ y to the tensile yield stress σ s is different for different materials. According to the convexity of yield surface, shear yield strengths are in the range of τ s=(0.5~0.667)σ s for those metallic materials that have same strength both in tension and compression. Yield stresses of metallic materials are higher than τ s /σ s =0.5. Many yield stresses of high-strength steel, high-strength alloys, and non-metallic materials are higher than τ s=0.667. These kinds of materials may be the SD (strength difference in tension and in compression) materials.

5.3 Reasonable Choice of a Yield Function for Non-SD Materials Because of the significant differences in shear strengths of materials, the yield function can be selected on the basis of the ratio of the shear yield stress τ s to the tensile yield stress σ s.

5.3 Reasonable Choice of a Yield Function for Non-SD Materials

101

According to the unified yield criterion f = σ1 − f′=

1 1+ b

1 1+ b

(bσ 2 + σ 3 ) = σs ,

σ2 ≤

if

( σ 1 + σ b 2 ) − σ 3 = σs ,

if

1 (σ 1 + σ 3 ) 2

σ2≥

1 (σ 1 + σ 3 ) 2

(5-2a) (5-2b)

where b is a yield criterion parameter that represents the effect of the intermediate principal shear stress on the yield of materials and lies in the range of 0 ≤ b ≤ 1 when the yield surfaces are convex. In the case of critical state in pure shear σ 1 = τ, σ 2 = 0 , σ 3 = −τ and τ = τ s , we have σ1

= τ s , σ 2 = 0 , σ 3 = −τ s , and

σ2

= (σ 1 + σ 3 ) / 2 = 0

(5-3)

hence, we can use the anyone of Eqs. (5-2a) or (5-2b). Substituting Eq. (5-3) into the equation of the unified yield criterion Eq.(5-2a) or Eq. (5-2b), the relation among the tensile yield stress σ s, shear yield stress τ s and the parameter b in the unified yield criterion is obtained as (5-4)

(2+b) τs =(1+b) σ s

The parameter b can be determined from the ratio of shear yield stress to tensile yield stress as follows: b=

2τs − σs σs

− τs

=

2 ατ −1 1 − ατ

,

(5-5)

Inversely, the ratio of shear yield stress to tensile yield stress can be given as ατ

=

τs σs

=

b +1 b+2

(5-6)

The unified yield criterion establishes clear and simple relations among the various yield criteria. It also provides a method to choose the appropriate yield criterion. It can be obtained from the unified yield criterion as follows: (1) First, we need know the tensile yield stress σ s and shear yield stress τ s; (2) Second, the ratio of the shear yield stress to the tensile yield stress α τ= τ s /σ s can be determined ; (3) then, substituting α τ into Eq. (5-5), the parameter b is determined; (4) at last, substituting b into Eq. (5-1a) and (5-1b), an appropriate yield criterion is obtained. For example, if the ratio of the shear yield stress to the tensile yield stress is α τ = τ s /σ s = 0.6, the parameter b can be determined from Eq. (5-5) is b=1/2. Substituting

102

5 Reasonable Choice of a Yield Function

b=1/2 into Eq.(5-2a) and (5-2b), then an appropriate yield criterion is given as follows: 1 1 when σ 2 ≤ (σ 1 + σ 3 ) (5-7a) f = σ 1 − (σ 2 + 2σ 3 ) = σ y , 2 3 f ′=

1 3

when σ 2 ≥

(2σ 1 + σ 2 ) − σ 3 = σ y ,

1 (σ + σ 3 ) 2 1

(5-7b)

This means that a new yield criterion is introduced. This new yield criterion can be approximated to the Huber-von Mises yield criterion. If the ratio of the shear yield stress to the tensile yield stress is α τ = τ s /σ s = 0.667, the parameter b can be determined from Eq. (5-5) is b=1. Substituting b=1 into Eq.(5-2a) and (5-2b), the yield criterion is given as follows: f

if

σ2 ≤

1 (σ + σ 3 ) 2 1

′ = (σ1 + σ 2 ) − σ 3 = σ s , if

σ2 ≥

1 (σ + σ 3 ) 2 1

1

= σ1 − (σ 2 + σ 3 ) = σ s , 2

1

(5-8a)

(5-8b) 2 It is the twin-shear yield criterion proposed by Yu in 1961. Various new yield criteria may be introduced when the ratio of the shear yield stress to the tensile yield stress is different. f

5.4 Experiments for Iron under σ–τ Stress State A combined σ –τ stress state can be produced in thin tube under axial force and torsion. For brittle materials, such as iron, the limit locus of the materials is asymmetrical in the τ –coordinate because its tensile strength is different from its compressive strength. Since the ratio of the tensile-compressive strength is different, two material constants are required, such as tensile strength σ t and compressive strength σc , tensile strength σ t and the tensile-compressive ratio α =σ t /σc , or compressive strength σ c and the compression-tension strength ratio m=σ c /σ t. For example, the limit loci corresponding to different tension-compression strength ratios of twin-shear yield function are shown in Fig. 5.5. The comparison of the experimental results of iron with the twin-shear yield function are given. A series of experiments of iron under σ −τ combined stress states were conducted by Grassir and Cornet (1949), Mair (1968) and Coffin (1950). Their experimental results are shown in Fig. 5.6.

5.5 Experiments for Concrete under Complex Stress

103

Fig. 5.5 Comparison between experimental results for iron and twin-shear strength theory (Grossir and Cornet 1949; Coffin 1950)

5.5 Experiments for Concrete under Complex Stress The experimental results of concrete with the twin-shear yield function are shown in Fig.5.6.

Fig. 5. 6 Comparison between experimental results for concrete and twin-shear stress theory

The primary experiments on limit loci in the ʌ-plane on concrete were conducted by Gachon and Launay of the French National Institute of Technology. A series of limit loci in the ʌ-plane for concrete are given under different hydrostatic pressures. Figs. 5.7 and 5.8 show the limit loci in the ʌ-plane for concrete (Gachon 1972, Launay and Gachon 1973). It can be seen from Figs. 5.7 and 5.8 that although smooth curves can approximate the results, the polygonal line in Fig. 5.8 is closer to the experimental results. Fig. 5.8 shows three groups of experimental limit loci and compares them with yield function. The limit locus of yield function shown in Fig. 5.8 is the unified strength theory with b=1/2. In order to enable comparison, the limit locus of the unified strength theory with b=0 and b=1 under 3p=4 and 8 are also given. Although there are only two data points when 3p=1, which cannot be compared with yield function, other experimental results all agree with the estimation of the unified strength theory with b=1/2. As to the experimental results in Fig. 5.8, they also agree with the unified strength theory with b=1/2.

104

5 Reasonable Choice of a Yield Function

Fig. 5.7 Limit loci in the ʌ-plane for concrete (Gachon 1972)

Fig. 5.8 Comparison between experimental limit loci of concrete and the unified strength theory with b=1/2

In the 1990s, many true triaxial experiments were conducted. Faruque and Chang conducted three groups of experiments on plain concrete. The stress states of these three groups of experiments were (σ 2=σ 3, σ 1), (σ 1 =–σ 3, σ 2) and (σ 1=σ 2, σ 3), i.e., triaxial tension, shear and compression, respectively. Their experimental results can be connected as shown in Fig. 5.9. It can be seen that the experimental results agree with the unified strength theory with b=1. The experimental results for steel fiber concrete obtained by Dong et al. (1993) also agree with twin-shear stress theory.

5.6 Experiments for Rock under Complex Stress

105

Fig. 5.9 Concrete (Faruque and Chang 1990)

From the above experimental results, it can be deduced that the limit loci of concrete in the ʌ-plane lies between the unified strength theory when b=1/2 and b=1. There are lots of experimental data on meridian lines for concrete (see Chen WF 1982). It can be expressed approximately by a two-parameter criterion, giving a straight limit meridian line. Generally, it must be expressed by three-parameter, four-parameter or five-parameter criteria, giving curved limit meridian lines.

5.6 Experiments for Rock under Complex Stress Michelis (1985, 1987) conducted many fine true triaxial experiments on rock and concrete. The results show that the effect of intermediate principal stress σ 2 is an important characteristic for geomaterials. According to the three series of experimental data (Michelis 1985, 1987) three limit loci may be drawn as shown in Fig. 5.10.

106

5 Reasonable Choice of a Yield Function

Fig. 5.10 Marble (Michelis 1987)

The biaxial experiments of rock have also been conducted at the same time. Fig. 5.11 shows the experimental result published by Amadei and Kuberan in the 24th Conference of Rock Mechanics of American in 1984. The dotted line in the figure is the limit line of Mohr-Coulomb strength theory in plane stress state. The solid line is the limit line of the unified strength theory with b=3/4. Compared with the experimental results, there is a large difference between the Mohr-Coulomb theory and the experimental results. Mohr-Coulomb strength theory is too conservative. The limit surface of the unified theory with b=3/4 is close to the experimental results, but in the region of biaxial compressive stress state, it is also too conservative.

Fig. 5.11 Experimental results under biaxial condition for limestone (Amadei et al, 1984)

A granite with properties such as high hardness, high density, high strength and high elastic modulus can be found in the upstream of the Yellow River (China). Its uniaxial compressive strength is σ c =157 MPa; it has elastic modulus G=50 Gpa,

5.6 Experiments for Rock under Complex Stress

107

tensile strength σ t =7.8 MPa, shear strength parameter C0=16 MPa, tgϕ =0.96, the unit weight r =2680 kg/m3 and Possion’s ratio ν = 0.2 . A series of experiments on rock corresponding to different high pressures under the same stress angle were carried out by the Northwest Design and Research Institute (China) and the Wuhan Institute of Rock and Soil Mechanics of the Chinese Academy of Science. The failure strength of rock corresponding to different hydraulic pressures with the same stress angle can be obtained, and then the limit meridian lines of rock under this stress angle can then be obtained. Five stress angles θ =0°, 13.9°, 30°, 46.1°, 60° are adopted, and the corresponding five limit meridian lines are shown in Fig. 5.12. Six sections are adopted in Fig. 5.12 within the range of p=80−200 MPa, and then six limit loci in the ʌ-plane corresponding to different values of p are obtained as shown in Fig. 5.12.

Fig. 5.12 Limit loci in meridian lines and the ʌ-plane

It can be seen that: 1. The strength of granite increases with increase of the hydraulic pressure p. 2. The length of vector q differs corresponding to different stress angles θ in the ʌ-plane when the hydraulic pressure p is constant. Granite shows an obvious stress angle effect. There is an obvious distinction between the circular limit loci of the Drucker–Prager criterion and the experimental results. 3. All the experimental points are located outside the limit loci of the Mohr–Coulomb yield function, and they are closer to that of the twin-shear yield function. 4. The limit meridian line changes with the stress angle. 5. In the process of varying stress angle from θ = 0° to θ = 60°, the value of q increases and reaches q = 262.2 MPa, and then decreases to q =255 MPa. This result agrees with the twin-shear stress theory.

108

5 Reasonable Choice of a Yield Function

5.7 Experiments on Clay and Loess under Complex Stress Soil is a widely used material in structural engineering and geotechnical engineering. The yield function is the basis of soil mechanics and foundation engineering. At present, the axisymmetric triaxial experiments on soil are the elementary tests in soil mechanics and have gradually developed into true triaxial experiments. The early research on failure criteria for soils under true triaxial stress states or plane strain states was done by Shibata and Karube (1965) at Kyoto University, Roscoe (1968), Roscoe and Burland (1968), Wood and Roth (1972) at Cambridge University, Ko and Scott (1967) at Colorado State University, Brown and Casbarian (1965), Sutherland and Mesdary (1969) at the University of Glasgow, Bishop (1971) and Green (1972a) at Imperial College. Fig. 5.13 indicates the experimental results for normally consolidated soil carried out by Shibata and Karube (1965). The experimental results on normally consolidated soil lie almost between the unified strength theory with b=1/4 and b=1/2. They do not agree with the Mohr-Coulomb yield function.

Fig. 5.13 Soil (Shibata and Karube 1965)

Fig. 5.14 shows the experimental results for compactive loess given by Fang in 1986. Fig. 5.15 shows the experimental results under true triaxial conditions for undisturbed loess and remolded loess given by Xing et al. at Xi’an Science and Technological University. The experimental results all agree with the unified strength theory with b=1/2.

5.8 Experiments on Sand under Complex Stress

Fig. 5.14 Compacted loess (Fang 1986)

109

Fig. 5.15 Loess (Xing et al. 1992)

Recently, the limit loci in ʌ-plane of undisturbed loess soils is obtained by Yoshimine et al. at Tokyo Metropolitan University, Tokyo, Japan. It is shown in Fig.5.16. It is in agreement with the twin-shear strength theory or the unified strength theory with b=1.

Fig. 5.16 Loci in ʌ-plane of undisturbed loess soils (Yoshimine et al. 2004)

5.8 Experiments on Sand under Complex Stress A well-known experiment on sand was carried out by Green and Bishop (1969). Fig. 5.17 shows the experimental results. Fig. 5.18 shows the dynamic strength for sand obtained by Zhang and Shao (1988). The results are close to the unified strength theory with b=3/4 and b=2/3, respectively.

110

5 Reasonable Choice of a Yield Function

Fig. 5.17 Sand (Green and Bishop 1969)

Fig. 5.18 Dynamic strength of sand (Zhang and Shao)

Fig. 5.19 shows the comparison between the unified strength theory (b=3/4) with experimental limit locus in the ʌ-plane for sand obtained by Nakai and Matsuoda (1983) in Japan.

Fig. 5.19 Limit locus in the ʌ-plane for Toyoura Sand (Nakai and Matsuoka)

Fig. 5.20 a, b shows the experimental results on loose sand and dense sand, given by Dakoulas and Sun (1992). The results agree with the unified strength theory with b=1/2 and b=3/4, respectively.

5.8 Experiments on Sand under Complex Stress

(a) loose sand

111

(b) dense sand

Fig. 5.20 Limit loci for Ottawa fine sand: (a) loose sand; (b) dense sand (Dakoulas and Sun 1992)

The limit loci in the ʌ-plane for sand obtained by Ko and Scott (1968) are shown in Figs. 5.21. The results agree with the unified strength theory with b=1/2.

Fig. 5.21 Limit locus in the ʌ–plane for medium sand (Ko and Scott 1968)

Fig. 5.22 shows the static and dynamic strength for saturated sand under complex stress states obtained by Zhang and Shao (1988).

112

5 Reasonable Choice of a Yield Function

Fig. 5.22 Static and dynamic limit loci for saturated sand (Zhang and Shao 1988)

These experimental data are situated between the limit loci of the unified strength theory with b=1/2 and b=1.

5.9 Reasonable Choice of a Yield Function for SD- Materials It is difficult to choose an appropriate failure criterion for SD (Strength Difference in tension and in compression) materials. The unified strength theory (unified strength theory) establishes a clear and simple relation among the various yield criteria. It also provides a method to choose the appropriate yield criterion. The reasonable choice method can be obtained from the unified strength theory as follows. First, we need know the tensile strength σ t and compressive strength σ c ; Second, the ratio α =σ t /σ c , i.e. the ratio of tensile strength σ t to compressive strength σ c, can be determined Third, if the ratio α =σ t /σ c=1, it means that the tensile strength equals the compressive strength. We can use the unified yield criterion and choose a resonable parameter b, as described in section 5.3 this chapter. At last, if the ratio α =σ t /σ cĮ1, or σ t Į σ c, it is the material with SD effect (effect of Strength Difference in tension and in compression). We have to use the two-parameters yield function. The unified strength theory can be used as a two-parameters yield function. The mathematical equation is expressed as follows:

when σ 2 ≤ σ 1 + α σ 3 1+α

(5-9a)

σ1 +α σ 3 1 (σ1 + bσ 2) −ασ3 = σ t, when σ 2 ≥ 1 +α 1+ b

(5-9b)

F = σ1 −

F'=

α

1+ b

(bσ 2 + σ 3) = σ t,

5.10 The Beauty of the Unified Strength Theory

113

It is linear and simple. The difficulty is how to choose the failure criterion parameter b. A method is using the true triaxial test for every material, however, it is expensive and difficult. One simple method is choosing the intermediate value of b, which is a mediated criterion between the lower bound (the Mohr-Coulomb strength theory) and upper bound (the twin-shear strength theory). The mathematical equation is also linear and simple, it is shown as follows: F = σ1 −

α

3

(σ 2 + 2σ 3 ) = σ t , σ 2 ≤

σ1 + ασ 3

1+α

1 σ +ασ 3 F′ = (2σ1 +σ 2 ) −ασ 3 = σ t , σ 2 ≥ 1 3 1+ α

(5-10a)

(5-10b)

This is a new failure criterion deduced from the unified strength theory with b=1/2. Since the Drucker–Prager criterion cannot match with the practice, this criterion is more reasonable and can be substituted for the Drucker–Prager criterion. According to the experimental data described in sections 5.4 to 5.8. The strength theory parameter b can be recommended as follows: b=1/2 to b=1 for concrete, rock and high strength steel and alloy; i.e. 1/2 ≤ b ≤ 1 b=1/4 to b=3/4 for soils and soft rock, i.e. 1/4 ≤ b ≤ 3/4.

5.10 The Beauty of the Unified Strength Theory What is the beauty of a thing? Beauty is the qualities that give pleasure to the senses or lift up the mind or spirit (Longman Dictionary of Contemporary English 1978). Beauty is the combination of qualities that give pleasure to the senses or to the moral sense or the intellect (The Oxford Advanced learner’s Dictionary of Current English 1963). A thing of beauty is a joy for ever (Keats, John 1795–1821). What is the beauty of science? Six elements of the beauty of mathematics and physics were described by Tzanakis (1997), Kosso (1999), Shen (2004) and others. Six relevant points about the beauty of mathematics and physics are: (a) Clarity: the conceptual clarity in the foundations and the development of a theory. (b) Simplicity, Elegant and economic reasoning. It is also said that: “Science advocates simplicity” (Shen ZJ 2004). (c) Unification of a priori unrelated concepts, methods, theories or phenomena. (d) The “naturality” of a theory. (e) Symmetry. (f) Analogy The beauty of the unified strength theory was first proposed and studied by Fan, et al. (2001) of Nanyang Technological University in Singapore. Fan, et al. (2001) a lecture at an International Congress on Computational Mechanics held at Sydney in 2001, Australia. The power and unification of the unified strength theory are discussed.

114

5 Reasonable Choice of a Yield Function

A closing lecture was delivered by Yu et al. at the International Symposium on the Developments in Plasticity and Fracture, Centenary of M.T.Huber Criterion, in Cracow, Poland (Yu et al. 2004). The Beauty of Strength Theories was discussed. The unified strength theory was derived based on the concept of multiple slip mechanism and the multi-shear element model or twin-shear element. Multi-shear element and twin-shear element are spatial equipartition available for continuum mechanics, which are shown in Fig. 5. 23.

Fig. 5.23 Multi-shear element and twin-shear element

It is obvious that this element model is different from the principal stress element used in common continuum mechanics. There are three sets of principal shear stress and normal stress acted on the sections, on which the principal shear stress is acted respectively. However, there are only two independent components in three principal shear stresses, because the maximum shear stress τ 13 equals the sum of the other two, i.e. τ 13 = τ 12 + τ 23 . Considering the two larger principal shear stresses and the corresponding normal stress and their different effects on failure of materials, the mathematical modeling of the unified strength theory can be formulated as (Yu-He 1991; Yu 1992, 1994) F = τ13 + bτ12 + β (σ 13 + bσ 12 ) = C , when τ12 + βσ 12 ≥ τ 23 + βσ 23

(5-11a)

F ' = τ13 + bτ 23 + β (σ 13 + bσ 23 ) = C , when τ12 + βσ 12 ≤ τ 23 + βσ 23

(5-11b)

where b is a coefficient of the effect of the other principal shear stresses on the strength of materials. Introducing a tension-compression strength ratio α = σ t σ c . The unified strength theory is expressed in terms of three principal stresses as follows F = σ1 − F '=

α (bσ + σ ) = σ t, 1+ b 2 3

when σ 2 ≤ σ 1 +ασ 3 1 +α

σ 1 +α σ 3 1 (σ1 + bσ 2 ) −ασ3 = σ t , when σ 2 ≥ 1 +α 1+ b

(5-12a)

(5-12b)

5.10 The Beauty of the Unified Strength Theory

115

The mathematical expression of the unified strength theory is simple and linear, but it has rich and varied contents, and can be easily changed to suit many new conditions. It possesses fundamentally all the expected characteristics for a unified strength theory. A series of limit loci of the unified strength theory on the deviatoric section are shown in Fig. 2 and Fig. 3 in Preface of this book. Several characteristics of the unified strength theory are discussed as follows: (1) Linearity and Simplicity

It is physically meaningful and can be expressed by mathematically simple equation. The formulation of the unified strength theory is linear and convenient to use in applications to analytical solution of plasticity and plastic analysis of structure and computational implementation for numerical solution. (2) Unification

According to Tzanakis (1997) one of six relevant points about the beauty of mathematics and physics is unification of a priori unrelated concepts, methods, theories or phenomena. All the yield criteria and failure criteria are single criterion having various model and expression. The limiting loci of the unified strength theory cover all regions from the Mohr-Coulomb theory to the twin-shear strength theory. The unified strength theory is not a single criterion. It is a series of failure criteria, a system of strength theory. This theory gives a series of new failure criteria, establishes a relationship among various failure criteria, and encompasses previous yield criteria, failure models and other smooth criteria or empirical criteria as special cases or linear approximations. The famous Tresca yield criterion, the Mohr-Coulomb strength theory, the twin-shear yield criterion, the twin-shear strength theory and some others are special criteria of the unified strength theory. The unification can be seen from Figs. 2 and 3 in the Preface and Fig. 4.22 in Chapter 4. The relation among the single-shear theory, the twin-shear theory and a series of new failure criteria can be seen in Fig. 5.24.

116

5 Reasonable Choice of a Yield Function

0 < b π / 2 is in a plane strain state. Boundary surface AE subjected to uniform pressure q, as shown in Fig.8.13. Determine the limit load puni on the surface AB. The slip lines field is illustrated in Fig.8.13. The twin-shear limit load can be expressed as follows. It was given by Zhang,Li and Yin in 1998. π ϕt ) ⋅ exp[ (2γ −π )tgϕt ] − Ct ⋅ ctgϕt 4 2

(8-51)

4sinϕ0 2+ (1+ sinϕ 0)

(8-17)

pt = (q + Ct ⋅ ctgϕt ) ⋅ tg2 ( +

where sinϕt =

Ct = 4C 0 ⋅cosϕ 0 1 , 2 + (1+sin ϕ 0)cosϕt

(8-18)

When q=ıt, the relation between limit loads pt and the ratio of tensile strength to compressive strength of material is shown in Fig. 8.14.

Fig. 8.13 Slip field of obtuse wedge

Fig. 8.14 Limit loads for different materials

8.6 Twin-shear Slip Line Field Theory for Plane Strain Problams

215

When q=0, it is a slope problem. The twin-shear limit load is π ϕt ) ⋅ exp [ (2γ − π )tgϕ t ] − Ct ⋅ ctgϕ t 4 2

pt = (Ct ⋅ ctg ϕt ) ⋅ tg2 ( +

(8-52)

When ĳt=ĳ0, it is the solution for the Mohr-Coulomb maerial. When ĳt=ĳ0=0, it is the solution for the twin-shear material in Į=1. The limit load is π 2

4 3

(8-53)

pt = (1 − + γ )σs

When ĳt=ĳ0=0, and Ct=C0, it is the conventional solution of the Tresca material. π 2

(8-54)

pt = (1 − + γ )σs

8.6.4. Example 4: Acute wedge The twin-shear solution for an acute wedge was obtained by Zhang, Li and Yin in 1998. The acute wedge with angle ∠BAD γ = < π / 2 is in a plane strain state, where ∠ BAC =δ , ∠CAD = ν , and δ + ν =γ . Boundary surface AD is subjected to uniform pressure q, as shown in Fig. 8.15. Determine the limit load pt on the surface AB. The slip lines field is illustrated in Fig. 8.15. The discontinuous line is denoted by AC, which divides the wedge into two regions. The angles between slip Į lines and ȕ lines are 2ȥ. The external load pt is assumed greater than pressure q, then the region ABC (Region I) is a active region. The twin-shear limit load can be expressed as follows: pt = (q + Ct ⋅ ctgϕ t ) ⋅

1 + sin ϕ t sin 2ν ⋅ − Ct ⋅ ctgϕt 1 − sin ϕ t sin 2δ

(8-55)

where ĳt and Ct are the same as those of obtuse wedge (Example 3). When q=ıt, the relation between limit loads pt and the ratio of tensile strength to compressive strength of material is shown in Fig. 8.16.

216

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Fig. 8.15 Slip field of obtuse wedge

Fig. 8.16 Limit loads for different materials

When q=0, it is a slope problem. The twin-shear limit load is pt = (Ct ⋅ ctgϕt ) ⋅

1 + sin ϕ t sin 2ν ⋅ − Ct ⋅ ctgϕ t 1 − sin ϕ t sin 2δ

(8-56)

When ĳt=ĳ0, it is the solution for the Mohr-Coulomb material. When ĳt=ĳ0=0, it is the solution for the twin-shear material in Į=1. The limit load is 4 3

pt = (1− cosγ )σs

(8-57)

When ĳt=ĳ0=0, and Ct=C0, it is the conventional solution of the Tresca material. pt = (1− cosγ )σs

(8-58)

8.6.5. Example 5: Earth Pressure Lateral earth pressure problem is one of important problems in soil mechanics, as shown in Figs. 8.17 and 8.18. Earth pressure problem deals with the magnitude and distribution of lateral earth pressure between a soil mass and an adjoining earthretaining structure. The classical theories on earth pressure are those due to Coulomb (1773) and Rankine (1857). Fig. 8.17 shows a passive earth pressure problem. Fig. 8.18 shows a active earth pressure problem.

8.6 Twin-shear Slip Line Field Theory for Plane Strain Problams

Fig. 8.17 Active earth pressure

217

Fig. 8.18 Passive earth pressure

This problem is also considered as a limit load problem of a slope. The top and the slope side can be looked upon as the limit load problem of wedge, as show in Fig. 8.19a ( γ ≥ π / 2 ) and Fig. 8.19b ( γ ≤ π / 2 ). The weight of soil is not taken into account.

Fig. 8.19 Earth pressure (a) ( γ ≥ π / 2 ) and (b) ( γ ≥ π / 2 )

The active earth pressure can be derived in the case of q >E and γ ≥ π / 2 as follows: π

ϕt

4

2

Eactive = ( q + Ct ⋅ ctgϕ t) ⋅ tg2( +

) ⋅ exp[(π

− 2γ ) ⋅ tgϕ t] − Ct ⋅ ctgϕ t

(8-59)

The passive earth pressure can be derived in the case of E > q and γ ≥ π / 2 as follows: π ϕt ) ⋅ exp[ (2γ − π )tgϕ t ] − Ct ⋅ ctg ϕ t 4 2

pt = (q + Ct ⋅ ctgϕt ) ⋅ tg2 ( +

(8-60)

The active earth pressure can be derived in the case of q >E and γ ≤ π / 2 as follows: pt = (q + Ct ⋅ ctgϕ t ) ⋅

1+ sinϕ t sin2δ ⋅ − Ct ⋅ ctgϕt 1−sinϕ t sin 2δ

(8-61)

218

8 Twin-Shear Slip-Line Field for Plane Strain Problem

The passive earth pressure can be derived in the case of E >q and γ ≤ π / 2 as follows: 1 + sinϕ t sin2ν ⋅ − Ct ⋅ ctgϕt pt = (q + Ct ⋅ ctgϕ t )⋅ 1 − sinϕ t sin2δ

(8-62)

It is the same as Eq.8-55

Summary The twin-shear slip line field theory for plane strain problems based on the twinshear yield function is described in this chapter. The twin-shear slip line field theory for plane strain problems includes orthogonal and non-orthogonal slip line field. It is different from the used orthogonal or non-orthogonal slip line field theories based on single-shear strength theories (Tresca and Mohr-Coulomb materials). The new method can reflect the effect of intermediate principal stress of plane strain, where the intermediate principal stress is the principal stress in z direction. The twin-shear slip theory can be used for those materials with obvious effect of the intermediate principal stress. Five examples are used to illustrate the applications of the twin-shear slip lines field.

Problems Problem 8.1 The extension of a strip with a sufficiently large circular hole for non-SD material was studied by Prager and Hodge (1951) and Kachanov (1971) as shown in Fig. P8.1. The Tresca yield criterion was used in these studies. Can you obtain another study on this subject using the twin-shear slip line field for non-SD material ( α = 1 )?

Fig. P8.1 Extension of a strip with a sufficiently large circular hole

Problems

219

Problem 8.2 Can you obtain a more complete study on the extension of a strip with a sufficiently large circular hole (Fig. P8.1) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.3. The extension of a strip with ideal cuts (crack) for non-SD material was given by Kachanov (1971) as shown in Fig. P8.2. The Tresca yield criterion was used in these studies. Can you obtain a more complete study on this subject using the twinshear slip line field for non-SD material ( α = 1 )?

Fig. P8.2 A ideal cuts (crack)

Fig. P8.3 An angular notches

Problem 8.4. Can you obtain a more complete study on the extension of a strip with ideal cuts (Fig. P8.2) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.5. The extension of a strip with angular notches for non-SD material was given by Kachanov (1971) as shown in Fig. P8.3. The Tresca yield criterion was used in the studies. Can you obtain a more complete study on this subject using the twin-shear slip line field ( α = 1 )? Problem 8.6. Can you obtain a more complete study on the extension of a strip with angular notches (Fig. P8.3) by using the twin-shear slip line field for SD materials (α ≠ 1 )? Problem 8.7. The extension of a strip with circular base for non-SD material was given by Kachanov (1971) as shown in Fig. P8.4. The Tresca yield criterion was used in the studies. Can you obtain a more complete study on this subject using the twin-shear slip line field ( α = 1 )?

220

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Fig. P8.4 Extension of a strip with a circular base

Problem 8.8. Can you obtain a more complete study on the extension of a strip with circular base (Fig. P8.2) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.9. Figure P8.5 shows the slip line field of indentation at the bottom of a flat trench. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.5 Flat trench

Fig. P8.6 Deep vertically sided

Problem 8.10. Figure P8.5 shows the slip line field of indentation at the bottom of a flat trench. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.11 Figure P8.6 shows the slip line field of indentation at the foot of a very deep vertically sided groove. Find the limit load by using the twin-shear slip line field ( α = 1 ). Problem 8.12. Figure P8.6 shows the slip line field of indentation at the foot of a very deep vertically sided groove. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ).

Problems

221

Problem 8.13 Figure P8.7 shows the slip line field of indentation at the top of a flat punch. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.7 Indentation at the top of a flat punch

Problem 8.14. Figure P8.7 shows the slip line field of indentation at the top of a flat punch. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.15. Pure bending of a strip weakened by notches of various shapes was investigated by Green (1953) and Kachanov (1971). Fig. P8.8 shows the slip line field of a strip weakened by one-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.8 Strip weakened by one-sided deep notch with a circular base

Problem 8.16. Figure P8.8 shows the slip line field of a strip weakened by one-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ).

222

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Problem 8.17. Figure P8.9 shows the slip line field of a strip weakened by two-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α = 1 ).

Fig. P8.9 Strip weakened by two-sided deep notch with a circular base

Problem 8.18. Figure P8.9 shows the slip line field of a strip weakened by two-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.19. Figure P8.10 shows a slip line field of a strip weakened by center crack for non-SD materials. Find the slip line field for SD materials.

Fig. P8.10 shows a slip line field of a strip weakened by center crack

Problem 8.20. Figure P8.11 shows the slip line field of a strip with a hole; find the limit pressure for non-SD materials and SD materials.

References and Bibliography

223

Fig. P8.11 Slip line field of a strip with a hole

Problem 8.21. The slip line field and limit pressure were widely studied by some researchers. Figure P8.12 shows the slip line field around a circular hole loaded uniformly with a pressure, find the limit pressure for non-SD materials and SD materials by using the twin-shear slip line field theory.

Fig. P8.12 Slip line field around a hole

References and Bibliography Collins IF (1990) Plane Strain Characteristics Theory for Soils and Granular Materials with Density Dependent Yield Criteria, J. Mech. Phys. Solids., 38(1), 1–25 . Collins IE and Dewhurs, P (1993) A matrix technique for constructing slip-line field solutions to a class of plane-strain plasticity problems. Int. J. Numer. Methods Eng., 7: 357–378. Drucker DC, Greenberg HJ and Prager W (1951) The safety factor of an elastic-plastic body in plane strain. J. Appl. Mech., 18: 371–378. Ford H (1954) The Theory of Plasticity in Relation to Engineering Application. J. AppL Math. Phys., 5: 1–35.

224

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Geiringer H (1930) Beit zum Vollstiindigen ebenen Plastizitits-problem, Proc 3rd Intern. Congr. Appl. Mech, 2: 185–190. Hencky H (1923) Ueber einige statisch bestimmte Faelle des Gleichgewichts in plastischen Koerpern, Z. angew. Math Mech., 3: 245–251. Hill R (1949) The Plastic Yielding of Notched Bars Under Tension, Quart. Mech. AppL Math., 2: 40–52. Hill R (1956), The Mechanics of Quasi-Static Plastic Deformation in Metals, In: Survey in Mechanics, G. K. Batcheler and R. M. Davis eds, Cambridge . Johnson W and Mellor PB (1962), Plasticity for Mechanical Engineers. Van Nostrand, Princeton, N.J. Johnson W, Sowerby R, Venter RD (1982), Plane-Strain Slip Line Fields for Metal Deformation Processes – A Source Book and Bibliography, Pergamon Press . Matsuoka H (2000) Soil Mechanics. Nagoya Technical Institute Press: Nagoya. (in Japanese; Chinese translation, 2004 by Yao NP and Lou T ) Moore ID and and Rowe RK (1991) Objective solutions for bearing capacity of strain-softening soils. In: Beer G, Booker JR and Carter JP eds. Computer Methods and Advances in Geomechanics. Rotterdam: A.A.Balkema, Vol.2,1183–1189. Prager W (1955) The Theory of Plasticity: A Survey of Recent Achievements. Proc. Inst. Mech. Eng., 169: 41–57. Prager W (1959) Introduction to Plasticity. Addison-Wesley, Reading, Mass. Prager W and Hodge P G Jr (1951) Theory of Perfectly Plastic Solids. Wiley, New York. Prandtl L (1920) l~ber die H~irte Plastischer Koerper, Goettinger Nachr., Math. Phys. KI., 74–85. Thomsen EG, Yang CT and Kobayashi S (1965) Mechanics of Plastic Deformation in Metal Processing. Macmillan, New York. Yu MH (1983), Twin Shear Stress Criterion, Int. J. of Mech. Sci., 25(1), 71–74 . Yu MH, He LN and Song, LY (1985), Twin Shear Stress Theory and Its Generalization, Scientia Sinica (Science in China), Series A, (English edn.), 28(11), 1174–1183. Yu MH and He LN (1991), A new model and theory on yield and failure of materials under complex stress state. In: Mechanical Behaviour of Matterials-VI, Pergamon, Oxford, Vol.3: 841–846. Yu MH, Liu CY and He LN (1992), Generalized Twin Shear Stress Yield Criterion and Its Generalization, Chinese Science Bulletin (English edn.), 37(24), 2085–2089. Yu Mao-hong, et al (1992), Computer Image Analysis of the Plastic Zone of Structure, Journal of Xi’an Jiaotong University, 26(2), 121–122 (in Chinese). Yu MH, Liu JY and Ma Guo-wei (1994), Twin-shear slip line theory: orthogonal and nonorthogonal slip line fields. Journal of Xi’an Jiaotong University, 28(2):122–126. Yu MH, Yang SY, Liu CY and Liu JY (1997) Unified plane-strain slip line theory. China Civil Engrg. J. 30(2), 14–26 (in Chinese, English abstract). Zhang YQ, Li JC and Yin ZN (1998) Application of twin-shear strength theory in wedge’s limit analysis. In: Yu MH and Fan SC eds: Strength Theory: Application, Development and Prospect for the 21st Century, New York, Beijing: Science Press, 1998, 1155 –1160.

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.1 Introduction The twin-shear slip line field theory based on the twin-shear yield criterion and generalized twin-shear criterion for plane strain problems has been described in Chapter 8. Most available slip line field theories for plane strain problems are based on the one of single yield function such as the Tresca criterion (Maximum shear stress criterion), the Mohr-Coulomb strength theory (single-shear criterion), the Hubervon Mises criterion, the twin-shear yield criterion and the generalized twin-shear strength theory. These kinds of slip line field theories can be used only for one kind of material, respectively, such as the Tresca material, the Mohr-Coulomb material, the Hubervon Mises material and the twin-shear material. The adaptability of various slip fields are illustrated in Table 9.1. Table 9.1 The adaptability of various slip fields

Applications of slip line fields theory Tresca slip line For ϕt = ϕ 0 = 0 and For σt = σc materials field τ = o ,5σ materials Orthogonal slip field

Slip line fields

s

Orthogonal slip Mises slip field line field

s

For ϕt = ϕ0 = 0 and

For σt = σc materials

τs = o,577σs materials

Orthogonal slip field

Twin-shear slip line field

For ϕt = ϕ0 = 0 and

For σt = σ c materials

τs = o,667σ s material

Orthogonal slip field

Mohr-Coulomb slip field

For ϕt ≠ ϕ0 ≠ 0 , i.e.

For σt ≠ σc materials

α ≠ 1 materials For ϕt > ϕ0 ≠ 0 , i.e.

Non-orthogonal slip For σt ≠ σc materials

Non-orthogonal Generalized slip field twin-shear slip field

α ≠ 1 materials

Non-orthogonal slip field

226

9 Unified Slip-Line Field Theory for Plane Strain Problem

It is seen that the single slip field theory can not be adapted for other kinds of materials. No relations among these slip field theories are available. In order to solve the above mentioned problems, the unified strength theory (Yu 1991) was used to extend the slip line field theory for plane strain problem by Yu-Yang-Liu in 1997. A new system of orthogonal and non-orthogonal unified slip line field theory for plane strain problems was proposed and developed. Various orthogonal and non-orthogonal plane strain slip line field theories based on different strength theories, such as the Tresca criterion, the Huber-von Mises criterion, the twin-shear yield criterion, the Mohr-Coulomb theory, and the generalized twin-shear strength theory, are special cases or linear approximation (Huber-von Mises) of the unified slip line field theory. Besides, a series of new unified slip line field can be introduced by different choice of strength criterion parameter b of the unified slip line field theory.

9.2 Unified Strength Theory in Plane Strain Condition The stress state of plane strain structure is the same as the description in chapter 8. The main results are expressed as follows: ε z = ε xz = ε yz = τ xz = τ yz = vz = 0 ,

(9-1)

z is a principal direction, and ız is a principal stress. The stress component in plane strain state have only four streses components ıx, ıy, Ĳxy and ız. The maximum principal stress ı1 and minimum principal stress ı3 (ı1 ı2 ı3) of plane strain problem are σ1

= σmax

σ3

=

σ min

=

σx + σy

2

2

§σ σ · ± ¨ x− y¸+ © 2 ¹

2

τ xy

(9-2)

Introducing a parameter m, the intermediate principal stress ı2 can be expressed as

σ2 =

m 2

(σ1 + σ3),

(9-3)

where m is the intermediate principal stress state parameter, 0 < m ≤ 1 for plane strain problem. The intermediate principal stress state parameter m can be determined by both theoretical and experimental analysis. Generally, m < 1 for elastic region, i.e. ız = m(ı1 + ı3)/2 < (ı1 + ı3)/2; and mė1 for plastic region. The stress state of plane strain can be expressed by two new variations R and p

9.2 Unified Strength Theory in Plane Strain Condition

p=

1 1 1 1 (σ 1 + σ3 ) = (σ x + σ y ) = σ 2 = σ z , m m 2 2

1

§ σ1 − σ3 = ¨ © 2

R=

227

σ x − σy

2

(9-4)

2

· 2 ¸ + τ xy , ¹

(9-5)

The relations between these stresses are σx = p + R cos 2θ σy = p − R cos 2 θ τ xy = R sin 2θ

(9-6)

= ( p + C 0 ⋅ cot ϕ ) sin ϕ ⋅ sin 2 ϕ

where © denote the angle from x coordinate to the direction of ı1. The mathematical formulae of the unified strength theory can be expressed in two equations as follows:

F = σ1 − F ′=

1 1+ b

α

1+b

( b σ 2 + σ3 ) = σ t , when

σ2 ≤

σ1

(σ1 + bσ2 ) − α σ3 = σ t , when σ2 ≥

+

α σ3

1+α σ + ασ 1 3

1+α

,

(9-7a) ,

(9-7b)

Where ıt and ıc are uniaxial tensile and compressive strength of material respectively. Material parameter α = ıt /ıc is tensile-compressive strength ratio, which reflects material's Strength Difference (SD) effect. It is seen from Eq (9-4) that b reflects the effect of intermediate principal stresses on the yield of materials. The unified strength theory can also be expressed in terms of shear strength parameter C0 and friction angle ĳ0 as follows:

F = [σ 1 −

or

1 1+ b

b (σ 2 + σ 3 )] + [σ 1 +

1

(b σ 2 + σ 3 )] sin ϕ 0 = 2 C 0 ⋅ cos ϕ 0 1+ b σ +σ σ −σ when σ 2 ≤ 1 3 + 1 3 sin ϕ 0, 2 2

when σ 2 ≤ p + R sin ϕ 0

F' =[

1 1+ b

(σ 1 + bσ 2 − σ3 ] + [

1 1+ b

(σ 1 + bσ2 ) + σ 3 ] s in ϕ 0 = 2C 0 ⋅ co s ϕ 0

(9-8a)

228

9 Unified Slip-Line Field Theory for Plane Strain Problem

when σ2 ≥

σ1 + σ3 σ1 − σ3 + sin ϕ0 , 2 2

when σ 2 ≤ p + R sin ϕ 0

or

(9-8b)

The unified strength theory can consider the different effects of the intermediate principal stress for different materials. It establishes the relations among available strength theories, and creates a series of new yield criteria. Because the intermediate principal stress equals σ 2 = mp ≤

p + R sin ϕ 0 =

1 2

(σ 1 + σ 3) +

1

(σ 1 − σ 3 ) sin ϕ 0 ,

2

(9-9)

it accords with the first expression of the unified strength theory Eq (9-8). Combining Eqs (9-8a), (9-5) and (9-6), we get

R=

2(1 + b ) C0 ⋅ cos ϕ 0 2 + b (1 + sin ϕ 0 )

+

b (1 − m ) + (2 + b + bm ) sin ϕ 0 2 + b (1 + sin ϕ 0 )

(9-10)

p

where the compressive stress is usually defined positive. We introduce two new parameters ĳuni and Cuni (Yu et al. 1997) as follows:

sin ϕ uni =

b (1 − m ) + ( 2 + b + bm ) sin ϕ 0

sin ϕ uni = Cuni =

2 + b (1 + sin ϕ 0 ) 2 (b + 1) sin ϕ 0 2 + b (1 + sin ϕ 0 ) 2 ( b + 1) C0 ⋅ cos ϕ 0

1

2 + b (1 + sin ϕ 0 )

cos ϕ uni

,

when m Į 1,

(9-11a)

when m = 1,

(9-11b) (9-11c)

The parameters ĳuni and Cuni are referred to as the unified friction angle and the unified cohesion, respectively. The relations of Cuni∼ b and ¶uni∼ b for different ĳ0 are shown in Fig. 9.1 and Fig. 9.2, respectively.

9.2 Unified Strength Theory in Plane Strain Condition

229

Cuni/c0

Fig. 9.1 Relation between unified cohesion Cuni and b

¶uni

Fig. 9.2 Relation between unified friction angle ĳuni and b

Substituting Eqs (9-11) into Eq (9-10), the equation of the unified strength theory for plane strain problem can be rewritten as

230

9 Unified Slip-Line Field Theory for Plane Strain Problem

R = p sin ϕ uni + Cuni cos ϕ uni ,

(9-12)

It is the new expression of the unified strength theory for plane strain condition.

9.3 Unified Slip Line Field Theory for Plane Strain Problem (Statically Admissible Field) Under plane strain condition, some restrictions as εz = d ε z = γ zx = d γ zx = γ zy = d γ zy = 0

(9-13)

The plane strain equilibrium differential equations can be written as (see: Hill 1950 or Johnson and Mellor 1962)

∂σ x ∂τ yx + = γ sin θ 0 ∂x ∂y

∂τ xy ∂x

+

∂σ y ∂y

(9-14)

= − γ cos θ 0

in which ¤ is specific weight and ș0 is the angle between the direction of gravity and the minus direction of y coordinate, as shown in Fig. 9.3.

Fig. 9.3 Stress state in any point of plane strain slip line field (dxė0, dyė0)

Solving Eqs (9-9), (9-11), and (9-12), the stress governing equations are obtained as follows:

9.3 Unified Slip Line Field Theory for Plane Strain Problem

231

b(1 − m) + (2 + b + bm)sin ϕ 0 ∂p ∂p b(1 − m) + (2 + b + bm)sin ϕ 0 (1 + cos 2θ ) + sin 2θ + ∂x 2 + b(1 + sin ϕ 0) ∂y 2 + b(1 + sin ϕ 0) ∂θ ∂θ cos 2θ − sin 2θ ) = γ sin θ 0 ∂y ∂x b(1 − m) + (2 + b + bm)sin ϕ0 ∂p b(1 − m) + (2 + b + bm)sin ϕ0 ∂p sin 2θ + (1 − cos 2θ ) + 2 + b(1 + sin ϕ0 ) 2 + b(1 + sin ϕ0 ) ∂x ∂y +2R(

+ 2 R(

∂θ ∂θ cos 2θ + sin 2θ ) = −γ cos θ 0 ∂x ∂y (9-15)

Equation (9-15) satisfies the unified strength theory (Eq. 9-10), and plane strain static equilibrium equations (Eq. 9-14). Equation (9-15) may be elliptic-type (two different real roots), parabolic-type (two same real roots) or hyperbolic-type (no real roots) pseudo-linear differential equations which can be solved by the method of characteristics

dy = tg (θ − µ) , dx dy £ family: = tg (θ + µ), dx

α family:

(9-16a) (9-16b)

in which µ =

π

4

−

ϕ uni .

2

We can see that the equations are elliptic-type pseudo-lineal differential equations. Equation (9-15) has not only two different real roots of the pseudolinear equation (9-14), but also two characteristic lines at the angle of 2 with each other. Substituting Eq.9-11 into Eq.9-15, the governing equations (9-15) change to

∂p ∂p ∂θ ∂θ (1 + sin ϕ uni⋅ cos 2θ ) + sin ϕuni ⋅ sin 2θ + 2R( cos 2θ − sin 2θ ) = γ sin θ 0 ∂x ∂y ∂y ∂x (9-17) ∂p ∂p ∂θ ∂θ sin ϕ uni⋅ sin 2θ + (1 − sin ϕ uni⋅ cos 2θ ) + 2R( cos 2θ + sin 2θ ) = −γ cosθ 0 ∂x ∂y ∂x ∂y It is interesting that Eq. (9-17) is similar to the conventional equation. It is only the substitution of Cuni and ĳuni for C0 and ĳ0. This substitution embodies the effect of yield criterion parameter b of the unified strength theory in an implicit way, builds the linkage of different slip line field theories and reflects

232

9 Unified Slip-Line Field Theory for Plane Strain Problem

the regular effect of intermediate principal stress in this new unified slip line field theory. The unified slip lines field theory can be degenerated to orthogonal and nonorthogonal theories based on the Tresca critereion (α=1,b=0), the Huber-von Mises criterion (α=1, b=1/2), the twin Shear criterion (α=1, b=1), the Mohr-Coulomb criterion (b=0) and the generalized twin shear criterion (b=1). Moreover, when we choose other values of parameter b, a series new theories can be introduced. Hence, the unified strength criterion parameter b can also be regarding as a parameter of choosing for yield function. In this section, the curvilinear coordinate system Sα and Sȕ coinciding with the slip lines α and β is choosed, as shown in Fig. 9.4.

Fig. 9.4 Stress state in any point of plane strain slip line field

According to the rules of directional derivative, the stress governing equations, Eq. (9-17), can be expressed in curvilinear coordinates Sα and Sȕ

α family: − sin 2 µ

∂p ∂ Sα

+ 2R

∂θ ∂ Sα

+ γ [sin(θ 0 + 2 µ )

∂x ∂ Sα

+ cos(θ 0 + 2 µ )

∂y ∂ Sα

] = 0 (9-18a)

β family: sin 2 µ

∂p ∂ Sβ

+ 2R

∂θ ∂ Sβ

+ γ [sin(θ 0 − 2 µ )

∂x ∂ Sβ

+ cos(θ 0 − 2 µ )

∂y ∂ Sβ

] = 0 . (9-18b)

Equations (9-17) and (9-18) are the stress governing equations (statically admissible) of the unified slip line field theory for plane strain problem. The equations differ from ordinary stress governing equations by substituting Cuni and ĳuni for C0 and ĳ0.

9.3 Unified Slip Line Field Theory for Plane Strain Problem

233

9.4. Unified Slip Line Field Theory for Plane Strain (Kinematically Admissible Field) In this section, the associated flow rule is adopted, namely

∂g

p

dε ij = d λ

= dλ

∂σ ij

∂f

,

∂σ ij

(9-19)

where the potential function is the equation of unified strength theory, which can be expressed as

1 1 f = (σ x + σ y )sin ϕuni − (σ x − σ y )2 + τ xy2 + Cuni ⋅ cos ϕuni = 0 , 2 4

(9-20)

The plastic strain rates under small deformation and rigid plastic condition can be obtained by ε&x =

ε& y =

γ& xy =

∂ u& x ∂ vx , = ∂x ∂x ∂ u&y ∂y

∂u& x ∂y

+

=

∂ vy

∂u& y ∂x

,

∂y =

∂v x ∂y

+

∂vy ∂x

,

(9-21)

Then we can get velocity governing equations of unified slip line field theory for plane strain problem α family:

dνα + [ν α ctg (

β family:

dνβ + [να csc(

π

2 π

2

− ϕ uni ) − νβ ⋅ csc(

π

2

− ϕ uni ) − νβ ⋅ ctg (

π

2

− ϕ uni )] dψ = 0 ,

− ϕ uni)] dψ = 0 .

(9-22a) (9-22b)

where ux and uy are displacement components, vx =du x /dt and vy =duy /dt are velocity components along x and y directions, whereas vα and vȕ are velocity components along α and β slip lines, respectively. Superimposed dot means derivative with respect to time.

234

9 Unified Slip-Line Field Theory for Plane Strain Problem

Substituting unified strength theory for plane strain into associated flue rule Eq. (9-19), and taking the rigid plastic postulate into consideration, we obtain

1 2 (σ y − σ x) ° ®sin ϕ uni + 2 ∂σ x 1 / 4 (σ x − σ y ) 2 + τ xy °¯ 1 2 (σ y − σ x) ∂f dλ ° =− dε y = − dλ ®sin ϕ uni − 2 ∂σ y 2 ° 1 4 (σ x − σ y ) 2 + τ xy ¯ τ xy ∂f dγ xy = 2 d ε xy = − 2 d λ = dλ 2 ∂ τ xy 1 4 (σ x − σ y )2 + τ x y

d ε x = − dλ

∂f

=−

dλ 2

½ ° ¾ °¿ ½ ° ¾ °¿

(9-23)

where the relation between shear strain ε xy and engineering shear strain Ȗxy , i.e., Ȗxy =2İxy , is used. The compressive normal stress is defined positive. Figure 9.5 gives the plane strain Mohr circle and the relation between the slip angles, were is the angle between α slip line and x direction, i.e. ψ = θ − µ = θ − (π / 4 − ϕ uni / 2) . Follow this definition, Eq. (9-23) can be simplified to

dλ [sin ϕ uni + sin(2ψ − ϕ uni )] 2 dλ dε y = − [sin ϕ uni − sin(2ψ − ϕ uni)] 2 d γ xy = d λ cos(2ψ − ϕ uni ) dε x = −

Fig. 9.5 Stress state and direction angle in any point of plane strain slip line field

(9-24)

9.4 Unified Slip Line Field Theory for Plane Strain

235

When the direction of slip line is along x direction, i.e. =0 (α line) or ψ = − (π 2 − ϕ uni ) (£ line), it follows from Eq. (9-24) that

dεx ψ =0 = d ε x

ψ =− (π 2 −ϕuni )

= 0

(9-25)

This equation indicates that the rigid strain rate will vanishes along slip lines. The relation in Fig. 9.5(b), i.e. the relation between velocity components along slip lines vα = u&α ( v β = u&β ) and velocity components along x (y) axis vx (vy), can be obtained by

v x = u& x =

vα sin(ψ + 2 µ ) − vβ sin ψ

v y = u& y =

sin 2 µ

.

(9-26)

vα cos(ψ + 2 µ ) − vβ cosψ − sin 2 µ

Combination of Eqs. (9-21), (9-25) and (9-26), gives,

dε x

ψ =0

= ε& x

ψ =0

dt =

∂ vx ∂x

ψ =0

dt

= { dvα + [ vα ctg ( π 2 − ϕ uni ) − vβ csc( π 2 − ϕ uni )] dψ } d t = 0

(9-27)

In the above equation, we have used the relation µ = π 4 − ϕ uni / 2 and definitions

dvα ≡ ( ∂ vα ∂ x )

ψ =0

and dψ ≡ ( ∂ ψ ∂ x ) . ψ =0

When slip line field generates plastic flow, by integrating Eq. (9-21), we can work out the velocity field that satisfies the boundary conditions of the problem. The velocity field solution complies with the unified strength theory, associated flow rule and rigid plastic small deformation condition. When ĳuni=ĳ0, which is the case of orthogonal slip line field, Eq. (9-22) can be simplified to the famous Geiringer velocity equations (Johnson and Mellor 1962)

α family: d vα − vβ dθ = 0 ,

(9-28a)

β family: dvβ + vα dθ = 0 .

(9-28b)

By now, we have extended the unified strength theory to slip line field theory for plane strain by means of the introduction of unified effective parameters: the

236

9 Unified Slip-Line Field Theory for Plane Strain Problem

unified internal cohesive Cuni and the unified friction angle ĳuni and got the governing equations of the unified slip line field theory for plane strain problem (Eqs 9-17, 9-18 and 9-22). Unified slip line field theory can be used to materials with obvious intermediate principal stress effect and give the linkage of various slip line field theories without theoretical difficulty. Moreover, the unified slip field theory contains infinite number of orthogonal and non-orthogonal slip line field theories. With the different choice of parameter (α, β, γ) or Cuni and ĳuni, we can get a series of special cases of the unified slip field theory.

9.5 Special Cases of the Unified Slip Line Field Theory 9.5.1 Case 1: ¤=0 This is the case when unified slip line field theory for plane strain problem is applied to materials where gravity is left out of consideration. In this case, velocity governing equations are the same as Eq. (9-22), whereas stress governing Eq. (9-18) can be simplified to

α family: − sin 2 µ β family: sin 2 µ

∂p ∂ Sα ∂p

∂ Sβ

+ 2R

+ 2R

∂θ ∂ Sα ∂θ

∂ Sβ

= 0,

=0

(9-29a) (9-29b)

Integrating the above equations, after simplification, we obtain

α family:

p = Cα ⋅ exp(2θ ⋅ ctg 2 µ ) − Cuni ⋅ ctg ϕ uni ,

(9-30a)

β family:

p = Cβ ⋅ exp( − 2θ ⋅ ctg 2 µ ) − Cuni ⋅ ctgϕ uni ,

(9-30b)

where Cα and Cȕ are integral constants, which will be determined by different boundary conditions. Parameters Cuni and ĳuni are defined in Eq. 9-11. This case is a new type of non-orthogonal slip line field. As an example, a strip footing of width AA and semi-infinite length carrying a uniform load on the surface of a semi-infinite, homogeneous and isotropic soil is show in Fig.9.6. The material strength parameters for the soil are C0 and ĳ0 but the unit weight is assumed to be zero. When the pressure becomes equal to the ultimate bearing capacity, the footing is pushed downwards into the soil mass

9.5 Special Cases of the Unified Slip Line Field Theory

237

producing a state of plastic equilibrium below the footing. The surface AA is assumed to be smooth.

Fig. 9.6 Slip lines field of weight-less soil under a strip footing

The slip field can be indivited into three regions with the angles AAD being (45º + ĳ /2) as shown in Fig.9.6. The downward movement of the wedge AAD forces the adjoining soil sideways, producing outward lateral forces on both sides of the wedge AAD. Passive zones AEF and AE’F’ therefore develop on both sides of the active wedge, with the angles EFA and E’F’A being (45º - ĳ /2). The transition between the downward movement of the active wedge and the lateral movement of the passive wedge takes place through zones of radial shear ADE and ADE’, and the surfaces DE and DE’ are logarithmic spirals to which the failure planes of the active and passive wedges are tangential. A state of plastic equilibrium thus exists above the surface EDF and DE’F’, and the remainder of the soil is in a state of elastic equilibrium. The following solution of limit load q is obtained by using the unified slip lines field theory. It is a new non-orthogonal slip line field system.

º ª 1 + sin ϕ uni q = C uni ⋅ ctg ϕ un i « e x p ( π t g ϕ uni ) − 1 » ¬ 1 − sin ϕ uni ¼

(9-31)

This solution differs from the traditional solutions in the substitution of Cuni and ĳuni for C0 and ĳ0, and the effect of intermediate principal stress is taken into account and establishs the relation of different solutions, as shown in Fig. 9.7 (Yang and Yu 1996).

238

9 Unified Slip-Line Field Theory for Plane Strain Problem

Fig. 9.7 Relation between limit load and unified strength parameter b of a strip footing

We can also draw the following conclusions: 1. when b=0, that is ĳuni=ĳ0 and Cuni = C0 (Eqs 9-16 and 9-17), the unified solution is simplified to the Tresca solution (α=1) or the Mohr-Coulomb solution (α Į 1). 2. when b (bĮ0) is fixed, the larger the value of ĳ0 is, the bigger the difference between the new solution and the Tresca solution (α =1) or the Mohr-Coulomb solution (α Į1) is. 3. when ĳ0 is fixed, the larger the value of b is, the bigger the difference of the two solutions is.

9.5.2 Case 2: ĳuni=0 This is the case of orthogonal unified slip line field theory for plane strain problems. Because of the perpendicularly of two families (α and £ ) of slip lines, 2 µ = π 2 − ϕuni = π 2 . In this case, it follows from Eqs (9-16) and (9-17) that ϕ uni = ϕ 0 = 0 ,

R = Cuni =

2(1 + b ) 2+b

C0 ,

α = 1.

(9-32)

Orthogonal unified slip line field theory for plane strain problem is used for nonSD materials, α =1. In another word, only this kind of materials can generate this case of orthogonal slip line field. Substituting 2µ =ʌ/2 into Eqs (9-18) and (9-22), we get the stress and velocity governing equations of this case α family

9.5 Special Cases of the Unified Slip Line Field Theory

−

∂p ∂S α

+ 2R

∂θ ∂Sα

∂x

+ γ [ cos θ 0

∂Sα

− sin θ 0

∂y ∂Sα

]=0

239

(9-33a)

dνα − νβ d θ = 0 β family

∂p ∂Sβ

+ 2R

∂θ

+ γ [ − cos θ 0

∂Sβ

∂x ∂Sβ

+ sin θ 0

∂y ∂Sβ

]= 0

.

(9-33b)

dνβ + να dθ = 0 Integrating the stress governing Eq. (9-33), we obtain

α family:

p − γ cos θ 0 x + γ sin θ 0 y − 2 Rθ = C α ,

(9-34a)

β family:

p − γ cos θ 0 x + γ sin θ 0 y + 2 Rθ = C β ,

(9-34b)

9.5.3 Case 3:

ϕ uni = 0

and ¤=0

This is the case of orthogonal unified slip line field theory for plane strain problem without consideration of gravity. From Eqs. (9-16) and (9-17), we can get the restrictions of this case ϕ uni = ϕ 0 = 0 , ∂

R = Cuni =

2 (1 + b) 2+b

C0 ,

(9-35)

γ = 0, α = 1

Substituting above equations into Eq. (9-35), we have the stress and velocity governing equations of this case

∂ ∂ Sα

( p − 2 Rθ ) = 0

,

α family

(9-36a)

β family

(9-36b)

dvα − vβ d θ = 0 ∂

∂Sβ

( p + 2 Rθ ) = 0

dv β − vα dθ = 0

.

240

9 Unified Slip-Line Field Theory for Plane Strain Problem

where the condition that R is constant with respect to Sα and Sȕ is used when material and strength theory is fixed Integrating Eq. (9-36), we can get the solutions of this case

α family:

p − 2 Rθ = Cα ,

(9-37a)

β family:

p + 2 Rθ = Cβ .

(9-37b)

where C α and C β are integral constants. Substitute ¤= 0 into Eq. (9-30), we can also get above equations. The form of Eqs (9-36) and (9-37) is similar to that of traditional solutions of orthogonal slip line field theories. But the definition of R is different. In this discussion, R is unified parameter and with different choice of yield criterion parameter b, the solution can be simplified to those of the Tresca, the Huber-von Mises and the twin-shear slip line field theories, they are: 1. b = 0, R = C 0 = σs 2 = 0.5σs , it is the Tresca solution; 2. b=1/2, R = 6/5 C 0 = 3/5 σs = 0.6σs , it is the linear approximations to the Huber-von Mises solution (exact solution is R = 1 3. b=1, R = 4 / 3C0 = 2 / 3σs = 0.667σs

3 σs = 0.58σs );

it is the solution of the twin-shear yield

criterion.

9.6 Applications of the Unified Slip Line Field Theory 9.6.1 Example 1: Trapezoid structure The trapezoid PVC specimen with a top angle 2¯ isconsidered. The uiform distributed load is applied on the top of the specimen, as shown in Fig. 9.8. The loading velocity is 1mm/min. The physical properties of the material are: Young's modules: 367.88 kN/cm2

Specific gravity: 1.35-1.45 g/cm3

Poisson's Ratio: 0.27

Tensile strength: 5.886 kN/cm2

Compressive strength: 7.575 kN/cm2 Determine the limit load.

Solution Friction angle and cohesion of this material can be determined by

9.6 Applications of the Unified Slip Line Field Theory

ϕ 0 = sin

C0 =

−1

σc − σ t = 7.208 0 σ c + σt

σ t (1 + sin ϕ 0 )

2 cos ϕ 0

241

(9-38)

= 3.339

It is assumed that the surfaces AA’ are smooth and there is no friction. It is also assumed that there is a constant pressure on the top. The rest of the boundary is stress-free.The slip line field is given in Fig.9.8.

Fig. 9.8. Slip lines field of a trapeziod structure (Yu 1998)

The slip line field can be divited into three regions:I, II, and III, where I and III are uniform stress regions, and II is a centered fan region. (1) The triangular region III (ABC) It is formed by free boundary AB and the slip lines AC and BC. This is a constant stress region. The slip lines are straight with α1=ʌ/4–ĳ/2. The mean stress is a constant and must satisfy condition throughout this region : ın=Ĳn=0, ı1=ıt, ı3=ın=0. Along the ȕ lines, we have

p =

− Cuni ⋅ cos ϕ uni 1 − sin ϕ uni

= Cβ ⋅ exp( 2 ξ ⋅ tg ϕ uni ) + Cuni ⋅ ctg ϕ uni

(9-39)

The integrate constant is determined by

Cβ =

− Cuni ⋅ cos ϕuni 1 − sin ϕuni

exp( − 2 ξ ⋅ tg ϕ uni )

(9-40)

242

9 Unified Slip-Line Field Theory for Plane Strain Problem

(2) The triangular region I (AA’D) It is formed by loading boundary AA’ and the slip lines AD and A’D. This is a constant stress region. The slip lines are straight with angle − ( π + ϕuni ) (α lines) 4 2 and ( π + ϕ uni ) ( ȕ lines). 4 2 The integrate constant is determined by

Cβ =

− q − C uni ⋅ ctg ϕuni

(9-41)

1 + sin ϕ uni

(3) Centered fan region II (ACD) This is a slip region. The α lines are straight with different angle acrossed at point A. ȕ lines are logarithmic spirals. The expression of the logarithmic spirals is

r1 = r0 exp(2 ξ ⋅ tg ϕ uni ) The length AC of a side of center fan is

AA '

r AD = 2 cos(

π

4

+

ϕ uni

2

)

The length AD of another side of center fan is

rAC =

AA ' exp ( 2 ξ ⋅ tg ϕ uni ) 2 cos(

π

4

+

ϕ uni

2

)

The limit loading of trapezoid specimen is obtained as follows

q = C uni ⋅ ctg ϕ uni [

1 + sin ϕ uni 1 − sin ϕ uni

exp ( 2ξ ⋅ tg ϕ uni ) − 1 ]

(9- 42)

With different choice of unified yield criterion parameter b, a series of limit loading are obtained as shown in Fig.9.9. The three curves are three results for three specimen, the top angles are: 2ξ = 120o, 2 ξ = 80o and 2ξ = 60o. Figure 9.10 is the variation of the slip angles with the variation of unified yield criterion parameter b. From Fig. 9.10, we can see that the result of Unified Slip Line Field Theory (2= 81.04o for b = 0.8) is much closer to the experimental result (2 =79.5o ) than that of the Mohr-Coulomb (2= 82.8o ).

9.6 Applications of the Unified Slip Line Field Theory

243

It is worthy to mention that not only the limit loading q but also the slip angle 2µ are different. They are different for different material. The variation of slip angle 2µ with the unified yield criterion parameter b is shown in Fig.9.10.

26 o

24

2ξ=120

22

2ξ=60

o

q (KN)

2ξ=80

o

20 18 16 14 12 0.0

0.2

0.4

0.6

0.8

1.0

b Fig. 9.9 Unified solutions of limit loading (Yang-Yu 1997)

83.0

2µ (degree)

82.5 82.0 81.5 81.0 80.5 0.0

0.2

0.4

0.6

0.8

1.0

b Fig. 9.10 Variation of slip angle 2µ with the unified yield criterion parameter b

244

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.6.2 Example 2: Strip footing The slip lines field of strip footing under uniform punch pressure is similar to

that of trapezoid structure as shown in Fig.9.11. The difference only in the angle ʌ and 2ȟ (2ȟ=2ș1 in Fig.9.11,b).

Fig. 9.11 Slip lines field of a semi-infinite surface (a) and a trapeziod structure (b)

The limit loading of strip footing can be obtained by 2ȟ=ʌ, which is given as follows q = C uni ⋅ ctg ϕ uni [

1 + sin ϕ uni 1 − sin ϕ uni

exp(π ⋅ tg ϕ uni ) − 1]

(9-43)

9.6.3 Example 3: Shallow strip footing A shallow strip footing is shown in Fig.9.12, and the material parameters are: C 0 = 9Kp a, ϕ 0 = 14 o, γ = 17.3KN / m 3, width of strip B=3m, depth d=1.5m. The shear strength of the soil between the surface and depth d is neglected.

This soil being considered only as a surcharge imposing a uniform pressure q=Ȗ0 d on the horizonal plane at foundation level. Determine the limit load for strip footing.

Fig. 9.12 Slip lines field of a falf space under shallow strip footing

9.6 Applications of the Unified Slip Line Field Theory

245

Solution Friction angle and cohesion of this material can be determined. The unified friction angle ĳuni and the unified cohesion Cuni can be determined by using Eqs.9-10 and 911. The relations of unified friction angle ĳuni and the unified cohesion Cuni with unified yield criterion parameter b, i.e. relations Cuni~b and ¶uni~b are shown in Figs. 9.13 and 9.14, respectively.

ϕ uni

20.00

15.00

10.00

5.00

b 0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.13Relations of unified friction angle ĳuni with unified yield criterion parameter b

C uni/c 0

1.20 1.00 0.80 0.60 0.40 0.20

b

0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.14Relations of unified cohesion Cuni with unified yield criterion parameter b

A series of slip line field and different results of limit loading were determined by Fan and Yu by using the unified slip field theory. The five slip line fields and relating limit loading are shown in Figs. 9.15 to 9.20.

246

9 Unified Slip-Line Field Theory for Plane Strain Problem

Pu =171.77

143.84

200.28

0.00

4.00

2.00

Fig. 9.15 Slip line field for b=0 material (Pu =171.77)

Pu =192.26

159.47

225.73

0.00

2.00

Fig. 9.16 Slip line field for b=0.2 material (Pu=192.26)

4.00

9.6 Applications of the Unified Slip Line Field Theory

pu=210.75 173.20

249.07

0.00

4.00

2.00

Fig. 9.17 Slip line field for b=0.4 material (pu=210.75)

pu=218.31 179.46

257.93

0.00

2.00

4.00

Fig. 9.18 Slip line field for b=0.5 material (pu=218.31)

247

248

9 Unified Slip-Line Field Theory for Plane Strain Problem

196.15

286.08

pu=240.68

0.00

2.00

4.00

Fig. 9.19 Slip line field for b=0.8 material (pu=240.68)

pu=252.38 205.81

299.83

0.00

2.00

4.00

Fig. 9.20 Slip line field for b=1.0 material (Twin-shear theory pu=252.38)

The limit loading of strip footing varies with the choice of the unified yield criterion parametere b. The relation of limit loading of strip footing with b is shown in Fig.9.21.

9.6 Applications of the Unified Slip Line Field Theory

249

Pu/c 50.00 40.00

30.00

20.00

10.00

b

0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.21Relations of limit loading with unified yield criterion parameter b

It is seen that a series of results can be obtained by using the unified slip lines field theory.

9.6.4 Example 4: Acute Wedge An acute wedge is in a plane strain state. Its top angle γ < π 2 , and surface AB is subjected to uniform pressure Pu , as shown in Fig. 9.22. Determine the limit pressure Pu on surface AB .

Fig. 9.22Acute wedge under unilateral pressure

Solution: The unified solution of acute wedge under unilateral pressure was given by Zhang, Hao and Yu in 2003. When 0 < γ < π 2 , a stress discontinuous line in the wedge will appear. The characteristic field is shown in Fig.9.22, where ∠BAC = δ , ∠CAD = ν, δ + ν = γ . The regions ABC and ACD are regions of constant biaxial

250

9 Unified Slip-Line Field Theory for Plane Strain Problem

compression and uniaxial compression, respectively. The constant stress regions ABC and ACD are separated by the line of stress discontinuity AC which is inclined to A B at an angle δ to be determined. The different values a quantity may assume in the regions ABC and ACD will be distinguished by subscripts 1 and 2, respectively. The angle between characteristics α and β is 2ψ . From the stress boundary condition of the wedge, we have σ 3 = − pu in region ABC , and σ 1 = 0 in region ACD . Thus it has ϕ1 =

π

2

−δ, ϕ2 = ν

(9-44)

It also has δ +ν = γ

(9- 45)

The unified limit load for acute wedge was given as follows

· § 1 + sin ϕ uni sin 2ν pu = Cuni ⋅ cot ϕ uni ¨¨ − 1¸¸ ¹ © 1 − sin ϕ uni sin 2δ

(9-46)

where ĳuni and Cuni were introduced by Yu et al. in 1997 and 1998, they are defined as

sin ϕ uni =

Cuni =

2 (b + 1) sin ϕ 2 + b (1+ sin ) ϕ

,

2 ( b + 1)C ⋅ cos ϕ

1 . 2 + b (1 + sin ϕ ) cos ϕ uni

(9-47)

ĳuni and Cuni are two parameters in the unified slip field theory. For the case of b = 0 and α ≠ 1 , the unified limit load reduces to

§ 1 + sin ϕ sin 2ν · pu ' = c cot ϕ ¨¨ − 1 ¸¸ © 1 − sin ϕ sin 2δ ¹

(9-48)

This is the solution on the basis of Mohr-Coulomb criterion (Shield 1954; Chen 1975).

9.6 Applications of the Unified Slip Line Field Theory

251

For the case of b = 0 and α = 1 , the unified limit load reduces to

p u " = lim p u ' = 2 c (1 − cos γ ) α →1

(9-49)

(ϕ → 0)

This is the solution on the basis of Tresca criterion (Chen 1975). When Ȗ=ʌ/3, the relation between the limit load pu and the unified yield criterion b at different ratio of α = ³t /³c are shown in Fig.9.23.

Fig. 9.23 The relation between limit load Pu and unified strength theory parameter b

It can be found that the SD effect of material and the influence of intermediate principal stress on the limit load are significant. Through the parameters α and b, the dependence of the result of the limit load on yield criterion is also reflected. As shown, at the same α , the Mohr-Coulomb criterion (b = 0 ) leads to the minimum value of pu σ t while the twin-shear strengrh theory (b = 1) leads to the maximum value of pu σt .

9.6.5 Example 5: Experiments A method of observing plastic zone in a structure under loading is applied. In order to obtain clear images of the development of structure's plastic zone, image analysis technique has been used.The plastic zone of structure under limit loading is obtained. Three trapeziod specimens are the same as example 1, in which the top angle are: 2ξ = 120o , 2 ξ = 80o and 2ξ = 60o . The three experimental results of limit loading are: 23.6kN for 2ξ = 120o, 18.5kN for 2 ξ = 80o , and 16.9kN for 2ξ = 60o . The theoretical results has been obtained as shown in Fig. 9.24.

252

9 Unified Slip-Line Field Theory for Plane Strain Problem

83.0

26 o

24

2ξ=120

22

2ξ=60

82.5

o

o

2µ (degree)

q (KN)

2ξ=80

20 18 16

81.5 81.0

14 12 0.0

82.0

0.2

0.4

0.6

b

0.8

1.0

80.5 0.0

0.2

0.4

0.6

0.8

1.0

b

Fig. 9.24 Variations of limt loads and slip angle with the unified yield criterion parameter b

We can see from Fig. 9.24 that the three experimental results q1=23.6kN, for 2 ξ = 120o , q2=18.5kN for 2 ξ = 80o , and q3=16.9kN for 2ξ = 60o are closed to the unified solution with bĬ0.8. Obvious error will be produced when we use the traditional Mohr-Coulomb slip line field solution (b=0). We can also assume that this material can be simulated by bĬ0.8, i.e. limit loads of cases with other top angles can be determined by Eq.9-42 with bĬ0.8. Furthermore, we can find from the experiment that the shape of slip line is nonorthogonal. The slip angle obtained by computer image analysis is 78o (for MohrCoulomb non-orthogonal slip line field theory, the angle is 82.8o ). The test gives the change of 2µ, the angle between two slip lines, with different choice of unified yield criterion parameter b. From Fig. 9.24, we can see that the slip angle o calculated through unified Slip Line Field Theory (2µ=81.04 when b=0.8) is much closer to the experiment result than the result based on the Mohr-Coulomb non-orthogonal slip line filed theory (2µ=82.8 o ).

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method Various finite element solutions for the bearing capacity of structures have been reported in the literature. Some are of very interesting and value. The development of plasticity in soil under a footing foundation were studied by Nayak and Zienkiewicz (1972) and Moore and Rowe (1991) et al. Fig. 9.25 to Fig. 9.28 show the results of plastic zones at footing displacement obtained by Moore and Rowe (1991). They used a 15 nodes element (as show at the right in Fig. 9.25) and a series of computational results were obtained. Each yielded integration point within the triangular elements has been marked with a small lines, where these lines are aligned with the direction of the shear deformation at those locations.The development of plastic zone at various footing penetrations are shown clearly.The

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method

253

final slip surface is shown in Fig. 9.28. It is observed that the soil materials collapses with a mechanism similar to that of Prandtl for perfectly plastic materials (Moore and Rowe 1991) .

Fig. 9.25 Fine mesh (Moore and Rowe 1991) Fig. 9.26 Initial plastic zone

Fig. 9.27 Development of plastic zone

Fig. 9.28 Final plastic zone

The velocity fields at the final displasment is shown in Fig. 9.29. The shape roughtly resembles the Prandtl mechanism for perfectly plastic materials, although only part of the solid material in motion is responding plastically, with both the block of material directly under the rigid footing and much of the solid within the “passive motion” behaving elastically. The shape is also similar the results obtained by the unified slip field theory.

254

9 Unified Slip-Line Field Theory for Plane Strain Problem

Fig. 9.29 Velocity fields at footing diaplacement (Moore and Rowe 1991)

The similar results were also obtained by other researcheres. A real-life problem in geomechanics were investigated by Wunderlich, Findeib and Cramer (Fig. 9.30) as well as Wunderlich, Findeib and Cramer Zimmermann and Commend et al.(Fig. 9.31). They showed the limit-load state obtained by the finite element analysis (2001). A localized failure in the shape of the well known Prandtle sliplines which have been derived on a analytical basis was given. The results of the finite element analysis are in close agreement with observations in reality.

Fig. 9.30 Limit-load state of strip footing (Wunderlich, Findeib and Cramer 2001)

Fig. 9.31 Limit-load state of strip footing (Zimmermann and Commend 2001)

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method

255

The numerical tests of a panel under compression were analyzed by de Borst et al (1995) and Chen and Baker (2001). The plastic strain develops in “X” shape. It is agreement with the experimental results shown in Fig. 9.32.

Fig. 9.32 The plastic strain develops in “X” shape (Chen and Baker 2001)

These kinds of results were obtained by Yu and Zeng in 1990. The calculation results by using two material models, i.e. the Mohr-Coulomb strength theory (b=0) and the twin-shear strength theory (b=1, Yu 1985) are illustrated in Fig.9.33 and Fig.9.34. Figure 9.33 is a result of thick plate with a hole under compression, and figure 9.34 is a result of thick plate with a hole under tension. It is seen that the four results are different.

Fig. 9.33 Different results of two models in compression and in tension (Yu and Zeng 1993, see: Yu 1998)

It is worth noting that the result of the finit element method is always a single result by using a single yield criterion. The result of convenient slip line field is also a single result. It is also worthy to note that the shape and angle of the plastic zone are also different for different yield criterion.

256

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.8 Comparison of the Unified Slip Line Field Theory with Experimental Results The experimental results of the plastic zones for a plate with different holes under tension are shown in Fig. 9.34 (see Yu 1998).

(a) Test results (Yu 1981)

(b) Test results (Liu 1989)

Fig. 9.34 Plastic zones of tensile plate with different holes

The comparison of three methods are shown in Fig. 9.35. The rectangular thick plate specimen with a circular hole at the center was applied under an uniform load at the edge. The material and the experimental procedure are same as those in example 1 and example 5. In Fig. 9.35, curve 1 is the experimental result of plastic zone, curve 2 is that of unified elasto-plastic finite element calculation (b=0.8), and curve 3 is of Unified Slip Line Field Theory.

Fig. 9.35 Comparison of three methods (see Yu 1998)

As can be seen, the plastic zones are different in tension and in compression for SD (strength different) maerials. Fig. 9.33(a) shows the computational results by

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain

257

using the twin-shear strength theory and the Mohr-Coulomb strength theory for the same material in compression. Fig. 9.33(b) shows the computational results by using the twin-shear strength theory and the Mohr-Coulomb strength theory for the same material in tension. The experimental results also present the difference of plastic zones in tension and in compression, as shown in Fig. 9.36.

Fig. 9.36 Different results in compression and in tension (Yu and Liu 1989)

In order to confirm the results of the unified slip line theory, the elasto-plastic finite element program UEPP based on the unified strength theory (UST) is used to compute the limit loading q of the same structures. UEPP was established by Yu, Zeng, Ma,Yang, Wang et al. in the period of 1993 to 1998 (Yu and Zeng 1994; Yu, Yang, Fan et al. 1997). From these comparisons, we can find that the result from the characteristics line theory are very close to those results from the experiments and finite element methods. The detail of numerical analysis of generalized plasticity will be discussed in another book : ĀComputational Plasticityā.

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain During the process of the elastic-plastic deformation, the continuity of velocity vanishes when it is passing the certain characteristics surface, with the development of the deformation, namely, the phenomenon of discontinuous bifurcations is produced. Hill (1958), Marciniak and Kuczynski (1967), Storen and Rice (1975), Rudnicki and Rice (1975), Hutchinson and Tvergaard (1980, 1981), Tvergaard, Needleman and Lo (1981), Raniecki and Bruhns (1981), Bruhns (1984), Li (1987), Runesson and Mroz (1989), Hill JM and Wu YH (1993),

258

9 Unified Slip-Line Field Theory for Plane Strain Problem

Zyczkowski (1999) et al. have done extensive researches for the discontinuous bifurcations. Ottosen and Runesson (1991) put forward a general description of discontinuous bifurcations for the plane problem of isotropic and elastic-plastic body plane problem, obeying the Mohr-Coulomb yield. criterion. Hill JM and Wu YH (1993) used the Ashton-Warren Spring yield equation. It is a Mohr-Coulomb typed yield equation, in which the maximum principal stress σ1 and the minimum principal stress σ3 are taken into account. Zyczkowski (1999) studied the discontinuous bifurcations in the case of the Burzynski-Torere yield criterion. The corresponding properties of discontinuous bifurcations have been obtained by using various yield criteria. For selection of the yield function, the intermediate principal stress is not considered in Mohr-coulomb Strength Theory, and this theory can not match the experimental results of much materials. The unified strength theory can be adapted for many kinds of materials, and make the former simple strength theories to be its special samples or its linear approach. Therefore, the unified strength theory is adopted to analyze the discontinuous bifurcations of materials for plane strain problem. The mathematical expression of the unified strength theory for plane strain problems is F = ( 1 + b ) ( 1 + sin φ ) σ1 − ( 1 − sin φ ) ( bσ 2 + σ3 ) − 2 ( 1 + b ) c cos φ = 0

When σ 2 ≤

1 2

(σ1 + σ3 ) +

sin φ 2

(σ 1 − σ 3)

(9-50a)

F ' = (1 + sin φ ) (σ 1 + bσ 2) − (1 − sin φ ) ( 1 + b ) σ 3 − 2 ( 1 + b ) c cos φ = 0

When σ 2 ≥

1 sin φ (σ + σ ) + (σ 1 − σ 3 ) 2 1 3 2

(9- 50b)

We chose the first equation of the unified strength theory (9-50a), because of the intermediate principal stress is σ2 =

m 1 sin φ (σ + σ ) ≤ (σ 1 + σ 3) + (σ 1 − σ 3) ( 0 < m 1) 2 1 3 2 2

(9-51)

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain

259

Substituting Eq. (9-51) into Eq.(9-50), we have F = ( 1 + b ) ( 1 + sin φ ) σ 1 −

1 2

( 1 − sin φ ) ( bmσ 1 + bmσ 3 + 2σ 3 ) − 2 ( 1 + b ) c cos φ = 0 (9-52)

definite f = ∂F , then we have ∂σ f1 = (1 + b ) ( 1 + sin φ ) σ 1 − f2 = −

1 2

bm 2

( 1 − sin φ ) (9-52)

( 1 − sin φ ) ( bm + 2 )

f3 = 0

The angle of shear band is obtained as follows (Zhang 2000) tg 2θ =

f1 f2

=

2(1 + b )(1 + sin ϕ ) − bm (1 − sin ϕ ) (1 − sin ϕ )(2 + bm )

(9-53)

The direction angle of shear band is

cos 2θ =

b (1 − m) + (2 + b + bm ) sin ϕ0 2 + b (1 + sin ϕ0 )

when mĮ1,

(9-54)

Equation (9-54) for plastic plane strain problems can be simplified to cos 2θ =

2(1 + b ) sin ϕ 0 2 + b (1 + sin ϕ 0)

when m=1,

(9-55)

This result is similar to that of the unified slip field theory for plane strain problems. The direction angle of shear band is sensitive to the failure criterion. The unified slip field theory give us a effective method to study this problems. The discontinuous bifurcations of elasto-plastic material for plane stress problems will be described in detail in Chapter 11.

260

9 Unified Slip-Line Field Theory for Plane Strain Problem

Summary A unified slip line field theory for plane strain problems based on the unified strength theory is described in this chapter. The unified slip line field theory for plane strain problems is composed of a group of orthogonal and non-orthogonal slip line fields. Many presently used orthogonal or non-orthogonal slip line field theories based on single shear strength theories are special cases (Tresca material slip field, Mohr-Coulomb material slip field and the twin-shear material slip field) or linear approximation (Huber-von Mises material) of the unified slip field theory system. By introducing an intermediate principal stress parameter, m, the new method can reflect the intermediate principal stress of plane strain problem, where the intermediate principal stress is the principal stress in z direction. Experiments and Elasto-Plastic Finite Element calculations have been used to verified the validity of the unified slip theory. The unified strength theory, the unified slip theory can be used in many engineering fields, especially for materials with obvious intermediate principal stress effect. The unified slip line field theory for plane strain problems has the following advantages: 1. It is a system of orthogonal and non-orthogonal slip line filed, which encompasses, in a piece-wise linear manner, other slip line field theories. All other slip line field theories are its special cases or linear approximations; 2. It can reflect the different effects of intermediate principal stress on different materials by introducing unified strength theory parameter b; 3. Giving a series of new slip line fields, and establishing the relations among available slip line field theories; 4. Introducing an intermediate principal stress parameter m, which can comply with different plane strain compressible and non-compressible materials. 5. It agrees with experimental results and can be easily used in many engineering fields.

Problems Problem 9.1 The extension of a strip with a sufficiently large circular hole for non-SD material was shown in Fig. P8.1 of chapter 8. Can you obtain a more complete study on this subject using the unified slip field theory for non-SD material ( α = 1 , and b= 0, b =1/2, b =1). Problem 9.2 The extension of a strip with a sufficiently large circular hole for non-SD material was shown in Fig. P8.1 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1).

Problems

261

Problem 9.3. The extension of a strip with ideal (infinitely thin) cuts (crack) for non-SD material was shown in Fig. P8.2 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory ( α = 1 , and b=0, b=1/2, b=1). Problem 9.4. The extension of a strip with ideal (infinitely thin) cuts (crack) for non-SD material was shown in Fig. P8.2 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1). Problem 9.5. The extension of a strip with angular notches for non-SD material was shown in Fig. P8.3 last chapter. Can you obtain a more complete study on this subject using the unified slip line field theory (α=1, and b=0, b=1/2, b=1). Problem 9.6. The extension of a strip with angular notches for non-SD material was shown in Fig. P8.3 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1). Problem 9.7. The extension of a strip with circular base for non-SD material was shown in Fig. P8.4 of chapter 8. Can you obtain a study on this subject using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.8. The extension of a strip with circular base for non-SD material was shown in Fig. P8.4 of chapter 8. Can you obtain a more complete study on this subject using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.9. The slip line field of indentation at the bottom of a flat trench was shown in Fig.P8.5 of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.10. The slip line field of indentation at the bottom of a flat trench was shown in Fig.P8.5 last chapter. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.11. The slip line field of indentation at the foot of a very deep vertically sided groove was shown in Fig.P8.6of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.12. The slip line field of indentation at the foot of a very deep vertically sided groove was shown in Fig.P8.6 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1).

262

9 Unified Slip-Line Field Theory for Plane Strain Problem

Problem 9.13. The slip line field of indentation at the top by a flat punch was shown in Fig.P8.7 of chapter 8. Find the limit load by using the unified slip line field theory for nonSD materials (α=1, and b=0, b=1/2, b=1). Problem 9.14. The slip line field of indentation at the top by a flat punch was shown in Fig.P8.7 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.15. The slip line field of a strip weakened by one-sided deep notch with a circular base was shown in Fig.P8.8 last chapter. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.16. The slip line field of a strip weakened by one-sided deep notch with a circular base was shown in Fig.P8.8 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.17. The slip line field of a strip weakened by two-sided deep notch with a circular base was shown in Fig.P8.9 of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.18. The slip line field of a strip weakened by two-sided deep notch with a circular base was shown in Fig.P8.9 last chapter. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.19. Figure P9.1 shows the slip line field of a pure bending strip weakened by two-sided angular notch. The limit moment for the Tresca material is

1 § · 2 π π − γ ¸ h σ s , for γ ≥ + M = ¨1 + 2 4 2 © ¹

Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.20.

Find the limit moment of a pure bending strip weakened by two-sided angular notch (Fig. P9.1) by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1).

Problems

Fig. P9.1 Two-sided angular notch

263

Fig. P9.2 One-sided angular notch

Problem 9.21. Figure P9.2 shows the slip line field of a pure bending strip weakened by one-sided angular notch. The limit moment for the Tresca material is

§ π + π − 2 γ · h2 σs , for γ ≥ 1 M = ¨¨ ¸¸ © 4 + π − 2γ ¹ 2

Find the limit moment by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.22. Find the limit moment of a pure bending strip weakened by one-sided angular notch by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.23. Figure P9.3 shows the slip line field of a pure bending strip weakened by one-sided angular notch with γ < 1 . Find the limit moment by using the unified slip line field theory for non-SD materials and SD materials

Fig. P9.3 Bending strip with angular notch

Fig. P9.4 Indentation of a semi-infinite mass

Problem 9.24. Figure P9.4 shows the slip line field of an indentation of a semi-infinite mass of rigid-perfectly plastic material by a rigid straight-sided, acute-angle indenter (Hill 1950; Johnson and Mellor 1961). The limit load for the Tresca material is

264

9 Unified Slip-Line Field Theory for Plane Strain Problem

P = 2 a (1 + γ )σs

Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.25. Find the limit load of an indentation of a semi-infinite mass of rigid-perfectly plastic material by a rigid straight-sided, acute-angle indenter by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.26. The slip line field of a thick-walled cylinder is shown in Fig.P9.5. The limit pressure for the Tresca material is

P = σs ln

b a

Find the limit pressure by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1).

Fig. P9.5 Slip line field of a thick-walled cylinder (Tresca material)

Problem 9.27. Find the limit pressure for a thick-walled cylinder by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.28. Comparing the results of the slip line field theory for a thick-walled cylinder with the elasto-plastic analysis in Chapter 15. Problem 9.29. Figure P9.6 shows a slip line field of a strip weakened by center crack for non-SD materials. Determine thelimit load by using the unified slip line field theory for SD materials (α 1, and b=0, b=1/2, b=1).

Problems

265

Fig. P9.6 A slip line field of a strip weakened by center crack

Problem 9.30. The slip line field of a strip with a hole under uniform pressure was shown in Fig. P8.9 last chapter. Find the limit pressurefor non-SD materials and SD materials by using the unified slip field theory. Problem 9.31. The slip line field of extrusion through a die over a smooth container wall was studied by Johnson et al (1962). Figure P9.7 shows the fan shaped slip line field The limit pressure were given by using the Tresca condition as follows P = §¨1 + π ·¸ h σs 2¹ © Find the limit pressure for SD materials by using the unified slip line field theory (α 1, and b=0, b=1/2, b=1).

Fig. P9.7 Extrusion through a die over a smooth container wall

Problem 9.32. Find the limit pressureof extrusion through a die over a smooth container wall for SD materials by using the unified slip line field theory (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.33. The slip line field of drawing of a strip was studied by Johnson et al (1962). Figure P9.8 shows the fan shaped slip line field. Limit drawing force for the Tresca material is

266

9 Unified Slip-Line Field Theory for Plane Strain Problem

P=

2 hσs (1 + γ ) sin γ 1 + 2 sin γ

o

when γ ≥ 42 27 ' , H = 2h

Find the drawing force for non-SD materials by using the unified slip line field theory (α=1, and b=0, b=1/2, b=1). Problem 9.34 . Find the drawing force for SD materials by using the unified slip line field theory (α ≠ 1, and b=0, b=1/2, b=1).

Fig. P9.8 Extrusion of a strip

Fig. P9.9

Problem 9.35 . The slip line field and limit pressure for extrusion problems were studied by Johnson et al. as shown in Fig. P9.9. The limit extrusion force for the Tresca material is π · § P = 2 ¨1 + ¸ a σs 2¹ ©

when b =2a

Find the limit pressure of extrusion by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.36 . Find the limit pressure of extrusion by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.37. Determine the limit load of a deep beam shown in Fig. P9.10

Problems

267

Fig. P9.10

Problem 9.38. A series of results can be obtained by using the unified slip line field theory for various plane strain problems. All the solutions of the problems in this chapter have not been studied before. Can you try to give a series of new results for these problems, and try to use in practice. Problem 9.39. The slip line field and limit pressure for slop stability problems were given by ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) for the Mohr-Coulomb material as shown in Fig. P9.11. The limit pressure is

1 + sin ϕ ½ q = C ⋅ cot ϕ ® exp ª¬(π − 2 χ ) tan ϕº¼ − 1¾ ϕ − 1 sin ¯ ¿

Fig. P9.11

Find the limit pressure of slop by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1) and SD materials (α ≠ 1, and b=0, b=1/2, b=1).

268

9 Unified Slip-Line Field Theory for Plane Strain Problem

References and Bibliography Chen G. and Baker G (2001). Gradient-dependent plasticity with a 3-node incompatible element for the plastic multiplier. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 1129–1134. de Borst R., Pamin J and Sluys LJ (1995) Computation issues in gradient plasticity, In: Continuum Models for Materials with Micro-structure, H.B. Mfihlhaus (ed.), Wiley: Chichester, 159–200. Drucker DC, Greenberg HJ and Prager W (1951) The safety factor of an elastic-plastic body in plane strain, J. Appl. Mech., 18: 371–378. Ford H (1954) The Theory of Plasticity in Relation to Engineering Application, J. AppL Math. Phys., 5: 1–35. Geiringer H (1930) Beit zum Vollstiindigen ebenen Plastizitits-problem, Proc 3rd Intern. Congr. Appl. Mech, 2: 185–190. Hencky H(1923) Ueber einige statisch bestimmte Faelle des Gleichgewichts in plastischen Koerpern Z. angew. Math Mech., 3: 245– 251. Hill R (1949) The Plastic Yielding of Notched Bars Under Tension, Quart. Mech. AppL Math., 2: 40– 52. Hill R(1956), The Mechanics of Quasi-Static Plastic Deformation in Metals, In: Survey in Mechanics, G. K. Batcheler and R. M. Davis eds, Cambridge, Johnson W and Mellor PB (1962), Plasticity for Mechanical Engineers, Van Nostrand, Princeton, N.J. Johnson W, Sowerby R, Venter RD (1982), Plane-Strain Slip Line Fields for Metal Deformation Processes--A Source Book and Bibliography, Pergamon Press, Oxford. Moore ID and and Rowe RK (1991) Objective solutions for bearing capacity of strainsoftening soils. In: Beer G, Booker JR and Carter JP eds. Computer Methods and Advances in Geomechanics. Rotterdam: A.A.Balkema, Vol.2,1183–1189. Panayotounakos D (1996) Ad Hoc Exact Solutions for the Stress and Velocity Fields in Rigid Perfectly Plastic Materials Under Plane-Strain Conditions. Int. J. Plast., 12:1069– 1190. Prager W (1955) The Theory of Plasticity: A Survey of Recent Achievements, Proc. Inst. Mech. Eng., 169: 41–57. Prager W (1959) Introduction to Plasticity, Addison-Wesley, Reading, Mass. Prager W and Hodge P G Jr (1951) Theory of Perfectly Plastic Solids, Wiley New York. Prandtl L (1920) l~ber die H~irte Plastischer Koerper, Goettinger Nachr., Math. Phys. KI.,74–85. Thomsen EG, Yang CT and Kobayashi S (1965) Mechanics of Plastic Deformation in Metal Processing, Macmillan, New York. Wunderlich, Findeib and Cramer in (2001) Finite element analysis of bearing capacities in geomechanics considering dilatant and contractant constitutive laws. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 2001, 533–538. Yu Mao-hong (1983), Twin Shear Stress Criterion, Int. J. of Mech. Sci., 25(1), 71–74, Yu Mao-hong, He, Li-nan, Song, Ling-yu (1985), Twin Shear Stress Theory and Its Generalization, Scientia Sinica (Science in China), Series A, (English edn.), 28(11), 1174–1183. Yu Mao-hong and He Li-nan (1991), A new model and theory on yield and failure of materials under complex stress state. In: Mechanical Behaviour of Matterials-VI. Yu Mao-hong, He Li-nan (1992), Generalized Twin Shear Stress Yield Criterion and Its Generalization, Chinese Science Bulletin (English edn.), 37(24), 2085–2089. Yu Mao-hong, et al (1992), Computer Image Analysis of the Plastic Zone of Structure, Journal of Xi'an Jiaotong University, 26(2), 121–122 (in Chinese).

References and Bibliography

269

Yu Mao-Hong, Liu Jian-Yu and Ma Guo-wei (1994), Twin-shear slip line theory: orthogonal and non-orthogonal slip line fields. Journal of Xi’an Jiaotong University, 28(2):122–126. Yu Mao-hong. (1998) Twin-shear Theory and Its Applications. Beijing: Science Press (in Chinese). Yu MH and Fan SC eds (1998) Strength Theory: Applications, Developments and Prospects for the 21st Century. New York, Beijing: Science Press. Yu Mao-hong. (2004) Unified Strength Theory and Its Applications. Berlin: Springer. Zenkiewicz OC(1992), Computational Mechanics Today, Int. J. Numer. Methods in Engrg., 34, 9–33. Zhang YQ (2000) Analysis of damage and Discontinuous bifurcations for Elarto-Plastic Geomaterials. Dissertation of Doctor at Xi’an Jiaotong University, Xi’an, China (in Chinese) Zhang YQ and Yu MH (2001) Discontinuous bifurcations of metallic materials for plane stress. Chinese J. of Mechanical Engineering, 37(4): 62–85 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of elasto-plastic materials for plane stress. Acta Mechanica Sinica, 33(5): 706–713 (in Chinese, English Abstract). Zimmermann Th and Commend S (2001) Stabilized finite element applications in geomechanics. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 2001, 533–538. Ȼɟɪɟɡɚɧɥɟɜ ȼȽ (1952) Ɉɫɟɫɢɦɦɟɬɪɢɱɧɚɹ Ɂɚɞɚɱɚ Ɍɟɨɪɢɢ ɉɪɟɞɟɥɶɧɨɝɨ Ɋɚɜɧɨɜɟɫɢɹ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. Ɇɨɫɤɜɚ: Ƚɨɫ. ɂɡɞ. Ɍɟɯ. Ɍɟɨ. Ʌɢɬɟɪɚɬɭɪɵ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1942) ɋɬɚɬɢɤɚ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. ɂɡɞ. Ⱥɇ ɋɋɋɊ, Ɇɨɫɤɜɚ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) ɋɬɚɬɢɤɚ ɋɵɩɭɟɣ ɋɪɟɞɵ (Third ed.).Ƚɨɫ. ɂɡɞ. Ɏɢɡ-Ɇɚɬ. Ʌɢɬɟɪɚɬɭɪɵ. Ɇɨɫɤɜɚ (in Russia)

10 Twin-Shear Characteristics Field for Plane Stress Problem

10.1 Introduction The twin-shear slip field and the unified slip line field theory for plane strain problems have been described in Chapters 8 and 9. This chapter deals with the twin-shear characteristics filed for plane stress problems. For plane stress problems, characteristic methods can be used to solve the quasi-linear differential equation systems of stress and velocity fields. Judgments on the types of these differential equation systems can be made using the theory of characteristics. They may be elliptic or hyperbolic, depending on the considered stress state. The methods of characteristics based on the Huber-von Mises and the Tresca criteria can be found in the literature of Kachanov (1971), Martin (1973), Yan (1988) and Panoyotomakos (1999) for plane stress problems. A new characteristics method for plane stress problems was established based on the twin-shear yield criterion (Yu 1961, 1983) by Yan and Bu in 1993 and 1996. The methods of characteristics based on the Huber-von Mises, the Tresca and the twin-shear criteria can be applied to the limit analysis of the plane stress problems. However, they are only adapted for the non-SD (strength differential) materials with τ 0 ≈ 0.58σ t , τ 0 = 0.5σ t and τ 0 = 2σ t /3, respectively, but fail for the SD materials. Although the method of characteristics based on the Mohr-Coulomb criterion takes account of SD effect, it is only adapted for the material with τ 0 =σ t σ c/ (σ t + σ c).

10.2 Characteristics Method based on the Tresca Criterion and the Huber-von Mises criterion 10.2.1 Characteristics Method based on the Tresca Criterion The Tresca criterion in plane stress state is shown in Fig. 10.1. If χ and λ are introduced for the cases of σ x σ y ≤ τ ²xy and σ xσ y ≥ τ² xy respectively, the following expressions of stresses satisfy automatically the Tresca criterion in plane stress state,

10.2 Tresca Criterion and the Huber-von Mises criterion

271

σ2 σs

F

E

σs

D

A

σ1

σs

B C

σs Fig. 10.1 Tresca criterion in plane stress state

σx = 2k χ + k cos 2ϕ

(10-1a)

σy = 2k χ − k cos 2ϕ

(10-1b)

τxy = k sin 2ϕ

(10-1c)

on lines AB and DE in Fig. 10.1. σ x = σ s [ s (1 − λ ) + λ cos 2ϕ ]

(10-2a)

σ y = σ s [ s (1 − λ ) − λ cos 2ϕ ]

(10-2b)

τ xy = k sin 2ϕ

(10-2c)

on lines BC, CD, EF and FA in Fig. 10.1, where 1 when σ1 > 0, σ2 > 0 ° s=® ° −1 when σ < 0, σ < 0 1 2 ¯

(10-3)

The equations of equilibrium determined by the stress components in Eq. (10-1) and Eq. (10-2) are of the hyperbolic type and the parabolic type, respectively. The equations of the characteristics are

272

10 Twin-Shear Characteristics Field for Plane Stress Problem

(10-4)

dy § · = tan ¨ϕ ± π ¸ 4¹ dx © dy s + cos 2ϕ − cot ϕ , =− =® dx sin 2ϕ ¯ tan ϕ ,

(10-5)

It can be seen that Eq. (10-4) has two orthogonal families of characteristics, which differentiate π/4 with the direction of principal stresses σ1 and σ2. It coincides with the definition of slip line. The two families of characteristics have the following forms, χ + ϕ = C1

(10-6a)

χ − ϕ = C2

(10-6b)

Eq. (10-6) is the same as Hencky equation for the plane strain problem, when assuming χ = σ/2k. Eq. (10-5) has only one family of characteristics, which is parallel to the intermediate principal stress by considering that it is a three-dimensional problem. The characteristic line is the intersecting line between xy-plane and the plane which offsets an angle of π/4 from the directions of the maximum and minimum stresses. This agrees with the explanation of the slip line equation (17-4), as long as considering the difference of the cases σ xσ y ≤τ ²xy and σ xσ y ≥τ ²xy . From the above analysis, if the Tresca criterion is applied, the characteristics with respect to the lines AB and DE (σ x σ y >τ ² xy) can be solved by the hyperbolic type equations. On other lines (σ x σ y >τ ² xy), it can be solved by integrating the differential equation directly.

10.2.2 Characteristics Method based on the Huber-von Mises Criterion The Huber-von Mises criterion in plane stress state is given in Fig. 10.2. If a variable ω is introduced, the stress components satisfy Huber-von Mises criterion can be obtained by σ x = k ( 3 cos ω + sin ω cos 2ϕ ) σy = k

(

3 cos ω − sin ω cos 2ϕ

τ xy = k sin ω sin 2ϕ

)

(10-7a) (10-7b) (10-7c)

10.2 Tresca Criterion and the Huber-von Mises criterion

σ2 ω= E′

5π 3

σs C′

D′ ω =

3π ω= 2 4π

F′ ω =

σs

G′

ω =π

ω=

273

ω =0 11π A 6 π ω = C σs 6

3

7π 6

E

D ω = π σ1 3

ω=

F G5π ω = 2π ω= 3 6

π

2

B

σs

Fig. 10.2 Huber-von Mises criterion in plane stress state

The characteristics of the equilibrium equation determined by Eq. (10-7) is dy 3 sin ω sin 2ϕ ± 3 − 4cos 2 ω = dx 3 sin ω cos 2ϕ − cos ω

(10-8)

It is obvious that there exist two families of characteristics only when 3 − 4cos 2 ω > 0 ( π / 6 < ω < 5π / 6 or 7π / 6 < ω < 11π / 6 ) (lines CG and C ′G ′ in Fig. 10.2). Otherwise, there is no characteristics ( 3 − 4cos 2 ω < 0 ) (lines CC ′ and GG ′ in Fig. 10.2) or there is only one family of the characteristics ( 3 − 4cos 2 ω = 0 ) (points C, C′, G, and G′ ). For the hyperbolic type, two supplementary incremental expressions are needed ψ =

χ =−

π

2

1 2

³

§ cot ω · 1 − cos −1 ¨ ¸ 2 © 3 ¹ ω π 6

3 − 4cos 2 ω dω sin ω

(10-9a)

(10-9b)

The equation of characteristics can then be obtained as

dy = tan(ϕ ± ψ ) dx

(10-10)

274

10 Twin-Shear Characteristics Field for Plane Stress Problem

Along these two families of the characteristics, it has χ + ϕ = C1

(10-11a)

χ − ϕ = C2

(10-11b)

which has the same form with Eq. (10-6), however, χ is much more complex than that in Eq. (10-6). Meanwhile, it can be found that the two families of characteristics are not orthogonal to each other. The angle between the two families of the characteristics is 2ψ, which varies with locations. From the above analysis, for Huber-von Mises criterion, the problem can be solved by the characteristics method of the hyperbolic type when π/6 < ω < 5π/6, or 7π/6 < ω < 11π/6, however, the process will be very tedious due to the non-orthogonal feature. On other segments it will be more difficult to solve the characteristics.

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion Characteristics method based on the twin-shear yield criterion was proposed by Yan and Bu in 1993. In(σ x, σ y, τ xy) plane stress states, three principal stresses are σ1 =

σ2 =

σx + σ y

2 σx + σ y

2

2

§ σx − σ y · 2 + ¨ ¸ + τ xy 2 © ¹

(10-12a)

2

§ σx − σ y · 2 − ¨ ¸ + τ xy 2 © ¹ σ3 = 0

(10-12b) (10-12c)

The twin-shear yield criterion has the following form, 1 3 1 f = σ 1 − (σ 2 + σ 3 ) = σ s = k , when σ 2 ≤ (σ 1 + σ 3) 2 2 2

(10-13a)

1 3 1 (σ 2 + σ 3) − σ 3 = σ s = k , when σ 2 ≥ (σ 1 + σ 3) 2 2 2

(10-13b)

f =

The yield loci of the twin-shear yield criterion in the plane stress state are shown in Fig. 10.3.

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion

275

Fig. 10.3 Twin-shear yield criterion in plane stress state

The functions of the six segments in Fig. 10.3 can be expressed as follows, f1 = 2σ 1 − σ 2 = 3k

(10-14a)

f2 = 2 σ 1 − σ 2 = −3k

(10-14b)

f3 = 2σ 2 − σ 1 = 3k

(10-14c)

f 4 = 2σ 2 − σ 1 = −3k

(10-14d)

f5 = σ 1 − σ 2 = −3k

(10-14e)

f 6 = σ 1 − σ 2 = 3k

(10-14f)

Substituting Eq. (10-10) into Eq. (10-14), we derive the twin-shear yield criterion function expressed in terms of the three principal stresses as follows, 1 1 σ x + σy + 3 (σ x − σ y ) 2 + τ 2xy = 3k , 2 4 when σ x + σ y ≤ 6

(10-15a)

1 (σ x − σ y ) 2 + τ 2 xy 4

1 (10-15b) ( σ x − σ y ) 2 + τ 2xy 4 Neglecting body force, the equations of equilibrium for plane stress problems are σ x + σ y = 3k , when

∂σ x ∂x

+

∂τ xy ∂y

σx + σy ≥ 6

= 0,

∂τ xy ∂x

+

∂σ y ∂y

=0

(10-16)

276

10 Twin-Shear Characteristics Field for Plane Stress Problem

10.3.1 Hyperbolic Type For the yield condition of Eq. (10-15a), assuming σ1 − σ 2

2

= λ k,

σ1 + σ 2

2

= 3(1 − λ ) sk

(10-17)

where S = 1, when σ1 + σ 2 > 0 ; S = 0, when σ 1 + σ 2 = 0 ;

(10-18)

S = −1, when σ 1 + σ 2 < 0 Combining Eqs. (10-10) and (10-17) gives 2

σx + σ y §σ x − σ y · 2 = 3(1 − λ ) sk ¨ ¸ + τ xy = λ k , 2 © 2 ¹

(10-19)

The corresponding stress components are σ x = k [ 3s (1 − λ ) + λ cos 2ϕ ]

(10-20a)

σ y = k [ 3s (1 − λ ) − λ cos 2ϕ ]

(10-20b)

τ xy = k λ sin 2ϕ

(10-20c)

The above stresses satisfy Eq. (10-15a) automatically, in which λ is in the range of 1 ≤ λ ≤1 2

(10-21)

Combining Eq. (10-20) and Eq. (10-16) derives

−3s

∂λ ∂λ ∂λ ∂λ ∂λ + cos 2ϕ − 2λ sin 2ϕ + sin 2ϕ + 2λ sos2ϕ =0 ∂x ∂x ∂x ∂y ∂y

∂λ ∂ϕ ∂λ ∂λ ∂ϕ − 3s − =0 sin 2ϕ + 2λ sos 2ϕ sos 2ϕ + 2λ sin 2ϕ ∂x ∂x ∂y ∂y ∂y For any line in xy-plane, increments of λ and ϕ can be written as dλ =

∂λ ∂λ dx + dy ∂x ∂y

(10-22a) (10-22b)

(10-23a)

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion

277

∂ϕ ∂ϕ (10-23b) dx + dy ∂x ∂y Eq. (10-22) together with Eq. (10-23) makes an algebraic equation system with ∂λ /∂ x, ∂λ /∂ y, ∂ϕ /∂ x, ∂ϕ /∂ y as unknowns. Let the determinant of coefficients vanish, i.e. dϕ =

−3s + cos 2ϕ sin 2ϕ ∆= dx 0

sin 2ϕ −3s − cos 2ϕ dy 0

−2λ sin 2ϕ 2λ cos 2ϕ 0 dx

2λ cos 2ϕ 2λ sin 2ϕ =0 0 dy

(10-24)

It is then obtained,

dy −3s sin 2ϕ ± 2 2 s = dx 1 − 3s cos 2ϕ

(10-25)

Assuming s = −3cos 2ϕ , Eq. (10-25) can be rewritten as

1 dy § s· = tan(ϕ B ψ ),ψ = cos −1 ¨ − ¸ 2 dx © 3¹

(10-26)

Eq. (10-26) determines two families of characteristics. As can be seen, the two families of characteristics differ angles ±ψ from the direction of the principal stress σ1 . Here those corresponding to the plus sign are assigned as family α and those to the minus sign as family β. In order to derive the relationship between λ and ϕ, from Eqs. (10-22), (10-23) and (10-24), it has ϕ + 2s ln λ = C1 (along α line)

(10-27a)

ϕ − 2 s ln λ = C2 (along β line)

(10-27b)

Thus, based on the twin-shear yield criterion, it can be solved by the characteristics method for stress state on lines of FA, BC, CD, EF (see Fig. (10.3)).

10.3. 2 Elliptic Type For the yield condition Eq. (10-15b) (AB and DE in Fig. (10.3)), it has

∂λ ∂ϕ ∂λ ∂ϕ cos 2ϕ − 2λ sin 2ϕ sin 2ϕ + 2λ cos 2ϕ + =0 ∂x ∂x ∂y ∂y

(10-28a)

∂λ ∂ϕ ∂λ ∂ϕ sin 2ϕ + 2λ cos 2ϕ cos 2ϕ + 2λ sin 2ϕ − =0 ∂x ∂x ∂y ∂y

(10-28b)

278

10 Twin-Shear Characteristics Field for Plane Stress Problem

where λ ≤ 1/2. Let the determinant of the coefficients of Eqs. (10-28) and (10-23) vanish, it has

cos 2ϕ sin 2ϕ ∆= dx 0

sin 2ϕ − cos 2ϕ dy 0

−2λ sin 2ϕ 2λ cos 2ϕ 0 dx

2λ cos 2ϕ 2λ sin 2ϕ =0 0 dy

(10-29)

Then it is obtained (dx) 2 + (dy ) 2 = 0

(10-30)

There is no real root for dy/dx. The equilibrium differential equation determined by the stress components which satisfy Eq. (10-15b) is an elliptic type, thus the characteristics do not exist. Based on the above analysis, it can be found that the problem of the stress state on the lines of FA, BC, CD, EF (see Fig. (10.3)) is of the hyperbolic type and can be solved by the characteristic method. However, the problem of the stress state on the other two lines AB and DE (see Fig. (10.3)) is of the elliptic type which can not be solved by the characteristic method. Nevertheless, the yield condition of Eq. (10-15b) is very simple and can be solved directly by using equilibrium equation and the yield function.

10.4 Twin-shear Characteristics Field for Plane Stress Problems (Velocity Field) 10.4.1 Velocity Field corresponding to Eq. (10-15b) Applying associate flow rule, the strain rate can be obtained from Eq. (10-15b) as ξ x = ξ y , ζ xy = 0

(10-31)

The velocity components are thus

∂Vx ∂Vy − =0 ∂x ∂y ∂Vx ∂V y + =0 ∂x ∂y The increments of the velocity components are ∂Vx ∂V dx + x dy = dVx ∂x ∂y

(10-32a)

(10-32b)

(10-33a)

10.4 Twin-shear Characteristics Field for Plane Stress Problems

∂Vy ∂x

dx +

∂V y ∂y

The determinant of coefficients of

279

(10-33b)

dy = dV y

∂Vx ∂Vx ∂V y ∂V y , , , in the above four ∂x ∂y ∂x ∂y

equations equal to 0, which gives

1 0 0 −1 0 1 1 0 ∆= =0 dx dy 0 0 0 0 dx dy

(10-34)

Then (dx)2 + ( dy ) 2 = 0

(10-35)

There is no real root for dy/dx. The equation is of the elliptic type and the characteristics do not exist.

10.4.2 Velocity Field corresponding Eq. (10-15a) Corresponding to the yield condition of Eq. (10-15), it has ζx = α

ª º σx − σ y ∂f s 1 » =α « + « 6 2 ( σ − σ ) 2 + 4τ 2 » ∂σ x x y xy ¼ «¬

(10-36a)

ζy = α

ª σx − σ y ∂f s 1 =α « − « 6 2 (σ − σ ) 2 + 4τ 2 ∂σ y x y xy ¬«

(10-36b)

ζ xy = α

º » » ¼»

2τ xy ∂f =α − ∂τ xy (σ x − σ y ) 2 + 4τ 2 xy

(10-36c)

where f is the twin-shear yield function, α ( > 0) is a scalar factor. Combining Eq. (10-20) and Eq. (10-36) derives

∂V y ∂Vx ∂Vy ∂Vx ∂V y ∂Vx + − ∂y ∂y ∂z ∂x ∂y ∂x = = = s 1 s 1 ϕ ϕ sin 2 cos 2 + cos 2ϕ − cos 2ϕ 6 2 6 2

(10-37)

280

10 Twin-Shear Characteristics Field for Plane Stress Problem

Eq. (10-37) can be rewritten as §s · ∂Vx § s · ∂V y − ¨ + cos 2ϕ ¸ =0 ¨ − cos 2ϕ ¸ ©3 ¹ ∂x © 3 ¹ ∂y

§ ∂V ∂V y · § ∂Vx ∂V y · cos 2ϕ ¨ x + − ¸ − sin 2ϕ ¨ ¸=0 ∂x ¹ ∂y ¹ © ∂y © ∂x The determinant of the coefficient must vanish, which gives s − cos 2ϕ 3 ∆ = − sin 2ϕ dx 0

0

0

cos 2ϕ dy

cos 2ϕ 0

0

dx

s − − cos 2ϕ 3 sin 2ϕ =0 0

(10-38a)

(10-38b)

(10-39)

dy

Then the following equation is obtained dy −3sin 2ϕ ± 2 2 −3sin 2ϕ ± 2 2 s = = dx s − 3cos 2ϕ 1 − 3s cos 2ϕ

(10-40)

Eq. (10-40) is the same with the characteristics of the stress field. Thus, the characteristics of the velocity field just coincide with those of the stress field for the twin-shear yield criterion, just like the Tresca criterion and the Huber-von Mises criterion. Combining Eqs. (10-33), (10-38) and (10-39) gives dVx + dV y

dy =0 dx

(10-41)

Corresponding velocity field can then be obtained through Eqs. (10-26) and (10-41)

dVx + dVy tan(ϕ − ψ ) = 0 , along α line

(10-42a)

dVx + dVy tan(ϕ + ψ ) = 0 , along β line

(10-42b)

Considering an arbitrary point P at an plane curve L on the xy plane, if local coordinate system (t, n) is applied, the first equation of Eq. (10-38) can be rewritten as

§s · ∂Vt § s · ∂V − ¨ + cos 2ϕ ¸ n ¨ − cos 2ϕ ¸ ∂ 3 3 t © ¹ © ¹ ∂n

(10-43)

where t and n are respectively in the tangential and normal directions of the curve L. Coefficients of ∂Vn/∂n of Eq. (10-43) equals to 0, then cos 2ϕ = − s / 3

(10-44)

10.5 Applications of the Twin-shear Characteristics Method

281

From Eq. (10-43), it has ζ t = ∂Vt / ∂t = 0

(10-45)

10.5 Applications of the Twin-shear Characteristics Method 10.5.1 Velocity Discontinuous Line in Uniaxial Tension In the plane stress problem, it is possible that velocity discontinuities exist not only in the tangential, but also in the normal direction of the slip line. A ‘necking’ deformation zone may be formed. Assuming that the neck has a small width b (in the limiting case b→0) and by a simple derivation, it can be seen that the line of velocity discontinuity is just one of the velocity characteristics, and the relative velocity v is perpendicular to the velocity characteristics of the other family (Kachanov 1971). In this example, σ y = σ 1, σ x = 0, τ xy = 0, so s = 1. There are two families of velocity characteristics, and the value of ψ (the angle between the velocity characteristics and the principal stress σ 1) is given by 1 § 1· (10-46) cos −1 ¨ − ¸ = 54° 44′ 2 © 3¹ Therefore, the angle γ between the relative velocity v and principal stress σ 1 is ψ =

γ = 90° − ψ = 35° 16′

(10-47)

Fig. 10.4 Plate specimen in uniaxial tension

It can be seen that by using the twin-shear yield criterion, the solution of this problem is simple and straightforward. The same value of ψ can also be obtained by using the Huber-von Mises yield criterion, but the process will be more cumbersome (Kachanov 1971). This value

282

10 Twin-Shear Characteristics Field for Plane Stress Problem

(54° 44′ ) has been verified by experiment (Nadai 1950) and coincide with the result of Huber-von Mises (Yan 1988). The line of velocity discontinuity is known as Lüder’s line. Based on the Tresca yield criterion, ψ can take an arbitrary value between 45° and 90° ; obviously, it is unreasonable.

10.5.2 Limit Load of an Infinite Thin Plate with a Circular Hole An infinite thin plate, having a circular hole with radius a (Fig. 10.5), is subjected to a two-directional uniform tension q at infinity. Find the limit load qs and the corresponding stress distribution.

Fig. 10.5 An infinite plate with a circular hole

It is obvious that this is a plane stress problem. As the hole is free and the plate experiences two-directional uniform tension at infinity, on the edge of the hole there will be σ θ > 0 and σ r = 0 and at infinity there will be σ θ = σ r > 0. Thus σ θ ≥ σ r ≥ 0 holds in the whole plate, and then s = +1. Near the hole, the stress satisfies Eq. (10-15a). And equations of the characteristics passing through the point A (r = a, θ = 0) will be θ =±

1 r ln , ‘+’ for α line, ‘−’for β line 2 a

(10-48)

Along AP , it has ϕ + 2 ln λ = C 1

From ϕ = θ + π /2 and σ r

r =a

(10-49)

= 0 , we know λ A=3/4, thus, it has 1/ 2

λ =

3§ a · ¨ ¸ 4© r ¹

(10-50)

10.5 Applications of the Twin-shear Characteristics Method

283

The stress components are derived as follows ª

σθ = 3k «1 −

«¬

1/ 2 º

1§ a· ¨ ¸ 2© r ¹

ª «¬

(10-51b)

1/ 2 º

§a· ¸ ©r¹

σ r = 3k «1 − ¨

(10-51a)

» »¼

» »¼

With r increasing, λ will decrease. When r = 9a/4, λ = 1/2, which is the critical value for the hyperbola. When r > 9a/4, the equation is ellipse. Stress components can be derived from differential equation and yield criterion. 2º

(10-52a)

2º

(10-52b)

σr =

3k ª 27 § a · «1 − ¨ ¸ 2 «¬ 16 © r ¹

σθ =

3k ª 27 § a · «1 + ¨ ¸ 2 «¬ 16 © r ¹

» »¼ » »¼

Thus, limit load is qs = σ r

r →∞

=

3k =σs 2

(10-53)

Expressions of corresponding stresses are ª § a ·1/ 2 º 9 ° 2 σ s «1 − ¨ ¸ » , a ≤ r ≤ a 4 °° ¬« © r ¹ ¼» σr = ® ª 27 § a · 2 º ° 9 ° σ s «1 − ¨ ¸ » , r > a 16 r 4 © ¹ »¼ «¬ °¯

ª 1 § a ·1/ 2 º 9 ° 2σ s «1 − ¨ ¸ » , a ≤ r ≤ a 4 °° «¬ 2 © r ¹ ¼» σθ = ® ª 27 § a ·2 º ° 9 ° σ s «1 + ¨ ¸ » , r > a 4 «¬ 16 © r ¹ »¼ ¯°

(10-54a)

(10-54b)

For comparison, characteristics and stress distribution under the three yield criterion are shown in Figs. 10.6, 10.7 and 10.8. The same value of limit load qs = σs is obtained based on each of the aforementioned three yield criterion (Kachanov 1971).

284

10 Twin-Shear Characteristics Field for Plane Stress Problem

Fig. 10.6 Results of example 2: Twin-shear criterion

Fig. 10.7 Result of example 2: von-Mises criterion

Fig. 10.8 Results of example 2: Tresca criterion

10.5 Applications of the Twin-shear Characteristics Method

285

10.5.3 Thin Circular Ring Plate subjected to a Uniform Internal Pressure A thin circular ring plate with inner radius a and outer b = 2a, subjected to a uniform internal pressure q (Fig. 10.9). Find the limit load and the corresponding stress distribution. Through analysis similar to that in example 2, near the outer edge of the ring plate

Fig. 10.9 Example 3

λ=

ª

σ θ = 3k «1 −

«¬

ª

σ r = 3k «1 −

«¬

3 § 2a · ¨ ¸ 4© r ¹

1 § 2a · ¨ ¸ 2© r ¹ 1 § 2a · ¨ ¸ 2© r ¹

(1/ 2)

(1/ 2) º

» (c≤r ≤b ) »¼

(1/ 2) º

» (c≤r ≤b ) »¼

(10-55)

(10-56a)

(10-56b)

With r decreasing, λ will increase, and λ = 1 is the limit of availability of Eq. (10-13). Take c to denote this radius; thus, from Eq. (10-10) 9 c= a 8

(10-57)

In the region a ≤ r ≤ (9/8)a, s = −1, thus σ θ = −(3 − 4λ )k ( a ≤ r ≤ c )

(10-58a)

σ r = −(3 − 2λ ) k ( a ≤ r ≤ c )

(10-58b)

ψ =

1 1 cos −1 = 35D16' 2 3

(10-59)

286

10 Twin-Shear Characteristics Field for Plane Stress Problem

The equations of characteristics passing through the point r = a, θ = 0, are θ = ± 2 ln

r (‘+’ for α line, ‘−’ for β line) a

(10-60)

Then, −

π

2

− 2 ln1 = −

π

2

+ θ − 2 ln λ = −

r + 2 ln − 2 ln λ 2 c π

(10-61)

Hence, λ =

r 8r = c 9a

(10-62)

Substituting Eq. (10-19) into Eq. (10-18) § ©

32 r · ¸ 27 a ¹

(10-63a)

§ ©

16 r · ¸ 27 a ¹

(10-63b)

σ θ = −3k ¨1 − σ r = −3k ¨ 1 −

Since σθ + σ r = 3k 2 − (48 / 27)( r / a ) ≤ 3k in the region a ≤ r ≤ (9/8) a, the yield condition Eq. (10-15a) is always applicable for this region. Thus, the limit load is qs = σ r

r =a

= 1.222k = 0.815σ s

The characteristics and stress distribution are shown in Fig. 10.10.

Fig. 10.10 Results of example 3

10.6 Comparison of these Different Methods

287

Based on the Huber-von Mises and Tresca yield criterion, the values of limit loads are qs = 1.330k = 0.768σ s for Huber-von Mises yield criterion; and q s = 1.386k = 0.693σ s for the Tresca yield criterion.

10.6 Comparison of These Different Methods Yan and Bu (1993) have compared the three different characteristic methods based respectively on the twin-shear yield criterion, the Tresca criterion, and the Huber-von Mises criterion. The advantages and disadvantages of these methods are shown in Table 10.1 and Table 10.2. Through the comparison, the following conclusions can be drawn: 1. It would be simpler to derive the characteristics based on the Tresca criterion and the twin-shear criterion than the Huber-von Mises criterion. 2. The twin-shear yield criterion has the advantage in describing the velocity discontinuity for the unixial tension example. 3. It is suggested to use the Tresca criterion if the experimental data of a certain material offset the Huber-von Mises ellipse toward the Tresca polygon. If the experimental data locates outside the Huber-von Mises ellipse, the twin-shear yield criterion is suggested. Thus, application of the Huber-von Mises criterion can be avoided.

Table 10.1. Comparison of the three yield criterion

Criterion

Range of hyperbolic type σ1

Tresca

von Mises Twin-shear

σ2 σ1 σ2

σ1 σ2

0

(11-70)

Then, from Eq. (11-51) D

θ = 90

,

H db l l' = − (1 + ν ) 2 2 SS ' 2µ

(11-71)

314

11 Unified Characteristics Field Theory for Plane Stress Problem

Due to Hdb ≤ 0, the discontinuous bifurcations don’t occur at the plastic hardening state, and the bifurcation mode is split mode. When b = 1, P1 =P2, Q1 = Q2, the direction of bifurcation is arbitrary. When b=0, as the intermediary of the two modes, the mode of discontinuous bifurcations belongs to either split mode or shear band mode. 2. case of σ 1 ≥ 0 ≥ σ 2, when σ 2 ≥ (1+sinφ)σ 1/( sinφ-1), through analysis, we can obtain 2

tan 2 θ =

2m1m '1 − m1m '3 − m3 m'1 H db 1 + ν ( m3m '1 − m1m' 3 ) = , 2µ 4 RR ' ( m1 − m3 )( m '1 − m '3 ) 2m3m' 3 − m1m' 3 − m3m' 1

(11-72)

where, R = m12 + m32 , R ' = m '12 + m '32 , from Eq. (11-72), Hdb ≥ 0, the bifurcations occur at plastic hardening or ideal plastic state, and the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of the unified strength theory b can be shown by Fig. 11.9.

Fig. 11.9 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

When σ 2 ≤ (1+sinφ)σ 1/( sinφ−1), 2

tan 2 θ =

2l1l '1 − l1l '3 − l3l '1 H db 1 + ν ( l3l '1 − l1l '3 ) = , 2l3l '3 − l1l '3 − l3l '1 2µ 4 SS ' ( l1 − l3 )( l '1 − l '3 )

(11-73)

11.6 Discontinuous Bifurcations of Non-associated Flow Elasto-plastic

315

where, S = l12 + l32 , S ' = l '12 + l '32 , from Eq. (11-73), Hdb ≥ 0, the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of the unified strength theory b can be shown by Fig. 11.10.

Fig. 11.10 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

3. case of 0 ≥ σ 1 ≥ σ 2, when σ 2 ≥ (1 + sinφ)σ 1/2, by calculation, when 0 ≤ b ≤ 1, D

θ =0

where, R = m22 + m32 ,

,

H db m m' = − (1 + ν ) 2 2 2µ RR '

(11-74)

R ' = m '22 + m '32 , from Eq. (11-74), Hdb ≤ 0, the

bifurcations occur at plastic softening or ideal plastic state, and the bifurcation mode is split mode (also shear band mode, as b = 0). When b = 1, an arbitrary direction can be the initial direction of the bifurcation, belonging to split mode, and the corresponding hardening modulus is

H db m m' m m' = − (1 + ν ) 2 2 = − (1 + ν ) 3 3 2µ RR ' RR '

(11-75)

316

11 Unified Characteristics Field Theory for Plane Stress Problem

When σ 2 ≥ (1+sinφ)σ 1 / 2, by calculation, 2l2l '2 − l2l '3 − l3l '2 2l3l '3 − l2l '3 − l3l '2

½ ° ° 2 ¾ H db 1 + ν ( l3l '2 − l2l '3 ) ° = 2µ 4 SS ' ( l2 − l3 )( l '2 − l '3 ) °¿

tan 2θ =

(11-76)

where, S = l22 + l32 , S ' = l '22 + l '32 , from Eq. (11-76), Hdb ≥ 0, the bifurcations occur at plastic hardening or ideal plastic state, and the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of strength theory b can be shown by Fig. 11.11.

Fig. 11.11 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

The results produced by the Yu unified strength theory above show that the initial angle of bifurcation obtained as b = 0 is just the solution of Mohr-Coulomb strength theory (1900); the angle obtained as b = 0, φ = 0 is just the solution of Tresca (1991) yield criterion and the angle obtained as b = 1/2, φ = 0 is the linear approach of the solution of Huber-von Mises yield criterion.

11.7 Discussion and Experimental Verification

317

11.7 Discussion and Experimental Verification 11.7.1 Discussion

Assume the material satisfy the associate flow law. A special case is discussed in this part and compared with the existing unified plane stress characteristics field theory (Yu et al. 1998, 1999). Define A = (σ1+σ2) / 2, B = (σ 1−σ2) / 2. For plane stress problem, materials are assumed satisfy the associate flow law, following conclusions are drawn: For σ1 ≥ σ2 ≥ 0 (viz. A ≥ B), when σ2 ≤ (1+sin φ)σ1/2, it is equal to A ≤ (2+α)B / α (α is the tension-compression ratio), discontinuous bifurcations are shear band mode. From Eq. (11-67) tan 2θ = −

m1 m2

(11-77)

then cos2θ = −

m1 + m2 1+ b −α b =− m1 − m2 1+ b +α b

(11-78)

Here, sinφ = (1−α)/(1+α) is used. In such a stress state, the angle of characteristics is given by unified characteristics theory as follows cos 2θ = −

m n

(11-79)

where, m = (1+b−αb) / (1+b), n = (1+b+αb) / (1+b). It is obviously that Eq. (11-78) and Eq. (11-79) have given the same result. When σ 2 ≥ (1+sinφ)σ 1/2 (viz. A ≥ (2+α)B / α), if 0 < b ≤ 1, discontinuous bifurcations are of split mode. In such a stress state, when 0 < b ≤ 1, from the unified plane stress characteristics field theory, we know that there is no characteristics, because there is no root for the characteristics angle cos2θ = −(1+b) / (1−b). When b = 0, these two will give the same results. The same conclusion will be drawn for the two cases of σ 1 ≥ 0 ≥ σ 2 (A ≤ B), and 0 ≥ σ1 ≥ σ2 (A ≤ − B). From the above analysis, following conclusions can be obtained: In the plane stress state, shear band mode bifurcations is the same with the characteristics in essence. Angle of the unified characteristics given by Yu et al. (1999) can be obtained by the degeneration of the angle of shear band. So, the bifurcation theory can be used to analyze the characteristics.

318

11 Unified Characteristics Field Theory for Plane Stress Problem

11.7.2 Experimental Verification

A rectangular thin plate, made of PVC hard plastic, is subjected to uniform tension on two short sides as shown in Fig. 11.12. Unixial tensile strength of the PVC material: σ t = 5.886kN/cm² ; unixial compressive strength: σ c = 7.575kN/cm² ; tension-compression ratio: α = σ t /σ c =0.777. When subjected to tension, local slip band, which has the angle θ =61° with the tensional direction, appeared in the specimen. Based on the present unified characteristic field theory, with different b, the result of the characteristics will be different and a series of solutions can be obtained. On the other words that different strength theory will lead to different azimuth angle of shear band. Localized shear band on the plate is observed after the stretching. The angle θ of the shear band from the force direction is 60° . From a back analysis, the angle θ is determined as 60.97° when b = 0.675. It implies that the commonly used Mohr-Coulomb criterion may give very different prediction (48.60° for this example) of the shear band direction. It can not coincide with the experimental result. So, b = 0.675 is used to simulate the PVC-like material, viz. the strength theory of b = 0.675 can be used for shear band analysis of this kind of material.

x1 σ

B

θ

x2

A

σ Fig. 11.12 Rectangular thin plate subjected to tension

Summary

319

In this section, unification of the maximum critical hardening modulus has been done for the discontinuous bifurcations of elastic-plastic materials. Based on this unification, the phenomenon of discontinuous bifurcations has been investigated and obtained the initial azimuth angle and unified analytical model of the corresponding hardening modulus of discontinuous bifurcations under the non-associated plastic flow condition. This solution can be adapted for many kinds of materials and make the former simplex strength theories to be its special samples or its linear approach. Through the analysis of the results we can know that the isomerism of compression and tension and the intermediate principal stress have so great influence on the discontinuous bifurcations that govern the stress state. Therefore, these two factors above can’t be ignored during the analysis of the bifurcation, or else the results obtained can’t accord with the results of actual practice. On the other hand, the influence of different strength criterion to the discontinuous bifurcations of elastic-plastic materials can be established by giving different value of parameter b. A conclusion can be drawn that the influence of strength criterion is relative to the stress state of material. Actually, the value of parameter b can be calculated from Eq. (11-57). Substituting it in the unified solution, the properties of bifurcation fit for the material can be obtained. Comparing with the theory of characteristics field of plane stress, we can know that the discontinuous bifurcations of shear band mode of plane stress coincide with the characteristics. Thus, the theory of bifurcation can be adopted to analyze the characteristics. Similar discontinuous bifurcations for plane strain problems can be seen in Chapter 9.

Summary Based on the unified strength theory the unified characteristics field theory for plastic plane stress problem is described in this chapter. It is the unification of the plastic characteristics methods based on the Tresca criterion, the Huber-von Mises criterion and the twin-shear yield criterion. A series of new results can be also obtained by using the unified characteristics field theory. The strength-differential effect (SD effect and the effect of intermediate principal stress are taken into account in the unified characteristics field theory. The unified solutions of two examples, i.e. an infinite thin plate with a hole and a trapezoidal plate under compression, are given. It concludes a series of new results. The discontinuous bifurcations problems under plane stress are also studied by using the unified strength theory in this chapter.

320

11 Unified Characteristics Field Theory for Plane Stress Problem

Problems Problem 11.1 Derive the characteristics field for plane stress problem by using the Mohr-Coulomb strength criterion or the Yu unified strength theory with b = 0. Problem 11.2 Derive the characteristics field for plane stress problem by using the twin-shear strength or the Yu unified strength theory with b=1. Problem 11.3 Derive the characteristics field for plane stress problem by using the Yu unified strength theory with b = 0.5. Problem 11.4 Discuss the discontinuous bifurcation based on the Mohr-Coulomb strength criterion or the Yu unified strength theory with b = 0. Problem 11.5 Discuss the discontinuous bifurcation based on the twin-shear strength or the Yu unified strength theory with b = 1. Problem 11.6 Discuss the discontinuous bifurcation based on the Yu unified strength theory with b = 0.5. Problem 11.7 Discuss the discontinuous bifurcation for plane strain problems (see chapters 8 and 9) based on the Yu unified strength theory with b = 0.5.

References and Bibliography Bruhns OT (1984) Bifurcation problems in plasticity. In: The Constitutive Law in Thermoplasticity, Lehmann Thed. Springer-Verlag, Wien, New York. Hill RA (1958) General theory of uniqueness and stability in elastic-plastic solids. J. Mech. and Phys. of Solids, 6: 236–249. Hill JM and Wu YH (1993) Plastic flows of granular materials of shear index n−1, (1) yield functions; (2) Plane and axially symmetric problems for n = 2, J. Mech. and Phys. of Solids, 40(1): 77–93; 95–115. Hutchinson JW and Tvergaard V (1980) Surface instabilities on statically strained plastic solids. Int. J. Mech. Sci., 22: 339−358. Hutchinson JW and Tvergaard V (1981) Shear band formation in plane strain. Int. J. Solids Struct., 17: 451−466. Li GC (1987) Shear band bifurcations of ductile materials. Acta Mechanics Sinica, 19, 61−68. Marciniak Z and Kuczynski K (1967) Limit strains in the process of stretch forming sheet metal. Int. J. Mech. Sci., 9: 609−619. Ranniecki B, Bruhns OT (1981) Bounds to bifurcation stresses in solids with non-associated flow law at finite strain. J. Mech. and Phys. of Solids. , 29: 153–172. Rudnicki JW and Rice JR (1975) Conditions for the localization of deformation in pressure-sensitive dilatant materials. J. Mech. Phys. Solids, 23: 231–241.

Summary

321

Runesson K, Mroz Z (1989) A note on non-associated plastic flow rules. International Journal of Plasticity, 5: 639–658. Runesson K, Ottosen N, Peric D (1991) Discontinuous bifurcations of elastic-plastic solutions at plane stress and plane strain. International Journal of Plasticity, 7: 99–121. Storen S and Rice JR (1975) Localized necking in thin sheets. J. Mech. and Phys. of Solids, 23: 421–433. Thomas TY (1961) Plastic Flow and Frature in Solids. , Academic Press, New York. Tvergaard V, Needleman A and Lo KK (1981) Flow localization in the plane strain tensile test. J. Mech. and Phys. of Solids. 29: 115–127. Yu MH (1961) General behaviour of isotropic yield function (in Chinese), Res. Report of Xi’an Jiaotong University. Xi’an. Yu MH (1983) Twin shear stress yield criterion. Int. J. Mech. Sci. 25: 71–74. Yu MH, He LN, S LY (1985) Twin shear stress theory and its generalization, Scientia Sinica (Science in China), Series A, 28(12): 1174–1183. Yu MH, He LN (1991) A New Model and Theory on Yiwld and Failure of Materials under Complex Stress State. Mechanical behaviour of materials-6, Pergamon Press, 3 : 841–846. Yu MH (1994) Unified Strength Theory for geomaterials and its applications. Chinese Journal of Geothechnical Engineering, 16(2): 1–10 (in Chinese). Yu MH (1998) Twin Shear Theory and Its Application. Berjing: Science Press (in Chinese). Yu MH, Zhang YQ, Yang SY (1998) Another important generalization of the unified strength theory. J. of Xi’an Jiaotong University. 32: 108–110 (in Chinese, English Abstract). Yu MH, Zhang YQ, Li JC (1999) The unified characteristics theory for plastic plane stress problems. J. of Xi’an Jiaotong University. 33(4) : 1–4 (in Chinese, English Abstract). Zhang YQ and Yu MH (1999) Solutions to plastic plane stress problems. J. of Xi’an Jiaotong University, 33(6): 60–63 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of metallic materials for plane stress. Chinese J. of Mechanical Engineering, 37(4): 62–85 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of elasto-plastic materials for plane stress. Acta Mechanica Sinica, 33(5): 706–713 (in Chinese, English Abstract). Zhang YQ, Hao H and Yu MH (2003) A unified characteristics theory for plastic plane stress and strain problems. J. of Applied Mechanics, 70: 649–654. Zyczkowski M (1999) Discontinuous bifurcations in the case of the Burzynski-Torere yield criterion. Acta Mechanica, 132: 19–35.

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

12.1 Introduction The twin-shear slipe-line field and the unified slipe-line field theory for plane strain problem and the twin-shear characteristics field and the unified characteristics field theory for plane stress problem have been described in Chapters 8, 9, 10 and 11. It can be applied to metal plastic forming, the limit analysis of structure in civil engineering and mechanical engineering. The partial differential equations of the axisymmetric problem are not exactly hyperbolic, they may be elliptical and parabolic. The two families of characteristics lines of the parabolic functions become one family, and there are no characteristics lines for the elliptical equations. The characteristics line field theories of the spatial axisymmetric problem is more complex. It is difficult to solve analytically, and still remains open. A lots of simplified methods were used to discuss the characteristics line theory of spatial axisymmetric problems. Levin (1953), Shield (1955) and Kachanov (1971) et al. used Haar von-Karman complete plasticity condition and the Tresca criterion. They studied the indentation problem of a punch, and assumed that circumferential stress σ θ is equal to one of the other two principal stresses, namely σ θ ≈ σ 1 or σθ ≈ σ 3 . The results of the characteristics line theory, however, did not agree well with the reality ( Hill 1950). Szczepinski (1979) used the hypotheses σθ ≈ σ r and the Tresca criterion to study the characteristics line theory of spatial axisymmetric problems. After that, the infinite differential method was also used for spatial axisymmetric problems (Shield 1955). Based on the same method, Cox analyzed the limit loading capability of cohesive circular smooth soil foundations ( c − ϕ soil and ρ = 0 ). Larkin analyzed circular shallow soil foundations ( ρ = 0 ) when c = 0 . The above analyzed results were summarized by Chen (1975). Shield and Cox used the single-sheer strength theory (Tresca-Mohr-Coulomb theory) and the hypotheses σθ = σ 2 < σ1 of Haar and von-Karnam. Some axisymmetric characteristics problems were solved by Ishlinsky (1944), and Sokolovsky (1942) using the Mohr-Coulomb theory. Figs. 12.1 and 12.2 show the two examples of axisymmetric characteristics field (from Ȼɟɪɟɡɚɧɥɟɜ 1960). Figure 12.3 is an example of the axisymmetric characteristics for a long-rod penetration in concrete target (Yu, Li, Wei and Chen, see Yu 2002a).

12.1 Introduction

323

Fig. 12.1. Characteristics field of an indentation of a circular head punch (non-SD material)

Fig. 12.2. Characteristics field of an indentation of a circular head punch (SD material)

-6

-4

-2

0

2

4

Fig. 12.3 Axisymmetric characteristics field of a long-rod in normal penetration

Most solutions can be adapted only for the Tresca material and the MohrCoulomb material A unified characteristics line field theory for axisymmetric problems which can be adapted for more materials was introduced by Yu et al. in 2001 (Yu, Li and Zhang 2001). It is based on the peculiarity of spatial axisymmetric plastic problems and the unified strength theory. The stress field and velocity field of the unified axisymmetric characteristics line field theory are described in this chapter, and two examples by using the new characteristics theory for axisymmetric plastic problem are given. The unified

324

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

axisymmetric characteristics line field theory is also used to solve the high velocity impact problem. The normal penetration of a long-rod under high velocity is described in this chapter.

12.2 The Unified Strength Theory The Yu unified strength theory has been described in Chapter 4. The mathematical expression of the unified strength theory is f = σ1 − f'=

α

1+ b

(bσ 2 + σ 3 ) = σ t

1 (σ 1 + bσ 2 ) − α σ 3 = σ t 1+ b

when σ 2 ≤

σ1 + α σ 3

1+ α σ1 + α σ 3 when σ 2 ≥ 1+ α

(12-1a) (12-1b)

The unified strength theory can be expressed in terms of internal cohesion c0 and the friction angle ϕ 0 as follows

f = [σ1− 1 (bσ 2+ σ 3)] + [σ1+ 1 (bσ 2 +σ 3) ]sin ϕ0 = 2c0cos ϕ 0, 1+b 1+b σ +σ 3 σ1 −σ 3 sin ϕ 0 + when σ 2 ≤ 1 2 2 or

when σ2 ≤ p + R sin ϕ 0 (12-2a) 1 1 f ' =[ ( σ 1 + bσ 2 ) − σ 3 ] + [ ( σ 1 + bσ 2 ) + σ 3 ]sin ϕ0 = 2c0 cos ϕ0 , 1+ b 1+ b σ + σ 3 σ1 − σ 3 when σ 2 ≥ 1 sin ϕ 0 + 2 2

or

when σ 2 ≤ p + R sin ϕ 0

(12-2b)

The relations among c0 , ϕ 0 and the other parameters of material are shown as α =

1 − sin ϕ 0 1 + sin ϕ0

σt =

2c0 cos ϕ 0 1 + sin ϕ 0

(12-3)

It is shown that the unified strength theory consists of a series of strength theories from the single shear strength theory (lower limit, Mohr-Coulomb 1900) to the twin shear strength theory (upper limit, Yu 1985). The variaties of yield loci of the unified strength theory on the deviatoric plane have been illustrated in Figure 2 in Preface and Fig. 4.7, 4.8 in Chapter 4.

12.3 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Stress Field) There are four non-zero stress components σ r , σθ , σ z and τ rz in the axisymmetric problem, the circumferential stress σθ must be one of principal stresses.

12.3 Unified Characteristics Line Field Theory

325

According to the stress state of a spatial axisymmetric problems, we introduce a parameter m for circumferential stress σθ ( 0 ≤ m ≤ 1 ) σ + σ3 σ −σ σθ = σ 3 + m( 1 − σ 3) = σ3 + m 1 3 2 2

(12-4)

For the axisymmetric problem, we define P=

σ 1 + σ3

2

,R=

σ1 − σ3

2

(12-5)

The following relations can be derived σ1 = P + R

σ 2 = σθ = P + ( m − 1) R

σ3 = P− R

(12-6)

The stresses of the problem can be expressed as σ r = P + R cos 2θ

½ ° ° ¾ (12-7) ° °¿

σ z = P − R cos 2θ τ rz = R sin 2θ σ θ = P + ( m − 1) R

where θ is the angle between the directions of the maximum principal stress and axis r. Using the first expression of the unified strength theory Eq.(12-2a) because the intermediate principal stress is σ 2 = σ θ = P + (m − 1) R ≤ P + R sin ϕ 0. Substituting Eq. (12-6) into Eq. (12-2), the unified strength theory for spatial axisymmetric problem is obtained as follows R=−

2(1 + b)sin ϕ 0 2(1 + b)c0 cos ϕ 0 P+ 2(1 + b) + mb(sin ϕ 0 − 1) 2(1 + b) + mb(sin ϕ 0 − 1)

(12-8)

The expression of the unified strength theory for spatial axisymmetric problem can be simplified to the simple expression as follows

R = −P sinϕ uni + cuni cos ϕ uni

(12-9)

where sinĳuni and Cuni are the unified material parameters introduced from the unified strength theory by Yu et al. (2001) for spatial axisymmetric problem. The parameter ĳuni and Cuni are referred to as the unified friction angle ĳuni and the unified internal cohesion Cuni, respectively.

sin ϕuni =

2(1+ b)sin ϕ 0 , 2(1+ b) + mb(sin ϕ0 −1)

(12-10)

326

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Cuni =

2(1+ b)c0 cos ϕ 0 1 ⋅ 2(1+ b) + mb(sinϕ 0 −1) cos ϕuni

(12-11)

When m = 0.5 , sinĳuni and Cuni can be expressed as

2(1+ b) sin ϕ 0 , 2(1+ b) + 0.5b(sin ϕ 0 −1)

(12-12)

2(1+ b) c0 cos ϕ 0 1 ⋅ 2(1+ b) + 0.5b(sinϕ 0 −1) cos ϕuni

(12-13)

sinϕuni =

Cuni =

The relations between the unified material parameters ĳ uni and C uni and the conventional material parameter ĳ0 and C0 are shown in Fig. 12.4 and Fig. 12.5.

1.14 1.12

0

ϕ0=5

Ct /C 0

1.10

C uni / C 0

0

ϕ0=10

1.08 1.06 1.04

0

ϕ0=15

1.02

0

ϕ0=20

1.00

0

ϕ0=25 0.0 0.0

0.2 0.2

0.4 0.4

0.6 0.6

0.8 0.8

1.0 1.0

b Fig. 12.4. Relation between unified cohesion Cuni and b

12.3 Unified Characteristics Line Field Theory

25

0

ϕ0=25

20

ϕt

327

0

ϕ0=20

15 0

ϕ0=15

ĳuni

10 0

ϕ0=10 5

0

0

ϕ0=5

0.0000000000.2000000030.4000000060.6000000090.8000000121.000000015 0.2 0.0 0.8 1.0

0.4

b

0.6

Fig. 12.5. Relation between unified internal friction angle ĳuni and b

When stress P presents compressive stress, the Eq.(12-9) changes to

R = P sin ϕ uni + cuni cos ϕ uni

(12-14)

The equilibrium differential equations of the axisymmetric problem are shown as ∂σ r ∂r ∂σz

∂z

+ +

∂τ rz ∂z ∂τ rz

∂r

+ +

σr −σ z =0

r

τ rz

r

=0

½ ¾ ¿

(12-15)

Substituting Eq. (12-7) and Eq. (12-14) into Eq.(12-15), the governing differential equations are expressed as ∂P (1+sin ϕ uni cos 2θ ) + ∂ P sin ϕ tuni sin 2θ + 2R ( ∂θ cos 2θ − ∂θ sin 2θ ) = R(m−1− cos 2θ ) r ∂r ∂z ∂z ∂r ∂P ∂P ∂θ ∂θ R sin ϕuni sin2θ + (1− sin ϕuni cos 2θ ) + 2R ( cos 2θ + sin 2θ ) =− sin 2θ ∂r ∂z ∂z ∂r r

(12-16)

Assuming that functions P and θ are given respectively along some curve z = z (r ) in the roz-plane, we get

328

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

dP =

∂P ∂r

∂P

dr +

∂z

dz , dθ =

∂θ ∂r

dr +

∂θ ∂z

dz

(12-17)

Eqs.(12-12) and (12-13) constitute a system of four linear inhomogeneous algebraic equations for the partial derivatives. The characteristics line equations of the solutions can be given, let the determinant of the algebraic and the relavant numerators are zero. Letting the determinant of the system equal to zero, we obtain the differential equations of the characteristics lines as follows

dz = tan(θ − µ) dr dz = tan(θ + µ ) β line group: dr

(12-18a)

α line group:

(12-18b)

There exist two families of characteristics lines, where the parameter 2µ is the angle between the characteristics lines Į and ȕ and the relation between parameters µ and ĳuni is µ=

π 4

ϕ − uni . 2

According to the direction derivation formulas ∂

= [sin(θ + µ )

∂r ∂ ∂z

∂ ∂ Sα

= − [cos(θ + µ )

− sin(θ − µ )

∂ ∂ Sα

∂ ∂ Sβ

− cos(θ − µ )

] sin 2µ ∂

∂ Sβ

] sin 2µ

(12-19a) (12-19b)

where Sα and Sβ are the convected coordinate system of the characteristics lines α and β , respectively. Therefore, the unified characteristics line equations are introduced as follows ∂z ∂r R R ∂z ( m − 1)(cos 2 µ + sin 2µ )+ r r ∂ Sα ∂ Sα ∂ Sα ∂ Sα ∂ Sα α line group (12-20a) ∂P ∂θ ∂z ∂r R R ∂z sin 2 µ − 2R = − (m − 1)(cos 2µ − sin 2 µ )− r r ∂ Sβ ∂ Sβ ∂ Sβ ∂ Sβ ∂ Sβ

sin 2µ

∂P

− 2R

∂θ

=

β line group

(12-20b)

It is the stress field of the unified characteristics line theory for axisymmetric problem.

12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems

329

12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Velocity field) The associated flow rule is d ε ijp = d λ

∂f

(12-21)

∂σ ij

The unified strength theory of the spatial axisymmetric problem can be derived from the Eq. (12-3) and Eq. (12-8) §σ r − σθ · 2 +τ 2 + C cosϕ = 0 (12-22) rz uni uni ¨ 2 ¸ © ¹ Under the small deformation condition, the strain rates can be expressed as 1 f = (σ r + σ θ )sinϕuni − 2

εr = εθ = εz =

γrz =

∂u ∂r

∂f

= −λ

∂σ r

∂f u = −λ ∂σ θ r ∂v ∂z

∂u ∂z

= −λ

+

∂f ∂σ z

∂v ∂r

= −λ

∂f

(12-23)

∂τ rz

From Eqs. (12-21), (12-22), (12-23) and Eq (12-10), we can get λ εr = − (sinϕuni − cos2θ ) 2 εz = −

λ (sinϕ + cos2θ ) uni

2 λ rz = λ sin 2θ

(12-24a) (12-24b) (12-24c)

where θ is the angle from the direction of principle stress σ r to the direction of axis r. When the angle between the characteristics line α and axis r is denoted by ψ , the relation between ϕ and θ is shown as π ϕ θ =ψ + µ =ψ + ( − uni )

4

2

(12-25)

Substituting the above relation into Eq. (12-20) derives λ εr =− [sin ϕuni + sin (2ψ −ϕuni )]

2

(12-26a)

330

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

λ εz =− [sin ϕ uni − sin(2ψ −ϕ uni)] 2

(12-26b)

λrz = λ cos(2ψ − ϕuni )

(12-26c)

When one of the characteristics lines α or β overlaps with axis r, namely ψ = 0 or ψ = −(

π − ϕ uni) , Eq. (12-21) can be simplified to 2

εr = (

∂ u ∂r

)ψ = 0 = 0 or εr = (

∂ u ∂r

)

ψ =− (

π

2

−ϕ uni )

=0

(12-27)

It shows that the strain rate is zero along the direction of the characteristics lines. If the velocities along the characteristics lines α and β are denoted by Vα and Vβ , the velocities along axes r and z are denoted by u and w , respectively, the

relations among them can be expressed as u = w=

Vα sin( ψ + 2 µ ) − Vβ sin ψ

(12-28a)

sin 2 µ Vα cos(ψ + 2µ ) − Vβ cos ψ

(12-28b)

− sin 2µ

It can derive the following equations by getting differential with respect to r and combining with Eq.(12-22)

§ ∂u · = ¨¨ ¸¸ © ∂ r ¹ψ = 0

§ ∂ Vα ¨¨ © ∂r

· + Vα cot 2 µ ¸¸ ¹ψ = 0

§ ∂ψ ¨¨ © ∂r

· − Vβ csc 2µ ¸¸ ¹ ψ =0

§ ∂ψ ¨¨ © ∂r

· =0 ¸¸ ¹ ψ =0 (12-29)

From the above equations, the velocity equation along the characteristics line α and line β are obtained as follows α line group: dV + ªV cot§π −ϕ · −V csc §π −ϕ ·º dψ = 0 uni¸ β uni¸» α «α ¨ ¨

©2 ¹ ©2 ¹¼ ¬ β line group: dV +ªV csc§π −ϕ · −V cot§π −ϕ ·º dψ =0 β « α ¨© 2 uni ¸¹ β ¨© 2 uni¸¹» ¬ ¼

(12-30a) (12-30b)

It is the velocity field of the unified characteristics line theory for axisymmetric problem.

12.5 Applications of the Unified Characteristics Field Theory

331

12.5 Applications of the Unified Characteristics Field Theory Example 1. Circular Cone under Compression A circular cone under compression is shown in Fig. 12.6. The top radius of the circular cone is 20mm and the side face at rest has the oblique angle 45 0 from axis r. The material parameters are: E = 210 GPa, C 0 = 120MPa, and ĳ 0 = 0. Assuming that the contact surface is smooth, determine the characteristics line field and the limit loading of an circular cone during compression based on the unified characteristics line field theory.

Fig. 12.6. Characteristics line field of circular cone under compression

Only the right part of the cone should be considered because of axisymmetry. π Due to ϕ 0 = 0 it can be obtained that ϕ t = 0 and µ = , which shows that the 4 characteristics lines are orthogonal with each other. According to this condition , the characteristics lines can be expressed as dz

π

= tan(θ − ) dr 4 dz π = tan(θ + ) β line group: dr 4 It can derive t he governing differential equations α line group:

α line group β line group:

∂P ∂ Sα ∂P ∂ Sβ

− 2R + 2R

∂θ ∂ Sα ∂θ

=

R ∂r ∂ z [(m − 1) + ] r ∂ Sα ∂ Sα

R ∂r ∂z = − [(1 − m) + ] r ∂ Sβ ∂ Sβ ∂ Sβ

(12-31a) (12-31b)

(12-32a) (12-32b)

If the parameter m is 0.5, the differential terms in Eq. (12-32) are substituted by differential coefficient terms and Eq. (12-32) can be solved by numerical integral. The stress field is divided into three regions I, II and III, which correspond to the sides AB and AC, AC and AD, AD and AO, resperctively.

332

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Firstly, we begin to construct the characteristics line field of the region I from no-stress side AB and get the values P and θ of the region. There are P = − R , 3π on the side AB. σ1 = σ 2 = 0 , σ 3 = 2R and θ = 4 Secondly, for the singularity of point A, the characteristics lines field of the region II is constructed with lines α and lines β which is orthogonal to lines α . The two families of lines form a center fan of characteristics line at point A. Finally, we can find that the characteristics line field of the region III is dependent on the sides AO and AD, and the value θ is zero along the side AO. Therefore, the values P and θ can be derived in the region II. If the total loading acted on the top surface is divided by the area of the surface, the ultimate pressure q can be obtained. The unified characteristics line field with b = 1 is shown in Fig. 12.6 for the circular cone of top angle 450 . In order to confirm the results of the theory, the elasto-plastic finite element program UEPP based on the unified strength theory (UST) is used to compute the limit loading q of the same cone. The relation between limit loading q and parameter b is shown in Fig. 12.7 with the two methods. Curve 1 is the solution of the characteristics line theory for spatial axisymmetric problem, curve 2 is the result from finite element method; curve 3 is the solution of the slip line theory for plane strain problem. From the Fig. 12.7, we can find that the result from the characteristics line theory are very chose to those from the two computer programs . When b = 0.8, the limit loading with the new method is close to the experiment data in Suh, Lee and Rogers (1968).

Fig. 12.7. Relation curves between limit loading

q and strength criterion parameter b

The relation between loading q A and displacement δ at the top point A is calculated with the finite element program UEPP. The two curves in Fig. 12.8 show that the limit loading of spatial axisymmetric problem (curve 1) is little bigger than that of plane strain problem (curve 2), which are close to the results in Fig. 12.7.

12.5 Applications of the Unified Characteristics Field Theory

Fig. 12.8. Relation curves between displacement δ and loading

333

qA

Example 12.2. Semi-Infinite Body under the Circular Punch Pressure q A semi-infinite body under the circular punch pressure q on the free surface is shown in Fig.12.9. The radium of the pressure region is 2m. The parameters are 0 c0 = 0.3MPa and ϕ 0 = 15 .

The right part of the characteristics line field is shown in Fig.12.9 when b = 1 (the twin-shear strength theory, Yu 1985). The relations between q / c0 and b is shown in Fig. 12.10. They are obtained by using the unified characteristics line field theory (curve 1) and the unified slip field theory (curve 2). The solution at b = 0 (q/c0 = 13.9) in Fig.12.10 is the complete solution of Cox (1961), which is based on the Haar von-Karman condition and the Mohr-Coulomb strength theory .

Fig. 12.9. Semi-infinite body under the compression and the characteristics line field

334

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Fig. 12.10. The relation between the limit loading

q

and the parameter

b

A series of results can be introduced for the SD materials with the different tensile-compression strength ( ϕ 0 ≠ 0 ) and the non-SD materials with same tensilecompression strength ( ϕ 0 = 0 ) by the unified characteristics line field theory. The solutions of the Mohr-Coulomb material and Tresca material are special cases of the solutions of the unified characteristics line theory.

12.6 Penetration of High Velocity Rod to Target 12.6.1 Penetration problems of long rod Much research has been reported on impact and penetration problems because of their importance in modern engineering applications and protective engineering. Due to the experimental, analytical and computational complexities involved in general cases, attention has been paid to the penetration of a long-rod, with different impact velocities, into a target. Studies on this subject are mainly based on tests and supplemented with analytical or numerical methods. The analytical models began with the work of Bishop et al. (1945), who developed equations for the quasi-static expansion of cylindrical and spherical cavities and used these equations to estimate forces on conical nose punches pushed slowly into metal targets. Later, Hill (1950) and Hopkins (1960) derived and discussed the dynamic, spherically symmetric, cavity-expansion equations for an incompressible target material. The cavity expansion theory was further developed by Luk and Forrestal (1987), Forrestal and Tzou (1997), Xu et al. (1997) and Mastilovic and Krajcinovic (1999) to model the penetration of projectiles through soil, porous rock, ceramic and concrete targets. Based on the characteristics line theory, Simmons et al. (1962) investigated the deformation of thin plates subjected to high-impact loads. Slip line field theory is used by Wijk (1999) to find the penetration resistance on the rod. An

12.6 Penetration of High Velocity Rod to Target

335

overview on projectiles penetrating into geological targets was given by Heuze (1990). The dynamic failure mechanism of concrete is intricate since discontinuities such as cleavage cracks and defects with different shapes and orientations are commonly encountered in concrete and they have significant influence on the deformation and failure characteristics of concrete. The initially existing cracks and defects will be nucleated, and will evolve until material loses strength, when subjected to dynamic loading. The damage theory has been considered to be more suitable for the cleavage analysis of the concrete material (Krajcinovic, 1996; Lorrain and Loland, 1983). In the previous studies of the impact and penetration to concrete target, the commonly used constitutive models are elastic-plastic and/or brittle damage models (Luk and Forrestal, 1987; Forrestal and Tzou, 1997; Xu et al., 1997; Mastilovic and Krajcinovic, 1999), where elastoplasticity and damage are treated separately. How to define the failure criterion of the targets is critical for better analyzing penetration problems (Zukas et al., 1978). The failure criteria such as the MohrCoulomb strength theory and the Tresca yield criterion were often applied to penetration problems, as can be seen from the above references. These criteria do not consider all of the stress components in stress space. The effect of intermediate principal stress is not taken into account in the Tresca criterion and the MohrCoulomb strength theory, which are not consistent with the test results of many materials. A unified strength theory, which was suggested by Yu (1991), considers all of the components in stress space. It covers a series of strength theories, such as the Mohr-Coulomb’s single-shear strength theory and the twin-shear strength theory when the tension and compression strengths of materials are different, as well as the Tresca criterion, the Huber-von Mises criterion and the twin-shear criterion when the tension and compression strengths of materials are the same. The unified strength theory was applied to model penetration problem by Yu, Li and Wei (see Yu 2002a), and a unified plasticity-damage penetration model related to the crack density is proposed. The relation between radial traction and velocity at cavity-surface can be obtained by analyzing the distributions of stress and velocity of the target material. Based on the cylindrical cavity expansion theory and spatial axisymmetrical unified characteristics line theory, the attacking capability of a long-rod can be assessed from the derived relation as the rod impacts and penetrates the target with initial velocities of 300 ~ 1100 m / s . The results are compared with those of the experiments available in the open literatures.

12.6.2 Damage modeling of target material For the present problems, the cracks of the target are mainly caused by tensile stress waves and developed along the radial orientation (Forrestal and Tzou, 1997; Xu et al., 1997; Mastilovic and Krajcinovic, 1999). Therefore, a damaged loading surface is defined based on an equivalent tensile strain. When concrete material is subjected to tension, it will not fail unless the value of the stress is larger than its tensile strength, assuming the damage is caused by the activation and growth of

336

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

initially existing micro cracks. Although the damage evolution is rate-dependent in general (Chen et al., 2001), it is assumed that the damage evolution in this paper is rate-independent and isotropic for the purpose of simplicity. The definition of effective stress σ ∗ by Kachanov (1986) is used and mode I cracking is considered. Since the penetration damage is accumulated as a function of time and applied stress, crack density is expressed as a function of the equivalent tensile strain and time which is similar to the model proposed by Liu and Katsabanis (1997)

c f = m1 < ε − εcr > m2 t

(12-33)

where the angular bracket < ⋅ > denotes the function is valid only when the value inside the bracket is larger than zero, cf is the total number of cracks per unit volume, m 1 and m 2 are material constants, ε cr is the static critical tensile strain which can be easily determined from uniaxial static tensile test results ( ε cr = σ st E ), and t represents the accumulated time in the evolution of damage. According to the definition suggested by Whittaker et al. (1992), the scalar damage ω is related to the crack density cf and expressed as ω = 1− e

− c f Vl

(12-34)

where Vl is the damaged volume. If the maximum principal strain is less than the critical value ε cr , there is no damage in the target and the probability of fracture is equal to zero. On the other hand, if the maximum principal strain exceeds ε cr , the material stiffness will degrade, based on the research by Huang et al. (1994).

12.6.3 Fundamental equations of the target A cylindrical symmetric cavity is expanded from an initial radius of zero at velocity v0r = v0r (t ) , as a rod penetrates a target. The expansion of cavity produces four regions of response as shown in Fig.12.11. The four regions are: (1) plastic region (the material reaches unified strength theory, v0rt ≤ r ≤ ct ); (2) damaged region (the material reaches its tensile strength, ct < r ≤ c1t ); (3) elastic region ( c1t < r ≤ cd t ) and (4) an undisturbed region ( r > cd t ). 0

vr is the cavity-expansion rate, which is rate-dependent and decreased with time t . c and c1 are interface velocities. c d is the elastic, dilatation velocity. r is radial Eulerian coordinate. There are three principal stresses, σ r , σ θ and σ z , which are radial, circumferential and axial stress components (positive in compression) and σ r ≥ σ z ≥ σθ for the problem.

12.6 Penetration of High Velocity Rod to Target

337

non-disturbed elastic damage plastic 0

vr t

ct

c1t

cdt

Fig. 12 .11. Cylindrical cavity-expansion

The target material is considered to be compressive and is assumed to satisfy linear pressure-volumetric strain relation σ m = K ε v = K (1 − ρ 0 ρ )

(12-35)

where ρ 0 and ρ are densities of the original and deformed material, respectively, ε v is the volumetric strain, K is the bulk modulus and σ m is given by σm =

σ r + σθ + σ z

3

(12-36)

According to the material characteristics of a cylindrical cavity-expansion, the strength theory can be deduced when the material comes into a plastic yielding state, namely σ r − σθ = At σ r + Bt

(12-37)

with

At =

2sin ϕ t , Bt = 2ct cos ϕt 1 + sin ϕ t 1 + sin ϕt

(12-38)

The equations of mass and momentum conservation in cylindrical coordinates take the forms of

1 dρ ∂v v , + =− ∂r r ρ dt

(12-39a)

∂σ r 1 dv + ( σ r − σθ ) = − ρ ∂r r dt

(12-39b)

338

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

At the two interfaces r = c1t and r = ct , the target material satisfies the Hugoniot jump condition that mass and momentum across the interface remain conservative,

[ ρ (v − vJ )] = 0 ,

(12-40a)

[σr + ρ v(v − vJ )] = 0

(12-40b)

where the brackets [...] stand for the magnitude of the discontinuity of the bracketed variable across the wave front (interface) that propagates with the velocity vJ .

12.7 Elastic-Damage-Plastic Analysis of the Target Define E0 , K 0 , ν 0 and E , K , ν to be the Young’s modulus, bulk modulus and Poission’s ratio of the original and damaged materials, respectively. Because an isotropic model is used, only two of three moduli are independent. σ r1 and σ r 2 , v1 and v2 , ρ1 and ρ 2 are the dimensionless radial stresses, velocities and densities of the damaged and plastic regions at r = ct , respectively. σ r 3 and σ r 4 , v3 and v4 are the dimensionless radial stresses and velocities of the elastic and damaged regions at r = c1t , respectively. σ ri = σ ri / K 0 , vi = vi / c and ρ j = ρ j / ρ 0 ( i = 1 ~ 4 , j = 1 ~ 2 ) are used for the dimensionless variables.

12.7.1 Elastic region ( c1t ≤ r ≤ cd t ) According to the linear elastic stress-strain relations, E0 ∂u uº ª °σ r = − (1 − 2ν ) (1 + ν ) «(1 − ν 0 ) ∂r + ν 0 r » ¼ 0 0 ¬ °° (12-41) ® ° ∂u º E0 u ª (1 − ν 0 ) + ν 0 » ° σθ = − (1 − 2ν 0 ) (1 + ν 0 ) ¬« ∂r ¼ r °¯ and Eq. (12-39), the differential equation of wave can be derived, with the dimensionless variables ξ = r ct and u = u ct , as follows: (1 − λ 2 ξ 2 )

d 2u dξ 2

+

1 du ξ dξ

−

1 ξ

2

u =0

(12-42)

12.7 Elastic-damage-plastic Analysis of the Target

339

where λ = c cd and u is radial particle displacement. The boundary conditions are u (r = cd t ) = 0 , σθ (r = c1t ) = − σ f

(12-43)

Solving Eqs. (12-42) and (12-43), the radial velocity and stress in the region can be found to be ª 1 − λ 2ξ 2 λξ 1 + 1 − λ 2ξ 2 º 1 du »G = −« + ln λξ c dt 2 « 2λξ » ¬ ¼

(12-44a)

1 − λ 2ξ 2 λ 1 + 1 − λ 2ξ 2 σ 3 [(1 − 2ν0 ) + ln σ r (ξ ) = r = − ]G λξ 1 +ν 0 2 K0 2λξ 2

(12-44b)

v(ξ ) =

where η = c c p , η1 = c1 cp , cp = K 0 ρ 0 , σ f is the static tensile strength of the material, and σ ª 3(1 − 2ν 0 ) η η 2 − λ 2η12 η + η 2 − λ 2η12 º 3λ » ln ⋅ − G=− f « 2(1 + ν 0 ) K0 « 1 + ν 0 λη1 » 2λη12 ¬ ¼

−1

(12-45)

12.7.2 Damaged region ( ct ≤ r ≤ c1t ) As the cracks appear and develop along the radial direction, the circumferential stress is zero, that is, σθ = 0 . The density ρ of the deformed material is a function of the scalar damage ω . At r = c1t , the material comes into plastic yielding, the radial stress can be expressed as σ r1 =

Bt 1 − At

(12-46)

where Bt = Bt K 0 . The distributions of the dimensionless stress and velocity, and the relationship between η1 and η can be derived from Eqs. (12-35) and (12-36) and Eq. (12-39), as ε v is very small and 1 − ε v ≈ 1 . σ r (ξ ) = − t1 ξ + t2 2

v(ξ ) = − t2 (η ξ ) + (1 + ν )t1 (3K )

(12-47) (12-48)

340

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

η12 (1+ν )σr4 + 3Kη1 ⋅ η v4

Bt = (1 − At )K0

2

η (1 +ν ) − 3K

η η ⋅η v4 + σr4 (12-49) − 3K ( 1 ) ⋅ 21 η η (1 +ν ) −3 K

where η

t1 = 3K ( 1 ) ⋅ η

t2 =

η1 ⋅ η v4 + σ r4

η 2 (1 +ν ) − 3K

η12 (1 + ν )σ r4 + 3Kη1 ⋅ η v4 η 2 (1 + ν ) − 3K

K = K K0

(12-50a) (12-50b) (12-50c)

12.7.3 Elastic-damaged and plastic-damaged interface ( r = c1t and r = ct )

The relations between radial stresses and velocities at r = c1t can be derived from Eq. (12-34) and Eq. (12-39), σ r 4= σ r3 +

3(η1 − η v3 )(η v4 − η v3) 3 − (1 + ν 0 )(σ r 3 − σ f )

η v4 = η v 3 +

1 +ν σ r4 ] K 3 − (1 +ν 0 )(σr3 − σ f )

(η1 −η v3)[(1 +ν 0 )(σr3 − σ f ) −

(12-51a)

(12-51b)

From Eqs. (12-35)~(12-37) and Eq. (12-40), the radial stress, velocity and density at r = ct can be obtained as below σ r2 =

2K [2K − ρ1(2K + Bt )]ρ1η 2 (1 − v1)2 σr 1+ 2K + 2 − At 2 K + 2 − At

2 2 2 2 ρ σ (2 − At) + ρ1 η (v1 −1) (2 − At) − ρ1(2K + Bt) +1 v2 = (v1 −1) ⋅ 1 r1 2 2 2 ρ1 η (v1 −1) (2 − At ) − 2K

ρ2 =

ρ1η 2 (1 − v1)2 (2 − At ) − 2K

σ r1(2 − At ) + ρ1η 2 (1 − v1 )2 (2 − At ) − (2K + Bt )

(12-52) (12-53) (12-54)

12.7.4 Plastic region ( v0rt İ r İ ct ) The boundary conditions are v(ξ = v0r c) = v0r c , v( r = ct ) = v2 , σ r (r = ct ) = σ r 2

(12-55)

12.7 Elastic-damage-plastic Analysis of the Target

341

The differential forms of radial stress and velocity can be derived, from Eqs. (1240), (12-35) and (12-37), to be dv 2 K (1 − ε v )2 v + (2 − At )( Atσ r + Bt )(ξ − v)(1 − ε v ) = 2 2 2 dξ ξ [(2 − At )η (ξ − v) − 2 K (1 − ε v ) ] dσ r 2 K (1 − ε v )[( Atσ r + Bt )(1 − ε v ) + η 2 (ξ − v)v] = 2 2 2 dξ ξ [(2 − At ) η (ξ − v) − 2 K (1 − ε v ) ]

(12-56) (12-57)

where ε v = [(2 − At )σ r − Bt ] (2K ) . The numerical solutions of Eqs. (12-55) and (12-56) for the plastic region can be got by using Runge-Kutta method. The radial stress and velocity of the cavity surface can be obtained when the condition v (ξ = v0r c) = v0r c is satisfied.

12.7.5 Solution procedure and the normal penetration dept For the purpose of simplicity, the solution is obtained with an inverse procedure from the elastic region to the plastic region, because the boundary condition of the cavity surface is unknown. The procedure is summarized as follows: (1). The mathematical expressions of v3 and σ r 3 in elastic region can be found from Eqs. (12-44a) and (12-44b). The mathematical expressions of v 4 and σ r 4 in damaged region can be found from Eqs. (12-50a) and (12-50b). The relationship between η 1 and η can be got when the above expressions v3 , σ r 3 , v 4 and σ r 4 are inserted into Eq. (12-48). (2). Choose a value for η and calculate η 1 from the relationship between η 1 and η. (3). The values of v3 , σ r 3 , v 4 and σ r 4 can be obtained by substituting η 1 and η into Eqs.(12-44a), (12-44b), (12-50a) and (12-50b). v 2 and σ r 2 can be derived by substituting v1 and σ r 1 into Eq.(12-51) to (12-53). (4). The calculations of Eqs. (12-55) and (12-56) are proceeded from the plasticitydamage interface ξ = 1 to the cavity surface ξ = v0r / c . The particle velocity and radial stress in the plastic region can then be obtained. When the boundary 0 condition v ξ = v0 c = v0r / c is satisfied, the value of v r corresponding to the chosen r value of η is determined. Since η vr0 = v0r / c p , v0r / c p can be obtained. An inverse procedure is used to calculate the interface velocity and the cavity-expansion velocity. The relation between the radial stress σ r0 and the cavity-expansion velocity v0r can then be obtained.

342

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

(5). After the numerical relationship between v0r and σ r0 are obtained, a mathematical penetration expression of σ r0 versus v0r can be deduced by curve fitting methods.

12.7.6 Final depth of normal penetration When a long-rod with an ogival nose penetrates vertically into a semi-infinite concrete target, f n and fτ are normal force and tangential force. Tangential force fτ = µ ⋅ f n , where µ is the friction parameter. The ogival nose is shown in Fig. 12.12, where s is the radius of the rod, and θ 0 and θ 1 are the center angles of the top and the side surface of the rod, respectively. Following Forrestal and Tzou (1997) it is assumed that the normal force f n on the ogive nose is actually equal to the force σ r0 (v0r ) needed to expand the cavity at 0 the rate vr . Letting Vz to be the penetration velocity of the rod, we have

vr0 = Vz ⋅ cosθ 1

(12-58)

If the rod is assumed to be rigid and the shank side resistance is neglected, the final normal depth after the rod completely penetrates into the target can be derived 0 0 from v r versus σ r and the Newton’s second law, namely zmax =

where m2 = 2 π s 2 A1K0

³

n2 = 2π s2 A3ρ 0

³

M n2 ln 1 + ⋅ V02 2n2 m2 − Mg 90 0 θ0

(12-59)

(sinθ 1 − sinθ 0 )(cos θ1 + µ sinθ 1)dθ 1 ,

900 ϑ0

(sinθ 1 − sinθ 0 )(cos θ 1+ µ sinθ 0 )cos2θ 1 dθ 1 , A1 and A3 are the

coefficients of curve-fit v0r versus σ r0 , M is the mass of the rod, and V0 is the impact velocity of the rod.

12.8 Comparison and Verification

343

Vz

r fn

s s

θ0 θ1

fτ

Fig. 12.12. Geometry of rod nose and traction components

12.8 Comparison and Verification A special concrete considered by Mastilovic and Krajcinovic (1999) is defined with the following parameters, ν 0 = 0.22 , E0 =11.3GPa , ρ 0 = 2260Kg / m3, σ f = 13MPa and µ = 0.1. The parameters of a long-rod with an ogival nose are M =1.6Kg , s = 0.0915m and the radius of the rod shank a = 0.0153 m. According to the test data (Forrestal and Tzou, 1997) and some of the numerical investigations of the damage evolution pattern (Mastilovic and Krajcinovic, 1999), the damage value is about 0.23 when the dynamic tensile stress reaches the dynamic failure stress, implying c f Vl can be derived. The degraded moduli due to damage can be obtained from the analysis of Huang et al. (1994). The relations of the plastic-damaged interface velocity c versus cavityexpansion velocity v0r and v0r versus σ r0 can be derived by using the methods from steps (1) to (5), which are described in 12.7.5. The relations are shown in Fig. 12.13 and Fig. 12.14. It is shown that the plastic-damaged interface velocity c is increased with the increase of expansion velocity v0r , as shown in Fig. 12.13. The radial stress σ r0 is also incresed with the expansion velocity v0r as shown in Fig. 12.14. For the same cavity-expansion velocity v 0r , the radial stress at cavity surface is changing for the different values of strength criterion parameter b . The radial stress σ r0 is increased with the increase of parameter b . The dimensionless radial stress σ r0 ( σ r0 = σ r0 / K 0 ) can be expressed as a second order polynomial of v0r K0 / ρ 0 , that is,

344

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

σ r 0 = A1 + A2 (v0r

K0 / ρ 0 ) + A3(v0r

K 0 / ρ 0 )2

(12-60)

0.8

c/c p

0.6 0.4

b=0.0 b=0.5 b=1.0

0.2 0.0 0.00

0.05

0.10

0.15

0.20

0.25

0.30

0.35

0.40

v r0 /c p Fig.12-13. Plastic-damage velocity vs cavity-expansion velocity 1.4 1.400000021 1.200000018 1.2

b=1.0 b=0.5 b=0.0

σr /K0

1.000000015 1.0

0

0.8 0.800000012 0.6 0.600000009 0.4 0.400000006 0.2 0.200000003 0.000000000 0.0

0.000000000 0.100000001 0.0 0.1 0.200000003 0.3 0.400000006 0.4 0.2 0.300000004

v r0 /c p Fig.12.14. Radial stress vs velocity of cavity-expansion

According to the conditions σ r0

v0r = 0

0 = σ r0st and dσ r

d v0r

=0,

(12-61)

v0r = 0

where σ 0rst is the dimensionless radial traction of quasi-static cavity-expansion. It 0 can be found that A1 = σ rst and A2 = 0. The value of σ 0rst can be derived from the spatial axisymmetric unified characteristics line theory (Yu et al., 2001). The spatial axisymmetric characteristics lines at the contact surface is shown as

12.8 Comparison and Verification

345

Fig. 12.3, in which the effect of surface friction is not taken into account. Based on the spatial axisymmetric characteristics line theory, we can get: (1) A1 = 0.03377 when b = 1; (2) A1 = 0.03203 when b = 0.5, which is close to the quasi-static cavity-expansion 0 radial limit stress σ rst = 0.0323 of Mastilovic and Krajcinovic (1999); (3) A1 = 0.03072 when b= 0. The value A3 can be obtained from the curve of Vr0 vs σ r0 , that is, A3 = 6.8~7.0 (when b = 1), A3 = 4.5~4.7 (when b = 0.5) and A3 = 2.2~2.5 (when b = 0). The final depths for the different values of strength criterion parameter b can be derived from Eqs. 12-58, 12-59 and 12-60. They are shown in Fig. 12.15. 3.0 2.5

z max (m)

2.0

b=0.0 b=0.15 b=0.5 b=1.0 test data

1.5 1.0 0.5 0.0 200

400

600

800

1000

1200

V0 (m/s) Fig. 12.15. Final depth vs initial impact velocity of long rod

When the impact velocity is V0 = 300m / s , the final depths Zmax = 0.236m for b = 1 are close to the test data Zmax = 0.23m (Forrestal and Tzou, 1997). When the impact velocity is V0 = 700m/s, Zmax = 0.915m for b = 0.5 are close to the test data Zmax = 0.9m. When the initial impact velocity is V0 = 1100m/s, Zmax = 2.02m for b = 0.15 are close to the test data Zmax = 2.06m. The penetration depths of the rod are situated within the area of 0 < b < 1. Fig. 12.16 shows the relationship between the rod mass and the final penetration depths when b = 1.0. The rod penetrates more deeply if its mass is heavier. The effect of the mass on the finial depth is more obvious when the initial impact velocity of the rod is higher. One reason why tungsten alloy rods (Rosenberg, 1997) are usually applied in modern arms is that their densities are higher.

346

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

2.5

V0=1100m/s V0=700m/s V0=300m/s

zmax (m )

2.0

1.5

1.0

0.5

0.0

1.5

1.8

2.1

2.4

2.7

M (Kg) Fig. 12.16. Final depth vs mass of the rod

Summary The characteristics line theory for spatial axisymmetric plastic problem is very important in the plasticity and engineering. The unified characteristics line field theory of spatial axisymmetric problem and its applications are described in this chapter. The effects of the intermediate principle stress σ2 and the SD effect of materials are taken into account in the unified characteristics field theory. A series of characteristics line field for spatial axisymmetric problem suitable for different kinds of materials can be derived from the new theory, the previous theories are special cases or linear approximation of the unified characteristics line theory. The new theory can be applied to the limit analysis of spatial axisymmetric plastic problems in plasticity and engineering. Based on the cylindrical cavity-expansion theory and the unified strength theory, a unified plastic-damage model is proposed for penetration problems. The proposed model is used to simulate penetration of a long-rod into a concrete target. The spatial axisymmetric characteristics line theory is used for the analysis of quasi-static normal penetration of a long-rod. The results show that: (1) The rod mass has obvious affect on the final penetration depth; (2) By comparison with the available test date, it appears that the proposed procedure is effective for penetration analysis. The test results are situated within the analysis results (0 < b < 1); (3) When the initial impact velocity of a rod is higher than 1500m/ s , the material behaviour and penetration process of rods and targets will change significantly.

Problems

347

Problems Problem 12.1 The characteristyics fields for indentation of a circular head punch are shown in Fig. P12.1. The limit pressures was obtained by using the Tresca yield criterion as follows. p b= σ s (1+ π ) 4 Find the limit pressure of indentation of a circular head punch by using the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1). .

Fig. P12.1. Circular head penestration into half space

Problem 12.2 Find the limit pressure of indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1).

Problem 12.3 The characteristyics fields for indentation of a circular head punch are shown in Fig. P12.2. This problem was studied by Hill (1950) Prager-Hodge (1951) and Levin (1953) by using the Tresca yield criterion. A is a initial situation; b is the indentation of the circular head; c is the deep indentation of the circular head and bar. The limit pressures are:

p b = σ s (1+ π ) and pc = σs (1 + 3π ) . 4 4 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1) .

348

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Fig. P12.2. Circular head penestration into infinit surface

Problem 12.4 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1) .

Problem 12.5 The characteristyics fields of indentation for non-SD materials under a circular head punch with a uniform pressure q shown in Fig. P12.3. The limit pressures was obtained by using the Tresca yield criterion. Find the limit pressure of indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1).

Fig. P12.3. Slip field under circular foundation for non-SD materials

Problem 12.6 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1).

References and Bibliography Bishop RF, Hill R and Mott NF (1945) The theory of indentation and hardness tests. The Proc. of the Phys. Soc. 57(3): 147–159. Chen WF (1975) Limit Analysis and Soil Plasticity. Elsevier, Amsterdam, New York.

References and Bibliography

349

Chen Z, Deng M and Chen EP (2001) Rate-dependent transition from the tensile damage to discrete fracture in dynamic brittle failure. Theoretical and Applied Fracture Mechanics. 35(3): 229–235. Collins IF, Dewhurst P (1975) A slip line field analysis of asymmetrical hot rolling. International Journal of Mechanical Science, (17): 643 . Forrestal, M. J., Tzou, D. Y., 1997. A spherical cavity-expansion penetration model for concrete targets. Int. J. Solids Structures 34, 4127-4146. Heuze FE (1990). An overview of projectile penetration into geological materials, with emphasis on rock. Int. J. Rock Mech. Min. Sci. and Geomech. Abstr. 27 (1), 1–14. Hill R (1950). The mathematical theory of plasticity. Clarendon Press, London. Hopkins HG (1960). Dynamic expansion of spherical cavities in metal. In: Progress in Solid Mechanics, Vol. 1, Chapter III, ed. I. N. Sneddon and R. Hill. North-Holland Publishing Company, Amsterdam, New York. Ishlinsky AYu (1944) Axisymmetrical plasticity problem and Brinell test. Appl. Math. Mech. 8 (in Russian). Johnson W, Sowerby R, Venter RD (1982) Plane strain slip line fields for metal deformation Processes-A source book and Bibliography. Oxford: Pergamon Press,. Kachanov LM (1975) Foundations of the Theory of Plasticity. North-Holland, London,. Kachanov LM (1986) Introduction to continuum damage mechanics. Martinus Nijhoff Publishers, Dordrecht, The Netherlands. Krajcinovic D (1996). Damage Mechanics. Elsevier, Amsterdam. Liu L, Katsabanis PD (1997). Development of a continuum damage model for blasting analysis. Int. Journal of Rock Mech. Min. Sci. 34, 217–231. Lorrain M and Loland KE (1983) Damage theory applied to concrete. Fracture Mechanics of Concrete, Edited by Writtmann. Luk VK and Forrestal MJ (1987) Penetration into semi-infinite reinforced-concrete targets with spherical and ogival nose projectiles. Int. J. Impact Eng. 6 (4): 291–301. Levin E (1953) Indentation pressure of a smooth circular punch. Quarterly. Appl. Math., (13), 133. Mastilovic S and Krajcinovic D (1999). High-velocity expansion of a cavity within a brittle material. Journal of the Mechanics and Physics of Solids 47, 577-610. Rosenberg Z, Dekal E, Hohler V, et al. (1997). Hypervelocity penetration of tungsten alloy rods into ceramic tiles: experiments and 2-D simulations. Int. J. of Impact Engineering 20, 675-683. Shield RT (1955) The Plastic Indentation of a Layer by a Flat Punch. Quarterly. Appl. Math., (13), 27. Simmons JˈHauser F, Dorn JE (1962) Mathematical Theories of Plastic Deformations under Impulsive Loading. Cambridge University Press, London, England. Sokolovsky VV (1960) Statics of Cohesionless Medium. Publ. Books on Phys. Math. Moscow (in Russian). Suh, NP., Lee RS., Rogers CR (1968).. The Yielding of Truncated Solid Cones under Quasi-Static and Dynamic Loading, J. Mech. Phys. Solids 16, 357. Szczepinski W (1979).. Introduction to the Mechanics of Plastic Forming of Metals. Sijthoff and Noordhoff, Netherlands,. Whittaker KT, Singh RH and Sun D (1992). Rock fracture mechanics principles, design and applications. Elsevier, Amsterdam. Wijk AG (1999). High-velocity projectile penetration into thick armor targets. Int. J. Impact Eng. 22, 45-54. Xu Y, Keer LM, Luk VK (1997) Elastic-cracked model for penetration into unreinforced concrete targets with ogival nose projectiles. Int. J. Solids Structures 34(12), 1479–1491. Yu MH, He LN, Song LY (1985) Twin shear stress theory and its generalization, Scientia Sinica (Science in China), English Edition, Series A, 28(11): 1113–1120. Yu MH, He LN (1991) A new Model and Theory on Yield and Failure of Materials Under Complex Stress State, Mechanical Behaviors of Materials̚6, Pergamon Press, Vol. 3: 841–846. Yu MH (1992) New System of Strength Theory. Xi’an Jiaotong Universitry Press, Xi’an (in Chinese). Yu MH (1994) Unified strength theory for geomaterials and its applications. Chinese J. Geot. Eng. 16(2): 1–10, (in Chinese, English Abstract).

350

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Yu MH, Yang SY, et al (1997). Unified Plane-strain slip Line field theory system. Chinese J. Civil Engineering, 30(2): 14̚26 (in Chinese, English Abstract) . Yu MH (1998) Twin Shear Theory and its Application. Science Press, Beijing 892 pp. (in Chinese). Yu MH, Li JC and Zhang YQ (2001) Unified characteristics line theory of spatial axisymmetric plastic problem. Science in China (Series E), English edn. 44(2), 207–215; Chinese edn. 44(4), 323–331. Yu MH (2002a) Concrete Strength Theory and Its Applications. Higher Education Press, Beijing (in Chinese). Yu MH (2002b) Advances of strength theories of materials under complex stress state in the 20th Century. Applied Mechanics Reviews, 55(3): 169-258. Zhao DW, Xu JZ, Yang H., et al (1998) Application of Twin Shear Stress Yield criterion in axisymmetric Indentation of a Semi-Infinite Medium. In : Strength Theory Science Press, New York, Beijing, 1079-1084. Zukas JA, Nicholas T, Swift HF, et al. (1982). Impact Dynamics. Wiley, New York. Ȼɟɪɟɡɚɧɥɟɜ ȼȽ (1952) Ɉɫɟɫɢɦɦɟɬɪɢɱɧɚɹ Ɂɚɞɚɱɚ Ɍɟɨɪɢɢ ɉɪɟɞɟɥɶɧɨɝɨ Ɋɚɜɧɨɜɟɫɢɹ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. Ɇɨɫɤɜɚ: Ƚɨɫ. ɂɡɞ. Ɍɟɯ. Ɍɟɨ. Ʌɢɬɟɪɚɬɭɪɵ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1942) ɋɬɚɬɢɤɚ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. ɂɡɞ. Ⱥɇ ɋɋɋɊ, Ɇɨɫɤɜɚ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) ɋɬɚɬɢɤɚ ɋɵɩɭɟɣ ɋɪɟɞɵ (Third ed.).Ƚɨɫ. ɂɡɞ. Ɏɢɡ-Ɇɚɬ. Ʌɢɬɟɪɚɬɭɪɵ. Ɇɨɫɤɜɚ (in Russia)

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

13.1 Introduction Estimation of the crack-tip plastic zone under small-scale yielding ( SSY ) is one of the important topics in elastic-plastic fracture mechanics. Literatures show that researchers have endeavored in finding the shape and size of mode-I, -II and -III crack-tip plastic zone under SSY. Dugdale (1960) and Barenblatt (1962) independently introduced their model representing a yield-strip or cohesive-strip zone around a crack-tip. It is called Dugdale yield-strip model or cohesive model. On the other hand, Irwin (1960) suggested an approximation method by increasing the effective length of a crack based on the anti-plane elastic-perfectly-plastic solution as well as Hult and McClintock (1957). It is known as the Irwin’s plastic-zone correction model. The shape and size of yielding zone were derived from the Huber-von Mises criterion. Irwin (1968) further extended his model for plane-strain condition by enhancing the yield stress by a factor of 3 . Broek (1982) presented his estimation using the Tresca criterion. The above-mentioned models are all based on the SSY condition and are constructed with the assumptions in the linear elastic fracture mechanics (LEFM). They yield reasonably good estimations for certain materials such as metals having equal tensile and compressive strength. Recent investigations revealed that the Tresca criterion do not take into account the effect of the intermediate principal stress properly, while the Huber-von Mises criterion only puts in place the average effect of the three principal stresses. In other words, Tresca criterion is only applicable for those materials governed by a shear-stress limit ( Ĳ s = 0.5ı s ), so is the Huber-von Mises criterion for materials governed by another shear-stress limit ( Ĳ s = 0.58ı s ). The twin-shear yield criterion, which is equivalent to a different shear-stress limit ( Ĳ s = 0.67ıs ). It agrees well with the results ( Ĳ s = 0.7ı s ) reported by the British Royal Air Force who conducted multi-axial tests for four groups of nickel alloy at 750° Celsius (Winston, 1984). Later, a unified strength theory (UST) was proposed (Yu et al. 1991, 1992). An influence parameter ‘b’ for the effect of intermediate principal stress and the effect of intermediate principal shear-stress was put in place. The parameter ‘b’ normally varies between 0 and 1. The earlier twin-shear yield criterion is embraced as a special case (b=1). The UST unifies prevailing strength criteria through the variable parameter ‘b’, which actually bears a physical meaning as a material parameter. Adopting specific values of ‘b’ can lead to results equivalent to those

352

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

through Tresca criterion, Huber-von Mises criterion or its varieties. In addition, stretching beyond the normally admissible range (b1) can generate a new series of strength criteria for unconventional materials, which strength envelope may not necessarily be convex. Against this background, estimations of crack-tip plastic zone under SSY are re-investigated using the UST by Qiang in 1998. It provides unified solutions for shapes and sizes of mode-I, mode-II and mode-III crack-tip plastic zone in the K-dominant region. The minimum and maximum crack-tip plastic zones can be deduced through the normally admissible lower-bound (b = 0) and upper-bound (b=1) respectively. Adopting a proper value of the material parameter ‘b’ can lead to accurate solutions. Estimations of the crack-tip plastic zones using different values of ‘b’ are illustrated and compared, including those deductions equivalent to the Tresca and the Huber-von Mises criteria. The influences on the resulting plastic zone due to strength-differential (SD) effect and Poisson’s ratio are also studied. The investigation of the SD effect has practical significance because most materials have unequal tensile and compressive strength. The present approach is also extended to include some non-conventional materials under unsteady state. The definition of ‘conventional material under steady state’ refers to Drucker’s postulate that its failure/yield strength envelope is of convex shape in the stress space (i.e. the ʌ-space). The convexity condition is satisfied when 0 b 1. Beyond this conventionally admissible range (i.e. b < 0 or b > 1), the UST is ready to be applied to a whole spectrum of non-conventional materials, which strength envelope is not necessarily of convex shape. The shape and size of crack-tip plastic zone of those unconventional materials are also presented.

13.2 Unified Strength Theory The UST has been described in detail in Chapter 4. The mathematical modeling and the mathematical formulation are expressed as follows. F = τ 13 + bτ 12 + β ( σ13 + bσ 12 ) = C

when Ĳ 12 + ȕı 12

F ' = τ 13 + bτ 23 + β (σ 13 + bσ 23 ) = C when Ĳ 12 + ȕı 12

≥ Ĳ 23 + ȕı 23

≤ Ĳ 23 + ȕı 23

(13-1)

principal shear stresses and τ ij = (σi − σ j ) / 2 are the σ ij = ( σ i + σ j ) / 2 are the associated normal stresses. σ i (i =1,2,3) are the

where

principal stresses. ȕ is a coefficient which accounts for the effect of the corresponding normal stresses. Both ȕ and C are strength characteristics of a material, which values can be determined from standard experimental procedures for uniaxial tensile and uniaxial compressive tests. The relations are as follows:

13.2 Unified Strength Theory

353

where ıt and ıc are the uniaxial tensile and compressive strength respectively, Į = ı t /ı c is the strength ratio. This ratio is a measure of the strength

differential (SD) effect. Substituting Eq. (13-2) into Eq. (13-1) leads to the alternative expressions in terms of the principal stresses ıi, the tensile strength ıt and the strength ratio Į as follows. σ1 −

1 1+ b

α

1+ b

( b σ2 + σ 3 ) = σ t when

(σ1 + b σ 2 ) − ασ 3 = σ t when

σ2

σ2

≥

≤

σ 1+ασ 3

1+α σ 1 +ασ 3

(13-3)

1+α

Equation (13-3) shows that the UST not only takes into account the effect of the intermediate principal shear stress but also the SD effect. It is a function of the strength ratio Į. It can be seen from the envelope plotted in the diviatoric plane (see Fig. 13.1). It should be noted that the envelopes have symmetrical characteristics at 60°-intervals. For the sake of clarity, envelopes corresponding to different values of ‘b’ are plotted only in the diagonally opposite sector bounded by ș = 0° and ș = 60°. Along the radiation line rt (at ș = 0°), the limiting value is the tensile strength. Along the radiation line rc (at ș = 60°), the limiting value is the compressive strength. The UST criterion is a bi-linear surface approximation for the envelope between the radiation lines rt and rc. For values of ‘b’ ranging between 0 and 1, the shape of the whole envelope (0°ș < 360°) is convex. Outside this range (i.e. b < 0 or b > 1), the shape of the whole envelope become corrugated, and hence it represents those material not obeying the Drucker’s convexity postulate. In this sense, the UST unified the prevailing strength criteria. Its main features are further elaborated below.

354

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

Twin Shear Unified Strength Theory (Yu,1985) σ

1

'

θ θb

rc

rt

rc

0

60

rt

o

rt

rc

Single Shear Strength Theory (Mohr-Coulomb,1900)

b=0

σ

2

b1

Fig. 13.1 Loci of the UST in π -plane having different values of ‘b’

a)

b)

c)

UST consists of two material parameters - b and ȕ (or its equivalent form Į), which enables it to represent the strength envelope in the deviatoric plane for all conventional materials. In other words, it embraces all traditional strength criteria. For example, setting b = 0 and Į = 1 leads to the well-known Tresca criterion, which neglects totally the effect of intermediate principal shear stress and is only meant for materials having equal tensile and compressive strength. Again, setting Į = 1 and b = 1/2 yields segmental linear envelope very close to the smooth envelope by Mises criterion. It is worth noting that setting b = 1 leads to Yu’s twin-shear criterion – an earlier version of the UST. The UST provides admissible lower and upper bounds of the strength envelope for materials obeying the Drucker’s convexity postulate. When b = 0, it sets the lower bounds. Amongst them, Tresca envelope (Į = 1) is the one for materials having equal tensile and compressive strength; Mohr-Coulomb envelope is another one but it is for materials having different tensile and compressive strengths (Į 1). On the other hand when b = 1, it sets the upper bounds. Yu’s twin-shear criterion is one of it. Hence, the UST can be used to find the minimum and maximum yield/failure zone. When the value of ‘b’ is chosen outside the conventionally admissible range (i.e. b < 0 or b > 1), the corresponding strength envelope becomes non-convex shape. It violates the Drucker’s convexity postulate. In this

13.3 Stress fields around crack-tip

355

range, the UST yields strength envelopes for a whole spectrum of non-conventional materials, which do not obey the Drucker’s postulate.

13.3 Stress Fields Around Crack-Tip By virtue of linear elastic fracture mechanics, the 2D stress field in the vicinity of a mode-I crack-tip can be described as follows (Kanninen, 1985). σ x ½ 1 − sin( θ / 2 ) sin( 3θ / 2 ) ½ KI ° ° ° ° σ θ = cos ( / 2 ) ® y¾ ®1 + sin( θ / 2 ) sin( 3θ / 2 ) ¾ 12 r π ( 2 ) ° sin( θ / 2 ) cos( 3θ / 2 ) ° °τ ° ¯ ¿ ¯ xy ¿

(13-4)

For mode-II crack-tip, σ x ½ − sin(θ / 2)[ 2 + cos(θ /2 ) cos( 3θ / 2)]½ K II ° ° ° (13-5) ° cos(θ / 2) ® sin(θ / 2) cos(θ /2 ) sin( 3θ / 2) ¾ ®σ y ¾ = 1 2 °τ ° ( 2π r ) ° cos(θ / 2)[1 − sin(θ /2 ) sin( 3θ / 2)] ° xy ¿ ¯ ¯ ¿

For mode-III crack-tip, τ zx ½ K III − sin( θ / 2 ) ½ ® ¾= ® ¾ τ ¯ zy ¿ ( 2π r )1 2 ¯ cos( θ / 2 ) ¿

(13-6)

in which K I , K II and K III are the stress-intensity factors for mode-I, mode-II and mode-III respectively. ıx, ıy are the normal stresses in x- and y-direction respectively, and Ĳxy, Ĳzx, Ĳzy are the shear stresses in the xy-, zx- and zy-plane respectively. Position vector is expressed in polar coordinates (r,ș) measured from the crack-tip. The stress components in Eqs. (13-4)-(13-6) can be expressed in terms of the corresponding principal stresses ıi. For 2-dimenional plane problems, the principal stresses are: σ1½

¾= σ 2¿

σ3

σ x +σ y

2

2

§ σ x −σ y · 2 ¸ + τ xy ± ¨¨ 2 ¸¹ ©

0 =® ¯ ν ( σ 1+ σ 2 )

for plane stress for plane strain

(13-7a) (13-7b)

in which ν is Poisson’s ratio. Due to symmetry, the following derivations are presented only for the half-plane ( θ ∈ [0,π ] ). By substituting Eqs. (13-4)-(13-6)

356

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

into Eqs (13-7a)-(13-7b) and arranging the resulting stresses in the order such that σ 1 ≥ σ 2 ≥ σ 3 , we have For mode-I (plane-stress case) σ1

½ θ θ KI cos (1 ± sin ) ¾= σ2 ¿ 2 2 2π r σ3 = 0

(13-8)

For mode-I (plane-strain case) σ1

½ ¾= σ2 ¿

2π r

2ν K I

=

σ3

KI

cos

cos

2π r

θ

θ

(1 ± sin

2

2

)

for 0 ≤ ș < 2 sin

−1

(1 − 2 Ȟ )

(13-9)

θ

2

and σ1

=

σ2

=

σ3

=

KI 2π r 2ν K I 2π r KI 2π r

θ

cos

2

θ

2

)

θ

cos cos

(1 + sin

for 2 sin

−1

(1 − 2 Ȟ ) ≤ ș < ʌ (13-10)

2 θ

2

(1 − sin

θ

2

)

For mode-II (plane-stress case)

K II

σ1

=

σ2

=0

σ3

=

2π r

K II 2π r

1 4 − 3 sin 2 θ ) (− sin θ + 2

2

for 0 ≤ ș < 2 sin

(− sin

θ

2

−

1 2

−1

1

(13-11)

3

4 − 3 sin 2 θ )

and σ1 = 0

1

for 2 sin −1 ≤ș 1. The non-convex material may be called the non-conventional materials. The

366

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

shape and size of plastic zone for non-conventional materials (b=−0.1, −0,25, −0.5) are also plotted. Figures 13.12 and 13.13 are for mode-I plane-stress and plane-strain case respectively, while Figs. 13.14 and 13.15 for mode-II plane-stress and plane-strain case respectively. 13.7.1 Mode-I crack-tip plastic zone for non-conventional materials (plane stress)

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY 3

Dimensionless 2πy(σt/KII)

2

2 1

Crack 0

OX

O

-1 -2 -3 -1

0

1

2

3 2

Dimensionless 2πx(σt/KI)

Fig. 13.12 Mode-I crack-tip plastic zone for unconventional materials in plane-stress state ( Į = 1, Ȟ = 1/3 )

13.7 Shape and size of plastic zone for non-conventional materials

2

Dime nsionless 2πy(σt/KI)

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY

2

1

Crack 0

OX

O

-1

-2 -0.8

-0.6

-0.4

-0.2

0.0

0.2

2

0.4

0.6

Dimensionless 2πx(σt/KI)

Fig. 13.13 Mode-I crack-tip plastic zone for unconventional materials in plane-strain state ( Į = 1, Ȟ = 1/3 )

13.7.2 Mode-I crack-tip plastic zone for non-conventional materials (plane stress) UTSS (b= -0.1)

OY

4

UTSS (b= -0.25) UTSS (b= -0.5)

Dimensionless 2πy(σt/KII)

2

3 2 1

Crack

0

OX

O

-1 -2 -3 -4

-6

-4

-2

0

2

4

Dimensionless 2πx(σt/KII)

6

8

10

2

Fig. 13.14 Mode-II crack-tip plastic zone for unconventional materials in plane-stress states ( Į = 1, Ȟ = 1/3 )

367

368

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY

5 4

Dimension less 2πy(σt/KII)

2

3 2

Crack

1 0

OX

O

-1 -2 -3 -4 -5

-8

-6

-4

-2

0

2

4

6

8

10

2

Dimensionless 2πx(σt/KII)

Fig. 13.15 Mode-II crack-tip plastic zone for unconventional materials in plane-strain state

( Į = 1 . 0 , Ȟ = 1/3 )

13.8 Effect of ‘b’ Value Parameter ‘ b’ represents the influence of the intermediate principal shear stress. For the same material, the extents of the influence are not the same under different crack-tip modes. It reflects in the resulting shape and size of the crack-tip plastic zone. On the other hand, various values of ‘b’ also correspond to a spectrum of strength criteria, including the well-known Tresca and Huber-von Mises. In other words, each ‘b’ value represents a strength criterion, which is only valid for a group of materials. What follows are observations of results obtained from different criteria through its equivalent value of ‘b’. • For mode-I: In both plane-stress and plane-strain cases, a general trend is observed that the larger the value of ‘b’, the smaller is the size of the plastic zone. In other words, the greater the influence of the intermediate shears, the smaller the size of the plastic zone. It can be seen from Figs. 13.2 and 13.3 that the Tresca criterion (equivalent to b = 0) leads to the largest zone, while Yu’s earlier full-twin-shear criterion (equivalent to b = 1) yields the smallest zone. The size of plastic zone by the Huber-von

13.7 Shape and size of plastic zone for non-conventional materials

369

Mises criterion is somewhere in-between the Tresca and the Yu’s twin-shear criterion, and is almost the same as that by UST with b = 0.5 . • For mode-II: Similar trend as in mode-I is observed. The larger the value of ‘b’, the smaller is the size of the plastic zone. Figure 13.4 shows the plane-stress case, while Fig. 13.5 shows the plane-strain case. In both cases, Tresca criterion (equivalent to b = 0 ) leads to the largest zone, while Yu’s full-twin-shear criterion (equivalent to b=1 ) yields the smallest zone. The Huber-von Mises criterion yields zone of intermediate sizes. Their shapes look similar. • For mode-III: Similar trend as in mode-I and mode-II is observed, except that the plastic zones are all of circular shape. • For unconventional materials (b < 0 ): Since the same mathematical expressions are used, the same trends are observed. The smaller the value of ‘b’ (more negative), the larger is the size of the plastic zone. Figures. 13.12 and 13.13 show the results for mode-I plane-stress and plane-strain respectively, while Figs 13.14 and 13.15 show the results for mode-II plane-stress and plane-strain respectively.

13.9 Influence of SD Effect Parameter ‘α ’ is the ratio of the uniaxial tensile strength to the uniaxial compressive strength. The ratio is a measure of the effect of strength differentials (SD). Definitely, it influences the sizes of the crack-tip plastic zone. Trends are observed in different crack modes but no common trend is noted. • In mode-I: The weaker-in-tension materials (Į = 0.5) always result in larger plastic zone (if not less) than the equal-strength materials (Į = 1), in both plane-stress and plane-strain cases. The sizes in plane-stress cases are usually bigger than those in plane-strain cases. It can be seen in Figs. 13.4 13.5 and 13.6 for b = 0, 0.5 and 1.0 respectively. • In mode-II: Contrary to the trend in Mode-I, the weaker-in-tension materials ( α = 0.5) always result in smaller plastic zone than the equal-strength materials (Į = 1), in both plane-stress and plane-strain cases. However, the sizes in plane-stress cases maintain the trend being bigger than those in plane-strain cases. It can be seen in Figs. 13.9, 13.10 and 13.11 for b = 0, 0.5 and 1.0 respectively.

370

•

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

In mode-III: The plastic zones are all of circular shape. The weaker-in-tension materials (α = 0.5) always result in smaller plastic zone than the equal-strength materials (α = 1), in both plane-stress and plane-strain cases. Again, the sizes in plane-stress cases are usually bigger than those in plane-strain cases.

13.10 Influence of Poisson’s Ratio Results for plane-stress cases are independent of the Poisson’s ratio. For Mode-I and -II plane-strain cases, the influence of Poisson’s ratio is similar to the trend observed in the variations of ‘b’ values. The larger the Poisson’s ratio, the smaller is the size of the plastic zone. Figure 13.16 shows the effect of Poisson’s ratio on mode-I crack-tip plastic zone, while Fig. 13.17 shows the Mode-II.

ν =1/3 ν =1/4 ν =1/5

OY

1.0 0.8

Dimensionless 2πy(σt/KI)

2

0.6 0.4

Crack

0.2 0.0 0

OX

O

-0.2 -0.4 -0.6 -0.8 -1.0 -0.5

-0.4

-0.3

-0.2

-0.1

0.0

0.1

0.2

0.3

0.4

0.5

2

Dimensionless 2π x(σt/KI)

Fig. 13.16 Effect of Poisson’s ratio on mode-I crack-tip plastic zone in plane-strain state ( Į = 1 .0 , b = 1 .0 )

Summary

2

Dimensionless 2πy(σt/KII)

ν=1/3 ν=1/4 ν=1/5

OY

2

371

1

Crack 0

O

OX

-1

-2

-4

-3

-2

-1

0

1

2

3

2

Dimensionless 2πx(σt/KII)

Fig. 13.17 Effect of Poisson’s ratio on mode-II crack-tip plastic zone in plane-strain state (Į = 1 .0 , b = 1 .0 )

Summary This chapter presents the estimations of crack-tip plastic zone under small-scale yielding (SSY) using the unified strength theory (UST). The UST unifies all prevailing strength criteria through a variable parameter ‘b’. It provides unified solutions for shapes and sizes of mode-I, -II, -III crack-tip plastic zone in the K-dominant region. The minimum and maximum crack-tip plastic zones can be deduced through the conventionally admissible lowerand upper-bound values of ‘b’ in the UST. Adopting a proper value of the material parameter ‘b’ can lead to accurate solutions. Other specific values of ‘b’ can yield solutions equivalent to those through the Tresca criterion, Huber-von Mises criterion or its varieties. In addition, stretching beyond the normally admissible range for the material parameter ‘b’ (1) can generate a new series of strength criteria for unconventional materials, which strength envelope may not necessarily be convex. Estimations of the crack-tip plastic zones using different values of ‘b’ are illustrated and compared. The influences on the resulting plastic zone due to strength-differential (SD) effect and Poisson’s ratio are also investigated. Embracing the SD effect broadens the applicability to most materials, which have unequal tensile and

372

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

compressive strength. It demonstrates the robustness of present method in the estimation of shape and size of the crack-tip plastic zone under SSY. It is seen that: (1) The Yu's unified strength theory is applied to the study of the shape and size of plastic zones of mode I, II, III cracks, and a complete solution of unified closed forms is obtained. The Tresca criterion and the Huber-von Mises criterion are special case and linear approximation of the Yu’s theory. (2) Except for mode III cracks, the boundary curves of mode I, II crack tip plastic zones are composed of two parts, which is resulted from the piece-wise linearity of the Yu's criterion. (3) Generally speaking, the plastic zone obtained by the Yu's theory is smaller than that by the Huber-von Mises and much smaller than that by the Tresca criterion, showing that a bigger τ s /σ s will lead to a smaller plastic zone and weaker ability to resist fracture. (4) Different values of b in Yu's theory will produce a family of different yield criterion which will help obtain a group of crack tip plastic zones applicable to various materials. The value of σ t also exerts certain influence on the tip plastic zone, but only affects the plane strain condition (except for mode III cracks). The results were obtained by analytical solution. The unified strength theory and unified elasto-plastic constitutive model can be also implemented into commercial finite element codes and other FEM codes. The effect of failure criterion on numerical calculations of finite element method (FEM) can be also observed. These problems will be summarized at another book entailed “Computational Plasticity based on the Unified Strength theory”

Problems Problem 13.1. The solution of crack tip problem can be also studied by using the slip field theory. Figure P16.1 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode I under plane strain. Can you given a new solution by using the twin-shear slip field method described in Chapter 8. Problem 13.2. The solution of crack tip problem can be also studied by using the slip field theory. Figure P16.1 shows a slip field with the Tresca yield criterion for Mode I under plane strain condition. Can you given a new solution by using

Problems

373

the unified slip field theory described in Chapter 9.

Fig. P16.1

Mode I

Fig. P16.2

Mode II

Fig. P16.3 Mixed Mode III

Problem 13.3. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.2 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode II under plane strain condition. Can you given a new solution by using the twin-shear slip field method described in Chapter 8. Problem 13.4. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.2 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode II under plane strain condition. Can you given a new solution by using the unified slip field theory described in Chapter 9. Problem 13.5. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.3 shows a kind of slip field with the Tresca yield criterion (single-shear theory) for Mixed Mode I and II under plane strain. Can you given a new solution by using the unified slip field method described in Chapter 9. Problem 13.6. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.3 shows a kind of slip field with the Tresca yield criterion (single-shear theory) for Mixed Mode I and II under plane strain. Can you given a new solution by using the unified slip field method described in Chapter 9.

374

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

References and Bibliography Barenblatt GI (1962) The mathematical theory of equilibrium cracks in brittle fracture. Advances in Applied Mechanics; 7: 55–129. Broek D (1982) Elementary Engineering Fracture Mechanics (3rd ed.) Martinus Nijihoff Publishers, The Hague. Dugdale DS (1960) Yielding of steel sheets containing slits. Journal of the Mechanics and Physics of Solids; 8: 100–108. Fan SC, Yu MH, Yang SY (2001) On the unification of yield criteria. Journal of Appllied Mechanics, 68: 341–343. Flugge S (1958). Encyclopedia of Physics. New York: Springer-Verlag. Hult JAH, McClintock FA (1957) Elastic-plastic stress and strain distributions around sharp notches under repeated shear, In: Proceedings of the Ninth International Congress for Applied Mechanics, University of Brussels, 51–58. Irwin GR (1960) Plastic zone near a crack and fracture toughness. In: Proceedings of the 7th Sagamore Ordnance Materials Conference, New York: Syracuse University Press, 1960: IV-63-78 Irwin GR (1968) Linear fracture mechanics, fracture transition and fracture control. Engineering Fracture Mechanics; 1: 241-257. Kanninen MF, Popelar CH (1985) Advanced Fracture Mechanics. Oxford University Press, New York, 563 pages. Qiang HF, Xu YH, Zhu JH (1998) Unified solutions of mixture type crack tip plastic zone under small scale yielding. In: Strength Theory: Applications, Developments and prospects for the 21st Century, MH Yu and SC Fan (eds), Science Press, Beijing, New York, 823–829. Qiang HF and Lu N (1999) Unified solutions of crack tip plastic zone under small scale yielding, Chin. J. Mech. Engrg., 35(1), 34–38. (in Chinese) Winstone MR (1984) Influence of prestress on the yield surface of the cast nickel super alloy Mar-Mooz at elevated temperature. Mechanical Behavior of Materials, Pergamon Press, Oxford 1984, Vol. 1, 199–205 Yang Wei. Macro-Micro Scope Fracture Mechanics. Beijing: National Defence Industry Press, 1995.(In Chinese) Yu MH (1983) Twin-shear stress yield criterion. Int. Journal of Mechanical Science, 25(1): 71–74. Yu MH (2002) Advances in strength theories for materials under complex stress state in the 20th century. Applied Mechanics Reviews, 55(3): 169–218. Yu MH (1983) Twin-shear stress strength criterion. International Journal of Mechanical Science, 25(1): 71–74. Yu MH, He LN, Song LY (985) Twin-shear stress theory and its generalization. Scientia Sinica (Science in China) Series A, 28: 1174–1183. Yu MH, He LN (1991) A new model and theory on yield and failure of materials under complex stress state. In: Jono M, Inoue T. Mechanical Behavior of Materials-VI. Pergamon Press. Oxford, 841–846. Yu Mao-hong, New System of Strength Theory. Xian: Xian Jiaotong University Press, 1992. (In Chinese) Yu MH (1998) Twin-shear Theory and Its Applications. Science Press, Beijing (in Chinese) Yu Mao-Hong, Advances in strength theories for materials under complex stress state in the 20th Century. Applied Mechanics Reviews, 55 (2002) 169-218. Yu Mao-hong. (2004) Unified Strength Theory and Its Applications. Springer, Berlin.

14 Unified Fracture Criterion for Mixed Mode Crack Initiation and Fatigue Crack Growth

14.1 Introduction Mixed-mode fracture and fatigue crack growth are one of the most commonly used failure forms of material in analyzing practical engineering problems. The research on the mixed fracture criterion and fatigue crack growth is significant in fracture mechanics and engineering. Many research works in this area have been conducted and some criteria for predicating the direction of the crack initiation angle and the critical fracture load of materials have been proposed by energy principles and the stress approach (Khan et al. 2000). Among the criteria of energy principle type, G-criterion (Hussian et al. 1974), S-criterion (Sih 1974) and T-criterion (Theocaris and Andrianopoulos 1982a, 1982b) are original and more important ones. Other fracture criteria are the maximum tangential stress criterion (Erdogan and Sih 1963), maximum shear stress criterion, maximum stress triaxiality criterion (Kong, Schluter and Dahl 1995), maximum octahedral shear stress criterion etc. The plastic zone radius criterion for crack initiation angle was proposed recently by Golos and Wasiluk (2000), Wasiluk and Golos (2000), Kahn and Khraisheh (2004) and Bian and Kim (2004). S-criterion states that the crack initiation takes place along the direction with the minimum strain energy density around a constant radius around crack tip and a crack extension starts in the initiation direction when strain energy density reaches a critical value. The region within this constant radius is assumed and the linear elastic fracture mechanics does not hold in this circular region. In fact, there is not any evidence supporting the assumption that this area is circular region with constant radius, which is an intuitively fixed value only. This region is firstly called core region by Theocaris (Theocaris and Andrianopoulos 1982a, 1982b) using the caustic method, and the various fracture criteria maybe applied with high accuracy defined by the radius of the initial curve of the respective caustic created by the different loading modes. Then Theocaris et al. modified S-criterion in two aspects, firstly, total strain energy is separated into two components: a dilatational component that mainly causes cavity nucleation and development around a crack tip and distortional component that changes the shape of an element; secondly, the Huber-von Mises elastic-plastic boundary as the core region is assumed by using a variable radius for the core region, therefore T-criterion was defined that the crack

376

14 Unified Fracture Criterion for Mixed Mode Crack Initiation

initiation occurs at the direction with maximum dilatational strain energy density along the contour of constant distortional strain energy. Theocaris et al. also performed experiments on polycarbonate (PCBC) specimen to support their criterion (Theocaris et al. 1982c). The investigation mentioned above showed that the introduction (including both size and shape) of core region is very important for definition of various fracture criteria. However, the studies were performed only by using Huber-von Mises yield criterion, because it coincided with distortional energy part in form. Little attention has been paid to investigate the influence of yield criterion on the core region of crack tip. In fact, the Tresca criterion is the lower bound of yield criteria and the twinshear stress criterion (or the maximum principal deviatoric stress criterion) is the upper bound of yield criteria for stable and isotropic ductile material (Yu 1983). The Huber-von Mises yield criterion is a special case mediated between the lower bound and upper bound. A linear Unified strength theory (UST) was proposed by Yu in 1991 and 1992 (see: Yu 2002, 2004). It is obtained by introducing twin-shear element naturally. It has two simple mathematical formulae, piecewise linear yield surfaces and physical significance. Varying the parameter b in the UST derives a family of convex criteria. Based on the UST, a generalized T-criterion for Strength Difference (SD) or non-SD materials is obtained by Qiang, Yu et al. in 2003 and 2004. A new closed form of plastic core region model and its derivatives are obtained by Qiang in 2004. The Tresca-core region is lower bound, and the twin-shear-core region is upper bound, the Huber-von Mises-core region mediated between these two bounds. They are all the special case of the plastic core region responses of the generalized T-criterion. A unified fracture criterion based directly on the unified strength theory was obtained by Yu, Fan, Che et al. in 2003, 2004. In this chapter, a variable radius for the plastic core region based on the UST elastic-plastic boundary is introduced and incorporated in the formulation of the T-criterion, the lower bound and upper bound plastic core region responses of T-criterion is derived. Comparisons of the three particular solutions with respect to the Tresca-core region, the Huber-von Mises-core region and the TS-core region are made mutually. a generalized T-criterion is obtained, called the UT-criterion. At last, a unified fracture criterion for mixed mode crack is described in detail. It is introduced directly from the formulation of the unified strength theory (Fan 2003, Yu, Fan and Che 2003, 2004). The relations of crack initial angle © with DQG unified strength parameter b for mode Ċcrack (©~~b curves), cracked initial angle with various fracture criteria, unified fracture criterion of mixed I-II mode for various α , unified fracture criterion of mixed I-III mode for various α , and the unified fracture criterion of mixed II-III mode for various α are obtained by using the numerical calculation method. A series of relations are illustrated in Figs. 14.17 to 14.25. The unified fracture criterion may be also used for the study of fatigue crack growth.

14.2 Main Idea of T-Criterion

377

14.2 Main Idea of T-Criterion Consider an elastic-perfectly plastic plate under plane stress condition containing an internal crack inclined by an angle ȕ to the direction of the uniaxial loading, as show in Fig. 14.1. The stresses around the crack-tip are: Y

σ0

r β

θ

o X

2a

σ0

Fig. 14.1 Slant crack under remote uniaxial load σx =

σy =

τ xy =

KI ª KI 3θ · 3θ ·º θ§ θ§ θ θ f x (θ ) «cos 2 ¨1 − sin 2 sin 2 ¸ − µ sin 2 ¨ 2 + cos 2 cos 2 ¸» = 2π r ¬ 2π r ¹¼ ¹ © © ª θ§ θ 3θ · 3θ º KI θ θ f y (θ ) (14-1) «cos 2 ¨1 + sin 2 sin 2 ¸ + µ sin 2 cos 2 cos 2 » = 2π r ¬ 2π r ¹ © ¼

KI

KI ª KI 3θ 3θ · º θ θ θ § θ f xy (θ ) « cos 2 sin 2 cos 2 + µ cos 2 ¨ 1 − sin 2 sin 2 ¸ » = 2π r ¬ 2π r © ¹¼

where ıx, ıy. and Ĳxy are the normal stresses and shear stress in x-y plane respectively; K I = σ 0 π a sin2 β , K II = σ 0 π a sin β cos β and µ = K II / K I are stress-intensity factors for mode-I, -II and its notation respectively, σ 0 is uniaxial loading of remote field, 2a is the crack length; f x (θ ) , f y (θ ) and fxy (θ ) are defined as above. Based on T-criterion, the dilatational and distortional parts of the strain energy density are given respectively by:

TV = TD =

1 − 2ν (σ + σ y )2 6E x

1+ν 2 2 (σ x + σ y2 − σ xσ y + 3τ xy ) 3E

(14-2a)

(14-2b)

378

14 Unified Fracture Criterion for Mixed Mode Crack Initiation

where E and ν are the modulus of elasticity and Poisson’s ratio of the material. Using the notation of equation (1), we obtain from Eqs. (14-2a) and (14-2b) respectively

(1 − 2ν ) K I2 ( f x + f y )2 12π Er

(14-3a)

(1+ ν ) K I2 2 ( f x + f y2 − f x f y + 3 f xy2 ) 6π Er

(14-3b)

TV =

TD =

Since the distortional strain energy is constant along the Huber-von Mises elastic plastic boundary, TD,0 can be considered as a material constant, i.e., (1 + ν ) σ s2 . Combining Eqs. (14-3a) and (14-3b), we get boundary of the TD,0 = 3E core region and the dilatational strain energy 2

TV =

KI

( f x2 + f y2 − f x f y + 3 f xy2 )

(14-4)

( f x + f y )2 (1 − 2ν ) σ s2 6E f x2 + f y2 − f x f y + 3 f xy2

(14-5)

r=

2πσ s2

So the T-criterion is defined as TV

θ =θ 0

≥ T V, cr TD = T D , 0

∂ TV ∂θ

θ =θ 0

=0

∂ 2TV ∂θ 2

Mao-Hong Yu Guo-Wei Ma Hong-Fu Qiang Yong-Qiang Zhang

Generalized Plasticity

With 315 Figures

Professor Mao-Hong Yu Xian Jiaotong University School of Civil Engineering and Mechanics 710049 Xian, People’s Republic of China E-mail: [email protected]

Co-Authors Guo-Wei Ma Nanyang Technological University, Singapore

Hong-Fu Qiang Yi’an Hi-Tech Research Institute, China

Yong-Qiang Zhang National University of Singapore, Singapore

Library of Congress Control Number: 2005932191

ISBN-10 3-540-25127-8 Springer Berlin Heidelberg New York ISBN-13 978-3-540-25127-0 Springer Berlin Heidelberg New York This work is subject to copyright. All rights are reserved, whether the whole or part of the material is concerned, specif ically the rights of translation, reprinting, reuse of illustrations, recitation, broadcasting, reproduction on microf ilm or in any other way, and storage in data banks. Duplication of this publication or parts thereof is permitted only under the provisions of the German Copyright Law of September 9, 1965, in its current version, and permission for use must always be obtained from Springer. Violations are liable to to prosecution under the German Copyright Law. Springer is a part of Springer Science+Business Media. springeronline.com © Springer-Verlag Berlin Heidelberg 2006 Printed in Germany The use of general descriptive names, registered names, trademarks, etc. in this publication does not imply, even in the absence of a specif ic statement, that such names are exempt from the relevant protective laws and regulations and therefore free for general use. Camera-ready by the Author and SPI, India Cover design: design & production GmbH, Heidelberg Printed on acid-free paper

SPIN 11009092

62/3141/SPI 5 4 3 2 1 0

Appreciate the beauty of the discover the truth of the universe.

universe;

Zhuang Zi (369 –286 B.C. China)

I have loved the principle of beauty in all things, and if I had had time I would have made myself remembered. Keats, John (1795 – 1821, UK)

A thing of beauty is a joy for ever. Keats, John (1795 – 1821, UK)

“Beauty is truth, truth is beauty,” — that is all ye know on earth, and all ye need to know. Keats, John (1795 – 1821, UK)

Preface

Generalized plasticity is a generalization of the unified strength theory to the theory of plasticity. It is the unification of metal plasticity for Tresca materials, Huber-von Mises materials, and twin-shear materials. It is also the unification of geomaterial plasticity for Mohr-Coulomb materials and generalized twin-shear materials. Moreover, it leads to unification of metal plasticity and plasticity of geomaterials, in general. It is a companion volume to Unified Strength Theory and Its Applications published by Springer in 2004. Generalized Plasticity is based on the lectures on the unified theory of materials and structures given by the author at the School of Civil Engineering and Mechanics, Xi’an Jiaotong University in Xi’an, China and at the Nanyang Technological University of Singapore in 1996. It is a course entitled “Generalized Plasticity” for Ph.D. students at Xi’an Jiaotong University since 1993. The main contents are the unified yield function (unified strength theory) of material, the unified slip line field theory for plane strain problem, unified characteristics field theory for plane stress problem, unified characteristics field theory for spatial axisymmetric problem, limit pressure and shakedown pressure of a pressure vessel, the plastic zone analysis at a crack tip under small-scale yielding and the unified fracture criterion. Several chapters in this book have been presented in conferences and published in various journals. They are: Unified Strength Theory (Yu, 1991, 1992, 1994, 2002, 2004); Unified Slip Line Field Theory for Plane Strain Problem (Yu, Yang, et al., 1997, 1999); Unified Characteristics Field Theory for Plane Stress Problem (Yu and Zhang, 1998, 1999; Zhang, Hao and Yu, et al., 2003); Unified Characteristics Field Theory for Spatial Axisymmetric Problem (Yu and Li, 2001); Unified Solution for Limit Pressure of a Pressure Vessel (Wang and Fan, 1998; Zhao et al., 1999); Unified Solution for Shakedown Pressure of a Pressure Vessel (Xu and Yu, 2004, 2005); Analysis of Plastic Zone at Crack Tip (Qiang et al., 1998, 2004); Unified Fracture Criterion (Yu, Fan, Che, Yoshimine, et al., 2003, 2004; Qiang and Yu, 2004). The beauty of the unified strength theory discussed in Chap. 5 is a part of a closing lecture delivered at the International Symposium on Developments in Plasticity and Fracture: Centenary of M.T. Huber Criterion, held at Cracow, Poland in 2004. The garden of the flowers of strength theory, the beauty of the Huber-von Mises criterion, and the beauty of the unified strength theory were discussed at the lecture. The analytical results of the generalized plasticity are a series of results. It is different from the conventional plasticity. As an example, a unified solution of bearing capacity of a plane strain structure by using the unified slip line field theory is shown in Fig. 1. The conventional solution of bearing capacity of a

VIII

Preface

structure is adapted only for one kind of material. It is shown in Fig. 1 at b = 0. This result is obtained by using the Mohr-Coulomb strength theory (inner bound or lower bound as shown in Fig. 2a), Fig. 2b is a special case for Į = 1 materials. It can also be obtained by using the unified strength theory with b = 0. The unified solution includes a series of solutions and encompasses the solution of the Mohr-Coulomb strength theory as a special case. It is also possible to obtain a series of new solutions for different values of parameter b and different ratios of tension and compression strength of material, i.e., Į = ıt/ıc 1.

Fig. 1 Limit loads of a plane strain structure.

(a) Į = ıt/ıc 1 materials

(b) Į = ıt/ıc = 1 materials

Fig. 2 Yield loci of the unified strength theory on the deviatoric plane.

Preface

IX

The unified strength theory and the unified slip line field theory for plane strain problem can be expressed in terms of another material parameter, such as friction angle ĳ, it is widely used in geomechanics and geotechnical engineering. The unified solutions for a plane strain problem in terms of the friction ĳ are shown in Fig. 3. The description of the unified solutions of plane strain problems can be seen in Chap. 9.

Fig. 3 Unified solutions of a plane strain problem in terms of the friction ĳ.

For the plane stress problems, the yield loci of the unified strength theory in plane stress state is shown in Fig. 4, and the unified solution of bearing capacity of a plane stress structure by using the unified characteristics line field theory is shown in Fig. 5. It can be seen that a series of new results are given whereas the Mohr-Coulomb theory and the Tresca criterion can give only one result. It is a special case of the unified solution by using the unified strength theory and the unified characteristics line theory with b = 0 and b = 0, Į = 1.

(a) Į = ıt/ıc 1 materials

(b) Į = ıt/ıc =1 materials

Fig. 4 Yield loci of the unified strength theory in plane stress state.

X

Preface

1.35

α = 0.2 α = 0.5 α = 0.8 α = 1.0

1.30 1.25 1.20

q

1.15 1.10 1.05 1.00 0.95

0.0

0.2

0.4

0.6

0.8

1.0

b

Fig. 5 Limit loads of a plane stress structure. The analytical results are clearly illustrated to show the effects of yield criterion on plastic limit behaviors for plane strain problems, plane stress problems, axisymmetric problems, other engineering structures, the shape and size of plastic zone at crack tip, discontinuous bifurcation, and angle of shear band. Generalized plasticity gives us a series of results, which can be adapted for different materials and structures. The contents of the book can be divided into five parts as follows: Part One. The unified strength theory, material parameters in the unified strength theory, yield surfaces, yield loci, reasonable choice of the yield criterion, and the beauty of the unified strength theory are described in Chaps. 4 and 5. Part Two. Plastic stress–strain relation and concrete plasticity, discussed in Chaps. 6 and 7. Part Three. Twin-shear slip field and the unified slip-line field theory for plane strain problems, twin-shear characteristics field and the unified characteristics line theory for plane stress problems, and unified characteristics line field theory for axisymmetric problems and high velocity penetration problem are explained in Chaps. 8–12. Part Four. The unified solution of plastic zone at crack tip under small-scale yielding is given. Based on the unified strength theory, a unified fracture criterion, a new closed form of plastic core region model, and variation for the angle of initial crack growth versus crack inclination under different loading conditions are obtained. They are described in Chaps. 13 and 14. Part Five. Chapter 15 is devoted to the unified solutions of limit loads and shakedown loads for pressure vessels. Stress state analysis and basic behaviors of materials under complex stress are discussed in Chaps. 2 and 3. The description of the stress state may be found in a number of books covering mechanics of materials, solid mechanics, and elasticity and plasticity. Only some basic formulae and figures as well as some new ideas are

Preface

XI

given here. Brief summaries, problems, and references and bibliography are given at the end of the chapters. I would like to express my gratitude for the support of the National Natural Science Foundation of China (Grants nos. 59779028, 59924033, and 50078046), the Ministry of Education of China, the China Academy of Launch Vehicle Technology, the Aircraft Strength Research Institute of China, the Department of Science and Technology of Xi’an Jiaotong University, as well as the School of Civil and Environmental Engineering, Nanyang Technological University, Singapore. I am indebted to many authors and colleagues, especially Dr Ma at Nangyang Technological University, Singapore, Prof. Qiang at Xi’an Hi-Tech Research Institute, and Dr Zhang at National University of Singapore for going through the manuscript of this book. I am also indebted to Dr Li YM, Dr Yang SY, Dr Zhao JH, Dr Wang F, Dr Li JC, Dr Song L, Dr Liu YH, Dr Fan W, Dr Zan YW, Dr Wei XY, Dr Xu SQ, Dr Yoshimine M, Dr Yang JH, Dr Zheng H, Dr Gao JP, Dr Liu FY, and Mr Liu JY and Ms Zeng WB for their research work at Xi’an Jiaotong University. Thanks are due to Ms He, Ms Lei, and others for their support during the course of writing this book. I would like to thank many professors from other universities and many research scientists and engineers from various institutions for their work in the research and application of the unified strength theory. I would also like to acknowledge the support from all other individuals and universities, research organizations, journals, and publishers. I would also like to express my sincere thanks to Dr Dieter Merkle, Editorial Director, Engineering and Editorial Department and International Engineering Department, Springer-Verlag, Germany, and his team for their excellent editorial work on this manuscript. The study of generalized plasticity based on the unified strength theory is just the beginning. A lot of research in generalized plasticity is still to be done. Mao-Hong Yu Spring 2005

Contents

Preface Notations 1

Introduction 1.1 1.2 1.3 1.4 1.5 1.6 1.7

2

Stress Space and Stress State 2.1 2.2 2.3 2.4 2.5 2.6 2.7

3

Linear Elasticity ................................................................................. Classical Plasticity ............................................................................. Concrete Plasticity ............................................................................. Soil Plasticity .................................................................................... Rock Plasticity ................................................................................... Generalized Plasticity ........................................................................ Generalized Plasticity Based on the Unified Strength Theory.......... References and Bibliography.............................................................

Elements ............................................................................................ Stress at a Point, Stress Invariants...................................................... Deviatoric Stress Tensor, Deviatoric Tensor Invariants..................... Stresses on the Oblique Plane ............................................................ Hexahedron, Octahedron, Dodecahedron .......................................... Stress Space ........................................................................................ Stress State Parameters....................................................................... Summary ............................................................................................ References ........................................................................................

Basic Characteristics of Yield of Materials under Complex Stress 3.1 3.2 3.3 3.4 3.5 3.6

Introduction ........................................................................................ Strength Difference Effect (SD effect) ............................................ Effect of Hydrostatic Stress ............................................................... Effect of Normal Stress...................................................................... Effect of Intermediate Principal Stress .............................................. Effect of Intermediate Principal Shear-Stress ...................................

1 1 2 5 6 7 8 8 10

15 15 15 16 17 21 22 27 31 31

33 33 33 35 37 38 43

XIV

Contents

3.7

Bounds of the Convex Strength Theories ........................................ Summary........................................................................................... References .......................................................................................

46 47 47

4 Unified Strength Theory and Its Material Parameters

50

4.1 4.2 4.3 4.4 4.5 4.6 4.7 4.8 4.9

Introduction ................................................................................... Mechanical Model of the Unified Strength Theory ....................... Unified Strength Theory ............................................................... Special Cases of the Unified Strength Theory ............................... Material Parameters of the Unified Strength Theory ..................... Other Material Parameters of the Unified Strength T heory ............ Yield Surfaces and Yield Loci........................................................ Yield Loci of the Unified Strength Theory in the π í Plane ........ Yield Surfaces of the Unified Strength Theory in Principal Stress Space .................................................................................... 4.10 Yield Loci of the Unified Strength Theory in Plane Stress State .. 4.11 Unified Strength Theory in Meridian Plane ................................... 4.12 Yield Surfaces of the Non-linear Unified Strength T heory ............. Summary ....................................................................................... Problems ............................................................................. References and Bibliography .........................................................

50 51 53 54 60 63 66 69 72 75 78 81 85 87 93

5 Reasonable Choice of a Yield Function 5.1 5.2 5.3 5.4 5.5 5.6 5.7 5.8 5.9 5.10

Introduction ..................................................................................... Some Experimental Data of Metallic Materials............................. Reasonable Choice of a Yield Function for Non-SD Materials.... Experiments for Iron under σ – τ Stress State................................. Experiments for Concrete under Complex Stress ......................... Experiments for Rock under Complex Stress ............................... Experiments on Clay and Loess under Complex Stress ............... Experiments on Sand under Complex Stress ................................ Reasonable Choice of a Yield Function for SD-Materials ........... The Beauty of the Unified Strength Theory.................................. Summary............................................................................................. Problems ............................................................................................. References and Bibliography ..............................................................

6 Elasto-Plastic Costitutive Relations 6.1 6.2

95

Introduction ....................................................................................... Plastic Deformation in Uniaxial Stress State....................................

95 96 100 102 103 105 108 109 112 113 117 118 119

122 122 122

6.3 6.4 6.5 6.6 6.7 6.8 6.9 6.10 6.11 6.12

7

XV

Three-dimensional Elastic Stress-strain Relation ........................... Plastic Work Hardening and Strain Hardening................................ Plastic Flow Rule............................................................................. Drucker’s Postulate – Convexity of the Loading Surface ................. Incremental Constitutive Equations in Matrix Formulation........... Determination of Flow Vector for Different Yield Functions........ Singularity of Piecewise-Linear Yield Functions ............................ Process of the Plastic Flow Singularity........................................... Suggested Methods.......................................................................... Unified Process of the Corner Singularity ...................................... Summary .......................................................................................... Problems........................................................................................... References and Bibliography...........................................................

124 125 127 129 132 135 137 142 145 148 152 152 153

Concrete Plasticity 7.1 7.2 7.3 7.4 7.5 7.6 7.7

8

Contents

Introduction....................................................................................... Multi-Parameter Yield Criteria......................................................... Multi-Parameter Unified Yield Criterion......................................... Yield and Loading Functions ........................................................... Processing of Corner Singularity ..................................................... Strain Softening Phenomena and Material Damage ........................ Applcations ....................................................................................... Summary ........................................................................................... Problems............................................................................................ References and Bibliography............................................................

Twin- Shear Slip-Line Field for Plane Strain Problem 8.1 8.2 8.3 8.4 8.5 8.6

Introduction....................................................................................... Stress State in Plane Strain Problem ................................................ Twin-Shear Strength Theory of Plane Strain Problem .................... Twin-Shear Line Field Theory for Plane Strain Problem (Statically Admissible Field) ............................................................................ Twin-Shear Slip Line Field Theory for Plane Strain Problem (Kinematically Admissible Field) .................................................. Applications of the Twin-Shear Slip Line Field Theory for Plane Strain Problems ................................................................. Summary........................................................................................... Problems ........................................................................................... References and Bibliography ...........................................................

155 155 157 162 168 176 179 182 192 192 193

195 195 198 200 202 204 209 218 218 223

XVI

9

Contents

Unified Slip- Line Field Theory for Plane Strain Problem 9.1 9.2 9.3 9.4 9.5 9.6 9.7 9.8 9.9

Introduction ...................................................................................... 225 Unified Strength Theory in Plane Strain Condition......................... 226 Unified Slip Line Field Theory for Plane Strain Problem (Statically Admissible Field) ............................................................................ 230 Unified Slip Line Field Theory for Plane Strain Problem (Kinematically Admissible Field) ............................................................................ 233 Special Cases of the Unified Slip Line Field Theory ...................... 236 Applications of the Unified Slip Line Field Theory ........................ 240 Comparison of the Unified Slip Line Field Theory with Finite Element Method ............................................................................... 252 Comparison of the Unified Slip Line Field Theory with Experimental Results........................................................................ 256 Discontinuous Bifurcations of Elasto-Plastic Material For Plane Strain Problem .................................................................................. 257 Summary........................................................................................... 260 Problems ........................................................................................... 260 References and Bibliography ........................................................... 268

10 Twin-Shear Characteristics Field for Plane Stress Problem 10.1 Introduction ................................................................................... 10.2 Characteristics Method Based on the Tresca Criterion and the Huber-von Mises Criterion ....................................................... 10.3 Characteristics Method Based on the Twin-Shear Yield Criterion 10.4 Twin-Shear Characteristics Field for Plane Stress Problems (Velocity Field) ............................................................................. 10.5 Applications of the Twin-Shear Characteristics Method............... 10.6 Comparison of These Different Methods ....................................... Summary......................................................................................... Problems ......................................................................................... References and Bibliography .........................................................

11 Unified Characteristics Field Theory for Plane Stress Problem 11.1 11.2 11.3 11.4

225

Introduction.................................................................................... Unified Yield Function in Plane Stress State.................................. Characteristics Filed for Plane Stress Problems ........................... Applications of the Unified Characteristics Field for Plane Stress Problems.............................................................................

270 270 270 274 278 281 287 288 288 292

293 293 293 296 302

Contents

XVII

11.5 Discontinuous Bifurcations of Elasto-Plastic Material for Plane Stress ............................................................................... 11.6 Discontinuous Bifurcations of Non-associated Flow Elasto-Plastic Materials Based on Yu Unified Strength Theory... 11.7 Discussion and Experimental Verification .................................... Summary......................................................................................... Problems ......................................................................................... References and Bibliography .........................................................

310 317 319 320 320

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

322

12.1 Introduction.................................................................................... 12.2 The Unified Strength Theory......................................................... 12.3 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Stress Field) ........................................ 12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Velocity Field) .................................... 12.5 Applications of the Unified Characteristics Field Theory ............ 12.6 Penetration of High Velocity Rod to Target .................................. 12.7 Elastic-Damage-Plastic Analysis of the Target ................................ 12.8 Comparison and Verification ......................................................... Summary............................................................................................. Problems ............................................................................................. References and Bibliography .............................................................

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding 13.1 Introduction................................................................................... 13.2 Unified Strength Theory ............................................................... 13.3 Stress Field Around Crack-Tip ..................................................... 13.4 Shape and Size of Plastic Zone for Mode-I Crack Tip ................ 13.5 Shape and Size of Plastic Zone for Mode-II Crack Tip ............... 13.6 Plastic Zone for Mode-III Crack Tip............................................ 13.7 Shape and Size of Plastic Zone for Non-Conventional Materials 13.8 Effect of b’ Value ........................................................................ 13.9 Influence of SD Effect................................................................... 13.10 Influence of Poisson’s Ratio .......................................................... Summary ....................................................................................... Problems ....................................................................................... References and Bibliography .......................................................

308

322 324 324 329 331 334 338 343 346 347 348

351 351 352 355 357 361 365 365 368 369 370 371 372 374

’

XVIII

Contents

14 Unified Fracture Criteria for Mixed Mode Crack Initiation and Fatigue Crack Growth 14.1 14.2 14.3 14.4 14.5 14.6

375

Introduction ................................................................................. Main Idea of T-Criterion .............................................................. A Generalization for T-Criterion Using UST .............................. Significance of Parameters b, α and v .......................................... Crack Initiation Angle of the Generalized T-Criterion................ Application of the Unified Strength Theory in Establishing the Mixed Fracture Criterion........................................................ 14.7 Unified Fracture Criterion ............................................................ 14.8 Unified Fracture Criterion of Mixed Mode I – III ....................... 14.9 Unified Fracture Criterion of Mixed Mode II – III....................... Summary........................................................................................ Problems....................................................................................... References and Bibliography.......................................................

375 377 378 384 388 389 392 395 396 397 398 399

15 Limit Load and Shakedown Load of Pressures Vessel

401

15.1 Introduction ............................................................................ 15.2 Theorems of Limit Analysis of Structures............................... 15.3 Unified Solution of Limit Pressures for Thin-Walled Pressure Vessel............................................................................. 15.4 Unified Solution of Elastic Limit Pressure for Thick-Walled Cylinders ............................................................... 15.5 Unified Solution of Plastic Limit Pressure for Thick-Walled Cylinder................................................................. 15.6 Statical Shakedown Theorem (Melan Theorem) ....................... 15.7 Unified Solution of Shakedown Pressure for Thick-Walled Cylinder................................................................. 15.8 Effects of Yield Function on the Plastic Limit Pressure and Shakedown Pressure of Thick-Walled Cylinders ................. 15.9 Connection between Shakedown Theorem and Limit Load Theorem ............................................................. Summary ....................................................................................... Problems.......................................................................................... References and Bibliography..........................................................

401 402 403 406 416 423 425 430 434 435 436 437

Indexes Author Index ..................................................................................................... Subject Index.....................................................................................................

441 445

Notations

Stresses and Invariants σ1 , σ 2 , σ 3 σ13 , σ 12 , σ23

m σr , σθ , σz r

r

σr , σ z , σθ σ ij σ τ 13 τ 12 , τ 23 µσ µ τ µτ ′

r

θ τ 8 or τ oct σ 8 or σ oct

I1 , I2 , I3

σm

S1 , S2 , S3 J1 , J2 , J3 K I , K II , K III

major principal stress, intermediate principal stress and minor principal stress normal stresses acted on the orthogonal octahedron element intermediate principal stress state parameter radial stress, circumferential stress and axial stress in polar coordinates residual stresses of the cylinder in polar coordinates stress tensor normal stress maximum principal shear stress intermediate shear stress or minimum shear stress Lode stress parameter twin-shear parameter for stress state µτ = τ 12 / τ 23 , µτ ′ = τ 23 / τ 13 stress angle corresponding to the twin-shear parameter octahedral shear stress octahedral normal stress invariants of the stress tensor σ ij hydrostatic stress or mean stress deviatoric stresses invariants of the deviatoric stress tensor stress-intensity factors for mode-I, mode -II and mode-III

Strain and Flow Vector İ1, İ2, İ3 İe İp dİe dİp d ε ij e

principal strain elastic strain plastic strain elastic strain increment plastic strain increment elastic strain increment tensor

XX

Notations

d ε ij p İij

ε r , εθ εz ε r , εθ

Cijkl dλ {a1}, {a2}, {a3} C1, C2, C3 or C1′ , C2′, C3′

plastic strain increment tensor strain tensor radial and circumferential strain longitudinal strain radial and circumferential strain stiffness tensor proportional positive scalar factor flow vectors parameters defining the yield surface

Material Parameters σy σt σc α

m τ 0 or τ y

b β

C0 Ct Cuni

ϕ0 ϕt ϕuni

E G λ ν κ

K I c , K II c , KIII c

yield stress uniaxial tensile strength uniaxial compressive strength ratio of tensile strength to compressive strength compressive-tensile strength ratio of materials pure shear strength or shear yield strength of materials failure criterion parameter in the unified strength theory coefficient in the unified strength theory that represents the effect of the normal stress on failure cohesive strength twin-shear cohesion unified cohesion friction angle twin-shear friction angle unified friction angle elastic modulus (Young’s modulus) shear modulus Lame constant Poisson’s ratio hardening parameter of material stress-intensity factors of materials under mode-I, mode -II and mode-III

Miscellaneous f, f ′ F, F ′ ρ

u , v, w [σ ] p

yield criterion function yield criterion function or fracture criterion function density of the material displacements σ allowable tensile stress, [ σ ] = t n internal pressure subjected to the cylinder

Notations

pe pp p max r ri , re rp

elastic limit pressure plastic limit pressure shakedown pressure of the cylinder radial variable the internal and external radii of the cylinder plastic zone radius of the cylinder subjected to internal pressure p

XXI

1 Introduction

1.1 Linear Elasticity A structure deforms when it is subjected to external forces. The deformation is elastic if it is reversible, that is, if the deformation vanishes instantaneously as the external forces are removed. It is also assumed that the relationships of forcedisplacement and stress-strain are linear. Most engineering materials possess to a certain extent the property of linear-elasticity. The stress states of materials in structures are usually biaxial and triaxial, or in general multiaxial or polyaxial. It is very important to see how the stress combinations affect the strength of material and structure. Serious errors may be resulted if the uniaxial stress assumptions are extended directly to the multiaxial stress state. It will be assumed that the material of an elastic structure is homogeneous and continuously distributed over its volume so that the smallest element cut from the structure possesses the same specific physical properties as the structure. It will also be considered that the material of a structure is isotropic, i.e., the properties are the same in all directions. On the other hand, engineering materials are generally very complicated in compositions. The important material steel, for instance, consists of various kinds of crystals oriented in different directions. The material is very far from being homogeneous in microscope scale. The solutions in view of the theory of elasticity, however, based on the assumptions of homogeneity and isotropy can be applied to steel structures with very great accuracy on the macro-scale level. The explanation is that the crystals are very small; there are millions of them in one cubic inch of space. While the elastic properties of a single crystal may be very different in different directions, the crystals are ordinarily distributed at random and the elastic properties of larger pieces of metal represent averages of the properties of the crystals. Therefore, as long as the geometrical dimensions of a structure are very huge in comparison with the dimensions of a single crystal the assumption of homogeneity can be used with very high accuracy. And if the crystals are orientated randomly the material can be treated as isotropic (Timoshenko and Goodier 1970; Fung 1977). The assumptions of isotropy and homogeneity for materials are also used in plasticity. Discussions of the plasticity for heterogeneous and anisotropic materials are not in the scope of this book.

2

1 Introduction

1.2 Classical Plasticity The deformation of a material is plastic if it is irreversible. A brittle material such as glass, concrete, or rock under tension has only elastic deformation before it fails. On the other hand, metals, rocks and concrete under high confining pressure can undergo substantial plastic deformation before failure and therefore show ductile material properties. The " Theory of Plasticity " or " Plasticity " is a branch of solid mechanics regarding the plastic deformation and the limit load carrying capacity of materials and structures. It deals with the theories and methods of yield initiation of materials under complex stress state and calculation of stresses and strains in a deformed structure after part or the whole structure has yielded. It is necessary, as for elasticity, to establish equations of equilibrium and compatibility and to determine the experimental relations between stress and strain, besides , a condition of yield initiation is needed. It is called yield criterion or yield function. In 1864, Tresca presented two notes dealing with the experimental investigations on plastic flow of metals under great pressure to the French Academy. He first postulated a yield condition for the continuum problem. It is the well-known Tresca yield criterion. Saint-Venant (Barre de Saint-Venant 1797–1886) was the first to set up the fundamental equations of plasticity and to use them to solve several practical problems. The fundamental equations of plasticity are based on the following assumptions. 1. The volume of materials does not change during plastic deformation; 2. The directions of principal strains coincide with the directions of principal stresses; 3. The maximum shearing stress at each point is equal to a specific constant. It means that the Tresca criterion was used as a yield condition. Sometimes, it is referred as the maximum shear stress criterion or single-shear criterion. The yield surface of the Tresca criterion in stress space and its yield locus in deviatoric plane are shown in Fig. 1.1. The yield loci and the yield surfaces will be described in detail in Chapter 6.

Fig. 1.1 Yield surface of the Tresca criterion in stress space

1.2 Classical Plasticity

3

Using these hypotheses, Saint-Venant solved several problems such as torsion of circular shafts, pure bending of rectangular prismatic bars, and the plastic deformation of hollow circular cylinders under the internal pressure. In fact, SaintVenant initiated the study of a complete new field of solid mechanics. SaintVenant called the new subject "Plasticodynamics" . Now plasticity has been the object of considerable research. Prandtl (Ludwig Prandtl 1875–1953) made further progress in the field of plasticity. He solved the more complicated two-dimensional problem of a semiinfinite body under a uniform pressure p distributed over a strip of width. He obtained the limit pressure plimit of strip as follows

§ π · p lim it = σ s ¨1 + ¸ © 2¹ The first systematic treatment of plasticity was given by Nadai in 1931. Rapid progress in plasticity began with the appearance of the paper of Prandtl and the book of Nadai. After the Second World War, the subject of plasticity constitutes an important branch in the solid mechanics. Some books relating the plasticity were published near 1950 by Sokolovsky (1946), Freudental (1950), Hill (1950), Nadai (1950), Prager and Hodge (1951) et. al. After the Tresca yield criterion, the Huber-von Mises yield criterion was proposed by Huber in 1904 and von Mises in 1913. The yield surface of the HuberMises yield criterion in stress space and its yield locus in deviatoric plane are shown in Fig.1.2.

Fig. 1.2 Yield surface of the Huber-von Mises criterion in stress space

The classical plasticity is widely applied in mechanical engineering and metal forming. It is assumed by the Tresca criterion and the Huber-von Mises criterion that these materials have the same strength in both tension and compression and the ratio of shear yield stress Ĳy to the tensile yield stress ıy is Ĳy/ıy=0.5 based on the Tresca criterion or 0.577 on the Huber-von Mises criterion.

4

1 Introduction

In 1961, a new yield criterion was proposed by Haythorthwaite and Yu. It is introduced from the maximum deviatoric stress by Haythorthwaite and the twinshear stresses by Yu, and referred to respectively as the maximum deviatoric stress yield criterion and the twin-shear yield criterion. The yield surface of the twinshear yield criterion in stress space and its yield locus in ʌ plane are shown in Fig.1.3. The twin-shear yield criterion is adapted for those material have the same strength in tension and compression and the ratio of the shear yield stress Ĳy to the tensile yield stress ıy is Ĳy/ıy = 0.667. The mathematical expression of the twinshear yield criterion is linear. It is convenient for analytical solution of limit analysis of structure.

Fig. 1.3 Yield surface of the Twin-shear criterion in stress space

The yield loci in deviatoric plane and meridian plane of the three yield criteria are shown in Fig.1.4.

Fig. 1.4 Yield loci of the three yield criteria

1.3 Concrete Plasticity

5

Classical plasticity is widely used for metallic materials. However, classical plasticity models are not able to predict basic failure phenomena of rocks, soils, concrete, polymers and other materials. Applications in concrete structural engineering, geotechnical engineering, mining and petroleum engineering, nuclear power plant, underground excavation, structure safety problems under earthquake, and solid mechanics problems at meso/micro scales call for more realistic and more accurate solutions. Now developments in plasticity theory is an active field of mechanics. The concrete plasticity, soil plasticity, rock plasticity and computational plasticity etc. are developed.

1.3 Concrete Plasticity Concrete as a structural material has been used widely in many major constructions such as tall buildings, bridge, dam, offshore platforms, reactor vessels, nuclear containment structures, etc. Plastic analysis of these structures has become increasingly important. Concrete is a composite material, consisting of coarse aggregate and a continuous matrix, which itself comprises a mixture of cement paste and smaller sand particles. Its physical behavior is quite complex. In engineering application, only the mechanical behavior instead of the composition of the material is concerned, which is developed on the basis of a homogeneous continuum. Also, the material is assumed to be initially isotropic. In recent years, a good progress has been achieved in the area of constitutive modeling of concrete materials. Various predictive models with two-parameter, three-parameter and multi-parameter have been proposed and used for analysis of concrete structures. The models are based on the principles of continuum mechanics, neglecting the microstructure effect of the concrete materials. To this end, nonlinear elasticity and plasticity are found adequate in characterizing the macroscopic stress-strain behavior of concrete. The theory of concrete plasticity, i.e. the basic concepts and applications of plasticity modeling to concrete materials were presented by Chen (1982) and Nielsen (1984, 1999). Systematical descriptions on the " Plasticity in Reinforced Concrete" and " Limit Analysis and Concrete Plasticity" were given. The Mohr-Coulomb strength theory and some multi-parameter criteria are widely used in concrete plasticity. The yield locus of the Mohr-Coulomb strength theory in deviatoric plane is shown in Fig.1.5. The solid line is the yield locus of the generalized twin-shear criterion (Yu et al. 1985).

6

1 Introduction

Fig. 1.5 Two bounds of the convex yield criteria

1.4 Soil Plasticity Soils are complex materials consisting of solid, air and water. It exhibits a wide range of behavior depending on classification, stress history, void ratio, density and characteristics of the disturbing force. The plastic behavior of soils was studied by Roscoe, Schofield and Thurairajah (1963), Roscoe (1968), Roscoe and Burland (1968), Schofield and Wroth (1968) et al in Cambridge University. Soil Plasticity was presented by Roscoe (1968), Schofield and Wroth (1968), Chen (1975) and Salencon (1977) in 60’s and 70’s of the last century and continued by Chen and Baladi (1985). The soil plasticity was also implemented into computational code by Zienkiewicz and Pande (1977), Zienkiewicz and Humpheson (1977), Zienkiewicz and Mroz (1984), Desai (1984), Vermeer and de Borst (1984), de Boer R (1988) and others. Over the last 30 years, significant advances in this area have led to the development of several constitutive models, which may efficiently represent the behavior of soils subjected to complex stress. Now, the soil plasticity is still one of the most active research areas. The Mohr-Coulomb strength theory (Mohr 1900) and the Drucker-Prager (1952) criterion are widely used in soil plasticity. The yield loci in deviatoric plane and meridian plane of the Drucker-Prager criteria and the Mohr-Coulomb criterion are shown in Figs.1.6 and 1.7. Two bounds of failure criteria are shown in Fig.1.8. Systematical descriptions on the soil mechanics and applications were given by Chen (1975), Salencon (1977) and Chen and Baladi (1985), Zeng, Shen and Gong (2002). Soil plasticity based on the Critical State Soil Mechanics were described by Schofield and Wroth (1968), Atkingson & Bransby (1978), Atkingson (1981) and Wood (1990).

1.5 Rock Plasticity

7

Fig. 1.6 Some varieties of the Drucker-Prager criteria

Fig. 1.7 Yield loci of the Drucker-Prager criteria

Fig. 1.8 Yield loci of the two bounds (single-shear and twin-shear criteria)

1.5 Rock Plasticity The plastic behavior of rock was not generally known until 60’s of the last century when the rigid test equipment was produced. The first congress of international society of rock mechanics was hold in Lisbon in 1966. The flow behavior of rocks were studied by Broms (1966), Goodman, Taylor and Brekke (1968) and others. The bearing capacity of rock and concrete block was studied by Chen and Drucker (1969). Non-associated plasticity for soils, concrete and rock were studied by Vermeer and de Borst (1984) et al.

8

1 Introduction

The Mohr-Coulomb strength theory and the Hoek-Browm (1980) criterion are widely used in rock plasticity. “Finite Element Code for Soil and Rock Plasticity” was presented by Vermeer (1991, 1998). The concept of plastic zone of rock is widely used for rock mechanics and engineering.

1.6 Generalized Plasticity The theory of plasticity was originally developed for the description of the behavior of metallic materials. From the microscopic point of view, the deformational mechanisms of metal are quite different from those of concrete, rock and soils. The former is due to the arrangement of dislocations of polycrystals, while the later is due to the initiation and nucleation of microcracks at the aggregate-mortar interface as well as through the mortar, air or cracks. However, if we do not limit our interpretations of the behavior "plastic" and "yielding" in the usual sense, the classical theory of plasticity can be extended to approximate the concrete, rock and soils behavior under various circumstances (Chen 1978). In other words, the theory of plasticity, when not interpreted too narrowly, provides a very flexible mathematical model that can be used to describe a wide variety of behaviors of concrete, rock and soils. The continuum theory of plasticity was given by Khan et al. (1995). The generalized stress-strain behaviour of wet clay was studied by Roscoe and Burland (1968). The generalized cap model for geological materials was studied by Sandler, DiMaggio and Baladi (1976). The term of Generalized Plasticity was introduced by Zienkiewicz and Mroz (1984), Pastor and Zienkiewicz (1986), and by Pastor, Zienkiewicz and Chan (1990). The word of ‘generalized’ means the extension of plastic conception for metallic materials to geomaterials. Now, generalized plasticity is widely studied and applied in literature and engineering.

1.7 Generalized Plasticity Based on the Unified Strength Theory Great effort has been devoted to the formulation of yield criteria for various materials during the past 100 years (Yu 2002). Most yield criteria are suitable for only a certain type of materials. The plasticity theory for metallic materials is mainly based on the Tresca yield criterion and the Huber-Mises yield criterion. The plasticity theory of soils is mainly based on the Drucker-Prager criterion; and the plasticity theory for concrete and rock is mainly based on the Mohr-Coulomb criterion. What is the relationship among various yield criteria and different “Plasticity”? Many scientists have devoted considerable effort to this topic. Based on a unified mechanical model that takes into account the effects of all the stress components on the failure of materials, a new unified strength theory that has a unified mathematical expression was proposed by Yu in 1991. The Mohr– Coulomb strength theory, the twin-shear stress theory, and many other new criteria

1.7 Generalized Plasticity based on the Unified Strength Theory

9

can be deduced from the unified strength theory. A relationship among most of the prevailing failure criteria and yield criteria is established The unified strength theory contains two families of yield criteria for metal materials and geomaterials. The first family is the convex yield criteria. A series of convex yield criteria can be deduced from the unified strength theory by giving a certain value to material parameter b (0 0, σ

2

= σ 3 < 0, uniaxial tension, equal biaxial compression stress state.

′

If µ τ = µ τ = 0.5 (stress angle equals θ = 30 o ), the corresponding stress states are as follows: 1. σ

2

2. σ

2

1 (σ 1 + σ 3 ) = 0 , pure shear stress state; 2 = (σ 1 + σ 3 ) / 2 > 0, biaxial tension and uniaxial compression stress state;

3. σ

2

= (σ 1 + σ 3 ) / 2 < 0, uniaxial tension and biaxial compression stress state.

=

If µ τ = 0 ( µ τ ′ = 1 , stress angle equals θ = 60 o ), then the corresponding stress states are as follows:

2.7 Stress State Parameters

29

1. σ 1 = σ 2 = 0, σ 3 < 0, uniaxial compression stress state; 2. σ 1 = σ 2 > 0, σ 3 = 0, equal biaxial tension stress state; 3. σ 1 = σ 2 > 0, σ 3 < 0, equal biaxial tension and uniaxial compression stress state. According to the twin-shear stress parameters and the magnitude of the two smaller principal shear stresses, the stress state can be divided into three kinds of conditions as follows: 1. Extended tension stress state, that is, τ 12 > τ 23 , 0≤ µτ ′ < 0.5 von Mises

Mild steel

Solid bars

0.45–0.49

Tresca

Tubes

–

von Mises

Tubes

–

Tubes

–

von Mises von Mises von Mises near twin shear

Review work

–

No one agreed

Tubes

–

Tresca, von Mises

Tubes

–

von Mises

Tubes

–

von Mises

Tubes

–

von Mises

Tubes

0.54

von Mises

Tubes

–

> von Mises

Tubes Tubes Tubes

– – –

von Mises > von Mises von Mises

Lode 1926 Ros & Eichinger 1926 Taylor & Quinney 1931 Marin 1936

Iron, mild steel, nickle, copper Mild steel Aluminum, copper, Mild steel Mild steel

Morrison Mild steel 1940, 1948 Davis 1945 Copper, Davis and Parker medium carbon 1948 steel Osgood 1947 Aluminum alloy Cunningham et al. Magnesium alloy 1947 Bishop and Hill 1951 Polycrystals Fikri and Johnson Mild steel 1955 Marin and Hu 1956 Mild steel Naghdi et al. 1958 Aluminum alloy Hu and Bratt 1958 Aluminum alloy

5.2 Some Experimental Data of Metallic Materials

99

Table 5.1. (Continue) Researchers

Materials

Ivey 1961 Aluminum alloy Bertsch and Findley 1962 Aluminum alloy

Specimen

Ĳ s /ı s

Tubes Tubes

o.66 –

Suitable Criterion

Twin shear von Mises

Mair and Pugh 1964

Copper

Tubes

–

Miastkowski 1965

Brass

–

–

von Mises Twin shear von Mises

Rogan 1969

Steel

tubes

0.5

Tresca

–

von Mises

0.64

near Twin shear between Tresca and von Mises

Low Pisarenko et al. 1969 Copper, Cr-steel temperature Dawson 1970 Polycrystals – Phillips et al. Elevated Aluminum 1970, 1972 temperature Deneshi et al. 1976

Aluminum, Copper

Winstone 1984

Nickel alloy

Ellyin 1989 Wu and Yeh 1991 Ellyin 1993 Ishikawa 1997

Titanium Aluminum stainless steel Titanium Stainless steel

Low temperature Elevated temperature Tubes Tubes Tubes Tubes

0.53 0.6

> von Mises

0.7

Twin shear

0.66

Twin shear

0.58 0.66–0.7 0.62–0.7 0.6–0.63

von Mises Twin shear – > von Mises

The unified strength theory under σ − τ combined stress can be expressed as 2+b b σ 2 + 4τ 2 + σ = σs , 2 + 2b 2 + 2b b 2+b f = σ 2 + 4τ 2 − σ = σs , 2 + 2b 2 + 2b f =

when σ ≥ 0

(5-1a)

when σ ≥ 0

(5-1b)

The corresponding yield loci are shown in Fig. 5.4.

Fig. 5.4 Yield loci of the unified yield criterion under σ − τ combined stress state

100

5 Reasonable Choice of a Yield Function

It is seen that: 1. The unified yield criterion almost encompasses various yield criteria of materials under (σ −τ ) combined stresses. 2. The yield loci are convex when the parameter b varies from 0 to 1. It should be noted that the yield loci in the three–dimensional stress state and the plane stress state will be nonconvex when b >1 or b < 0. The nonconvex yield surfaces have been discussed in Chap. 3. 3. The differences between various yield functions are obvious under simple shear stress. The ratios of pure shear yield stress τ s to tensile yield stress σ s of some typical yield criteria are shown as follows: single-shear yield criterion (Tresca yield criterion): τ s = 0.5σ s; Huber-von Mises yield criterion: τ s=0.577σ s; twin-shear yield criterion: τ s = 0.667σ s; maximum tensile strain theory: τ s=0.769σ s (ν=0.3); maximum normal stress theory: τ y =1.0σ y. After the comparison of the shear yield strength and tensile yield strength among the 30 materials, Kishkin and Ratner (see Onksov 1963) divided the metals into four kinds according to the ratio of the shear yield strength to tensile yield strength τ s /σs as follows: 1. τ s /σ s ≅ 0.50 (0.48̢0.53, five materials), which agrees with the single-shear yield criterion (Tresca yield criterion) or with the unified yield criterion when b=0. 2. τ s /σ s ≅ 0.58 (0.54̢0.62, nine materials), which agrees with the Huber-von Mises yield criterion, or with the unified yield criterion when b =1+ 1/(1+ 3 ) or b=1/2. 3. τ s /σ s ≅ 0.68 (0.67̢0.71, eight materials), which agrees with the twin-shear yield criterion, or with the unified yield criterion when b = 1 . 4. τ s /σ s < 0.40 (0.31̢0.41, eight materials), which gives a nonconvex result that does not agree with existing criteria. This kind of result is not indicated by any theoretical criterion, but matches the unified yield criterion when b=̢1/3.

With regard to the ratio of shear strength to tensile strength of metals, the values in some manuals are 0.52~0.63 (carbon steel) and 0.65~0.78 (alloy steel). Generally, the ratio of shear yield stress τ y to the tensile yield stress σ s is different for different materials. According to the convexity of yield surface, shear yield strengths are in the range of τ s=(0.5~0.667)σ s for those metallic materials that have same strength both in tension and compression. Yield stresses of metallic materials are higher than τ s /σ s =0.5. Many yield stresses of high-strength steel, high-strength alloys, and non-metallic materials are higher than τ s=0.667. These kinds of materials may be the SD (strength difference in tension and in compression) materials.

5.3 Reasonable Choice of a Yield Function for Non-SD Materials Because of the significant differences in shear strengths of materials, the yield function can be selected on the basis of the ratio of the shear yield stress τ s to the tensile yield stress σ s.

5.3 Reasonable Choice of a Yield Function for Non-SD Materials

101

According to the unified yield criterion f = σ1 − f′=

1 1+ b

1 1+ b

(bσ 2 + σ 3 ) = σs ,

σ2 ≤

if

( σ 1 + σ b 2 ) − σ 3 = σs ,

if

1 (σ 1 + σ 3 ) 2

σ2≥

1 (σ 1 + σ 3 ) 2

(5-2a) (5-2b)

where b is a yield criterion parameter that represents the effect of the intermediate principal shear stress on the yield of materials and lies in the range of 0 ≤ b ≤ 1 when the yield surfaces are convex. In the case of critical state in pure shear σ 1 = τ, σ 2 = 0 , σ 3 = −τ and τ = τ s , we have σ1

= τ s , σ 2 = 0 , σ 3 = −τ s , and

σ2

= (σ 1 + σ 3 ) / 2 = 0

(5-3)

hence, we can use the anyone of Eqs. (5-2a) or (5-2b). Substituting Eq. (5-3) into the equation of the unified yield criterion Eq.(5-2a) or Eq. (5-2b), the relation among the tensile yield stress σ s, shear yield stress τ s and the parameter b in the unified yield criterion is obtained as (5-4)

(2+b) τs =(1+b) σ s

The parameter b can be determined from the ratio of shear yield stress to tensile yield stress as follows: b=

2τs − σs σs

− τs

=

2 ατ −1 1 − ατ

,

(5-5)

Inversely, the ratio of shear yield stress to tensile yield stress can be given as ατ

=

τs σs

=

b +1 b+2

(5-6)

The unified yield criterion establishes clear and simple relations among the various yield criteria. It also provides a method to choose the appropriate yield criterion. It can be obtained from the unified yield criterion as follows: (1) First, we need know the tensile yield stress σ s and shear yield stress τ s; (2) Second, the ratio of the shear yield stress to the tensile yield stress α τ= τ s /σ s can be determined ; (3) then, substituting α τ into Eq. (5-5), the parameter b is determined; (4) at last, substituting b into Eq. (5-1a) and (5-1b), an appropriate yield criterion is obtained. For example, if the ratio of the shear yield stress to the tensile yield stress is α τ = τ s /σ s = 0.6, the parameter b can be determined from Eq. (5-5) is b=1/2. Substituting

102

5 Reasonable Choice of a Yield Function

b=1/2 into Eq.(5-2a) and (5-2b), then an appropriate yield criterion is given as follows: 1 1 when σ 2 ≤ (σ 1 + σ 3 ) (5-7a) f = σ 1 − (σ 2 + 2σ 3 ) = σ y , 2 3 f ′=

1 3

when σ 2 ≥

(2σ 1 + σ 2 ) − σ 3 = σ y ,

1 (σ + σ 3 ) 2 1

(5-7b)

This means that a new yield criterion is introduced. This new yield criterion can be approximated to the Huber-von Mises yield criterion. If the ratio of the shear yield stress to the tensile yield stress is α τ = τ s /σ s = 0.667, the parameter b can be determined from Eq. (5-5) is b=1. Substituting b=1 into Eq.(5-2a) and (5-2b), the yield criterion is given as follows: f

if

σ2 ≤

1 (σ + σ 3 ) 2 1

′ = (σ1 + σ 2 ) − σ 3 = σ s , if

σ2 ≥

1 (σ + σ 3 ) 2 1

1

= σ1 − (σ 2 + σ 3 ) = σ s , 2

1

(5-8a)

(5-8b) 2 It is the twin-shear yield criterion proposed by Yu in 1961. Various new yield criteria may be introduced when the ratio of the shear yield stress to the tensile yield stress is different. f

5.4 Experiments for Iron under σ–τ Stress State A combined σ –τ stress state can be produced in thin tube under axial force and torsion. For brittle materials, such as iron, the limit locus of the materials is asymmetrical in the τ –coordinate because its tensile strength is different from its compressive strength. Since the ratio of the tensile-compressive strength is different, two material constants are required, such as tensile strength σ t and compressive strength σc , tensile strength σ t and the tensile-compressive ratio α =σ t /σc , or compressive strength σ c and the compression-tension strength ratio m=σ c /σ t. For example, the limit loci corresponding to different tension-compression strength ratios of twin-shear yield function are shown in Fig. 5.5. The comparison of the experimental results of iron with the twin-shear yield function are given. A series of experiments of iron under σ −τ combined stress states were conducted by Grassir and Cornet (1949), Mair (1968) and Coffin (1950). Their experimental results are shown in Fig. 5.6.

5.5 Experiments for Concrete under Complex Stress

103

Fig. 5.5 Comparison between experimental results for iron and twin-shear strength theory (Grossir and Cornet 1949; Coffin 1950)

5.5 Experiments for Concrete under Complex Stress The experimental results of concrete with the twin-shear yield function are shown in Fig.5.6.

Fig. 5. 6 Comparison between experimental results for concrete and twin-shear stress theory

The primary experiments on limit loci in the ʌ-plane on concrete were conducted by Gachon and Launay of the French National Institute of Technology. A series of limit loci in the ʌ-plane for concrete are given under different hydrostatic pressures. Figs. 5.7 and 5.8 show the limit loci in the ʌ-plane for concrete (Gachon 1972, Launay and Gachon 1973). It can be seen from Figs. 5.7 and 5.8 that although smooth curves can approximate the results, the polygonal line in Fig. 5.8 is closer to the experimental results. Fig. 5.8 shows three groups of experimental limit loci and compares them with yield function. The limit locus of yield function shown in Fig. 5.8 is the unified strength theory with b=1/2. In order to enable comparison, the limit locus of the unified strength theory with b=0 and b=1 under 3p=4 and 8 are also given. Although there are only two data points when 3p=1, which cannot be compared with yield function, other experimental results all agree with the estimation of the unified strength theory with b=1/2. As to the experimental results in Fig. 5.8, they also agree with the unified strength theory with b=1/2.

104

5 Reasonable Choice of a Yield Function

Fig. 5.7 Limit loci in the ʌ-plane for concrete (Gachon 1972)

Fig. 5.8 Comparison between experimental limit loci of concrete and the unified strength theory with b=1/2

In the 1990s, many true triaxial experiments were conducted. Faruque and Chang conducted three groups of experiments on plain concrete. The stress states of these three groups of experiments were (σ 2=σ 3, σ 1), (σ 1 =–σ 3, σ 2) and (σ 1=σ 2, σ 3), i.e., triaxial tension, shear and compression, respectively. Their experimental results can be connected as shown in Fig. 5.9. It can be seen that the experimental results agree with the unified strength theory with b=1. The experimental results for steel fiber concrete obtained by Dong et al. (1993) also agree with twin-shear stress theory.

5.6 Experiments for Rock under Complex Stress

105

Fig. 5.9 Concrete (Faruque and Chang 1990)

From the above experimental results, it can be deduced that the limit loci of concrete in the ʌ-plane lies between the unified strength theory when b=1/2 and b=1. There are lots of experimental data on meridian lines for concrete (see Chen WF 1982). It can be expressed approximately by a two-parameter criterion, giving a straight limit meridian line. Generally, it must be expressed by three-parameter, four-parameter or five-parameter criteria, giving curved limit meridian lines.

5.6 Experiments for Rock under Complex Stress Michelis (1985, 1987) conducted many fine true triaxial experiments on rock and concrete. The results show that the effect of intermediate principal stress σ 2 is an important characteristic for geomaterials. According to the three series of experimental data (Michelis 1985, 1987) three limit loci may be drawn as shown in Fig. 5.10.

106

5 Reasonable Choice of a Yield Function

Fig. 5.10 Marble (Michelis 1987)

The biaxial experiments of rock have also been conducted at the same time. Fig. 5.11 shows the experimental result published by Amadei and Kuberan in the 24th Conference of Rock Mechanics of American in 1984. The dotted line in the figure is the limit line of Mohr-Coulomb strength theory in plane stress state. The solid line is the limit line of the unified strength theory with b=3/4. Compared with the experimental results, there is a large difference between the Mohr-Coulomb theory and the experimental results. Mohr-Coulomb strength theory is too conservative. The limit surface of the unified theory with b=3/4 is close to the experimental results, but in the region of biaxial compressive stress state, it is also too conservative.

Fig. 5.11 Experimental results under biaxial condition for limestone (Amadei et al, 1984)

A granite with properties such as high hardness, high density, high strength and high elastic modulus can be found in the upstream of the Yellow River (China). Its uniaxial compressive strength is σ c =157 MPa; it has elastic modulus G=50 Gpa,

5.6 Experiments for Rock under Complex Stress

107

tensile strength σ t =7.8 MPa, shear strength parameter C0=16 MPa, tgϕ =0.96, the unit weight r =2680 kg/m3 and Possion’s ratio ν = 0.2 . A series of experiments on rock corresponding to different high pressures under the same stress angle were carried out by the Northwest Design and Research Institute (China) and the Wuhan Institute of Rock and Soil Mechanics of the Chinese Academy of Science. The failure strength of rock corresponding to different hydraulic pressures with the same stress angle can be obtained, and then the limit meridian lines of rock under this stress angle can then be obtained. Five stress angles θ =0°, 13.9°, 30°, 46.1°, 60° are adopted, and the corresponding five limit meridian lines are shown in Fig. 5.12. Six sections are adopted in Fig. 5.12 within the range of p=80−200 MPa, and then six limit loci in the ʌ-plane corresponding to different values of p are obtained as shown in Fig. 5.12.

Fig. 5.12 Limit loci in meridian lines and the ʌ-plane

It can be seen that: 1. The strength of granite increases with increase of the hydraulic pressure p. 2. The length of vector q differs corresponding to different stress angles θ in the ʌ-plane when the hydraulic pressure p is constant. Granite shows an obvious stress angle effect. There is an obvious distinction between the circular limit loci of the Drucker–Prager criterion and the experimental results. 3. All the experimental points are located outside the limit loci of the Mohr–Coulomb yield function, and they are closer to that of the twin-shear yield function. 4. The limit meridian line changes with the stress angle. 5. In the process of varying stress angle from θ = 0° to θ = 60°, the value of q increases and reaches q = 262.2 MPa, and then decreases to q =255 MPa. This result agrees with the twin-shear stress theory.

108

5 Reasonable Choice of a Yield Function

5.7 Experiments on Clay and Loess under Complex Stress Soil is a widely used material in structural engineering and geotechnical engineering. The yield function is the basis of soil mechanics and foundation engineering. At present, the axisymmetric triaxial experiments on soil are the elementary tests in soil mechanics and have gradually developed into true triaxial experiments. The early research on failure criteria for soils under true triaxial stress states or plane strain states was done by Shibata and Karube (1965) at Kyoto University, Roscoe (1968), Roscoe and Burland (1968), Wood and Roth (1972) at Cambridge University, Ko and Scott (1967) at Colorado State University, Brown and Casbarian (1965), Sutherland and Mesdary (1969) at the University of Glasgow, Bishop (1971) and Green (1972a) at Imperial College. Fig. 5.13 indicates the experimental results for normally consolidated soil carried out by Shibata and Karube (1965). The experimental results on normally consolidated soil lie almost between the unified strength theory with b=1/4 and b=1/2. They do not agree with the Mohr-Coulomb yield function.

Fig. 5.13 Soil (Shibata and Karube 1965)

Fig. 5.14 shows the experimental results for compactive loess given by Fang in 1986. Fig. 5.15 shows the experimental results under true triaxial conditions for undisturbed loess and remolded loess given by Xing et al. at Xi’an Science and Technological University. The experimental results all agree with the unified strength theory with b=1/2.

5.8 Experiments on Sand under Complex Stress

Fig. 5.14 Compacted loess (Fang 1986)

109

Fig. 5.15 Loess (Xing et al. 1992)

Recently, the limit loci in ʌ-plane of undisturbed loess soils is obtained by Yoshimine et al. at Tokyo Metropolitan University, Tokyo, Japan. It is shown in Fig.5.16. It is in agreement with the twin-shear strength theory or the unified strength theory with b=1.

Fig. 5.16 Loci in ʌ-plane of undisturbed loess soils (Yoshimine et al. 2004)

5.8 Experiments on Sand under Complex Stress A well-known experiment on sand was carried out by Green and Bishop (1969). Fig. 5.17 shows the experimental results. Fig. 5.18 shows the dynamic strength for sand obtained by Zhang and Shao (1988). The results are close to the unified strength theory with b=3/4 and b=2/3, respectively.

110

5 Reasonable Choice of a Yield Function

Fig. 5.17 Sand (Green and Bishop 1969)

Fig. 5.18 Dynamic strength of sand (Zhang and Shao)

Fig. 5.19 shows the comparison between the unified strength theory (b=3/4) with experimental limit locus in the ʌ-plane for sand obtained by Nakai and Matsuoda (1983) in Japan.

Fig. 5.19 Limit locus in the ʌ-plane for Toyoura Sand (Nakai and Matsuoka)

Fig. 5.20 a, b shows the experimental results on loose sand and dense sand, given by Dakoulas and Sun (1992). The results agree with the unified strength theory with b=1/2 and b=3/4, respectively.

5.8 Experiments on Sand under Complex Stress

(a) loose sand

111

(b) dense sand

Fig. 5.20 Limit loci for Ottawa fine sand: (a) loose sand; (b) dense sand (Dakoulas and Sun 1992)

The limit loci in the ʌ-plane for sand obtained by Ko and Scott (1968) are shown in Figs. 5.21. The results agree with the unified strength theory with b=1/2.

Fig. 5.21 Limit locus in the ʌ–plane for medium sand (Ko and Scott 1968)

Fig. 5.22 shows the static and dynamic strength for saturated sand under complex stress states obtained by Zhang and Shao (1988).

112

5 Reasonable Choice of a Yield Function

Fig. 5.22 Static and dynamic limit loci for saturated sand (Zhang and Shao 1988)

These experimental data are situated between the limit loci of the unified strength theory with b=1/2 and b=1.

5.9 Reasonable Choice of a Yield Function for SD- Materials It is difficult to choose an appropriate failure criterion for SD (Strength Difference in tension and in compression) materials. The unified strength theory (unified strength theory) establishes a clear and simple relation among the various yield criteria. It also provides a method to choose the appropriate yield criterion. The reasonable choice method can be obtained from the unified strength theory as follows. First, we need know the tensile strength σ t and compressive strength σ c ; Second, the ratio α =σ t /σ c , i.e. the ratio of tensile strength σ t to compressive strength σ c, can be determined Third, if the ratio α =σ t /σ c=1, it means that the tensile strength equals the compressive strength. We can use the unified yield criterion and choose a resonable parameter b, as described in section 5.3 this chapter. At last, if the ratio α =σ t /σ cĮ1, or σ t Į σ c, it is the material with SD effect (effect of Strength Difference in tension and in compression). We have to use the two-parameters yield function. The unified strength theory can be used as a two-parameters yield function. The mathematical equation is expressed as follows:

when σ 2 ≤ σ 1 + α σ 3 1+α

(5-9a)

σ1 +α σ 3 1 (σ1 + bσ 2) −ασ3 = σ t, when σ 2 ≥ 1 +α 1+ b

(5-9b)

F = σ1 −

F'=

α

1+ b

(bσ 2 + σ 3) = σ t,

5.10 The Beauty of the Unified Strength Theory

113

It is linear and simple. The difficulty is how to choose the failure criterion parameter b. A method is using the true triaxial test for every material, however, it is expensive and difficult. One simple method is choosing the intermediate value of b, which is a mediated criterion between the lower bound (the Mohr-Coulomb strength theory) and upper bound (the twin-shear strength theory). The mathematical equation is also linear and simple, it is shown as follows: F = σ1 −

α

3

(σ 2 + 2σ 3 ) = σ t , σ 2 ≤

σ1 + ασ 3

1+α

1 σ +ασ 3 F′ = (2σ1 +σ 2 ) −ασ 3 = σ t , σ 2 ≥ 1 3 1+ α

(5-10a)

(5-10b)

This is a new failure criterion deduced from the unified strength theory with b=1/2. Since the Drucker–Prager criterion cannot match with the practice, this criterion is more reasonable and can be substituted for the Drucker–Prager criterion. According to the experimental data described in sections 5.4 to 5.8. The strength theory parameter b can be recommended as follows: b=1/2 to b=1 for concrete, rock and high strength steel and alloy; i.e. 1/2 ≤ b ≤ 1 b=1/4 to b=3/4 for soils and soft rock, i.e. 1/4 ≤ b ≤ 3/4.

5.10 The Beauty of the Unified Strength Theory What is the beauty of a thing? Beauty is the qualities that give pleasure to the senses or lift up the mind or spirit (Longman Dictionary of Contemporary English 1978). Beauty is the combination of qualities that give pleasure to the senses or to the moral sense or the intellect (The Oxford Advanced learner’s Dictionary of Current English 1963). A thing of beauty is a joy for ever (Keats, John 1795–1821). What is the beauty of science? Six elements of the beauty of mathematics and physics were described by Tzanakis (1997), Kosso (1999), Shen (2004) and others. Six relevant points about the beauty of mathematics and physics are: (a) Clarity: the conceptual clarity in the foundations and the development of a theory. (b) Simplicity, Elegant and economic reasoning. It is also said that: “Science advocates simplicity” (Shen ZJ 2004). (c) Unification of a priori unrelated concepts, methods, theories or phenomena. (d) The “naturality” of a theory. (e) Symmetry. (f) Analogy The beauty of the unified strength theory was first proposed and studied by Fan, et al. (2001) of Nanyang Technological University in Singapore. Fan, et al. (2001) a lecture at an International Congress on Computational Mechanics held at Sydney in 2001, Australia. The power and unification of the unified strength theory are discussed.

114

5 Reasonable Choice of a Yield Function

A closing lecture was delivered by Yu et al. at the International Symposium on the Developments in Plasticity and Fracture, Centenary of M.T.Huber Criterion, in Cracow, Poland (Yu et al. 2004). The Beauty of Strength Theories was discussed. The unified strength theory was derived based on the concept of multiple slip mechanism and the multi-shear element model or twin-shear element. Multi-shear element and twin-shear element are spatial equipartition available for continuum mechanics, which are shown in Fig. 5. 23.

Fig. 5.23 Multi-shear element and twin-shear element

It is obvious that this element model is different from the principal stress element used in common continuum mechanics. There are three sets of principal shear stress and normal stress acted on the sections, on which the principal shear stress is acted respectively. However, there are only two independent components in three principal shear stresses, because the maximum shear stress τ 13 equals the sum of the other two, i.e. τ 13 = τ 12 + τ 23 . Considering the two larger principal shear stresses and the corresponding normal stress and their different effects on failure of materials, the mathematical modeling of the unified strength theory can be formulated as (Yu-He 1991; Yu 1992, 1994) F = τ13 + bτ12 + β (σ 13 + bσ 12 ) = C , when τ12 + βσ 12 ≥ τ 23 + βσ 23

(5-11a)

F ' = τ13 + bτ 23 + β (σ 13 + bσ 23 ) = C , when τ12 + βσ 12 ≤ τ 23 + βσ 23

(5-11b)

where b is a coefficient of the effect of the other principal shear stresses on the strength of materials. Introducing a tension-compression strength ratio α = σ t σ c . The unified strength theory is expressed in terms of three principal stresses as follows F = σ1 − F '=

α (bσ + σ ) = σ t, 1+ b 2 3

when σ 2 ≤ σ 1 +ασ 3 1 +α

σ 1 +α σ 3 1 (σ1 + bσ 2 ) −ασ3 = σ t , when σ 2 ≥ 1 +α 1+ b

(5-12a)

(5-12b)

5.10 The Beauty of the Unified Strength Theory

115

The mathematical expression of the unified strength theory is simple and linear, but it has rich and varied contents, and can be easily changed to suit many new conditions. It possesses fundamentally all the expected characteristics for a unified strength theory. A series of limit loci of the unified strength theory on the deviatoric section are shown in Fig. 2 and Fig. 3 in Preface of this book. Several characteristics of the unified strength theory are discussed as follows: (1) Linearity and Simplicity

It is physically meaningful and can be expressed by mathematically simple equation. The formulation of the unified strength theory is linear and convenient to use in applications to analytical solution of plasticity and plastic analysis of structure and computational implementation for numerical solution. (2) Unification

According to Tzanakis (1997) one of six relevant points about the beauty of mathematics and physics is unification of a priori unrelated concepts, methods, theories or phenomena. All the yield criteria and failure criteria are single criterion having various model and expression. The limiting loci of the unified strength theory cover all regions from the Mohr-Coulomb theory to the twin-shear strength theory. The unified strength theory is not a single criterion. It is a series of failure criteria, a system of strength theory. This theory gives a series of new failure criteria, establishes a relationship among various failure criteria, and encompasses previous yield criteria, failure models and other smooth criteria or empirical criteria as special cases or linear approximations. The famous Tresca yield criterion, the Mohr-Coulomb strength theory, the twin-shear yield criterion, the twin-shear strength theory and some others are special criteria of the unified strength theory. The unification can be seen from Figs. 2 and 3 in the Preface and Fig. 4.22 in Chapter 4. The relation among the single-shear theory, the twin-shear theory and a series of new failure criteria can be seen in Fig. 5.24.

116

5 Reasonable Choice of a Yield Function

0 < b π / 2 is in a plane strain state. Boundary surface AE subjected to uniform pressure q, as shown in Fig.8.13. Determine the limit load puni on the surface AB. The slip lines field is illustrated in Fig.8.13. The twin-shear limit load can be expressed as follows. It was given by Zhang,Li and Yin in 1998. π ϕt ) ⋅ exp[ (2γ −π )tgϕt ] − Ct ⋅ ctgϕt 4 2

(8-51)

4sinϕ0 2+ (1+ sinϕ 0)

(8-17)

pt = (q + Ct ⋅ ctgϕt ) ⋅ tg2 ( +

where sinϕt =

Ct = 4C 0 ⋅cosϕ 0 1 , 2 + (1+sin ϕ 0)cosϕt

(8-18)

When q=ıt, the relation between limit loads pt and the ratio of tensile strength to compressive strength of material is shown in Fig. 8.14.

Fig. 8.13 Slip field of obtuse wedge

Fig. 8.14 Limit loads for different materials

8.6 Twin-shear Slip Line Field Theory for Plane Strain Problams

215

When q=0, it is a slope problem. The twin-shear limit load is π ϕt ) ⋅ exp [ (2γ − π )tgϕ t ] − Ct ⋅ ctgϕ t 4 2

pt = (Ct ⋅ ctg ϕt ) ⋅ tg2 ( +

(8-52)

When ĳt=ĳ0, it is the solution for the Mohr-Coulomb maerial. When ĳt=ĳ0=0, it is the solution for the twin-shear material in Į=1. The limit load is π 2

4 3

(8-53)

pt = (1 − + γ )σs

When ĳt=ĳ0=0, and Ct=C0, it is the conventional solution of the Tresca material. π 2

(8-54)

pt = (1 − + γ )σs

8.6.4. Example 4: Acute wedge The twin-shear solution for an acute wedge was obtained by Zhang, Li and Yin in 1998. The acute wedge with angle ∠BAD γ = < π / 2 is in a plane strain state, where ∠ BAC =δ , ∠CAD = ν , and δ + ν =γ . Boundary surface AD is subjected to uniform pressure q, as shown in Fig. 8.15. Determine the limit load pt on the surface AB. The slip lines field is illustrated in Fig. 8.15. The discontinuous line is denoted by AC, which divides the wedge into two regions. The angles between slip Į lines and ȕ lines are 2ȥ. The external load pt is assumed greater than pressure q, then the region ABC (Region I) is a active region. The twin-shear limit load can be expressed as follows: pt = (q + Ct ⋅ ctgϕ t ) ⋅

1 + sin ϕ t sin 2ν ⋅ − Ct ⋅ ctgϕt 1 − sin ϕ t sin 2δ

(8-55)

where ĳt and Ct are the same as those of obtuse wedge (Example 3). When q=ıt, the relation between limit loads pt and the ratio of tensile strength to compressive strength of material is shown in Fig. 8.16.

216

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Fig. 8.15 Slip field of obtuse wedge

Fig. 8.16 Limit loads for different materials

When q=0, it is a slope problem. The twin-shear limit load is pt = (Ct ⋅ ctgϕt ) ⋅

1 + sin ϕ t sin 2ν ⋅ − Ct ⋅ ctgϕ t 1 − sin ϕ t sin 2δ

(8-56)

When ĳt=ĳ0, it is the solution for the Mohr-Coulomb material. When ĳt=ĳ0=0, it is the solution for the twin-shear material in Į=1. The limit load is 4 3

pt = (1− cosγ )σs

(8-57)

When ĳt=ĳ0=0, and Ct=C0, it is the conventional solution of the Tresca material. pt = (1− cosγ )σs

(8-58)

8.6.5. Example 5: Earth Pressure Lateral earth pressure problem is one of important problems in soil mechanics, as shown in Figs. 8.17 and 8.18. Earth pressure problem deals with the magnitude and distribution of lateral earth pressure between a soil mass and an adjoining earthretaining structure. The classical theories on earth pressure are those due to Coulomb (1773) and Rankine (1857). Fig. 8.17 shows a passive earth pressure problem. Fig. 8.18 shows a active earth pressure problem.

8.6 Twin-shear Slip Line Field Theory for Plane Strain Problams

Fig. 8.17 Active earth pressure

217

Fig. 8.18 Passive earth pressure

This problem is also considered as a limit load problem of a slope. The top and the slope side can be looked upon as the limit load problem of wedge, as show in Fig. 8.19a ( γ ≥ π / 2 ) and Fig. 8.19b ( γ ≤ π / 2 ). The weight of soil is not taken into account.

Fig. 8.19 Earth pressure (a) ( γ ≥ π / 2 ) and (b) ( γ ≥ π / 2 )

The active earth pressure can be derived in the case of q >E and γ ≥ π / 2 as follows: π

ϕt

4

2

Eactive = ( q + Ct ⋅ ctgϕ t) ⋅ tg2( +

) ⋅ exp[(π

− 2γ ) ⋅ tgϕ t] − Ct ⋅ ctgϕ t

(8-59)

The passive earth pressure can be derived in the case of E > q and γ ≥ π / 2 as follows: π ϕt ) ⋅ exp[ (2γ − π )tgϕ t ] − Ct ⋅ ctg ϕ t 4 2

pt = (q + Ct ⋅ ctgϕt ) ⋅ tg2 ( +

(8-60)

The active earth pressure can be derived in the case of q >E and γ ≤ π / 2 as follows: pt = (q + Ct ⋅ ctgϕ t ) ⋅

1+ sinϕ t sin2δ ⋅ − Ct ⋅ ctgϕt 1−sinϕ t sin 2δ

(8-61)

218

8 Twin-Shear Slip-Line Field for Plane Strain Problem

The passive earth pressure can be derived in the case of E >q and γ ≤ π / 2 as follows: 1 + sinϕ t sin2ν ⋅ − Ct ⋅ ctgϕt pt = (q + Ct ⋅ ctgϕ t )⋅ 1 − sinϕ t sin2δ

(8-62)

It is the same as Eq.8-55

Summary The twin-shear slip line field theory for plane strain problems based on the twinshear yield function is described in this chapter. The twin-shear slip line field theory for plane strain problems includes orthogonal and non-orthogonal slip line field. It is different from the used orthogonal or non-orthogonal slip line field theories based on single-shear strength theories (Tresca and Mohr-Coulomb materials). The new method can reflect the effect of intermediate principal stress of plane strain, where the intermediate principal stress is the principal stress in z direction. The twin-shear slip theory can be used for those materials with obvious effect of the intermediate principal stress. Five examples are used to illustrate the applications of the twin-shear slip lines field.

Problems Problem 8.1 The extension of a strip with a sufficiently large circular hole for non-SD material was studied by Prager and Hodge (1951) and Kachanov (1971) as shown in Fig. P8.1. The Tresca yield criterion was used in these studies. Can you obtain another study on this subject using the twin-shear slip line field for non-SD material ( α = 1 )?

Fig. P8.1 Extension of a strip with a sufficiently large circular hole

Problems

219

Problem 8.2 Can you obtain a more complete study on the extension of a strip with a sufficiently large circular hole (Fig. P8.1) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.3. The extension of a strip with ideal cuts (crack) for non-SD material was given by Kachanov (1971) as shown in Fig. P8.2. The Tresca yield criterion was used in these studies. Can you obtain a more complete study on this subject using the twinshear slip line field for non-SD material ( α = 1 )?

Fig. P8.2 A ideal cuts (crack)

Fig. P8.3 An angular notches

Problem 8.4. Can you obtain a more complete study on the extension of a strip with ideal cuts (Fig. P8.2) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.5. The extension of a strip with angular notches for non-SD material was given by Kachanov (1971) as shown in Fig. P8.3. The Tresca yield criterion was used in the studies. Can you obtain a more complete study on this subject using the twin-shear slip line field ( α = 1 )? Problem 8.6. Can you obtain a more complete study on the extension of a strip with angular notches (Fig. P8.3) by using the twin-shear slip line field for SD materials (α ≠ 1 )? Problem 8.7. The extension of a strip with circular base for non-SD material was given by Kachanov (1971) as shown in Fig. P8.4. The Tresca yield criterion was used in the studies. Can you obtain a more complete study on this subject using the twin-shear slip line field ( α = 1 )?

220

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Fig. P8.4 Extension of a strip with a circular base

Problem 8.8. Can you obtain a more complete study on the extension of a strip with circular base (Fig. P8.2) by using the twin-shear slip line field for SD materials ( α ≠ 1 )? Problem 8.9. Figure P8.5 shows the slip line field of indentation at the bottom of a flat trench. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.5 Flat trench

Fig. P8.6 Deep vertically sided

Problem 8.10. Figure P8.5 shows the slip line field of indentation at the bottom of a flat trench. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.11 Figure P8.6 shows the slip line field of indentation at the foot of a very deep vertically sided groove. Find the limit load by using the twin-shear slip line field ( α = 1 ). Problem 8.12. Figure P8.6 shows the slip line field of indentation at the foot of a very deep vertically sided groove. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ).

Problems

221

Problem 8.13 Figure P8.7 shows the slip line field of indentation at the top of a flat punch. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.7 Indentation at the top of a flat punch

Problem 8.14. Figure P8.7 shows the slip line field of indentation at the top of a flat punch. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.15. Pure bending of a strip weakened by notches of various shapes was investigated by Green (1953) and Kachanov (1971). Fig. P8.8 shows the slip line field of a strip weakened by one-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field ( α = 1 ).

Fig. P8.8 Strip weakened by one-sided deep notch with a circular base

Problem 8.16. Figure P8.8 shows the slip line field of a strip weakened by one-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ).

222

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Problem 8.17. Figure P8.9 shows the slip line field of a strip weakened by two-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α = 1 ).

Fig. P8.9 Strip weakened by two-sided deep notch with a circular base

Problem 8.18. Figure P8.9 shows the slip line field of a strip weakened by two-sided deep notch with a circular base. Find the limit load by using the twin-shear slip line field for SD materials ( α ≠ 1 ). Problem 8.19. Figure P8.10 shows a slip line field of a strip weakened by center crack for non-SD materials. Find the slip line field for SD materials.

Fig. P8.10 shows a slip line field of a strip weakened by center crack

Problem 8.20. Figure P8.11 shows the slip line field of a strip with a hole; find the limit pressure for non-SD materials and SD materials.

References and Bibliography

223

Fig. P8.11 Slip line field of a strip with a hole

Problem 8.21. The slip line field and limit pressure were widely studied by some researchers. Figure P8.12 shows the slip line field around a circular hole loaded uniformly with a pressure, find the limit pressure for non-SD materials and SD materials by using the twin-shear slip line field theory.

Fig. P8.12 Slip line field around a hole

References and Bibliography Collins IF (1990) Plane Strain Characteristics Theory for Soils and Granular Materials with Density Dependent Yield Criteria, J. Mech. Phys. Solids., 38(1), 1–25 . Collins IE and Dewhurs, P (1993) A matrix technique for constructing slip-line field solutions to a class of plane-strain plasticity problems. Int. J. Numer. Methods Eng., 7: 357–378. Drucker DC, Greenberg HJ and Prager W (1951) The safety factor of an elastic-plastic body in plane strain. J. Appl. Mech., 18: 371–378. Ford H (1954) The Theory of Plasticity in Relation to Engineering Application. J. AppL Math. Phys., 5: 1–35.

224

8 Twin-Shear Slip-Line Field for Plane Strain Problem

Geiringer H (1930) Beit zum Vollstiindigen ebenen Plastizitits-problem, Proc 3rd Intern. Congr. Appl. Mech, 2: 185–190. Hencky H (1923) Ueber einige statisch bestimmte Faelle des Gleichgewichts in plastischen Koerpern, Z. angew. Math Mech., 3: 245–251. Hill R (1949) The Plastic Yielding of Notched Bars Under Tension, Quart. Mech. AppL Math., 2: 40–52. Hill R (1956), The Mechanics of Quasi-Static Plastic Deformation in Metals, In: Survey in Mechanics, G. K. Batcheler and R. M. Davis eds, Cambridge . Johnson W and Mellor PB (1962), Plasticity for Mechanical Engineers. Van Nostrand, Princeton, N.J. Johnson W, Sowerby R, Venter RD (1982), Plane-Strain Slip Line Fields for Metal Deformation Processes – A Source Book and Bibliography, Pergamon Press . Matsuoka H (2000) Soil Mechanics. Nagoya Technical Institute Press: Nagoya. (in Japanese; Chinese translation, 2004 by Yao NP and Lou T ) Moore ID and and Rowe RK (1991) Objective solutions for bearing capacity of strain-softening soils. In: Beer G, Booker JR and Carter JP eds. Computer Methods and Advances in Geomechanics. Rotterdam: A.A.Balkema, Vol.2,1183–1189. Prager W (1955) The Theory of Plasticity: A Survey of Recent Achievements. Proc. Inst. Mech. Eng., 169: 41–57. Prager W (1959) Introduction to Plasticity. Addison-Wesley, Reading, Mass. Prager W and Hodge P G Jr (1951) Theory of Perfectly Plastic Solids. Wiley, New York. Prandtl L (1920) l~ber die H~irte Plastischer Koerper, Goettinger Nachr., Math. Phys. KI., 74–85. Thomsen EG, Yang CT and Kobayashi S (1965) Mechanics of Plastic Deformation in Metal Processing. Macmillan, New York. Yu MH (1983), Twin Shear Stress Criterion, Int. J. of Mech. Sci., 25(1), 71–74 . Yu MH, He LN and Song, LY (1985), Twin Shear Stress Theory and Its Generalization, Scientia Sinica (Science in China), Series A, (English edn.), 28(11), 1174–1183. Yu MH and He LN (1991), A new model and theory on yield and failure of materials under complex stress state. In: Mechanical Behaviour of Matterials-VI, Pergamon, Oxford, Vol.3: 841–846. Yu MH, Liu CY and He LN (1992), Generalized Twin Shear Stress Yield Criterion and Its Generalization, Chinese Science Bulletin (English edn.), 37(24), 2085–2089. Yu Mao-hong, et al (1992), Computer Image Analysis of the Plastic Zone of Structure, Journal of Xi’an Jiaotong University, 26(2), 121–122 (in Chinese). Yu MH, Liu JY and Ma Guo-wei (1994), Twin-shear slip line theory: orthogonal and nonorthogonal slip line fields. Journal of Xi’an Jiaotong University, 28(2):122–126. Yu MH, Yang SY, Liu CY and Liu JY (1997) Unified plane-strain slip line theory. China Civil Engrg. J. 30(2), 14–26 (in Chinese, English abstract). Zhang YQ, Li JC and Yin ZN (1998) Application of twin-shear strength theory in wedge’s limit analysis. In: Yu MH and Fan SC eds: Strength Theory: Application, Development and Prospect for the 21st Century, New York, Beijing: Science Press, 1998, 1155 –1160.

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.1 Introduction The twin-shear slip line field theory based on the twin-shear yield criterion and generalized twin-shear criterion for plane strain problems has been described in Chapter 8. Most available slip line field theories for plane strain problems are based on the one of single yield function such as the Tresca criterion (Maximum shear stress criterion), the Mohr-Coulomb strength theory (single-shear criterion), the Hubervon Mises criterion, the twin-shear yield criterion and the generalized twin-shear strength theory. These kinds of slip line field theories can be used only for one kind of material, respectively, such as the Tresca material, the Mohr-Coulomb material, the Hubervon Mises material and the twin-shear material. The adaptability of various slip fields are illustrated in Table 9.1. Table 9.1 The adaptability of various slip fields

Applications of slip line fields theory Tresca slip line For ϕt = ϕ 0 = 0 and For σt = σc materials field τ = o ,5σ materials Orthogonal slip field

Slip line fields

s

Orthogonal slip Mises slip field line field

s

For ϕt = ϕ0 = 0 and

For σt = σc materials

τs = o,577σs materials

Orthogonal slip field

Twin-shear slip line field

For ϕt = ϕ0 = 0 and

For σt = σ c materials

τs = o,667σ s material

Orthogonal slip field

Mohr-Coulomb slip field

For ϕt ≠ ϕ0 ≠ 0 , i.e.

For σt ≠ σc materials

α ≠ 1 materials For ϕt > ϕ0 ≠ 0 , i.e.

Non-orthogonal slip For σt ≠ σc materials

Non-orthogonal Generalized slip field twin-shear slip field

α ≠ 1 materials

Non-orthogonal slip field

226

9 Unified Slip-Line Field Theory for Plane Strain Problem

It is seen that the single slip field theory can not be adapted for other kinds of materials. No relations among these slip field theories are available. In order to solve the above mentioned problems, the unified strength theory (Yu 1991) was used to extend the slip line field theory for plane strain problem by Yu-Yang-Liu in 1997. A new system of orthogonal and non-orthogonal unified slip line field theory for plane strain problems was proposed and developed. Various orthogonal and non-orthogonal plane strain slip line field theories based on different strength theories, such as the Tresca criterion, the Huber-von Mises criterion, the twin-shear yield criterion, the Mohr-Coulomb theory, and the generalized twin-shear strength theory, are special cases or linear approximation (Huber-von Mises) of the unified slip line field theory. Besides, a series of new unified slip line field can be introduced by different choice of strength criterion parameter b of the unified slip line field theory.

9.2 Unified Strength Theory in Plane Strain Condition The stress state of plane strain structure is the same as the description in chapter 8. The main results are expressed as follows: ε z = ε xz = ε yz = τ xz = τ yz = vz = 0 ,

(9-1)

z is a principal direction, and ız is a principal stress. The stress component in plane strain state have only four streses components ıx, ıy, Ĳxy and ız. The maximum principal stress ı1 and minimum principal stress ı3 (ı1 ı2 ı3) of plane strain problem are σ1

= σmax

σ3

=

σ min

=

σx + σy

2

2

§σ σ · ± ¨ x− y¸+ © 2 ¹

2

τ xy

(9-2)

Introducing a parameter m, the intermediate principal stress ı2 can be expressed as

σ2 =

m 2

(σ1 + σ3),

(9-3)

where m is the intermediate principal stress state parameter, 0 < m ≤ 1 for plane strain problem. The intermediate principal stress state parameter m can be determined by both theoretical and experimental analysis. Generally, m < 1 for elastic region, i.e. ız = m(ı1 + ı3)/2 < (ı1 + ı3)/2; and mė1 for plastic region. The stress state of plane strain can be expressed by two new variations R and p

9.2 Unified Strength Theory in Plane Strain Condition

p=

1 1 1 1 (σ 1 + σ3 ) = (σ x + σ y ) = σ 2 = σ z , m m 2 2

1

§ σ1 − σ3 = ¨ © 2

R=

227

σ x − σy

2

(9-4)

2

· 2 ¸ + τ xy , ¹

(9-5)

The relations between these stresses are σx = p + R cos 2θ σy = p − R cos 2 θ τ xy = R sin 2θ

(9-6)

= ( p + C 0 ⋅ cot ϕ ) sin ϕ ⋅ sin 2 ϕ

where © denote the angle from x coordinate to the direction of ı1. The mathematical formulae of the unified strength theory can be expressed in two equations as follows:

F = σ1 − F ′=

1 1+ b

α

1+b

( b σ 2 + σ3 ) = σ t , when

σ2 ≤

σ1

(σ1 + bσ2 ) − α σ3 = σ t , when σ2 ≥

+

α σ3

1+α σ + ασ 1 3

1+α

,

(9-7a) ,

(9-7b)

Where ıt and ıc are uniaxial tensile and compressive strength of material respectively. Material parameter α = ıt /ıc is tensile-compressive strength ratio, which reflects material's Strength Difference (SD) effect. It is seen from Eq (9-4) that b reflects the effect of intermediate principal stresses on the yield of materials. The unified strength theory can also be expressed in terms of shear strength parameter C0 and friction angle ĳ0 as follows:

F = [σ 1 −

or

1 1+ b

b (σ 2 + σ 3 )] + [σ 1 +

1

(b σ 2 + σ 3 )] sin ϕ 0 = 2 C 0 ⋅ cos ϕ 0 1+ b σ +σ σ −σ when σ 2 ≤ 1 3 + 1 3 sin ϕ 0, 2 2

when σ 2 ≤ p + R sin ϕ 0

F' =[

1 1+ b

(σ 1 + bσ 2 − σ3 ] + [

1 1+ b

(σ 1 + bσ2 ) + σ 3 ] s in ϕ 0 = 2C 0 ⋅ co s ϕ 0

(9-8a)

228

9 Unified Slip-Line Field Theory for Plane Strain Problem

when σ2 ≥

σ1 + σ3 σ1 − σ3 + sin ϕ0 , 2 2

when σ 2 ≤ p + R sin ϕ 0

or

(9-8b)

The unified strength theory can consider the different effects of the intermediate principal stress for different materials. It establishes the relations among available strength theories, and creates a series of new yield criteria. Because the intermediate principal stress equals σ 2 = mp ≤

p + R sin ϕ 0 =

1 2

(σ 1 + σ 3) +

1

(σ 1 − σ 3 ) sin ϕ 0 ,

2

(9-9)

it accords with the first expression of the unified strength theory Eq (9-8). Combining Eqs (9-8a), (9-5) and (9-6), we get

R=

2(1 + b ) C0 ⋅ cos ϕ 0 2 + b (1 + sin ϕ 0 )

+

b (1 − m ) + (2 + b + bm ) sin ϕ 0 2 + b (1 + sin ϕ 0 )

(9-10)

p

where the compressive stress is usually defined positive. We introduce two new parameters ĳuni and Cuni (Yu et al. 1997) as follows:

sin ϕ uni =

b (1 − m ) + ( 2 + b + bm ) sin ϕ 0

sin ϕ uni = Cuni =

2 + b (1 + sin ϕ 0 ) 2 (b + 1) sin ϕ 0 2 + b (1 + sin ϕ 0 ) 2 ( b + 1) C0 ⋅ cos ϕ 0

1

2 + b (1 + sin ϕ 0 )

cos ϕ uni

,

when m Į 1,

(9-11a)

when m = 1,

(9-11b) (9-11c)

The parameters ĳuni and Cuni are referred to as the unified friction angle and the unified cohesion, respectively. The relations of Cuni∼ b and ¶uni∼ b for different ĳ0 are shown in Fig. 9.1 and Fig. 9.2, respectively.

9.2 Unified Strength Theory in Plane Strain Condition

229

Cuni/c0

Fig. 9.1 Relation between unified cohesion Cuni and b

¶uni

Fig. 9.2 Relation between unified friction angle ĳuni and b

Substituting Eqs (9-11) into Eq (9-10), the equation of the unified strength theory for plane strain problem can be rewritten as

230

9 Unified Slip-Line Field Theory for Plane Strain Problem

R = p sin ϕ uni + Cuni cos ϕ uni ,

(9-12)

It is the new expression of the unified strength theory for plane strain condition.

9.3 Unified Slip Line Field Theory for Plane Strain Problem (Statically Admissible Field) Under plane strain condition, some restrictions as εz = d ε z = γ zx = d γ zx = γ zy = d γ zy = 0

(9-13)

The plane strain equilibrium differential equations can be written as (see: Hill 1950 or Johnson and Mellor 1962)

∂σ x ∂τ yx + = γ sin θ 0 ∂x ∂y

∂τ xy ∂x

+

∂σ y ∂y

(9-14)

= − γ cos θ 0

in which ¤ is specific weight and ș0 is the angle between the direction of gravity and the minus direction of y coordinate, as shown in Fig. 9.3.

Fig. 9.3 Stress state in any point of plane strain slip line field (dxė0, dyė0)

Solving Eqs (9-9), (9-11), and (9-12), the stress governing equations are obtained as follows:

9.3 Unified Slip Line Field Theory for Plane Strain Problem

231

b(1 − m) + (2 + b + bm)sin ϕ 0 ∂p ∂p b(1 − m) + (2 + b + bm)sin ϕ 0 (1 + cos 2θ ) + sin 2θ + ∂x 2 + b(1 + sin ϕ 0) ∂y 2 + b(1 + sin ϕ 0) ∂θ ∂θ cos 2θ − sin 2θ ) = γ sin θ 0 ∂y ∂x b(1 − m) + (2 + b + bm)sin ϕ0 ∂p b(1 − m) + (2 + b + bm)sin ϕ0 ∂p sin 2θ + (1 − cos 2θ ) + 2 + b(1 + sin ϕ0 ) 2 + b(1 + sin ϕ0 ) ∂x ∂y +2R(

+ 2 R(

∂θ ∂θ cos 2θ + sin 2θ ) = −γ cos θ 0 ∂x ∂y (9-15)

Equation (9-15) satisfies the unified strength theory (Eq. 9-10), and plane strain static equilibrium equations (Eq. 9-14). Equation (9-15) may be elliptic-type (two different real roots), parabolic-type (two same real roots) or hyperbolic-type (no real roots) pseudo-linear differential equations which can be solved by the method of characteristics

dy = tg (θ − µ) , dx dy £ family: = tg (θ + µ), dx

α family:

(9-16a) (9-16b)

in which µ =

π

4

−

ϕ uni .

2

We can see that the equations are elliptic-type pseudo-lineal differential equations. Equation (9-15) has not only two different real roots of the pseudolinear equation (9-14), but also two characteristic lines at the angle of 2 with each other. Substituting Eq.9-11 into Eq.9-15, the governing equations (9-15) change to

∂p ∂p ∂θ ∂θ (1 + sin ϕ uni⋅ cos 2θ ) + sin ϕuni ⋅ sin 2θ + 2R( cos 2θ − sin 2θ ) = γ sin θ 0 ∂x ∂y ∂y ∂x (9-17) ∂p ∂p ∂θ ∂θ sin ϕ uni⋅ sin 2θ + (1 − sin ϕ uni⋅ cos 2θ ) + 2R( cos 2θ + sin 2θ ) = −γ cosθ 0 ∂x ∂y ∂x ∂y It is interesting that Eq. (9-17) is similar to the conventional equation. It is only the substitution of Cuni and ĳuni for C0 and ĳ0. This substitution embodies the effect of yield criterion parameter b of the unified strength theory in an implicit way, builds the linkage of different slip line field theories and reflects

232

9 Unified Slip-Line Field Theory for Plane Strain Problem

the regular effect of intermediate principal stress in this new unified slip line field theory. The unified slip lines field theory can be degenerated to orthogonal and nonorthogonal theories based on the Tresca critereion (α=1,b=0), the Huber-von Mises criterion (α=1, b=1/2), the twin Shear criterion (α=1, b=1), the Mohr-Coulomb criterion (b=0) and the generalized twin shear criterion (b=1). Moreover, when we choose other values of parameter b, a series new theories can be introduced. Hence, the unified strength criterion parameter b can also be regarding as a parameter of choosing for yield function. In this section, the curvilinear coordinate system Sα and Sȕ coinciding with the slip lines α and β is choosed, as shown in Fig. 9.4.

Fig. 9.4 Stress state in any point of plane strain slip line field

According to the rules of directional derivative, the stress governing equations, Eq. (9-17), can be expressed in curvilinear coordinates Sα and Sȕ

α family: − sin 2 µ

∂p ∂ Sα

+ 2R

∂θ ∂ Sα

+ γ [sin(θ 0 + 2 µ )

∂x ∂ Sα

+ cos(θ 0 + 2 µ )

∂y ∂ Sα

] = 0 (9-18a)

β family: sin 2 µ

∂p ∂ Sβ

+ 2R

∂θ ∂ Sβ

+ γ [sin(θ 0 − 2 µ )

∂x ∂ Sβ

+ cos(θ 0 − 2 µ )

∂y ∂ Sβ

] = 0 . (9-18b)

Equations (9-17) and (9-18) are the stress governing equations (statically admissible) of the unified slip line field theory for plane strain problem. The equations differ from ordinary stress governing equations by substituting Cuni and ĳuni for C0 and ĳ0.

9.3 Unified Slip Line Field Theory for Plane Strain Problem

233

9.4. Unified Slip Line Field Theory for Plane Strain (Kinematically Admissible Field) In this section, the associated flow rule is adopted, namely

∂g

p

dε ij = d λ

= dλ

∂σ ij

∂f

,

∂σ ij

(9-19)

where the potential function is the equation of unified strength theory, which can be expressed as

1 1 f = (σ x + σ y )sin ϕuni − (σ x − σ y )2 + τ xy2 + Cuni ⋅ cos ϕuni = 0 , 2 4

(9-20)

The plastic strain rates under small deformation and rigid plastic condition can be obtained by ε&x =

ε& y =

γ& xy =

∂ u& x ∂ vx , = ∂x ∂x ∂ u&y ∂y

∂u& x ∂y

+

=

∂ vy

∂u& y ∂x

,

∂y =

∂v x ∂y

+

∂vy ∂x

,

(9-21)

Then we can get velocity governing equations of unified slip line field theory for plane strain problem α family:

dνα + [ν α ctg (

β family:

dνβ + [να csc(

π

2 π

2

− ϕ uni ) − νβ ⋅ csc(

π

2

− ϕ uni ) − νβ ⋅ ctg (

π

2

− ϕ uni )] dψ = 0 ,

− ϕ uni)] dψ = 0 .

(9-22a) (9-22b)

where ux and uy are displacement components, vx =du x /dt and vy =duy /dt are velocity components along x and y directions, whereas vα and vȕ are velocity components along α and β slip lines, respectively. Superimposed dot means derivative with respect to time.

234

9 Unified Slip-Line Field Theory for Plane Strain Problem

Substituting unified strength theory for plane strain into associated flue rule Eq. (9-19), and taking the rigid plastic postulate into consideration, we obtain

1 2 (σ y − σ x) ° ®sin ϕ uni + 2 ∂σ x 1 / 4 (σ x − σ y ) 2 + τ xy °¯ 1 2 (σ y − σ x) ∂f dλ ° =− dε y = − dλ ®sin ϕ uni − 2 ∂σ y 2 ° 1 4 (σ x − σ y ) 2 + τ xy ¯ τ xy ∂f dγ xy = 2 d ε xy = − 2 d λ = dλ 2 ∂ τ xy 1 4 (σ x − σ y )2 + τ x y

d ε x = − dλ

∂f

=−

dλ 2

½ ° ¾ °¿ ½ ° ¾ °¿

(9-23)

where the relation between shear strain ε xy and engineering shear strain Ȗxy , i.e., Ȗxy =2İxy , is used. The compressive normal stress is defined positive. Figure 9.5 gives the plane strain Mohr circle and the relation between the slip angles, were is the angle between α slip line and x direction, i.e. ψ = θ − µ = θ − (π / 4 − ϕ uni / 2) . Follow this definition, Eq. (9-23) can be simplified to

dλ [sin ϕ uni + sin(2ψ − ϕ uni )] 2 dλ dε y = − [sin ϕ uni − sin(2ψ − ϕ uni)] 2 d γ xy = d λ cos(2ψ − ϕ uni ) dε x = −

Fig. 9.5 Stress state and direction angle in any point of plane strain slip line field

(9-24)

9.4 Unified Slip Line Field Theory for Plane Strain

235

When the direction of slip line is along x direction, i.e. =0 (α line) or ψ = − (π 2 − ϕ uni ) (£ line), it follows from Eq. (9-24) that

dεx ψ =0 = d ε x

ψ =− (π 2 −ϕuni )

= 0

(9-25)

This equation indicates that the rigid strain rate will vanishes along slip lines. The relation in Fig. 9.5(b), i.e. the relation between velocity components along slip lines vα = u&α ( v β = u&β ) and velocity components along x (y) axis vx (vy), can be obtained by

v x = u& x =

vα sin(ψ + 2 µ ) − vβ sin ψ

v y = u& y =

sin 2 µ

.

(9-26)

vα cos(ψ + 2 µ ) − vβ cosψ − sin 2 µ

Combination of Eqs. (9-21), (9-25) and (9-26), gives,

dε x

ψ =0

= ε& x

ψ =0

dt =

∂ vx ∂x

ψ =0

dt

= { dvα + [ vα ctg ( π 2 − ϕ uni ) − vβ csc( π 2 − ϕ uni )] dψ } d t = 0

(9-27)

In the above equation, we have used the relation µ = π 4 − ϕ uni / 2 and definitions

dvα ≡ ( ∂ vα ∂ x )

ψ =0

and dψ ≡ ( ∂ ψ ∂ x ) . ψ =0

When slip line field generates plastic flow, by integrating Eq. (9-21), we can work out the velocity field that satisfies the boundary conditions of the problem. The velocity field solution complies with the unified strength theory, associated flow rule and rigid plastic small deformation condition. When ĳuni=ĳ0, which is the case of orthogonal slip line field, Eq. (9-22) can be simplified to the famous Geiringer velocity equations (Johnson and Mellor 1962)

α family: d vα − vβ dθ = 0 ,

(9-28a)

β family: dvβ + vα dθ = 0 .

(9-28b)

By now, we have extended the unified strength theory to slip line field theory for plane strain by means of the introduction of unified effective parameters: the

236

9 Unified Slip-Line Field Theory for Plane Strain Problem

unified internal cohesive Cuni and the unified friction angle ĳuni and got the governing equations of the unified slip line field theory for plane strain problem (Eqs 9-17, 9-18 and 9-22). Unified slip line field theory can be used to materials with obvious intermediate principal stress effect and give the linkage of various slip line field theories without theoretical difficulty. Moreover, the unified slip field theory contains infinite number of orthogonal and non-orthogonal slip line field theories. With the different choice of parameter (α, β, γ) or Cuni and ĳuni, we can get a series of special cases of the unified slip field theory.

9.5 Special Cases of the Unified Slip Line Field Theory 9.5.1 Case 1: ¤=0 This is the case when unified slip line field theory for plane strain problem is applied to materials where gravity is left out of consideration. In this case, velocity governing equations are the same as Eq. (9-22), whereas stress governing Eq. (9-18) can be simplified to

α family: − sin 2 µ β family: sin 2 µ

∂p ∂ Sα ∂p

∂ Sβ

+ 2R

+ 2R

∂θ ∂ Sα ∂θ

∂ Sβ

= 0,

=0

(9-29a) (9-29b)

Integrating the above equations, after simplification, we obtain

α family:

p = Cα ⋅ exp(2θ ⋅ ctg 2 µ ) − Cuni ⋅ ctg ϕ uni ,

(9-30a)

β family:

p = Cβ ⋅ exp( − 2θ ⋅ ctg 2 µ ) − Cuni ⋅ ctgϕ uni ,

(9-30b)

where Cα and Cȕ are integral constants, which will be determined by different boundary conditions. Parameters Cuni and ĳuni are defined in Eq. 9-11. This case is a new type of non-orthogonal slip line field. As an example, a strip footing of width AA and semi-infinite length carrying a uniform load on the surface of a semi-infinite, homogeneous and isotropic soil is show in Fig.9.6. The material strength parameters for the soil are C0 and ĳ0 but the unit weight is assumed to be zero. When the pressure becomes equal to the ultimate bearing capacity, the footing is pushed downwards into the soil mass

9.5 Special Cases of the Unified Slip Line Field Theory

237

producing a state of plastic equilibrium below the footing. The surface AA is assumed to be smooth.

Fig. 9.6 Slip lines field of weight-less soil under a strip footing

The slip field can be indivited into three regions with the angles AAD being (45º + ĳ /2) as shown in Fig.9.6. The downward movement of the wedge AAD forces the adjoining soil sideways, producing outward lateral forces on both sides of the wedge AAD. Passive zones AEF and AE’F’ therefore develop on both sides of the active wedge, with the angles EFA and E’F’A being (45º - ĳ /2). The transition between the downward movement of the active wedge and the lateral movement of the passive wedge takes place through zones of radial shear ADE and ADE’, and the surfaces DE and DE’ are logarithmic spirals to which the failure planes of the active and passive wedges are tangential. A state of plastic equilibrium thus exists above the surface EDF and DE’F’, and the remainder of the soil is in a state of elastic equilibrium. The following solution of limit load q is obtained by using the unified slip lines field theory. It is a new non-orthogonal slip line field system.

º ª 1 + sin ϕ uni q = C uni ⋅ ctg ϕ un i « e x p ( π t g ϕ uni ) − 1 » ¬ 1 − sin ϕ uni ¼

(9-31)

This solution differs from the traditional solutions in the substitution of Cuni and ĳuni for C0 and ĳ0, and the effect of intermediate principal stress is taken into account and establishs the relation of different solutions, as shown in Fig. 9.7 (Yang and Yu 1996).

238

9 Unified Slip-Line Field Theory for Plane Strain Problem

Fig. 9.7 Relation between limit load and unified strength parameter b of a strip footing

We can also draw the following conclusions: 1. when b=0, that is ĳuni=ĳ0 and Cuni = C0 (Eqs 9-16 and 9-17), the unified solution is simplified to the Tresca solution (α=1) or the Mohr-Coulomb solution (α Į 1). 2. when b (bĮ0) is fixed, the larger the value of ĳ0 is, the bigger the difference between the new solution and the Tresca solution (α =1) or the Mohr-Coulomb solution (α Į1) is. 3. when ĳ0 is fixed, the larger the value of b is, the bigger the difference of the two solutions is.

9.5.2 Case 2: ĳuni=0 This is the case of orthogonal unified slip line field theory for plane strain problems. Because of the perpendicularly of two families (α and £ ) of slip lines, 2 µ = π 2 − ϕuni = π 2 . In this case, it follows from Eqs (9-16) and (9-17) that ϕ uni = ϕ 0 = 0 ,

R = Cuni =

2(1 + b ) 2+b

C0 ,

α = 1.

(9-32)

Orthogonal unified slip line field theory for plane strain problem is used for nonSD materials, α =1. In another word, only this kind of materials can generate this case of orthogonal slip line field. Substituting 2µ =ʌ/2 into Eqs (9-18) and (9-22), we get the stress and velocity governing equations of this case α family

9.5 Special Cases of the Unified Slip Line Field Theory

−

∂p ∂S α

+ 2R

∂θ ∂Sα

∂x

+ γ [ cos θ 0

∂Sα

− sin θ 0

∂y ∂Sα

]=0

239

(9-33a)

dνα − νβ d θ = 0 β family

∂p ∂Sβ

+ 2R

∂θ

+ γ [ − cos θ 0

∂Sβ

∂x ∂Sβ

+ sin θ 0

∂y ∂Sβ

]= 0

.

(9-33b)

dνβ + να dθ = 0 Integrating the stress governing Eq. (9-33), we obtain

α family:

p − γ cos θ 0 x + γ sin θ 0 y − 2 Rθ = C α ,

(9-34a)

β family:

p − γ cos θ 0 x + γ sin θ 0 y + 2 Rθ = C β ,

(9-34b)

9.5.3 Case 3:

ϕ uni = 0

and ¤=0

This is the case of orthogonal unified slip line field theory for plane strain problem without consideration of gravity. From Eqs. (9-16) and (9-17), we can get the restrictions of this case ϕ uni = ϕ 0 = 0 , ∂

R = Cuni =

2 (1 + b) 2+b

C0 ,

(9-35)

γ = 0, α = 1

Substituting above equations into Eq. (9-35), we have the stress and velocity governing equations of this case

∂ ∂ Sα

( p − 2 Rθ ) = 0

,

α family

(9-36a)

β family

(9-36b)

dvα − vβ d θ = 0 ∂

∂Sβ

( p + 2 Rθ ) = 0

dv β − vα dθ = 0

.

240

9 Unified Slip-Line Field Theory for Plane Strain Problem

where the condition that R is constant with respect to Sα and Sȕ is used when material and strength theory is fixed Integrating Eq. (9-36), we can get the solutions of this case

α family:

p − 2 Rθ = Cα ,

(9-37a)

β family:

p + 2 Rθ = Cβ .

(9-37b)

where C α and C β are integral constants. Substitute ¤= 0 into Eq. (9-30), we can also get above equations. The form of Eqs (9-36) and (9-37) is similar to that of traditional solutions of orthogonal slip line field theories. But the definition of R is different. In this discussion, R is unified parameter and with different choice of yield criterion parameter b, the solution can be simplified to those of the Tresca, the Huber-von Mises and the twin-shear slip line field theories, they are: 1. b = 0, R = C 0 = σs 2 = 0.5σs , it is the Tresca solution; 2. b=1/2, R = 6/5 C 0 = 3/5 σs = 0.6σs , it is the linear approximations to the Huber-von Mises solution (exact solution is R = 1 3. b=1, R = 4 / 3C0 = 2 / 3σs = 0.667σs

3 σs = 0.58σs );

it is the solution of the twin-shear yield

criterion.

9.6 Applications of the Unified Slip Line Field Theory 9.6.1 Example 1: Trapezoid structure The trapezoid PVC specimen with a top angle 2¯ isconsidered. The uiform distributed load is applied on the top of the specimen, as shown in Fig. 9.8. The loading velocity is 1mm/min. The physical properties of the material are: Young's modules: 367.88 kN/cm2

Specific gravity: 1.35-1.45 g/cm3

Poisson's Ratio: 0.27

Tensile strength: 5.886 kN/cm2

Compressive strength: 7.575 kN/cm2 Determine the limit load.

Solution Friction angle and cohesion of this material can be determined by

9.6 Applications of the Unified Slip Line Field Theory

ϕ 0 = sin

C0 =

−1

σc − σ t = 7.208 0 σ c + σt

σ t (1 + sin ϕ 0 )

2 cos ϕ 0

241

(9-38)

= 3.339

It is assumed that the surfaces AA’ are smooth and there is no friction. It is also assumed that there is a constant pressure on the top. The rest of the boundary is stress-free.The slip line field is given in Fig.9.8.

Fig. 9.8. Slip lines field of a trapeziod structure (Yu 1998)

The slip line field can be divited into three regions:I, II, and III, where I and III are uniform stress regions, and II is a centered fan region. (1) The triangular region III (ABC) It is formed by free boundary AB and the slip lines AC and BC. This is a constant stress region. The slip lines are straight with α1=ʌ/4–ĳ/2. The mean stress is a constant and must satisfy condition throughout this region : ın=Ĳn=0, ı1=ıt, ı3=ın=0. Along the ȕ lines, we have

p =

− Cuni ⋅ cos ϕ uni 1 − sin ϕ uni

= Cβ ⋅ exp( 2 ξ ⋅ tg ϕ uni ) + Cuni ⋅ ctg ϕ uni

(9-39)

The integrate constant is determined by

Cβ =

− Cuni ⋅ cos ϕuni 1 − sin ϕuni

exp( − 2 ξ ⋅ tg ϕ uni )

(9-40)

242

9 Unified Slip-Line Field Theory for Plane Strain Problem

(2) The triangular region I (AA’D) It is formed by loading boundary AA’ and the slip lines AD and A’D. This is a constant stress region. The slip lines are straight with angle − ( π + ϕuni ) (α lines) 4 2 and ( π + ϕ uni ) ( ȕ lines). 4 2 The integrate constant is determined by

Cβ =

− q − C uni ⋅ ctg ϕuni

(9-41)

1 + sin ϕ uni

(3) Centered fan region II (ACD) This is a slip region. The α lines are straight with different angle acrossed at point A. ȕ lines are logarithmic spirals. The expression of the logarithmic spirals is

r1 = r0 exp(2 ξ ⋅ tg ϕ uni ) The length AC of a side of center fan is

AA '

r AD = 2 cos(

π

4

+

ϕ uni

2

)

The length AD of another side of center fan is

rAC =

AA ' exp ( 2 ξ ⋅ tg ϕ uni ) 2 cos(

π

4

+

ϕ uni

2

)

The limit loading of trapezoid specimen is obtained as follows

q = C uni ⋅ ctg ϕ uni [

1 + sin ϕ uni 1 − sin ϕ uni

exp ( 2ξ ⋅ tg ϕ uni ) − 1 ]

(9- 42)

With different choice of unified yield criterion parameter b, a series of limit loading are obtained as shown in Fig.9.9. The three curves are three results for three specimen, the top angles are: 2ξ = 120o, 2 ξ = 80o and 2ξ = 60o. Figure 9.10 is the variation of the slip angles with the variation of unified yield criterion parameter b. From Fig. 9.10, we can see that the result of Unified Slip Line Field Theory (2= 81.04o for b = 0.8) is much closer to the experimental result (2 =79.5o ) than that of the Mohr-Coulomb (2= 82.8o ).

9.6 Applications of the Unified Slip Line Field Theory

243

It is worthy to mention that not only the limit loading q but also the slip angle 2µ are different. They are different for different material. The variation of slip angle 2µ with the unified yield criterion parameter b is shown in Fig.9.10.

26 o

24

2ξ=120

22

2ξ=60

o

q (KN)

2ξ=80

o

20 18 16 14 12 0.0

0.2

0.4

0.6

0.8

1.0

b Fig. 9.9 Unified solutions of limit loading (Yang-Yu 1997)

83.0

2µ (degree)

82.5 82.0 81.5 81.0 80.5 0.0

0.2

0.4

0.6

0.8

1.0

b Fig. 9.10 Variation of slip angle 2µ with the unified yield criterion parameter b

244

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.6.2 Example 2: Strip footing The slip lines field of strip footing under uniform punch pressure is similar to

that of trapezoid structure as shown in Fig.9.11. The difference only in the angle ʌ and 2ȟ (2ȟ=2ș1 in Fig.9.11,b).

Fig. 9.11 Slip lines field of a semi-infinite surface (a) and a trapeziod structure (b)

The limit loading of strip footing can be obtained by 2ȟ=ʌ, which is given as follows q = C uni ⋅ ctg ϕ uni [

1 + sin ϕ uni 1 − sin ϕ uni

exp(π ⋅ tg ϕ uni ) − 1]

(9-43)

9.6.3 Example 3: Shallow strip footing A shallow strip footing is shown in Fig.9.12, and the material parameters are: C 0 = 9Kp a, ϕ 0 = 14 o, γ = 17.3KN / m 3, width of strip B=3m, depth d=1.5m. The shear strength of the soil between the surface and depth d is neglected.

This soil being considered only as a surcharge imposing a uniform pressure q=Ȗ0 d on the horizonal plane at foundation level. Determine the limit load for strip footing.

Fig. 9.12 Slip lines field of a falf space under shallow strip footing

9.6 Applications of the Unified Slip Line Field Theory

245

Solution Friction angle and cohesion of this material can be determined. The unified friction angle ĳuni and the unified cohesion Cuni can be determined by using Eqs.9-10 and 911. The relations of unified friction angle ĳuni and the unified cohesion Cuni with unified yield criterion parameter b, i.e. relations Cuni~b and ¶uni~b are shown in Figs. 9.13 and 9.14, respectively.

ϕ uni

20.00

15.00

10.00

5.00

b 0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.13Relations of unified friction angle ĳuni with unified yield criterion parameter b

C uni/c 0

1.20 1.00 0.80 0.60 0.40 0.20

b

0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.14Relations of unified cohesion Cuni with unified yield criterion parameter b

A series of slip line field and different results of limit loading were determined by Fan and Yu by using the unified slip field theory. The five slip line fields and relating limit loading are shown in Figs. 9.15 to 9.20.

246

9 Unified Slip-Line Field Theory for Plane Strain Problem

Pu =171.77

143.84

200.28

0.00

4.00

2.00

Fig. 9.15 Slip line field for b=0 material (Pu =171.77)

Pu =192.26

159.47

225.73

0.00

2.00

Fig. 9.16 Slip line field for b=0.2 material (Pu=192.26)

4.00

9.6 Applications of the Unified Slip Line Field Theory

pu=210.75 173.20

249.07

0.00

4.00

2.00

Fig. 9.17 Slip line field for b=0.4 material (pu=210.75)

pu=218.31 179.46

257.93

0.00

2.00

4.00

Fig. 9.18 Slip line field for b=0.5 material (pu=218.31)

247

248

9 Unified Slip-Line Field Theory for Plane Strain Problem

196.15

286.08

pu=240.68

0.00

2.00

4.00

Fig. 9.19 Slip line field for b=0.8 material (pu=240.68)

pu=252.38 205.81

299.83

0.00

2.00

4.00

Fig. 9.20 Slip line field for b=1.0 material (Twin-shear theory pu=252.38)

The limit loading of strip footing varies with the choice of the unified yield criterion parametere b. The relation of limit loading of strip footing with b is shown in Fig.9.21.

9.6 Applications of the Unified Slip Line Field Theory

249

Pu/c 50.00 40.00

30.00

20.00

10.00

b

0.00 0.00

0.20

0.40

0.60

0.80

1.00

Fig. 9.21Relations of limit loading with unified yield criterion parameter b

It is seen that a series of results can be obtained by using the unified slip lines field theory.

9.6.4 Example 4: Acute Wedge An acute wedge is in a plane strain state. Its top angle γ < π 2 , and surface AB is subjected to uniform pressure Pu , as shown in Fig. 9.22. Determine the limit pressure Pu on surface AB .

Fig. 9.22Acute wedge under unilateral pressure

Solution: The unified solution of acute wedge under unilateral pressure was given by Zhang, Hao and Yu in 2003. When 0 < γ < π 2 , a stress discontinuous line in the wedge will appear. The characteristic field is shown in Fig.9.22, where ∠BAC = δ , ∠CAD = ν, δ + ν = γ . The regions ABC and ACD are regions of constant biaxial

250

9 Unified Slip-Line Field Theory for Plane Strain Problem

compression and uniaxial compression, respectively. The constant stress regions ABC and ACD are separated by the line of stress discontinuity AC which is inclined to A B at an angle δ to be determined. The different values a quantity may assume in the regions ABC and ACD will be distinguished by subscripts 1 and 2, respectively. The angle between characteristics α and β is 2ψ . From the stress boundary condition of the wedge, we have σ 3 = − pu in region ABC , and σ 1 = 0 in region ACD . Thus it has ϕ1 =

π

2

−δ, ϕ2 = ν

(9-44)

It also has δ +ν = γ

(9- 45)

The unified limit load for acute wedge was given as follows

· § 1 + sin ϕ uni sin 2ν pu = Cuni ⋅ cot ϕ uni ¨¨ − 1¸¸ ¹ © 1 − sin ϕ uni sin 2δ

(9-46)

where ĳuni and Cuni were introduced by Yu et al. in 1997 and 1998, they are defined as

sin ϕ uni =

Cuni =

2 (b + 1) sin ϕ 2 + b (1+ sin ) ϕ

,

2 ( b + 1)C ⋅ cos ϕ

1 . 2 + b (1 + sin ϕ ) cos ϕ uni

(9-47)

ĳuni and Cuni are two parameters in the unified slip field theory. For the case of b = 0 and α ≠ 1 , the unified limit load reduces to

§ 1 + sin ϕ sin 2ν · pu ' = c cot ϕ ¨¨ − 1 ¸¸ © 1 − sin ϕ sin 2δ ¹

(9-48)

This is the solution on the basis of Mohr-Coulomb criterion (Shield 1954; Chen 1975).

9.6 Applications of the Unified Slip Line Field Theory

251

For the case of b = 0 and α = 1 , the unified limit load reduces to

p u " = lim p u ' = 2 c (1 − cos γ ) α →1

(9-49)

(ϕ → 0)

This is the solution on the basis of Tresca criterion (Chen 1975). When Ȗ=ʌ/3, the relation between the limit load pu and the unified yield criterion b at different ratio of α = ³t /³c are shown in Fig.9.23.

Fig. 9.23 The relation between limit load Pu and unified strength theory parameter b

It can be found that the SD effect of material and the influence of intermediate principal stress on the limit load are significant. Through the parameters α and b, the dependence of the result of the limit load on yield criterion is also reflected. As shown, at the same α , the Mohr-Coulomb criterion (b = 0 ) leads to the minimum value of pu σ t while the twin-shear strengrh theory (b = 1) leads to the maximum value of pu σt .

9.6.5 Example 5: Experiments A method of observing plastic zone in a structure under loading is applied. In order to obtain clear images of the development of structure's plastic zone, image analysis technique has been used.The plastic zone of structure under limit loading is obtained. Three trapeziod specimens are the same as example 1, in which the top angle are: 2ξ = 120o , 2 ξ = 80o and 2ξ = 60o . The three experimental results of limit loading are: 23.6kN for 2ξ = 120o, 18.5kN for 2 ξ = 80o , and 16.9kN for 2ξ = 60o . The theoretical results has been obtained as shown in Fig. 9.24.

252

9 Unified Slip-Line Field Theory for Plane Strain Problem

83.0

26 o

24

2ξ=120

22

2ξ=60

82.5

o

o

2µ (degree)

q (KN)

2ξ=80

20 18 16

81.5 81.0

14 12 0.0

82.0

0.2

0.4

0.6

b

0.8

1.0

80.5 0.0

0.2

0.4

0.6

0.8

1.0

b

Fig. 9.24 Variations of limt loads and slip angle with the unified yield criterion parameter b

We can see from Fig. 9.24 that the three experimental results q1=23.6kN, for 2 ξ = 120o , q2=18.5kN for 2 ξ = 80o , and q3=16.9kN for 2ξ = 60o are closed to the unified solution with bĬ0.8. Obvious error will be produced when we use the traditional Mohr-Coulomb slip line field solution (b=0). We can also assume that this material can be simulated by bĬ0.8, i.e. limit loads of cases with other top angles can be determined by Eq.9-42 with bĬ0.8. Furthermore, we can find from the experiment that the shape of slip line is nonorthogonal. The slip angle obtained by computer image analysis is 78o (for MohrCoulomb non-orthogonal slip line field theory, the angle is 82.8o ). The test gives the change of 2µ, the angle between two slip lines, with different choice of unified yield criterion parameter b. From Fig. 9.24, we can see that the slip angle o calculated through unified Slip Line Field Theory (2µ=81.04 when b=0.8) is much closer to the experiment result than the result based on the Mohr-Coulomb non-orthogonal slip line filed theory (2µ=82.8 o ).

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method Various finite element solutions for the bearing capacity of structures have been reported in the literature. Some are of very interesting and value. The development of plasticity in soil under a footing foundation were studied by Nayak and Zienkiewicz (1972) and Moore and Rowe (1991) et al. Fig. 9.25 to Fig. 9.28 show the results of plastic zones at footing displacement obtained by Moore and Rowe (1991). They used a 15 nodes element (as show at the right in Fig. 9.25) and a series of computational results were obtained. Each yielded integration point within the triangular elements has been marked with a small lines, where these lines are aligned with the direction of the shear deformation at those locations.The development of plastic zone at various footing penetrations are shown clearly.The

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method

253

final slip surface is shown in Fig. 9.28. It is observed that the soil materials collapses with a mechanism similar to that of Prandtl for perfectly plastic materials (Moore and Rowe 1991) .

Fig. 9.25 Fine mesh (Moore and Rowe 1991) Fig. 9.26 Initial plastic zone

Fig. 9.27 Development of plastic zone

Fig. 9.28 Final plastic zone

The velocity fields at the final displasment is shown in Fig. 9.29. The shape roughtly resembles the Prandtl mechanism for perfectly plastic materials, although only part of the solid material in motion is responding plastically, with both the block of material directly under the rigid footing and much of the solid within the “passive motion” behaving elastically. The shape is also similar the results obtained by the unified slip field theory.

254

9 Unified Slip-Line Field Theory for Plane Strain Problem

Fig. 9.29 Velocity fields at footing diaplacement (Moore and Rowe 1991)

The similar results were also obtained by other researcheres. A real-life problem in geomechanics were investigated by Wunderlich, Findeib and Cramer (Fig. 9.30) as well as Wunderlich, Findeib and Cramer Zimmermann and Commend et al.(Fig. 9.31). They showed the limit-load state obtained by the finite element analysis (2001). A localized failure in the shape of the well known Prandtle sliplines which have been derived on a analytical basis was given. The results of the finite element analysis are in close agreement with observations in reality.

Fig. 9.30 Limit-load state of strip footing (Wunderlich, Findeib and Cramer 2001)

Fig. 9.31 Limit-load state of strip footing (Zimmermann and Commend 2001)

9.7 Comparison of the Unified Slip Line Field Theory with Finite Element Method

255

The numerical tests of a panel under compression were analyzed by de Borst et al (1995) and Chen and Baker (2001). The plastic strain develops in “X” shape. It is agreement with the experimental results shown in Fig. 9.32.

Fig. 9.32 The plastic strain develops in “X” shape (Chen and Baker 2001)

These kinds of results were obtained by Yu and Zeng in 1990. The calculation results by using two material models, i.e. the Mohr-Coulomb strength theory (b=0) and the twin-shear strength theory (b=1, Yu 1985) are illustrated in Fig.9.33 and Fig.9.34. Figure 9.33 is a result of thick plate with a hole under compression, and figure 9.34 is a result of thick plate with a hole under tension. It is seen that the four results are different.

Fig. 9.33 Different results of two models in compression and in tension (Yu and Zeng 1993, see: Yu 1998)

It is worth noting that the result of the finit element method is always a single result by using a single yield criterion. The result of convenient slip line field is also a single result. It is also worthy to note that the shape and angle of the plastic zone are also different for different yield criterion.

256

9 Unified Slip-Line Field Theory for Plane Strain Problem

9.8 Comparison of the Unified Slip Line Field Theory with Experimental Results The experimental results of the plastic zones for a plate with different holes under tension are shown in Fig. 9.34 (see Yu 1998).

(a) Test results (Yu 1981)

(b) Test results (Liu 1989)

Fig. 9.34 Plastic zones of tensile plate with different holes

The comparison of three methods are shown in Fig. 9.35. The rectangular thick plate specimen with a circular hole at the center was applied under an uniform load at the edge. The material and the experimental procedure are same as those in example 1 and example 5. In Fig. 9.35, curve 1 is the experimental result of plastic zone, curve 2 is that of unified elasto-plastic finite element calculation (b=0.8), and curve 3 is of Unified Slip Line Field Theory.

Fig. 9.35 Comparison of three methods (see Yu 1998)

As can be seen, the plastic zones are different in tension and in compression for SD (strength different) maerials. Fig. 9.33(a) shows the computational results by

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain

257

using the twin-shear strength theory and the Mohr-Coulomb strength theory for the same material in compression. Fig. 9.33(b) shows the computational results by using the twin-shear strength theory and the Mohr-Coulomb strength theory for the same material in tension. The experimental results also present the difference of plastic zones in tension and in compression, as shown in Fig. 9.36.

Fig. 9.36 Different results in compression and in tension (Yu and Liu 1989)

In order to confirm the results of the unified slip line theory, the elasto-plastic finite element program UEPP based on the unified strength theory (UST) is used to compute the limit loading q of the same structures. UEPP was established by Yu, Zeng, Ma,Yang, Wang et al. in the period of 1993 to 1998 (Yu and Zeng 1994; Yu, Yang, Fan et al. 1997). From these comparisons, we can find that the result from the characteristics line theory are very close to those results from the experiments and finite element methods. The detail of numerical analysis of generalized plasticity will be discussed in another book : ĀComputational Plasticityā.

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain During the process of the elastic-plastic deformation, the continuity of velocity vanishes when it is passing the certain characteristics surface, with the development of the deformation, namely, the phenomenon of discontinuous bifurcations is produced. Hill (1958), Marciniak and Kuczynski (1967), Storen and Rice (1975), Rudnicki and Rice (1975), Hutchinson and Tvergaard (1980, 1981), Tvergaard, Needleman and Lo (1981), Raniecki and Bruhns (1981), Bruhns (1984), Li (1987), Runesson and Mroz (1989), Hill JM and Wu YH (1993),

258

9 Unified Slip-Line Field Theory for Plane Strain Problem

Zyczkowski (1999) et al. have done extensive researches for the discontinuous bifurcations. Ottosen and Runesson (1991) put forward a general description of discontinuous bifurcations for the plane problem of isotropic and elastic-plastic body plane problem, obeying the Mohr-Coulomb yield. criterion. Hill JM and Wu YH (1993) used the Ashton-Warren Spring yield equation. It is a Mohr-Coulomb typed yield equation, in which the maximum principal stress σ1 and the minimum principal stress σ3 are taken into account. Zyczkowski (1999) studied the discontinuous bifurcations in the case of the Burzynski-Torere yield criterion. The corresponding properties of discontinuous bifurcations have been obtained by using various yield criteria. For selection of the yield function, the intermediate principal stress is not considered in Mohr-coulomb Strength Theory, and this theory can not match the experimental results of much materials. The unified strength theory can be adapted for many kinds of materials, and make the former simple strength theories to be its special samples or its linear approach. Therefore, the unified strength theory is adopted to analyze the discontinuous bifurcations of materials for plane strain problem. The mathematical expression of the unified strength theory for plane strain problems is F = ( 1 + b ) ( 1 + sin φ ) σ1 − ( 1 − sin φ ) ( bσ 2 + σ3 ) − 2 ( 1 + b ) c cos φ = 0

When σ 2 ≤

1 2

(σ1 + σ3 ) +

sin φ 2

(σ 1 − σ 3)

(9-50a)

F ' = (1 + sin φ ) (σ 1 + bσ 2) − (1 − sin φ ) ( 1 + b ) σ 3 − 2 ( 1 + b ) c cos φ = 0

When σ 2 ≥

1 sin φ (σ + σ ) + (σ 1 − σ 3 ) 2 1 3 2

(9- 50b)

We chose the first equation of the unified strength theory (9-50a), because of the intermediate principal stress is σ2 =

m 1 sin φ (σ + σ ) ≤ (σ 1 + σ 3) + (σ 1 − σ 3) ( 0 < m 1) 2 1 3 2 2

(9-51)

9.9 Discontinuous Bifurcations of Elasto-plastic Material for Plane Strain

259

Substituting Eq. (9-51) into Eq.(9-50), we have F = ( 1 + b ) ( 1 + sin φ ) σ 1 −

1 2

( 1 − sin φ ) ( bmσ 1 + bmσ 3 + 2σ 3 ) − 2 ( 1 + b ) c cos φ = 0 (9-52)

definite f = ∂F , then we have ∂σ f1 = (1 + b ) ( 1 + sin φ ) σ 1 − f2 = −

1 2

bm 2

( 1 − sin φ ) (9-52)

( 1 − sin φ ) ( bm + 2 )

f3 = 0

The angle of shear band is obtained as follows (Zhang 2000) tg 2θ =

f1 f2

=

2(1 + b )(1 + sin ϕ ) − bm (1 − sin ϕ ) (1 − sin ϕ )(2 + bm )

(9-53)

The direction angle of shear band is

cos 2θ =

b (1 − m) + (2 + b + bm ) sin ϕ0 2 + b (1 + sin ϕ0 )

when mĮ1,

(9-54)

Equation (9-54) for plastic plane strain problems can be simplified to cos 2θ =

2(1 + b ) sin ϕ 0 2 + b (1 + sin ϕ 0)

when m=1,

(9-55)

This result is similar to that of the unified slip field theory for plane strain problems. The direction angle of shear band is sensitive to the failure criterion. The unified slip field theory give us a effective method to study this problems. The discontinuous bifurcations of elasto-plastic material for plane stress problems will be described in detail in Chapter 11.

260

9 Unified Slip-Line Field Theory for Plane Strain Problem

Summary A unified slip line field theory for plane strain problems based on the unified strength theory is described in this chapter. The unified slip line field theory for plane strain problems is composed of a group of orthogonal and non-orthogonal slip line fields. Many presently used orthogonal or non-orthogonal slip line field theories based on single shear strength theories are special cases (Tresca material slip field, Mohr-Coulomb material slip field and the twin-shear material slip field) or linear approximation (Huber-von Mises material) of the unified slip field theory system. By introducing an intermediate principal stress parameter, m, the new method can reflect the intermediate principal stress of plane strain problem, where the intermediate principal stress is the principal stress in z direction. Experiments and Elasto-Plastic Finite Element calculations have been used to verified the validity of the unified slip theory. The unified strength theory, the unified slip theory can be used in many engineering fields, especially for materials with obvious intermediate principal stress effect. The unified slip line field theory for plane strain problems has the following advantages: 1. It is a system of orthogonal and non-orthogonal slip line filed, which encompasses, in a piece-wise linear manner, other slip line field theories. All other slip line field theories are its special cases or linear approximations; 2. It can reflect the different effects of intermediate principal stress on different materials by introducing unified strength theory parameter b; 3. Giving a series of new slip line fields, and establishing the relations among available slip line field theories; 4. Introducing an intermediate principal stress parameter m, which can comply with different plane strain compressible and non-compressible materials. 5. It agrees with experimental results and can be easily used in many engineering fields.

Problems Problem 9.1 The extension of a strip with a sufficiently large circular hole for non-SD material was shown in Fig. P8.1 of chapter 8. Can you obtain a more complete study on this subject using the unified slip field theory for non-SD material ( α = 1 , and b= 0, b =1/2, b =1). Problem 9.2 The extension of a strip with a sufficiently large circular hole for non-SD material was shown in Fig. P8.1 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1).

Problems

261

Problem 9.3. The extension of a strip with ideal (infinitely thin) cuts (crack) for non-SD material was shown in Fig. P8.2 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory ( α = 1 , and b=0, b=1/2, b=1). Problem 9.4. The extension of a strip with ideal (infinitely thin) cuts (crack) for non-SD material was shown in Fig. P8.2 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1). Problem 9.5. The extension of a strip with angular notches for non-SD material was shown in Fig. P8.3 last chapter. Can you obtain a more complete study on this subject using the unified slip line field theory (α=1, and b=0, b=1/2, b=1). Problem 9.6. The extension of a strip with angular notches for non-SD material was shown in Fig. P8.3 of chapter 8. Can you obtain a more complete study on this subject using the unified slip line field theory for SD materials (α ≠ 1, and b=0,b=1/2, b=1). Problem 9.7. The extension of a strip with circular base for non-SD material was shown in Fig. P8.4 of chapter 8. Can you obtain a study on this subject using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.8. The extension of a strip with circular base for non-SD material was shown in Fig. P8.4 of chapter 8. Can you obtain a more complete study on this subject using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.9. The slip line field of indentation at the bottom of a flat trench was shown in Fig.P8.5 of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.10. The slip line field of indentation at the bottom of a flat trench was shown in Fig.P8.5 last chapter. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.11. The slip line field of indentation at the foot of a very deep vertically sided groove was shown in Fig.P8.6of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.12. The slip line field of indentation at the foot of a very deep vertically sided groove was shown in Fig.P8.6 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1).

262

9 Unified Slip-Line Field Theory for Plane Strain Problem

Problem 9.13. The slip line field of indentation at the top by a flat punch was shown in Fig.P8.7 of chapter 8. Find the limit load by using the unified slip line field theory for nonSD materials (α=1, and b=0, b=1/2, b=1). Problem 9.14. The slip line field of indentation at the top by a flat punch was shown in Fig.P8.7 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.15. The slip line field of a strip weakened by one-sided deep notch with a circular base was shown in Fig.P8.8 last chapter. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.16. The slip line field of a strip weakened by one-sided deep notch with a circular base was shown in Fig.P8.8 of chapter 8. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.17. The slip line field of a strip weakened by two-sided deep notch with a circular base was shown in Fig.P8.9 of chapter 8. Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.18. The slip line field of a strip weakened by two-sided deep notch with a circular base was shown in Fig.P8.9 last chapter. Find the limit load by using the unified slip field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.19. Figure P9.1 shows the slip line field of a pure bending strip weakened by two-sided angular notch. The limit moment for the Tresca material is

1 § · 2 π π − γ ¸ h σ s , for γ ≥ + M = ¨1 + 2 4 2 © ¹

Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.20.

Find the limit moment of a pure bending strip weakened by two-sided angular notch (Fig. P9.1) by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1).

Problems

Fig. P9.1 Two-sided angular notch

263

Fig. P9.2 One-sided angular notch

Problem 9.21. Figure P9.2 shows the slip line field of a pure bending strip weakened by one-sided angular notch. The limit moment for the Tresca material is

§ π + π − 2 γ · h2 σs , for γ ≥ 1 M = ¨¨ ¸¸ © 4 + π − 2γ ¹ 2

Find the limit moment by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.22. Find the limit moment of a pure bending strip weakened by one-sided angular notch by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.23. Figure P9.3 shows the slip line field of a pure bending strip weakened by one-sided angular notch with γ < 1 . Find the limit moment by using the unified slip line field theory for non-SD materials and SD materials

Fig. P9.3 Bending strip with angular notch

Fig. P9.4 Indentation of a semi-infinite mass

Problem 9.24. Figure P9.4 shows the slip line field of an indentation of a semi-infinite mass of rigid-perfectly plastic material by a rigid straight-sided, acute-angle indenter (Hill 1950; Johnson and Mellor 1961). The limit load for the Tresca material is

264

9 Unified Slip-Line Field Theory for Plane Strain Problem

P = 2 a (1 + γ )σs

Find the limit load by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.25. Find the limit load of an indentation of a semi-infinite mass of rigid-perfectly plastic material by a rigid straight-sided, acute-angle indenter by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.26. The slip line field of a thick-walled cylinder is shown in Fig.P9.5. The limit pressure for the Tresca material is

P = σs ln

b a

Find the limit pressure by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1).

Fig. P9.5 Slip line field of a thick-walled cylinder (Tresca material)

Problem 9.27. Find the limit pressure for a thick-walled cylinder by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.28. Comparing the results of the slip line field theory for a thick-walled cylinder with the elasto-plastic analysis in Chapter 15. Problem 9.29. Figure P9.6 shows a slip line field of a strip weakened by center crack for non-SD materials. Determine thelimit load by using the unified slip line field theory for SD materials (α 1, and b=0, b=1/2, b=1).

Problems

265

Fig. P9.6 A slip line field of a strip weakened by center crack

Problem 9.30. The slip line field of a strip with a hole under uniform pressure was shown in Fig. P8.9 last chapter. Find the limit pressurefor non-SD materials and SD materials by using the unified slip field theory. Problem 9.31. The slip line field of extrusion through a die over a smooth container wall was studied by Johnson et al (1962). Figure P9.7 shows the fan shaped slip line field The limit pressure were given by using the Tresca condition as follows P = §¨1 + π ·¸ h σs 2¹ © Find the limit pressure for SD materials by using the unified slip line field theory (α 1, and b=0, b=1/2, b=1).

Fig. P9.7 Extrusion through a die over a smooth container wall

Problem 9.32. Find the limit pressureof extrusion through a die over a smooth container wall for SD materials by using the unified slip line field theory (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.33. The slip line field of drawing of a strip was studied by Johnson et al (1962). Figure P9.8 shows the fan shaped slip line field. Limit drawing force for the Tresca material is

266

9 Unified Slip-Line Field Theory for Plane Strain Problem

P=

2 hσs (1 + γ ) sin γ 1 + 2 sin γ

o

when γ ≥ 42 27 ' , H = 2h

Find the drawing force for non-SD materials by using the unified slip line field theory (α=1, and b=0, b=1/2, b=1). Problem 9.34 . Find the drawing force for SD materials by using the unified slip line field theory (α ≠ 1, and b=0, b=1/2, b=1).

Fig. P9.8 Extrusion of a strip

Fig. P9.9

Problem 9.35 . The slip line field and limit pressure for extrusion problems were studied by Johnson et al. as shown in Fig. P9.9. The limit extrusion force for the Tresca material is π · § P = 2 ¨1 + ¸ a σs 2¹ ©

when b =2a

Find the limit pressure of extrusion by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1). Problem 9.36 . Find the limit pressure of extrusion by using the unified slip line field theory for SD materials (α ≠ 1, and b=0, b=1/2, b=1). Problem 9.37. Determine the limit load of a deep beam shown in Fig. P9.10

Problems

267

Fig. P9.10

Problem 9.38. A series of results can be obtained by using the unified slip line field theory for various plane strain problems. All the solutions of the problems in this chapter have not been studied before. Can you try to give a series of new results for these problems, and try to use in practice. Problem 9.39. The slip line field and limit pressure for slop stability problems were given by ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) for the Mohr-Coulomb material as shown in Fig. P9.11. The limit pressure is

1 + sin ϕ ½ q = C ⋅ cot ϕ ® exp ª¬(π − 2 χ ) tan ϕº¼ − 1¾ ϕ − 1 sin ¯ ¿

Fig. P9.11

Find the limit pressure of slop by using the unified slip line field theory for non-SD materials (α=1, and b=0, b=1/2, b=1) and SD materials (α ≠ 1, and b=0, b=1/2, b=1).

268

9 Unified Slip-Line Field Theory for Plane Strain Problem

References and Bibliography Chen G. and Baker G (2001). Gradient-dependent plasticity with a 3-node incompatible element for the plastic multiplier. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 1129–1134. de Borst R., Pamin J and Sluys LJ (1995) Computation issues in gradient plasticity, In: Continuum Models for Materials with Micro-structure, H.B. Mfihlhaus (ed.), Wiley: Chichester, 159–200. Drucker DC, Greenberg HJ and Prager W (1951) The safety factor of an elastic-plastic body in plane strain, J. Appl. Mech., 18: 371–378. Ford H (1954) The Theory of Plasticity in Relation to Engineering Application, J. AppL Math. Phys., 5: 1–35. Geiringer H (1930) Beit zum Vollstiindigen ebenen Plastizitits-problem, Proc 3rd Intern. Congr. Appl. Mech, 2: 185–190. Hencky H(1923) Ueber einige statisch bestimmte Faelle des Gleichgewichts in plastischen Koerpern Z. angew. Math Mech., 3: 245– 251. Hill R (1949) The Plastic Yielding of Notched Bars Under Tension, Quart. Mech. AppL Math., 2: 40– 52. Hill R(1956), The Mechanics of Quasi-Static Plastic Deformation in Metals, In: Survey in Mechanics, G. K. Batcheler and R. M. Davis eds, Cambridge, Johnson W and Mellor PB (1962), Plasticity for Mechanical Engineers, Van Nostrand, Princeton, N.J. Johnson W, Sowerby R, Venter RD (1982), Plane-Strain Slip Line Fields for Metal Deformation Processes--A Source Book and Bibliography, Pergamon Press, Oxford. Moore ID and and Rowe RK (1991) Objective solutions for bearing capacity of strainsoftening soils. In: Beer G, Booker JR and Carter JP eds. Computer Methods and Advances in Geomechanics. Rotterdam: A.A.Balkema, Vol.2,1183–1189. Panayotounakos D (1996) Ad Hoc Exact Solutions for the Stress and Velocity Fields in Rigid Perfectly Plastic Materials Under Plane-Strain Conditions. Int. J. Plast., 12:1069– 1190. Prager W (1955) The Theory of Plasticity: A Survey of Recent Achievements, Proc. Inst. Mech. Eng., 169: 41–57. Prager W (1959) Introduction to Plasticity, Addison-Wesley, Reading, Mass. Prager W and Hodge P G Jr (1951) Theory of Perfectly Plastic Solids, Wiley New York. Prandtl L (1920) l~ber die H~irte Plastischer Koerper, Goettinger Nachr., Math. Phys. KI.,74–85. Thomsen EG, Yang CT and Kobayashi S (1965) Mechanics of Plastic Deformation in Metal Processing, Macmillan, New York. Wunderlich, Findeib and Cramer in (2001) Finite element analysis of bearing capacities in geomechanics considering dilatant and contractant constitutive laws. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 2001, 533–538. Yu Mao-hong (1983), Twin Shear Stress Criterion, Int. J. of Mech. Sci., 25(1), 71–74, Yu Mao-hong, He, Li-nan, Song, Ling-yu (1985), Twin Shear Stress Theory and Its Generalization, Scientia Sinica (Science in China), Series A, (English edn.), 28(11), 1174–1183. Yu Mao-hong and He Li-nan (1991), A new model and theory on yield and failure of materials under complex stress state. In: Mechanical Behaviour of Matterials-VI. Yu Mao-hong, He Li-nan (1992), Generalized Twin Shear Stress Yield Criterion and Its Generalization, Chinese Science Bulletin (English edn.), 37(24), 2085–2089. Yu Mao-hong, et al (1992), Computer Image Analysis of the Plastic Zone of Structure, Journal of Xi'an Jiaotong University, 26(2), 121–122 (in Chinese).

References and Bibliography

269

Yu Mao-Hong, Liu Jian-Yu and Ma Guo-wei (1994), Twin-shear slip line theory: orthogonal and non-orthogonal slip line fields. Journal of Xi’an Jiaotong University, 28(2):122–126. Yu Mao-hong. (1998) Twin-shear Theory and Its Applications. Beijing: Science Press (in Chinese). Yu MH and Fan SC eds (1998) Strength Theory: Applications, Developments and Prospects for the 21st Century. New York, Beijing: Science Press. Yu Mao-hong. (2004) Unified Strength Theory and Its Applications. Berlin: Springer. Zenkiewicz OC(1992), Computational Mechanics Today, Int. J. Numer. Methods in Engrg., 34, 9–33. Zhang YQ (2000) Analysis of damage and Discontinuous bifurcations for Elarto-Plastic Geomaterials. Dissertation of Doctor at Xi’an Jiaotong University, Xi’an, China (in Chinese) Zhang YQ and Yu MH (2001) Discontinuous bifurcations of metallic materials for plane stress. Chinese J. of Mechanical Engineering, 37(4): 62–85 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of elasto-plastic materials for plane stress. Acta Mechanica Sinica, 33(5): 706–713 (in Chinese, English Abstract). Zimmermann Th and Commend S (2001) Stabilized finite element applications in geomechanics. In: Valliappan S and Khalili N eds., Computational Mechanics : New Frontiers for the New Millennium, Amsterdam: Elsevier, 2001, 533–538. Ȼɟɪɟɡɚɧɥɟɜ ȼȽ (1952) Ɉɫɟɫɢɦɦɟɬɪɢɱɧɚɹ Ɂɚɞɚɱɚ Ɍɟɨɪɢɢ ɉɪɟɞɟɥɶɧɨɝɨ Ɋɚɜɧɨɜɟɫɢɹ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. Ɇɨɫɤɜɚ: Ƚɨɫ. ɂɡɞ. Ɍɟɯ. Ɍɟɨ. Ʌɢɬɟɪɚɬɭɪɵ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1942) ɋɬɚɬɢɤɚ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. ɂɡɞ. Ⱥɇ ɋɋɋɊ, Ɇɨɫɤɜɚ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) ɋɬɚɬɢɤɚ ɋɵɩɭɟɣ ɋɪɟɞɵ (Third ed.).Ƚɨɫ. ɂɡɞ. Ɏɢɡ-Ɇɚɬ. Ʌɢɬɟɪɚɬɭɪɵ. Ɇɨɫɤɜɚ (in Russia)

10 Twin-Shear Characteristics Field for Plane Stress Problem

10.1 Introduction The twin-shear slip field and the unified slip line field theory for plane strain problems have been described in Chapters 8 and 9. This chapter deals with the twin-shear characteristics filed for plane stress problems. For plane stress problems, characteristic methods can be used to solve the quasi-linear differential equation systems of stress and velocity fields. Judgments on the types of these differential equation systems can be made using the theory of characteristics. They may be elliptic or hyperbolic, depending on the considered stress state. The methods of characteristics based on the Huber-von Mises and the Tresca criteria can be found in the literature of Kachanov (1971), Martin (1973), Yan (1988) and Panoyotomakos (1999) for plane stress problems. A new characteristics method for plane stress problems was established based on the twin-shear yield criterion (Yu 1961, 1983) by Yan and Bu in 1993 and 1996. The methods of characteristics based on the Huber-von Mises, the Tresca and the twin-shear criteria can be applied to the limit analysis of the plane stress problems. However, they are only adapted for the non-SD (strength differential) materials with τ 0 ≈ 0.58σ t , τ 0 = 0.5σ t and τ 0 = 2σ t /3, respectively, but fail for the SD materials. Although the method of characteristics based on the Mohr-Coulomb criterion takes account of SD effect, it is only adapted for the material with τ 0 =σ t σ c/ (σ t + σ c).

10.2 Characteristics Method based on the Tresca Criterion and the Huber-von Mises criterion 10.2.1 Characteristics Method based on the Tresca Criterion The Tresca criterion in plane stress state is shown in Fig. 10.1. If χ and λ are introduced for the cases of σ x σ y ≤ τ ²xy and σ xσ y ≥ τ² xy respectively, the following expressions of stresses satisfy automatically the Tresca criterion in plane stress state,

10.2 Tresca Criterion and the Huber-von Mises criterion

271

σ2 σs

F

E

σs

D

A

σ1

σs

B C

σs Fig. 10.1 Tresca criterion in plane stress state

σx = 2k χ + k cos 2ϕ

(10-1a)

σy = 2k χ − k cos 2ϕ

(10-1b)

τxy = k sin 2ϕ

(10-1c)

on lines AB and DE in Fig. 10.1. σ x = σ s [ s (1 − λ ) + λ cos 2ϕ ]

(10-2a)

σ y = σ s [ s (1 − λ ) − λ cos 2ϕ ]

(10-2b)

τ xy = k sin 2ϕ

(10-2c)

on lines BC, CD, EF and FA in Fig. 10.1, where 1 when σ1 > 0, σ2 > 0 ° s=® ° −1 when σ < 0, σ < 0 1 2 ¯

(10-3)

The equations of equilibrium determined by the stress components in Eq. (10-1) and Eq. (10-2) are of the hyperbolic type and the parabolic type, respectively. The equations of the characteristics are

272

10 Twin-Shear Characteristics Field for Plane Stress Problem

(10-4)

dy § · = tan ¨ϕ ± π ¸ 4¹ dx © dy s + cos 2ϕ − cot ϕ , =− =® dx sin 2ϕ ¯ tan ϕ ,

(10-5)

It can be seen that Eq. (10-4) has two orthogonal families of characteristics, which differentiate π/4 with the direction of principal stresses σ1 and σ2. It coincides with the definition of slip line. The two families of characteristics have the following forms, χ + ϕ = C1

(10-6a)

χ − ϕ = C2

(10-6b)

Eq. (10-6) is the same as Hencky equation for the plane strain problem, when assuming χ = σ/2k. Eq. (10-5) has only one family of characteristics, which is parallel to the intermediate principal stress by considering that it is a three-dimensional problem. The characteristic line is the intersecting line between xy-plane and the plane which offsets an angle of π/4 from the directions of the maximum and minimum stresses. This agrees with the explanation of the slip line equation (17-4), as long as considering the difference of the cases σ xσ y ≤τ ²xy and σ xσ y ≥τ ²xy . From the above analysis, if the Tresca criterion is applied, the characteristics with respect to the lines AB and DE (σ x σ y >τ ² xy) can be solved by the hyperbolic type equations. On other lines (σ x σ y >τ ² xy), it can be solved by integrating the differential equation directly.

10.2.2 Characteristics Method based on the Huber-von Mises Criterion The Huber-von Mises criterion in plane stress state is given in Fig. 10.2. If a variable ω is introduced, the stress components satisfy Huber-von Mises criterion can be obtained by σ x = k ( 3 cos ω + sin ω cos 2ϕ ) σy = k

(

3 cos ω − sin ω cos 2ϕ

τ xy = k sin ω sin 2ϕ

)

(10-7a) (10-7b) (10-7c)

10.2 Tresca Criterion and the Huber-von Mises criterion

σ2 ω= E′

5π 3

σs C′

D′ ω =

3π ω= 2 4π

F′ ω =

σs

G′

ω =π

ω=

273

ω =0 11π A 6 π ω = C σs 6

3

7π 6

E

D ω = π σ1 3

ω=

F G5π ω = 2π ω= 3 6

π

2

B

σs

Fig. 10.2 Huber-von Mises criterion in plane stress state

The characteristics of the equilibrium equation determined by Eq. (10-7) is dy 3 sin ω sin 2ϕ ± 3 − 4cos 2 ω = dx 3 sin ω cos 2ϕ − cos ω

(10-8)

It is obvious that there exist two families of characteristics only when 3 − 4cos 2 ω > 0 ( π / 6 < ω < 5π / 6 or 7π / 6 < ω < 11π / 6 ) (lines CG and C ′G ′ in Fig. 10.2). Otherwise, there is no characteristics ( 3 − 4cos 2 ω < 0 ) (lines CC ′ and GG ′ in Fig. 10.2) or there is only one family of the characteristics ( 3 − 4cos 2 ω = 0 ) (points C, C′, G, and G′ ). For the hyperbolic type, two supplementary incremental expressions are needed ψ =

χ =−

π

2

1 2

³

§ cot ω · 1 − cos −1 ¨ ¸ 2 © 3 ¹ ω π 6

3 − 4cos 2 ω dω sin ω

(10-9a)

(10-9b)

The equation of characteristics can then be obtained as

dy = tan(ϕ ± ψ ) dx

(10-10)

274

10 Twin-Shear Characteristics Field for Plane Stress Problem

Along these two families of the characteristics, it has χ + ϕ = C1

(10-11a)

χ − ϕ = C2

(10-11b)

which has the same form with Eq. (10-6), however, χ is much more complex than that in Eq. (10-6). Meanwhile, it can be found that the two families of characteristics are not orthogonal to each other. The angle between the two families of the characteristics is 2ψ, which varies with locations. From the above analysis, for Huber-von Mises criterion, the problem can be solved by the characteristics method of the hyperbolic type when π/6 < ω < 5π/6, or 7π/6 < ω < 11π/6, however, the process will be very tedious due to the non-orthogonal feature. On other segments it will be more difficult to solve the characteristics.

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion Characteristics method based on the twin-shear yield criterion was proposed by Yan and Bu in 1993. In(σ x, σ y, τ xy) plane stress states, three principal stresses are σ1 =

σ2 =

σx + σ y

2 σx + σ y

2

2

§ σx − σ y · 2 + ¨ ¸ + τ xy 2 © ¹

(10-12a)

2

§ σx − σ y · 2 − ¨ ¸ + τ xy 2 © ¹ σ3 = 0

(10-12b) (10-12c)

The twin-shear yield criterion has the following form, 1 3 1 f = σ 1 − (σ 2 + σ 3 ) = σ s = k , when σ 2 ≤ (σ 1 + σ 3) 2 2 2

(10-13a)

1 3 1 (σ 2 + σ 3) − σ 3 = σ s = k , when σ 2 ≥ (σ 1 + σ 3) 2 2 2

(10-13b)

f =

The yield loci of the twin-shear yield criterion in the plane stress state are shown in Fig. 10.3.

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion

275

Fig. 10.3 Twin-shear yield criterion in plane stress state

The functions of the six segments in Fig. 10.3 can be expressed as follows, f1 = 2σ 1 − σ 2 = 3k

(10-14a)

f2 = 2 σ 1 − σ 2 = −3k

(10-14b)

f3 = 2σ 2 − σ 1 = 3k

(10-14c)

f 4 = 2σ 2 − σ 1 = −3k

(10-14d)

f5 = σ 1 − σ 2 = −3k

(10-14e)

f 6 = σ 1 − σ 2 = 3k

(10-14f)

Substituting Eq. (10-10) into Eq. (10-14), we derive the twin-shear yield criterion function expressed in terms of the three principal stresses as follows, 1 1 σ x + σy + 3 (σ x − σ y ) 2 + τ 2xy = 3k , 2 4 when σ x + σ y ≤ 6

(10-15a)

1 (σ x − σ y ) 2 + τ 2 xy 4

1 (10-15b) ( σ x − σ y ) 2 + τ 2xy 4 Neglecting body force, the equations of equilibrium for plane stress problems are σ x + σ y = 3k , when

∂σ x ∂x

+

∂τ xy ∂y

σx + σy ≥ 6

= 0,

∂τ xy ∂x

+

∂σ y ∂y

=0

(10-16)

276

10 Twin-Shear Characteristics Field for Plane Stress Problem

10.3.1 Hyperbolic Type For the yield condition of Eq. (10-15a), assuming σ1 − σ 2

2

= λ k,

σ1 + σ 2

2

= 3(1 − λ ) sk

(10-17)

where S = 1, when σ1 + σ 2 > 0 ; S = 0, when σ 1 + σ 2 = 0 ;

(10-18)

S = −1, when σ 1 + σ 2 < 0 Combining Eqs. (10-10) and (10-17) gives 2

σx + σ y §σ x − σ y · 2 = 3(1 − λ ) sk ¨ ¸ + τ xy = λ k , 2 © 2 ¹

(10-19)

The corresponding stress components are σ x = k [ 3s (1 − λ ) + λ cos 2ϕ ]

(10-20a)

σ y = k [ 3s (1 − λ ) − λ cos 2ϕ ]

(10-20b)

τ xy = k λ sin 2ϕ

(10-20c)

The above stresses satisfy Eq. (10-15a) automatically, in which λ is in the range of 1 ≤ λ ≤1 2

(10-21)

Combining Eq. (10-20) and Eq. (10-16) derives

−3s

∂λ ∂λ ∂λ ∂λ ∂λ + cos 2ϕ − 2λ sin 2ϕ + sin 2ϕ + 2λ sos2ϕ =0 ∂x ∂x ∂x ∂y ∂y

∂λ ∂ϕ ∂λ ∂λ ∂ϕ − 3s − =0 sin 2ϕ + 2λ sos 2ϕ sos 2ϕ + 2λ sin 2ϕ ∂x ∂x ∂y ∂y ∂y For any line in xy-plane, increments of λ and ϕ can be written as dλ =

∂λ ∂λ dx + dy ∂x ∂y

(10-22a) (10-22b)

(10-23a)

10.3 Characteristics Method Based on the Twin-Shear Yield Criterion

277

∂ϕ ∂ϕ (10-23b) dx + dy ∂x ∂y Eq. (10-22) together with Eq. (10-23) makes an algebraic equation system with ∂λ /∂ x, ∂λ /∂ y, ∂ϕ /∂ x, ∂ϕ /∂ y as unknowns. Let the determinant of coefficients vanish, i.e. dϕ =

−3s + cos 2ϕ sin 2ϕ ∆= dx 0

sin 2ϕ −3s − cos 2ϕ dy 0

−2λ sin 2ϕ 2λ cos 2ϕ 0 dx

2λ cos 2ϕ 2λ sin 2ϕ =0 0 dy

(10-24)

It is then obtained,

dy −3s sin 2ϕ ± 2 2 s = dx 1 − 3s cos 2ϕ

(10-25)

Assuming s = −3cos 2ϕ , Eq. (10-25) can be rewritten as

1 dy § s· = tan(ϕ B ψ ),ψ = cos −1 ¨ − ¸ 2 dx © 3¹

(10-26)

Eq. (10-26) determines two families of characteristics. As can be seen, the two families of characteristics differ angles ±ψ from the direction of the principal stress σ1 . Here those corresponding to the plus sign are assigned as family α and those to the minus sign as family β. In order to derive the relationship between λ and ϕ, from Eqs. (10-22), (10-23) and (10-24), it has ϕ + 2s ln λ = C1 (along α line)

(10-27a)

ϕ − 2 s ln λ = C2 (along β line)

(10-27b)

Thus, based on the twin-shear yield criterion, it can be solved by the characteristics method for stress state on lines of FA, BC, CD, EF (see Fig. (10.3)).

10.3. 2 Elliptic Type For the yield condition Eq. (10-15b) (AB and DE in Fig. (10.3)), it has

∂λ ∂ϕ ∂λ ∂ϕ cos 2ϕ − 2λ sin 2ϕ sin 2ϕ + 2λ cos 2ϕ + =0 ∂x ∂x ∂y ∂y

(10-28a)

∂λ ∂ϕ ∂λ ∂ϕ sin 2ϕ + 2λ cos 2ϕ cos 2ϕ + 2λ sin 2ϕ − =0 ∂x ∂x ∂y ∂y

(10-28b)

278

10 Twin-Shear Characteristics Field for Plane Stress Problem

where λ ≤ 1/2. Let the determinant of the coefficients of Eqs. (10-28) and (10-23) vanish, it has

cos 2ϕ sin 2ϕ ∆= dx 0

sin 2ϕ − cos 2ϕ dy 0

−2λ sin 2ϕ 2λ cos 2ϕ 0 dx

2λ cos 2ϕ 2λ sin 2ϕ =0 0 dy

(10-29)

Then it is obtained (dx) 2 + (dy ) 2 = 0

(10-30)

There is no real root for dy/dx. The equilibrium differential equation determined by the stress components which satisfy Eq. (10-15b) is an elliptic type, thus the characteristics do not exist. Based on the above analysis, it can be found that the problem of the stress state on the lines of FA, BC, CD, EF (see Fig. (10.3)) is of the hyperbolic type and can be solved by the characteristic method. However, the problem of the stress state on the other two lines AB and DE (see Fig. (10.3)) is of the elliptic type which can not be solved by the characteristic method. Nevertheless, the yield condition of Eq. (10-15b) is very simple and can be solved directly by using equilibrium equation and the yield function.

10.4 Twin-shear Characteristics Field for Plane Stress Problems (Velocity Field) 10.4.1 Velocity Field corresponding to Eq. (10-15b) Applying associate flow rule, the strain rate can be obtained from Eq. (10-15b) as ξ x = ξ y , ζ xy = 0

(10-31)

The velocity components are thus

∂Vx ∂Vy − =0 ∂x ∂y ∂Vx ∂V y + =0 ∂x ∂y The increments of the velocity components are ∂Vx ∂V dx + x dy = dVx ∂x ∂y

(10-32a)

(10-32b)

(10-33a)

10.4 Twin-shear Characteristics Field for Plane Stress Problems

∂Vy ∂x

dx +

∂V y ∂y

The determinant of coefficients of

279

(10-33b)

dy = dV y

∂Vx ∂Vx ∂V y ∂V y , , , in the above four ∂x ∂y ∂x ∂y

equations equal to 0, which gives

1 0 0 −1 0 1 1 0 ∆= =0 dx dy 0 0 0 0 dx dy

(10-34)

Then (dx)2 + ( dy ) 2 = 0

(10-35)

There is no real root for dy/dx. The equation is of the elliptic type and the characteristics do not exist.

10.4.2 Velocity Field corresponding Eq. (10-15a) Corresponding to the yield condition of Eq. (10-15), it has ζx = α

ª º σx − σ y ∂f s 1 » =α « + « 6 2 ( σ − σ ) 2 + 4τ 2 » ∂σ x x y xy ¼ «¬

(10-36a)

ζy = α

ª σx − σ y ∂f s 1 =α « − « 6 2 (σ − σ ) 2 + 4τ 2 ∂σ y x y xy ¬«

(10-36b)

ζ xy = α

º » » ¼»

2τ xy ∂f =α − ∂τ xy (σ x − σ y ) 2 + 4τ 2 xy

(10-36c)

where f is the twin-shear yield function, α ( > 0) is a scalar factor. Combining Eq. (10-20) and Eq. (10-36) derives

∂V y ∂Vx ∂Vy ∂Vx ∂V y ∂Vx + − ∂y ∂y ∂z ∂x ∂y ∂x = = = s 1 s 1 ϕ ϕ sin 2 cos 2 + cos 2ϕ − cos 2ϕ 6 2 6 2

(10-37)

280

10 Twin-Shear Characteristics Field for Plane Stress Problem

Eq. (10-37) can be rewritten as §s · ∂Vx § s · ∂V y − ¨ + cos 2ϕ ¸ =0 ¨ − cos 2ϕ ¸ ©3 ¹ ∂x © 3 ¹ ∂y

§ ∂V ∂V y · § ∂Vx ∂V y · cos 2ϕ ¨ x + − ¸ − sin 2ϕ ¨ ¸=0 ∂x ¹ ∂y ¹ © ∂y © ∂x The determinant of the coefficient must vanish, which gives s − cos 2ϕ 3 ∆ = − sin 2ϕ dx 0

0

0

cos 2ϕ dy

cos 2ϕ 0

0

dx

s − − cos 2ϕ 3 sin 2ϕ =0 0

(10-38a)

(10-38b)

(10-39)

dy

Then the following equation is obtained dy −3sin 2ϕ ± 2 2 −3sin 2ϕ ± 2 2 s = = dx s − 3cos 2ϕ 1 − 3s cos 2ϕ

(10-40)

Eq. (10-40) is the same with the characteristics of the stress field. Thus, the characteristics of the velocity field just coincide with those of the stress field for the twin-shear yield criterion, just like the Tresca criterion and the Huber-von Mises criterion. Combining Eqs. (10-33), (10-38) and (10-39) gives dVx + dV y

dy =0 dx

(10-41)

Corresponding velocity field can then be obtained through Eqs. (10-26) and (10-41)

dVx + dVy tan(ϕ − ψ ) = 0 , along α line

(10-42a)

dVx + dVy tan(ϕ + ψ ) = 0 , along β line

(10-42b)

Considering an arbitrary point P at an plane curve L on the xy plane, if local coordinate system (t, n) is applied, the first equation of Eq. (10-38) can be rewritten as

§s · ∂Vt § s · ∂V − ¨ + cos 2ϕ ¸ n ¨ − cos 2ϕ ¸ ∂ 3 3 t © ¹ © ¹ ∂n

(10-43)

where t and n are respectively in the tangential and normal directions of the curve L. Coefficients of ∂Vn/∂n of Eq. (10-43) equals to 0, then cos 2ϕ = − s / 3

(10-44)

10.5 Applications of the Twin-shear Characteristics Method

281

From Eq. (10-43), it has ζ t = ∂Vt / ∂t = 0

(10-45)

10.5 Applications of the Twin-shear Characteristics Method 10.5.1 Velocity Discontinuous Line in Uniaxial Tension In the plane stress problem, it is possible that velocity discontinuities exist not only in the tangential, but also in the normal direction of the slip line. A ‘necking’ deformation zone may be formed. Assuming that the neck has a small width b (in the limiting case b→0) and by a simple derivation, it can be seen that the line of velocity discontinuity is just one of the velocity characteristics, and the relative velocity v is perpendicular to the velocity characteristics of the other family (Kachanov 1971). In this example, σ y = σ 1, σ x = 0, τ xy = 0, so s = 1. There are two families of velocity characteristics, and the value of ψ (the angle between the velocity characteristics and the principal stress σ 1) is given by 1 § 1· (10-46) cos −1 ¨ − ¸ = 54° 44′ 2 © 3¹ Therefore, the angle γ between the relative velocity v and principal stress σ 1 is ψ =

γ = 90° − ψ = 35° 16′

(10-47)

Fig. 10.4 Plate specimen in uniaxial tension

It can be seen that by using the twin-shear yield criterion, the solution of this problem is simple and straightforward. The same value of ψ can also be obtained by using the Huber-von Mises yield criterion, but the process will be more cumbersome (Kachanov 1971). This value

282

10 Twin-Shear Characteristics Field for Plane Stress Problem

(54° 44′ ) has been verified by experiment (Nadai 1950) and coincide with the result of Huber-von Mises (Yan 1988). The line of velocity discontinuity is known as Lüder’s line. Based on the Tresca yield criterion, ψ can take an arbitrary value between 45° and 90° ; obviously, it is unreasonable.

10.5.2 Limit Load of an Infinite Thin Plate with a Circular Hole An infinite thin plate, having a circular hole with radius a (Fig. 10.5), is subjected to a two-directional uniform tension q at infinity. Find the limit load qs and the corresponding stress distribution.

Fig. 10.5 An infinite plate with a circular hole

It is obvious that this is a plane stress problem. As the hole is free and the plate experiences two-directional uniform tension at infinity, on the edge of the hole there will be σ θ > 0 and σ r = 0 and at infinity there will be σ θ = σ r > 0. Thus σ θ ≥ σ r ≥ 0 holds in the whole plate, and then s = +1. Near the hole, the stress satisfies Eq. (10-15a). And equations of the characteristics passing through the point A (r = a, θ = 0) will be θ =±

1 r ln , ‘+’ for α line, ‘−’for β line 2 a

(10-48)

Along AP , it has ϕ + 2 ln λ = C 1

From ϕ = θ + π /2 and σ r

r =a

(10-49)

= 0 , we know λ A=3/4, thus, it has 1/ 2

λ =

3§ a · ¨ ¸ 4© r ¹

(10-50)

10.5 Applications of the Twin-shear Characteristics Method

283

The stress components are derived as follows ª

σθ = 3k «1 −

«¬

1/ 2 º

1§ a· ¨ ¸ 2© r ¹

ª «¬

(10-51b)

1/ 2 º

§a· ¸ ©r¹

σ r = 3k «1 − ¨

(10-51a)

» »¼

» »¼

With r increasing, λ will decrease. When r = 9a/4, λ = 1/2, which is the critical value for the hyperbola. When r > 9a/4, the equation is ellipse. Stress components can be derived from differential equation and yield criterion. 2º

(10-52a)

2º

(10-52b)

σr =

3k ª 27 § a · «1 − ¨ ¸ 2 «¬ 16 © r ¹

σθ =

3k ª 27 § a · «1 + ¨ ¸ 2 «¬ 16 © r ¹

» »¼ » »¼

Thus, limit load is qs = σ r

r →∞

=

3k =σs 2

(10-53)

Expressions of corresponding stresses are ª § a ·1/ 2 º 9 ° 2 σ s «1 − ¨ ¸ » , a ≤ r ≤ a 4 °° ¬« © r ¹ ¼» σr = ® ª 27 § a · 2 º ° 9 ° σ s «1 − ¨ ¸ » , r > a 16 r 4 © ¹ »¼ «¬ °¯

ª 1 § a ·1/ 2 º 9 ° 2σ s «1 − ¨ ¸ » , a ≤ r ≤ a 4 °° «¬ 2 © r ¹ ¼» σθ = ® ª 27 § a ·2 º ° 9 ° σ s «1 + ¨ ¸ » , r > a 4 «¬ 16 © r ¹ »¼ ¯°

(10-54a)

(10-54b)

For comparison, characteristics and stress distribution under the three yield criterion are shown in Figs. 10.6, 10.7 and 10.8. The same value of limit load qs = σs is obtained based on each of the aforementioned three yield criterion (Kachanov 1971).

284

10 Twin-Shear Characteristics Field for Plane Stress Problem

Fig. 10.6 Results of example 2: Twin-shear criterion

Fig. 10.7 Result of example 2: von-Mises criterion

Fig. 10.8 Results of example 2: Tresca criterion

10.5 Applications of the Twin-shear Characteristics Method

285

10.5.3 Thin Circular Ring Plate subjected to a Uniform Internal Pressure A thin circular ring plate with inner radius a and outer b = 2a, subjected to a uniform internal pressure q (Fig. 10.9). Find the limit load and the corresponding stress distribution. Through analysis similar to that in example 2, near the outer edge of the ring plate

Fig. 10.9 Example 3

λ=

ª

σ θ = 3k «1 −

«¬

ª

σ r = 3k «1 −

«¬

3 § 2a · ¨ ¸ 4© r ¹

1 § 2a · ¨ ¸ 2© r ¹ 1 § 2a · ¨ ¸ 2© r ¹

(1/ 2)

(1/ 2) º

» (c≤r ≤b ) »¼

(1/ 2) º

» (c≤r ≤b ) »¼

(10-55)

(10-56a)

(10-56b)

With r decreasing, λ will increase, and λ = 1 is the limit of availability of Eq. (10-13). Take c to denote this radius; thus, from Eq. (10-10) 9 c= a 8

(10-57)

In the region a ≤ r ≤ (9/8)a, s = −1, thus σ θ = −(3 − 4λ )k ( a ≤ r ≤ c )

(10-58a)

σ r = −(3 − 2λ ) k ( a ≤ r ≤ c )

(10-58b)

ψ =

1 1 cos −1 = 35D16' 2 3

(10-59)

286

10 Twin-Shear Characteristics Field for Plane Stress Problem

The equations of characteristics passing through the point r = a, θ = 0, are θ = ± 2 ln

r (‘+’ for α line, ‘−’ for β line) a

(10-60)

Then, −

π

2

− 2 ln1 = −

π

2

+ θ − 2 ln λ = −

r + 2 ln − 2 ln λ 2 c π

(10-61)

Hence, λ =

r 8r = c 9a

(10-62)

Substituting Eq. (10-19) into Eq. (10-18) § ©

32 r · ¸ 27 a ¹

(10-63a)

§ ©

16 r · ¸ 27 a ¹

(10-63b)

σ θ = −3k ¨1 − σ r = −3k ¨ 1 −

Since σθ + σ r = 3k 2 − (48 / 27)( r / a ) ≤ 3k in the region a ≤ r ≤ (9/8) a, the yield condition Eq. (10-15a) is always applicable for this region. Thus, the limit load is qs = σ r

r =a

= 1.222k = 0.815σ s

The characteristics and stress distribution are shown in Fig. 10.10.

Fig. 10.10 Results of example 3

10.6 Comparison of these Different Methods

287

Based on the Huber-von Mises and Tresca yield criterion, the values of limit loads are qs = 1.330k = 0.768σ s for Huber-von Mises yield criterion; and q s = 1.386k = 0.693σ s for the Tresca yield criterion.

10.6 Comparison of These Different Methods Yan and Bu (1993) have compared the three different characteristic methods based respectively on the twin-shear yield criterion, the Tresca criterion, and the Huber-von Mises criterion. The advantages and disadvantages of these methods are shown in Table 10.1 and Table 10.2. Through the comparison, the following conclusions can be drawn: 1. It would be simpler to derive the characteristics based on the Tresca criterion and the twin-shear criterion than the Huber-von Mises criterion. 2. The twin-shear yield criterion has the advantage in describing the velocity discontinuity for the unixial tension example. 3. It is suggested to use the Tresca criterion if the experimental data of a certain material offset the Huber-von Mises ellipse toward the Tresca polygon. If the experimental data locates outside the Huber-von Mises ellipse, the twin-shear yield criterion is suggested. Thus, application of the Huber-von Mises criterion can be avoided.

Table 10.1. Comparison of the three yield criterion

Criterion

Range of hyperbolic type σ1

Tresca

von Mises Twin-shear

σ2 σ1 σ2

σ1 σ2

0

(11-70)

Then, from Eq. (11-51) D

θ = 90

,

H db l l' = − (1 + ν ) 2 2 SS ' 2µ

(11-71)

314

11 Unified Characteristics Field Theory for Plane Stress Problem

Due to Hdb ≤ 0, the discontinuous bifurcations don’t occur at the plastic hardening state, and the bifurcation mode is split mode. When b = 1, P1 =P2, Q1 = Q2, the direction of bifurcation is arbitrary. When b=0, as the intermediary of the two modes, the mode of discontinuous bifurcations belongs to either split mode or shear band mode. 2. case of σ 1 ≥ 0 ≥ σ 2, when σ 2 ≥ (1+sinφ)σ 1/( sinφ-1), through analysis, we can obtain 2

tan 2 θ =

2m1m '1 − m1m '3 − m3 m'1 H db 1 + ν ( m3m '1 − m1m' 3 ) = , 2µ 4 RR ' ( m1 − m3 )( m '1 − m '3 ) 2m3m' 3 − m1m' 3 − m3m' 1

(11-72)

where, R = m12 + m32 , R ' = m '12 + m '32 , from Eq. (11-72), Hdb ≥ 0, the bifurcations occur at plastic hardening or ideal plastic state, and the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of the unified strength theory b can be shown by Fig. 11.9.

Fig. 11.9 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

When σ 2 ≤ (1+sinφ)σ 1/( sinφ−1), 2

tan 2 θ =

2l1l '1 − l1l '3 − l3l '1 H db 1 + ν ( l3l '1 − l1l '3 ) = , 2l3l '3 − l1l '3 − l3l '1 2µ 4 SS ' ( l1 − l3 )( l '1 − l '3 )

(11-73)

11.6 Discontinuous Bifurcations of Non-associated Flow Elasto-plastic

315

where, S = l12 + l32 , S ' = l '12 + l '32 , from Eq. (11-73), Hdb ≥ 0, the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of the unified strength theory b can be shown by Fig. 11.10.

Fig. 11.10 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

3. case of 0 ≥ σ 1 ≥ σ 2, when σ 2 ≥ (1 + sinφ)σ 1/2, by calculation, when 0 ≤ b ≤ 1, D

θ =0

where, R = m22 + m32 ,

,

H db m m' = − (1 + ν ) 2 2 2µ RR '

(11-74)

R ' = m '22 + m '32 , from Eq. (11-74), Hdb ≤ 0, the

bifurcations occur at plastic softening or ideal plastic state, and the bifurcation mode is split mode (also shear band mode, as b = 0). When b = 1, an arbitrary direction can be the initial direction of the bifurcation, belonging to split mode, and the corresponding hardening modulus is

H db m m' m m' = − (1 + ν ) 2 2 = − (1 + ν ) 3 3 2µ RR ' RR '

(11-75)

316

11 Unified Characteristics Field Theory for Plane Stress Problem

When σ 2 ≥ (1+sinφ)σ 1 / 2, by calculation, 2l2l '2 − l2l '3 − l3l '2 2l3l '3 − l2l '3 − l3l '2

½ ° ° 2 ¾ H db 1 + ν ( l3l '2 − l2l '3 ) ° = 2µ 4 SS ' ( l2 − l3 )( l '2 − l '3 ) °¿

tan 2θ =

(11-76)

where, S = l22 + l32 , S ' = l '22 + l '32 , from Eq. (11-76), Hdb ≥ 0, the bifurcations occur at plastic hardening or ideal plastic state, and the bifurcation mode is shear band mode. With ignoring the different tensile and compressive property (φ = ψ = 0) of materials, the relationship between the initial bifurcation angle θ and the parameter of strength theory b can be shown by Fig. 11.11.

Fig. 11.11 Relation of the unified strength theory parameter b with initial direction of discontinuous bifurcation

The results produced by the Yu unified strength theory above show that the initial angle of bifurcation obtained as b = 0 is just the solution of Mohr-Coulomb strength theory (1900); the angle obtained as b = 0, φ = 0 is just the solution of Tresca (1991) yield criterion and the angle obtained as b = 1/2, φ = 0 is the linear approach of the solution of Huber-von Mises yield criterion.

11.7 Discussion and Experimental Verification

317

11.7 Discussion and Experimental Verification 11.7.1 Discussion

Assume the material satisfy the associate flow law. A special case is discussed in this part and compared with the existing unified plane stress characteristics field theory (Yu et al. 1998, 1999). Define A = (σ1+σ2) / 2, B = (σ 1−σ2) / 2. For plane stress problem, materials are assumed satisfy the associate flow law, following conclusions are drawn: For σ1 ≥ σ2 ≥ 0 (viz. A ≥ B), when σ2 ≤ (1+sin φ)σ1/2, it is equal to A ≤ (2+α)B / α (α is the tension-compression ratio), discontinuous bifurcations are shear band mode. From Eq. (11-67) tan 2θ = −

m1 m2

(11-77)

then cos2θ = −

m1 + m2 1+ b −α b =− m1 − m2 1+ b +α b

(11-78)

Here, sinφ = (1−α)/(1+α) is used. In such a stress state, the angle of characteristics is given by unified characteristics theory as follows cos 2θ = −

m n

(11-79)

where, m = (1+b−αb) / (1+b), n = (1+b+αb) / (1+b). It is obviously that Eq. (11-78) and Eq. (11-79) have given the same result. When σ 2 ≥ (1+sinφ)σ 1/2 (viz. A ≥ (2+α)B / α), if 0 < b ≤ 1, discontinuous bifurcations are of split mode. In such a stress state, when 0 < b ≤ 1, from the unified plane stress characteristics field theory, we know that there is no characteristics, because there is no root for the characteristics angle cos2θ = −(1+b) / (1−b). When b = 0, these two will give the same results. The same conclusion will be drawn for the two cases of σ 1 ≥ 0 ≥ σ 2 (A ≤ B), and 0 ≥ σ1 ≥ σ2 (A ≤ − B). From the above analysis, following conclusions can be obtained: In the plane stress state, shear band mode bifurcations is the same with the characteristics in essence. Angle of the unified characteristics given by Yu et al. (1999) can be obtained by the degeneration of the angle of shear band. So, the bifurcation theory can be used to analyze the characteristics.

318

11 Unified Characteristics Field Theory for Plane Stress Problem

11.7.2 Experimental Verification

A rectangular thin plate, made of PVC hard plastic, is subjected to uniform tension on two short sides as shown in Fig. 11.12. Unixial tensile strength of the PVC material: σ t = 5.886kN/cm² ; unixial compressive strength: σ c = 7.575kN/cm² ; tension-compression ratio: α = σ t /σ c =0.777. When subjected to tension, local slip band, which has the angle θ =61° with the tensional direction, appeared in the specimen. Based on the present unified characteristic field theory, with different b, the result of the characteristics will be different and a series of solutions can be obtained. On the other words that different strength theory will lead to different azimuth angle of shear band. Localized shear band on the plate is observed after the stretching. The angle θ of the shear band from the force direction is 60° . From a back analysis, the angle θ is determined as 60.97° when b = 0.675. It implies that the commonly used Mohr-Coulomb criterion may give very different prediction (48.60° for this example) of the shear band direction. It can not coincide with the experimental result. So, b = 0.675 is used to simulate the PVC-like material, viz. the strength theory of b = 0.675 can be used for shear band analysis of this kind of material.

x1 σ

B

θ

x2

A

σ Fig. 11.12 Rectangular thin plate subjected to tension

Summary

319

In this section, unification of the maximum critical hardening modulus has been done for the discontinuous bifurcations of elastic-plastic materials. Based on this unification, the phenomenon of discontinuous bifurcations has been investigated and obtained the initial azimuth angle and unified analytical model of the corresponding hardening modulus of discontinuous bifurcations under the non-associated plastic flow condition. This solution can be adapted for many kinds of materials and make the former simplex strength theories to be its special samples or its linear approach. Through the analysis of the results we can know that the isomerism of compression and tension and the intermediate principal stress have so great influence on the discontinuous bifurcations that govern the stress state. Therefore, these two factors above can’t be ignored during the analysis of the bifurcation, or else the results obtained can’t accord with the results of actual practice. On the other hand, the influence of different strength criterion to the discontinuous bifurcations of elastic-plastic materials can be established by giving different value of parameter b. A conclusion can be drawn that the influence of strength criterion is relative to the stress state of material. Actually, the value of parameter b can be calculated from Eq. (11-57). Substituting it in the unified solution, the properties of bifurcation fit for the material can be obtained. Comparing with the theory of characteristics field of plane stress, we can know that the discontinuous bifurcations of shear band mode of plane stress coincide with the characteristics. Thus, the theory of bifurcation can be adopted to analyze the characteristics. Similar discontinuous bifurcations for plane strain problems can be seen in Chapter 9.

Summary Based on the unified strength theory the unified characteristics field theory for plastic plane stress problem is described in this chapter. It is the unification of the plastic characteristics methods based on the Tresca criterion, the Huber-von Mises criterion and the twin-shear yield criterion. A series of new results can be also obtained by using the unified characteristics field theory. The strength-differential effect (SD effect and the effect of intermediate principal stress are taken into account in the unified characteristics field theory. The unified solutions of two examples, i.e. an infinite thin plate with a hole and a trapezoidal plate under compression, are given. It concludes a series of new results. The discontinuous bifurcations problems under plane stress are also studied by using the unified strength theory in this chapter.

320

11 Unified Characteristics Field Theory for Plane Stress Problem

Problems Problem 11.1 Derive the characteristics field for plane stress problem by using the Mohr-Coulomb strength criterion or the Yu unified strength theory with b = 0. Problem 11.2 Derive the characteristics field for plane stress problem by using the twin-shear strength or the Yu unified strength theory with b=1. Problem 11.3 Derive the characteristics field for plane stress problem by using the Yu unified strength theory with b = 0.5. Problem 11.4 Discuss the discontinuous bifurcation based on the Mohr-Coulomb strength criterion or the Yu unified strength theory with b = 0. Problem 11.5 Discuss the discontinuous bifurcation based on the twin-shear strength or the Yu unified strength theory with b = 1. Problem 11.6 Discuss the discontinuous bifurcation based on the Yu unified strength theory with b = 0.5. Problem 11.7 Discuss the discontinuous bifurcation for plane strain problems (see chapters 8 and 9) based on the Yu unified strength theory with b = 0.5.

References and Bibliography Bruhns OT (1984) Bifurcation problems in plasticity. In: The Constitutive Law in Thermoplasticity, Lehmann Thed. Springer-Verlag, Wien, New York. Hill RA (1958) General theory of uniqueness and stability in elastic-plastic solids. J. Mech. and Phys. of Solids, 6: 236–249. Hill JM and Wu YH (1993) Plastic flows of granular materials of shear index n−1, (1) yield functions; (2) Plane and axially symmetric problems for n = 2, J. Mech. and Phys. of Solids, 40(1): 77–93; 95–115. Hutchinson JW and Tvergaard V (1980) Surface instabilities on statically strained plastic solids. Int. J. Mech. Sci., 22: 339−358. Hutchinson JW and Tvergaard V (1981) Shear band formation in plane strain. Int. J. Solids Struct., 17: 451−466. Li GC (1987) Shear band bifurcations of ductile materials. Acta Mechanics Sinica, 19, 61−68. Marciniak Z and Kuczynski K (1967) Limit strains in the process of stretch forming sheet metal. Int. J. Mech. Sci., 9: 609−619. Ranniecki B, Bruhns OT (1981) Bounds to bifurcation stresses in solids with non-associated flow law at finite strain. J. Mech. and Phys. of Solids. , 29: 153–172. Rudnicki JW and Rice JR (1975) Conditions for the localization of deformation in pressure-sensitive dilatant materials. J. Mech. Phys. Solids, 23: 231–241.

Summary

321

Runesson K, Mroz Z (1989) A note on non-associated plastic flow rules. International Journal of Plasticity, 5: 639–658. Runesson K, Ottosen N, Peric D (1991) Discontinuous bifurcations of elastic-plastic solutions at plane stress and plane strain. International Journal of Plasticity, 7: 99–121. Storen S and Rice JR (1975) Localized necking in thin sheets. J. Mech. and Phys. of Solids, 23: 421–433. Thomas TY (1961) Plastic Flow and Frature in Solids. , Academic Press, New York. Tvergaard V, Needleman A and Lo KK (1981) Flow localization in the plane strain tensile test. J. Mech. and Phys. of Solids. 29: 115–127. Yu MH (1961) General behaviour of isotropic yield function (in Chinese), Res. Report of Xi’an Jiaotong University. Xi’an. Yu MH (1983) Twin shear stress yield criterion. Int. J. Mech. Sci. 25: 71–74. Yu MH, He LN, S LY (1985) Twin shear stress theory and its generalization, Scientia Sinica (Science in China), Series A, 28(12): 1174–1183. Yu MH, He LN (1991) A New Model and Theory on Yiwld and Failure of Materials under Complex Stress State. Mechanical behaviour of materials-6, Pergamon Press, 3 : 841–846. Yu MH (1994) Unified Strength Theory for geomaterials and its applications. Chinese Journal of Geothechnical Engineering, 16(2): 1–10 (in Chinese). Yu MH (1998) Twin Shear Theory and Its Application. Berjing: Science Press (in Chinese). Yu MH, Zhang YQ, Yang SY (1998) Another important generalization of the unified strength theory. J. of Xi’an Jiaotong University. 32: 108–110 (in Chinese, English Abstract). Yu MH, Zhang YQ, Li JC (1999) The unified characteristics theory for plastic plane stress problems. J. of Xi’an Jiaotong University. 33(4) : 1–4 (in Chinese, English Abstract). Zhang YQ and Yu MH (1999) Solutions to plastic plane stress problems. J. of Xi’an Jiaotong University, 33(6): 60–63 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of metallic materials for plane stress. Chinese J. of Mechanical Engineering, 37(4): 62–85 (in Chinese, English Abstract). Zhang YQ and Yu MH (2001) Discontinuous bifurcations of elasto-plastic materials for plane stress. Acta Mechanica Sinica, 33(5): 706–713 (in Chinese, English Abstract). Zhang YQ, Hao H and Yu MH (2003) A unified characteristics theory for plastic plane stress and strain problems. J. of Applied Mechanics, 70: 649–654. Zyczkowski M (1999) Discontinuous bifurcations in the case of the Burzynski-Torere yield criterion. Acta Mechanica, 132: 19–35.

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

12.1 Introduction The twin-shear slipe-line field and the unified slipe-line field theory for plane strain problem and the twin-shear characteristics field and the unified characteristics field theory for plane stress problem have been described in Chapters 8, 9, 10 and 11. It can be applied to metal plastic forming, the limit analysis of structure in civil engineering and mechanical engineering. The partial differential equations of the axisymmetric problem are not exactly hyperbolic, they may be elliptical and parabolic. The two families of characteristics lines of the parabolic functions become one family, and there are no characteristics lines for the elliptical equations. The characteristics line field theories of the spatial axisymmetric problem is more complex. It is difficult to solve analytically, and still remains open. A lots of simplified methods were used to discuss the characteristics line theory of spatial axisymmetric problems. Levin (1953), Shield (1955) and Kachanov (1971) et al. used Haar von-Karman complete plasticity condition and the Tresca criterion. They studied the indentation problem of a punch, and assumed that circumferential stress σ θ is equal to one of the other two principal stresses, namely σ θ ≈ σ 1 or σθ ≈ σ 3 . The results of the characteristics line theory, however, did not agree well with the reality ( Hill 1950). Szczepinski (1979) used the hypotheses σθ ≈ σ r and the Tresca criterion to study the characteristics line theory of spatial axisymmetric problems. After that, the infinite differential method was also used for spatial axisymmetric problems (Shield 1955). Based on the same method, Cox analyzed the limit loading capability of cohesive circular smooth soil foundations ( c − ϕ soil and ρ = 0 ). Larkin analyzed circular shallow soil foundations ( ρ = 0 ) when c = 0 . The above analyzed results were summarized by Chen (1975). Shield and Cox used the single-sheer strength theory (Tresca-Mohr-Coulomb theory) and the hypotheses σθ = σ 2 < σ1 of Haar and von-Karnam. Some axisymmetric characteristics problems were solved by Ishlinsky (1944), and Sokolovsky (1942) using the Mohr-Coulomb theory. Figs. 12.1 and 12.2 show the two examples of axisymmetric characteristics field (from Ȼɟɪɟɡɚɧɥɟɜ 1960). Figure 12.3 is an example of the axisymmetric characteristics for a long-rod penetration in concrete target (Yu, Li, Wei and Chen, see Yu 2002a).

12.1 Introduction

323

Fig. 12.1. Characteristics field of an indentation of a circular head punch (non-SD material)

Fig. 12.2. Characteristics field of an indentation of a circular head punch (SD material)

-6

-4

-2

0

2

4

Fig. 12.3 Axisymmetric characteristics field of a long-rod in normal penetration

Most solutions can be adapted only for the Tresca material and the MohrCoulomb material A unified characteristics line field theory for axisymmetric problems which can be adapted for more materials was introduced by Yu et al. in 2001 (Yu, Li and Zhang 2001). It is based on the peculiarity of spatial axisymmetric plastic problems and the unified strength theory. The stress field and velocity field of the unified axisymmetric characteristics line field theory are described in this chapter, and two examples by using the new characteristics theory for axisymmetric plastic problem are given. The unified

324

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

axisymmetric characteristics line field theory is also used to solve the high velocity impact problem. The normal penetration of a long-rod under high velocity is described in this chapter.

12.2 The Unified Strength Theory The Yu unified strength theory has been described in Chapter 4. The mathematical expression of the unified strength theory is f = σ1 − f'=

α

1+ b

(bσ 2 + σ 3 ) = σ t

1 (σ 1 + bσ 2 ) − α σ 3 = σ t 1+ b

when σ 2 ≤

σ1 + α σ 3

1+ α σ1 + α σ 3 when σ 2 ≥ 1+ α

(12-1a) (12-1b)

The unified strength theory can be expressed in terms of internal cohesion c0 and the friction angle ϕ 0 as follows

f = [σ1− 1 (bσ 2+ σ 3)] + [σ1+ 1 (bσ 2 +σ 3) ]sin ϕ0 = 2c0cos ϕ 0, 1+b 1+b σ +σ 3 σ1 −σ 3 sin ϕ 0 + when σ 2 ≤ 1 2 2 or

when σ2 ≤ p + R sin ϕ 0 (12-2a) 1 1 f ' =[ ( σ 1 + bσ 2 ) − σ 3 ] + [ ( σ 1 + bσ 2 ) + σ 3 ]sin ϕ0 = 2c0 cos ϕ0 , 1+ b 1+ b σ + σ 3 σ1 − σ 3 when σ 2 ≥ 1 sin ϕ 0 + 2 2

or

when σ 2 ≤ p + R sin ϕ 0

(12-2b)

The relations among c0 , ϕ 0 and the other parameters of material are shown as α =

1 − sin ϕ 0 1 + sin ϕ0

σt =

2c0 cos ϕ 0 1 + sin ϕ 0

(12-3)

It is shown that the unified strength theory consists of a series of strength theories from the single shear strength theory (lower limit, Mohr-Coulomb 1900) to the twin shear strength theory (upper limit, Yu 1985). The variaties of yield loci of the unified strength theory on the deviatoric plane have been illustrated in Figure 2 in Preface and Fig. 4.7, 4.8 in Chapter 4.

12.3 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Stress Field) There are four non-zero stress components σ r , σθ , σ z and τ rz in the axisymmetric problem, the circumferential stress σθ must be one of principal stresses.

12.3 Unified Characteristics Line Field Theory

325

According to the stress state of a spatial axisymmetric problems, we introduce a parameter m for circumferential stress σθ ( 0 ≤ m ≤ 1 ) σ + σ3 σ −σ σθ = σ 3 + m( 1 − σ 3) = σ3 + m 1 3 2 2

(12-4)

For the axisymmetric problem, we define P=

σ 1 + σ3

2

,R=

σ1 − σ3

2

(12-5)

The following relations can be derived σ1 = P + R

σ 2 = σθ = P + ( m − 1) R

σ3 = P− R

(12-6)

The stresses of the problem can be expressed as σ r = P + R cos 2θ

½ ° ° ¾ (12-7) ° °¿

σ z = P − R cos 2θ τ rz = R sin 2θ σ θ = P + ( m − 1) R

where θ is the angle between the directions of the maximum principal stress and axis r. Using the first expression of the unified strength theory Eq.(12-2a) because the intermediate principal stress is σ 2 = σ θ = P + (m − 1) R ≤ P + R sin ϕ 0. Substituting Eq. (12-6) into Eq. (12-2), the unified strength theory for spatial axisymmetric problem is obtained as follows R=−

2(1 + b)sin ϕ 0 2(1 + b)c0 cos ϕ 0 P+ 2(1 + b) + mb(sin ϕ 0 − 1) 2(1 + b) + mb(sin ϕ 0 − 1)

(12-8)

The expression of the unified strength theory for spatial axisymmetric problem can be simplified to the simple expression as follows

R = −P sinϕ uni + cuni cos ϕ uni

(12-9)

where sinĳuni and Cuni are the unified material parameters introduced from the unified strength theory by Yu et al. (2001) for spatial axisymmetric problem. The parameter ĳuni and Cuni are referred to as the unified friction angle ĳuni and the unified internal cohesion Cuni, respectively.

sin ϕuni =

2(1+ b)sin ϕ 0 , 2(1+ b) + mb(sin ϕ0 −1)

(12-10)

326

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Cuni =

2(1+ b)c0 cos ϕ 0 1 ⋅ 2(1+ b) + mb(sinϕ 0 −1) cos ϕuni

(12-11)

When m = 0.5 , sinĳuni and Cuni can be expressed as

2(1+ b) sin ϕ 0 , 2(1+ b) + 0.5b(sin ϕ 0 −1)

(12-12)

2(1+ b) c0 cos ϕ 0 1 ⋅ 2(1+ b) + 0.5b(sinϕ 0 −1) cos ϕuni

(12-13)

sinϕuni =

Cuni =

The relations between the unified material parameters ĳ uni and C uni and the conventional material parameter ĳ0 and C0 are shown in Fig. 12.4 and Fig. 12.5.

1.14 1.12

0

ϕ0=5

Ct /C 0

1.10

C uni / C 0

0

ϕ0=10

1.08 1.06 1.04

0

ϕ0=15

1.02

0

ϕ0=20

1.00

0

ϕ0=25 0.0 0.0

0.2 0.2

0.4 0.4

0.6 0.6

0.8 0.8

1.0 1.0

b Fig. 12.4. Relation between unified cohesion Cuni and b

12.3 Unified Characteristics Line Field Theory

25

0

ϕ0=25

20

ϕt

327

0

ϕ0=20

15 0

ϕ0=15

ĳuni

10 0

ϕ0=10 5

0

0

ϕ0=5

0.0000000000.2000000030.4000000060.6000000090.8000000121.000000015 0.2 0.0 0.8 1.0

0.4

b

0.6

Fig. 12.5. Relation between unified internal friction angle ĳuni and b

When stress P presents compressive stress, the Eq.(12-9) changes to

R = P sin ϕ uni + cuni cos ϕ uni

(12-14)

The equilibrium differential equations of the axisymmetric problem are shown as ∂σ r ∂r ∂σz

∂z

+ +

∂τ rz ∂z ∂τ rz

∂r

+ +

σr −σ z =0

r

τ rz

r

=0

½ ¾ ¿

(12-15)

Substituting Eq. (12-7) and Eq. (12-14) into Eq.(12-15), the governing differential equations are expressed as ∂P (1+sin ϕ uni cos 2θ ) + ∂ P sin ϕ tuni sin 2θ + 2R ( ∂θ cos 2θ − ∂θ sin 2θ ) = R(m−1− cos 2θ ) r ∂r ∂z ∂z ∂r ∂P ∂P ∂θ ∂θ R sin ϕuni sin2θ + (1− sin ϕuni cos 2θ ) + 2R ( cos 2θ + sin 2θ ) =− sin 2θ ∂r ∂z ∂z ∂r r

(12-16)

Assuming that functions P and θ are given respectively along some curve z = z (r ) in the roz-plane, we get

328

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

dP =

∂P ∂r

∂P

dr +

∂z

dz , dθ =

∂θ ∂r

dr +

∂θ ∂z

dz

(12-17)

Eqs.(12-12) and (12-13) constitute a system of four linear inhomogeneous algebraic equations for the partial derivatives. The characteristics line equations of the solutions can be given, let the determinant of the algebraic and the relavant numerators are zero. Letting the determinant of the system equal to zero, we obtain the differential equations of the characteristics lines as follows

dz = tan(θ − µ) dr dz = tan(θ + µ ) β line group: dr

(12-18a)

α line group:

(12-18b)

There exist two families of characteristics lines, where the parameter 2µ is the angle between the characteristics lines Į and ȕ and the relation between parameters µ and ĳuni is µ=

π 4

ϕ − uni . 2

According to the direction derivation formulas ∂

= [sin(θ + µ )

∂r ∂ ∂z

∂ ∂ Sα

= − [cos(θ + µ )

− sin(θ − µ )

∂ ∂ Sα

∂ ∂ Sβ

− cos(θ − µ )

] sin 2µ ∂

∂ Sβ

] sin 2µ

(12-19a) (12-19b)

where Sα and Sβ are the convected coordinate system of the characteristics lines α and β , respectively. Therefore, the unified characteristics line equations are introduced as follows ∂z ∂r R R ∂z ( m − 1)(cos 2 µ + sin 2µ )+ r r ∂ Sα ∂ Sα ∂ Sα ∂ Sα ∂ Sα α line group (12-20a) ∂P ∂θ ∂z ∂r R R ∂z sin 2 µ − 2R = − (m − 1)(cos 2µ − sin 2 µ )− r r ∂ Sβ ∂ Sβ ∂ Sβ ∂ Sβ ∂ Sβ

sin 2µ

∂P

− 2R

∂θ

=

β line group

(12-20b)

It is the stress field of the unified characteristics line theory for axisymmetric problem.

12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems

329

12.4 Unified Characteristics Line Field Theory for Spatial Axisymmetric Problems (Velocity field) The associated flow rule is d ε ijp = d λ

∂f

(12-21)

∂σ ij

The unified strength theory of the spatial axisymmetric problem can be derived from the Eq. (12-3) and Eq. (12-8) §σ r − σθ · 2 +τ 2 + C cosϕ = 0 (12-22) rz uni uni ¨ 2 ¸ © ¹ Under the small deformation condition, the strain rates can be expressed as 1 f = (σ r + σ θ )sinϕuni − 2

εr = εθ = εz =

γrz =

∂u ∂r

∂f

= −λ

∂σ r

∂f u = −λ ∂σ θ r ∂v ∂z

∂u ∂z

= −λ

+

∂f ∂σ z

∂v ∂r

= −λ

∂f

(12-23)

∂τ rz

From Eqs. (12-21), (12-22), (12-23) and Eq (12-10), we can get λ εr = − (sinϕuni − cos2θ ) 2 εz = −

λ (sinϕ + cos2θ ) uni

2 λ rz = λ sin 2θ

(12-24a) (12-24b) (12-24c)

where θ is the angle from the direction of principle stress σ r to the direction of axis r. When the angle between the characteristics line α and axis r is denoted by ψ , the relation between ϕ and θ is shown as π ϕ θ =ψ + µ =ψ + ( − uni )

4

2

(12-25)

Substituting the above relation into Eq. (12-20) derives λ εr =− [sin ϕuni + sin (2ψ −ϕuni )]

2

(12-26a)

330

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

λ εz =− [sin ϕ uni − sin(2ψ −ϕ uni)] 2

(12-26b)

λrz = λ cos(2ψ − ϕuni )

(12-26c)

When one of the characteristics lines α or β overlaps with axis r, namely ψ = 0 or ψ = −(

π − ϕ uni) , Eq. (12-21) can be simplified to 2

εr = (

∂ u ∂r

)ψ = 0 = 0 or εr = (

∂ u ∂r

)

ψ =− (

π

2

−ϕ uni )

=0

(12-27)

It shows that the strain rate is zero along the direction of the characteristics lines. If the velocities along the characteristics lines α and β are denoted by Vα and Vβ , the velocities along axes r and z are denoted by u and w , respectively, the

relations among them can be expressed as u = w=

Vα sin( ψ + 2 µ ) − Vβ sin ψ

(12-28a)

sin 2 µ Vα cos(ψ + 2µ ) − Vβ cos ψ

(12-28b)

− sin 2µ

It can derive the following equations by getting differential with respect to r and combining with Eq.(12-22)

§ ∂u · = ¨¨ ¸¸ © ∂ r ¹ψ = 0

§ ∂ Vα ¨¨ © ∂r

· + Vα cot 2 µ ¸¸ ¹ψ = 0

§ ∂ψ ¨¨ © ∂r

· − Vβ csc 2µ ¸¸ ¹ ψ =0

§ ∂ψ ¨¨ © ∂r

· =0 ¸¸ ¹ ψ =0 (12-29)

From the above equations, the velocity equation along the characteristics line α and line β are obtained as follows α line group: dV + ªV cot§π −ϕ · −V csc §π −ϕ ·º dψ = 0 uni¸ β uni¸» α «α ¨ ¨

©2 ¹ ©2 ¹¼ ¬ β line group: dV +ªV csc§π −ϕ · −V cot§π −ϕ ·º dψ =0 β « α ¨© 2 uni ¸¹ β ¨© 2 uni¸¹» ¬ ¼

(12-30a) (12-30b)

It is the velocity field of the unified characteristics line theory for axisymmetric problem.

12.5 Applications of the Unified Characteristics Field Theory

331

12.5 Applications of the Unified Characteristics Field Theory Example 1. Circular Cone under Compression A circular cone under compression is shown in Fig. 12.6. The top radius of the circular cone is 20mm and the side face at rest has the oblique angle 45 0 from axis r. The material parameters are: E = 210 GPa, C 0 = 120MPa, and ĳ 0 = 0. Assuming that the contact surface is smooth, determine the characteristics line field and the limit loading of an circular cone during compression based on the unified characteristics line field theory.

Fig. 12.6. Characteristics line field of circular cone under compression

Only the right part of the cone should be considered because of axisymmetry. π Due to ϕ 0 = 0 it can be obtained that ϕ t = 0 and µ = , which shows that the 4 characteristics lines are orthogonal with each other. According to this condition , the characteristics lines can be expressed as dz

π

= tan(θ − ) dr 4 dz π = tan(θ + ) β line group: dr 4 It can derive t he governing differential equations α line group:

α line group β line group:

∂P ∂ Sα ∂P ∂ Sβ

− 2R + 2R

∂θ ∂ Sα ∂θ

=

R ∂r ∂ z [(m − 1) + ] r ∂ Sα ∂ Sα

R ∂r ∂z = − [(1 − m) + ] r ∂ Sβ ∂ Sβ ∂ Sβ

(12-31a) (12-31b)

(12-32a) (12-32b)

If the parameter m is 0.5, the differential terms in Eq. (12-32) are substituted by differential coefficient terms and Eq. (12-32) can be solved by numerical integral. The stress field is divided into three regions I, II and III, which correspond to the sides AB and AC, AC and AD, AD and AO, resperctively.

332

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Firstly, we begin to construct the characteristics line field of the region I from no-stress side AB and get the values P and θ of the region. There are P = − R , 3π on the side AB. σ1 = σ 2 = 0 , σ 3 = 2R and θ = 4 Secondly, for the singularity of point A, the characteristics lines field of the region II is constructed with lines α and lines β which is orthogonal to lines α . The two families of lines form a center fan of characteristics line at point A. Finally, we can find that the characteristics line field of the region III is dependent on the sides AO and AD, and the value θ is zero along the side AO. Therefore, the values P and θ can be derived in the region II. If the total loading acted on the top surface is divided by the area of the surface, the ultimate pressure q can be obtained. The unified characteristics line field with b = 1 is shown in Fig. 12.6 for the circular cone of top angle 450 . In order to confirm the results of the theory, the elasto-plastic finite element program UEPP based on the unified strength theory (UST) is used to compute the limit loading q of the same cone. The relation between limit loading q and parameter b is shown in Fig. 12.7 with the two methods. Curve 1 is the solution of the characteristics line theory for spatial axisymmetric problem, curve 2 is the result from finite element method; curve 3 is the solution of the slip line theory for plane strain problem. From the Fig. 12.7, we can find that the result from the characteristics line theory are very chose to those from the two computer programs . When b = 0.8, the limit loading with the new method is close to the experiment data in Suh, Lee and Rogers (1968).

Fig. 12.7. Relation curves between limit loading

q and strength criterion parameter b

The relation between loading q A and displacement δ at the top point A is calculated with the finite element program UEPP. The two curves in Fig. 12.8 show that the limit loading of spatial axisymmetric problem (curve 1) is little bigger than that of plane strain problem (curve 2), which are close to the results in Fig. 12.7.

12.5 Applications of the Unified Characteristics Field Theory

Fig. 12.8. Relation curves between displacement δ and loading

333

qA

Example 12.2. Semi-Infinite Body under the Circular Punch Pressure q A semi-infinite body under the circular punch pressure q on the free surface is shown in Fig.12.9. The radium of the pressure region is 2m. The parameters are 0 c0 = 0.3MPa and ϕ 0 = 15 .

The right part of the characteristics line field is shown in Fig.12.9 when b = 1 (the twin-shear strength theory, Yu 1985). The relations between q / c0 and b is shown in Fig. 12.10. They are obtained by using the unified characteristics line field theory (curve 1) and the unified slip field theory (curve 2). The solution at b = 0 (q/c0 = 13.9) in Fig.12.10 is the complete solution of Cox (1961), which is based on the Haar von-Karman condition and the Mohr-Coulomb strength theory .

Fig. 12.9. Semi-infinite body under the compression and the characteristics line field

334

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Fig. 12.10. The relation between the limit loading

q

and the parameter

b

A series of results can be introduced for the SD materials with the different tensile-compression strength ( ϕ 0 ≠ 0 ) and the non-SD materials with same tensilecompression strength ( ϕ 0 = 0 ) by the unified characteristics line field theory. The solutions of the Mohr-Coulomb material and Tresca material are special cases of the solutions of the unified characteristics line theory.

12.6 Penetration of High Velocity Rod to Target 12.6.1 Penetration problems of long rod Much research has been reported on impact and penetration problems because of their importance in modern engineering applications and protective engineering. Due to the experimental, analytical and computational complexities involved in general cases, attention has been paid to the penetration of a long-rod, with different impact velocities, into a target. Studies on this subject are mainly based on tests and supplemented with analytical or numerical methods. The analytical models began with the work of Bishop et al. (1945), who developed equations for the quasi-static expansion of cylindrical and spherical cavities and used these equations to estimate forces on conical nose punches pushed slowly into metal targets. Later, Hill (1950) and Hopkins (1960) derived and discussed the dynamic, spherically symmetric, cavity-expansion equations for an incompressible target material. The cavity expansion theory was further developed by Luk and Forrestal (1987), Forrestal and Tzou (1997), Xu et al. (1997) and Mastilovic and Krajcinovic (1999) to model the penetration of projectiles through soil, porous rock, ceramic and concrete targets. Based on the characteristics line theory, Simmons et al. (1962) investigated the deformation of thin plates subjected to high-impact loads. Slip line field theory is used by Wijk (1999) to find the penetration resistance on the rod. An

12.6 Penetration of High Velocity Rod to Target

335

overview on projectiles penetrating into geological targets was given by Heuze (1990). The dynamic failure mechanism of concrete is intricate since discontinuities such as cleavage cracks and defects with different shapes and orientations are commonly encountered in concrete and they have significant influence on the deformation and failure characteristics of concrete. The initially existing cracks and defects will be nucleated, and will evolve until material loses strength, when subjected to dynamic loading. The damage theory has been considered to be more suitable for the cleavage analysis of the concrete material (Krajcinovic, 1996; Lorrain and Loland, 1983). In the previous studies of the impact and penetration to concrete target, the commonly used constitutive models are elastic-plastic and/or brittle damage models (Luk and Forrestal, 1987; Forrestal and Tzou, 1997; Xu et al., 1997; Mastilovic and Krajcinovic, 1999), where elastoplasticity and damage are treated separately. How to define the failure criterion of the targets is critical for better analyzing penetration problems (Zukas et al., 1978). The failure criteria such as the MohrCoulomb strength theory and the Tresca yield criterion were often applied to penetration problems, as can be seen from the above references. These criteria do not consider all of the stress components in stress space. The effect of intermediate principal stress is not taken into account in the Tresca criterion and the MohrCoulomb strength theory, which are not consistent with the test results of many materials. A unified strength theory, which was suggested by Yu (1991), considers all of the components in stress space. It covers a series of strength theories, such as the Mohr-Coulomb’s single-shear strength theory and the twin-shear strength theory when the tension and compression strengths of materials are different, as well as the Tresca criterion, the Huber-von Mises criterion and the twin-shear criterion when the tension and compression strengths of materials are the same. The unified strength theory was applied to model penetration problem by Yu, Li and Wei (see Yu 2002a), and a unified plasticity-damage penetration model related to the crack density is proposed. The relation between radial traction and velocity at cavity-surface can be obtained by analyzing the distributions of stress and velocity of the target material. Based on the cylindrical cavity expansion theory and spatial axisymmetrical unified characteristics line theory, the attacking capability of a long-rod can be assessed from the derived relation as the rod impacts and penetrates the target with initial velocities of 300 ~ 1100 m / s . The results are compared with those of the experiments available in the open literatures.

12.6.2 Damage modeling of target material For the present problems, the cracks of the target are mainly caused by tensile stress waves and developed along the radial orientation (Forrestal and Tzou, 1997; Xu et al., 1997; Mastilovic and Krajcinovic, 1999). Therefore, a damaged loading surface is defined based on an equivalent tensile strain. When concrete material is subjected to tension, it will not fail unless the value of the stress is larger than its tensile strength, assuming the damage is caused by the activation and growth of

336

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

initially existing micro cracks. Although the damage evolution is rate-dependent in general (Chen et al., 2001), it is assumed that the damage evolution in this paper is rate-independent and isotropic for the purpose of simplicity. The definition of effective stress σ ∗ by Kachanov (1986) is used and mode I cracking is considered. Since the penetration damage is accumulated as a function of time and applied stress, crack density is expressed as a function of the equivalent tensile strain and time which is similar to the model proposed by Liu and Katsabanis (1997)

c f = m1 < ε − εcr > m2 t

(12-33)

where the angular bracket < ⋅ > denotes the function is valid only when the value inside the bracket is larger than zero, cf is the total number of cracks per unit volume, m 1 and m 2 are material constants, ε cr is the static critical tensile strain which can be easily determined from uniaxial static tensile test results ( ε cr = σ st E ), and t represents the accumulated time in the evolution of damage. According to the definition suggested by Whittaker et al. (1992), the scalar damage ω is related to the crack density cf and expressed as ω = 1− e

− c f Vl

(12-34)

where Vl is the damaged volume. If the maximum principal strain is less than the critical value ε cr , there is no damage in the target and the probability of fracture is equal to zero. On the other hand, if the maximum principal strain exceeds ε cr , the material stiffness will degrade, based on the research by Huang et al. (1994).

12.6.3 Fundamental equations of the target A cylindrical symmetric cavity is expanded from an initial radius of zero at velocity v0r = v0r (t ) , as a rod penetrates a target. The expansion of cavity produces four regions of response as shown in Fig.12.11. The four regions are: (1) plastic region (the material reaches unified strength theory, v0rt ≤ r ≤ ct ); (2) damaged region (the material reaches its tensile strength, ct < r ≤ c1t ); (3) elastic region ( c1t < r ≤ cd t ) and (4) an undisturbed region ( r > cd t ). 0

vr is the cavity-expansion rate, which is rate-dependent and decreased with time t . c and c1 are interface velocities. c d is the elastic, dilatation velocity. r is radial Eulerian coordinate. There are three principal stresses, σ r , σ θ and σ z , which are radial, circumferential and axial stress components (positive in compression) and σ r ≥ σ z ≥ σθ for the problem.

12.6 Penetration of High Velocity Rod to Target

337

non-disturbed elastic damage plastic 0

vr t

ct

c1t

cdt

Fig. 12 .11. Cylindrical cavity-expansion

The target material is considered to be compressive and is assumed to satisfy linear pressure-volumetric strain relation σ m = K ε v = K (1 − ρ 0 ρ )

(12-35)

where ρ 0 and ρ are densities of the original and deformed material, respectively, ε v is the volumetric strain, K is the bulk modulus and σ m is given by σm =

σ r + σθ + σ z

3

(12-36)

According to the material characteristics of a cylindrical cavity-expansion, the strength theory can be deduced when the material comes into a plastic yielding state, namely σ r − σθ = At σ r + Bt

(12-37)

with

At =

2sin ϕ t , Bt = 2ct cos ϕt 1 + sin ϕ t 1 + sin ϕt

(12-38)

The equations of mass and momentum conservation in cylindrical coordinates take the forms of

1 dρ ∂v v , + =− ∂r r ρ dt

(12-39a)

∂σ r 1 dv + ( σ r − σθ ) = − ρ ∂r r dt

(12-39b)

338

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

At the two interfaces r = c1t and r = ct , the target material satisfies the Hugoniot jump condition that mass and momentum across the interface remain conservative,

[ ρ (v − vJ )] = 0 ,

(12-40a)

[σr + ρ v(v − vJ )] = 0

(12-40b)

where the brackets [...] stand for the magnitude of the discontinuity of the bracketed variable across the wave front (interface) that propagates with the velocity vJ .

12.7 Elastic-Damage-Plastic Analysis of the Target Define E0 , K 0 , ν 0 and E , K , ν to be the Young’s modulus, bulk modulus and Poission’s ratio of the original and damaged materials, respectively. Because an isotropic model is used, only two of three moduli are independent. σ r1 and σ r 2 , v1 and v2 , ρ1 and ρ 2 are the dimensionless radial stresses, velocities and densities of the damaged and plastic regions at r = ct , respectively. σ r 3 and σ r 4 , v3 and v4 are the dimensionless radial stresses and velocities of the elastic and damaged regions at r = c1t , respectively. σ ri = σ ri / K 0 , vi = vi / c and ρ j = ρ j / ρ 0 ( i = 1 ~ 4 , j = 1 ~ 2 ) are used for the dimensionless variables.

12.7.1 Elastic region ( c1t ≤ r ≤ cd t ) According to the linear elastic stress-strain relations, E0 ∂u uº ª °σ r = − (1 − 2ν ) (1 + ν ) «(1 − ν 0 ) ∂r + ν 0 r » ¼ 0 0 ¬ °° (12-41) ® ° ∂u º E0 u ª (1 − ν 0 ) + ν 0 » ° σθ = − (1 − 2ν 0 ) (1 + ν 0 ) ¬« ∂r ¼ r °¯ and Eq. (12-39), the differential equation of wave can be derived, with the dimensionless variables ξ = r ct and u = u ct , as follows: (1 − λ 2 ξ 2 )

d 2u dξ 2

+

1 du ξ dξ

−

1 ξ

2

u =0

(12-42)

12.7 Elastic-damage-plastic Analysis of the Target

339

where λ = c cd and u is radial particle displacement. The boundary conditions are u (r = cd t ) = 0 , σθ (r = c1t ) = − σ f

(12-43)

Solving Eqs. (12-42) and (12-43), the radial velocity and stress in the region can be found to be ª 1 − λ 2ξ 2 λξ 1 + 1 − λ 2ξ 2 º 1 du »G = −« + ln λξ c dt 2 « 2λξ » ¬ ¼

(12-44a)

1 − λ 2ξ 2 λ 1 + 1 − λ 2ξ 2 σ 3 [(1 − 2ν0 ) + ln σ r (ξ ) = r = − ]G λξ 1 +ν 0 2 K0 2λξ 2

(12-44b)

v(ξ ) =

where η = c c p , η1 = c1 cp , cp = K 0 ρ 0 , σ f is the static tensile strength of the material, and σ ª 3(1 − 2ν 0 ) η η 2 − λ 2η12 η + η 2 − λ 2η12 º 3λ » ln ⋅ − G=− f « 2(1 + ν 0 ) K0 « 1 + ν 0 λη1 » 2λη12 ¬ ¼

−1

(12-45)

12.7.2 Damaged region ( ct ≤ r ≤ c1t ) As the cracks appear and develop along the radial direction, the circumferential stress is zero, that is, σθ = 0 . The density ρ of the deformed material is a function of the scalar damage ω . At r = c1t , the material comes into plastic yielding, the radial stress can be expressed as σ r1 =

Bt 1 − At

(12-46)

where Bt = Bt K 0 . The distributions of the dimensionless stress and velocity, and the relationship between η1 and η can be derived from Eqs. (12-35) and (12-36) and Eq. (12-39), as ε v is very small and 1 − ε v ≈ 1 . σ r (ξ ) = − t1 ξ + t2 2

v(ξ ) = − t2 (η ξ ) + (1 + ν )t1 (3K )

(12-47) (12-48)

340

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

η12 (1+ν )σr4 + 3Kη1 ⋅ η v4

Bt = (1 − At )K0

2

η (1 +ν ) − 3K

η η ⋅η v4 + σr4 (12-49) − 3K ( 1 ) ⋅ 21 η η (1 +ν ) −3 K

where η

t1 = 3K ( 1 ) ⋅ η

t2 =

η1 ⋅ η v4 + σ r4

η 2 (1 +ν ) − 3K

η12 (1 + ν )σ r4 + 3Kη1 ⋅ η v4 η 2 (1 + ν ) − 3K

K = K K0

(12-50a) (12-50b) (12-50c)

12.7.3 Elastic-damaged and plastic-damaged interface ( r = c1t and r = ct )

The relations between radial stresses and velocities at r = c1t can be derived from Eq. (12-34) and Eq. (12-39), σ r 4= σ r3 +

3(η1 − η v3 )(η v4 − η v3) 3 − (1 + ν 0 )(σ r 3 − σ f )

η v4 = η v 3 +

1 +ν σ r4 ] K 3 − (1 +ν 0 )(σr3 − σ f )

(η1 −η v3)[(1 +ν 0 )(σr3 − σ f ) −

(12-51a)

(12-51b)

From Eqs. (12-35)~(12-37) and Eq. (12-40), the radial stress, velocity and density at r = ct can be obtained as below σ r2 =

2K [2K − ρ1(2K + Bt )]ρ1η 2 (1 − v1)2 σr 1+ 2K + 2 − At 2 K + 2 − At

2 2 2 2 ρ σ (2 − At) + ρ1 η (v1 −1) (2 − At) − ρ1(2K + Bt) +1 v2 = (v1 −1) ⋅ 1 r1 2 2 2 ρ1 η (v1 −1) (2 − At ) − 2K

ρ2 =

ρ1η 2 (1 − v1)2 (2 − At ) − 2K

σ r1(2 − At ) + ρ1η 2 (1 − v1 )2 (2 − At ) − (2K + Bt )

(12-52) (12-53) (12-54)

12.7.4 Plastic region ( v0rt İ r İ ct ) The boundary conditions are v(ξ = v0r c) = v0r c , v( r = ct ) = v2 , σ r (r = ct ) = σ r 2

(12-55)

12.7 Elastic-damage-plastic Analysis of the Target

341

The differential forms of radial stress and velocity can be derived, from Eqs. (1240), (12-35) and (12-37), to be dv 2 K (1 − ε v )2 v + (2 − At )( Atσ r + Bt )(ξ − v)(1 − ε v ) = 2 2 2 dξ ξ [(2 − At )η (ξ − v) − 2 K (1 − ε v ) ] dσ r 2 K (1 − ε v )[( Atσ r + Bt )(1 − ε v ) + η 2 (ξ − v)v] = 2 2 2 dξ ξ [(2 − At ) η (ξ − v) − 2 K (1 − ε v ) ]

(12-56) (12-57)

where ε v = [(2 − At )σ r − Bt ] (2K ) . The numerical solutions of Eqs. (12-55) and (12-56) for the plastic region can be got by using Runge-Kutta method. The radial stress and velocity of the cavity surface can be obtained when the condition v (ξ = v0r c) = v0r c is satisfied.

12.7.5 Solution procedure and the normal penetration dept For the purpose of simplicity, the solution is obtained with an inverse procedure from the elastic region to the plastic region, because the boundary condition of the cavity surface is unknown. The procedure is summarized as follows: (1). The mathematical expressions of v3 and σ r 3 in elastic region can be found from Eqs. (12-44a) and (12-44b). The mathematical expressions of v 4 and σ r 4 in damaged region can be found from Eqs. (12-50a) and (12-50b). The relationship between η 1 and η can be got when the above expressions v3 , σ r 3 , v 4 and σ r 4 are inserted into Eq. (12-48). (2). Choose a value for η and calculate η 1 from the relationship between η 1 and η. (3). The values of v3 , σ r 3 , v 4 and σ r 4 can be obtained by substituting η 1 and η into Eqs.(12-44a), (12-44b), (12-50a) and (12-50b). v 2 and σ r 2 can be derived by substituting v1 and σ r 1 into Eq.(12-51) to (12-53). (4). The calculations of Eqs. (12-55) and (12-56) are proceeded from the plasticitydamage interface ξ = 1 to the cavity surface ξ = v0r / c . The particle velocity and radial stress in the plastic region can then be obtained. When the boundary 0 condition v ξ = v0 c = v0r / c is satisfied, the value of v r corresponding to the chosen r value of η is determined. Since η vr0 = v0r / c p , v0r / c p can be obtained. An inverse procedure is used to calculate the interface velocity and the cavity-expansion velocity. The relation between the radial stress σ r0 and the cavity-expansion velocity v0r can then be obtained.

342

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

(5). After the numerical relationship between v0r and σ r0 are obtained, a mathematical penetration expression of σ r0 versus v0r can be deduced by curve fitting methods.

12.7.6 Final depth of normal penetration When a long-rod with an ogival nose penetrates vertically into a semi-infinite concrete target, f n and fτ are normal force and tangential force. Tangential force fτ = µ ⋅ f n , where µ is the friction parameter. The ogival nose is shown in Fig. 12.12, where s is the radius of the rod, and θ 0 and θ 1 are the center angles of the top and the side surface of the rod, respectively. Following Forrestal and Tzou (1997) it is assumed that the normal force f n on the ogive nose is actually equal to the force σ r0 (v0r ) needed to expand the cavity at 0 the rate vr . Letting Vz to be the penetration velocity of the rod, we have

vr0 = Vz ⋅ cosθ 1

(12-58)

If the rod is assumed to be rigid and the shank side resistance is neglected, the final normal depth after the rod completely penetrates into the target can be derived 0 0 from v r versus σ r and the Newton’s second law, namely zmax =

where m2 = 2 π s 2 A1K0

³

n2 = 2π s2 A3ρ 0

³

M n2 ln 1 + ⋅ V02 2n2 m2 − Mg 90 0 θ0

(12-59)

(sinθ 1 − sinθ 0 )(cos θ1 + µ sinθ 1)dθ 1 ,

900 ϑ0

(sinθ 1 − sinθ 0 )(cos θ 1+ µ sinθ 0 )cos2θ 1 dθ 1 , A1 and A3 are the

coefficients of curve-fit v0r versus σ r0 , M is the mass of the rod, and V0 is the impact velocity of the rod.

12.8 Comparison and Verification

343

Vz

r fn

s s

θ0 θ1

fτ

Fig. 12.12. Geometry of rod nose and traction components

12.8 Comparison and Verification A special concrete considered by Mastilovic and Krajcinovic (1999) is defined with the following parameters, ν 0 = 0.22 , E0 =11.3GPa , ρ 0 = 2260Kg / m3, σ f = 13MPa and µ = 0.1. The parameters of a long-rod with an ogival nose are M =1.6Kg , s = 0.0915m and the radius of the rod shank a = 0.0153 m. According to the test data (Forrestal and Tzou, 1997) and some of the numerical investigations of the damage evolution pattern (Mastilovic and Krajcinovic, 1999), the damage value is about 0.23 when the dynamic tensile stress reaches the dynamic failure stress, implying c f Vl can be derived. The degraded moduli due to damage can be obtained from the analysis of Huang et al. (1994). The relations of the plastic-damaged interface velocity c versus cavityexpansion velocity v0r and v0r versus σ r0 can be derived by using the methods from steps (1) to (5), which are described in 12.7.5. The relations are shown in Fig. 12.13 and Fig. 12.14. It is shown that the plastic-damaged interface velocity c is increased with the increase of expansion velocity v0r , as shown in Fig. 12.13. The radial stress σ r0 is also incresed with the expansion velocity v0r as shown in Fig. 12.14. For the same cavity-expansion velocity v 0r , the radial stress at cavity surface is changing for the different values of strength criterion parameter b . The radial stress σ r0 is increased with the increase of parameter b . The dimensionless radial stress σ r0 ( σ r0 = σ r0 / K 0 ) can be expressed as a second order polynomial of v0r K0 / ρ 0 , that is,

344

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

σ r 0 = A1 + A2 (v0r

K0 / ρ 0 ) + A3(v0r

K 0 / ρ 0 )2

(12-60)

0.8

c/c p

0.6 0.4

b=0.0 b=0.5 b=1.0

0.2 0.0 0.00

0.05

0.10

0.15

0.20

0.25

0.30

0.35

0.40

v r0 /c p Fig.12-13. Plastic-damage velocity vs cavity-expansion velocity 1.4 1.400000021 1.200000018 1.2

b=1.0 b=0.5 b=0.0

σr /K0

1.000000015 1.0

0

0.8 0.800000012 0.6 0.600000009 0.4 0.400000006 0.2 0.200000003 0.000000000 0.0

0.000000000 0.100000001 0.0 0.1 0.200000003 0.3 0.400000006 0.4 0.2 0.300000004

v r0 /c p Fig.12.14. Radial stress vs velocity of cavity-expansion

According to the conditions σ r0

v0r = 0

0 = σ r0st and dσ r

d v0r

=0,

(12-61)

v0r = 0

where σ 0rst is the dimensionless radial traction of quasi-static cavity-expansion. It 0 can be found that A1 = σ rst and A2 = 0. The value of σ 0rst can be derived from the spatial axisymmetric unified characteristics line theory (Yu et al., 2001). The spatial axisymmetric characteristics lines at the contact surface is shown as

12.8 Comparison and Verification

345

Fig. 12.3, in which the effect of surface friction is not taken into account. Based on the spatial axisymmetric characteristics line theory, we can get: (1) A1 = 0.03377 when b = 1; (2) A1 = 0.03203 when b = 0.5, which is close to the quasi-static cavity-expansion 0 radial limit stress σ rst = 0.0323 of Mastilovic and Krajcinovic (1999); (3) A1 = 0.03072 when b= 0. The value A3 can be obtained from the curve of Vr0 vs σ r0 , that is, A3 = 6.8~7.0 (when b = 1), A3 = 4.5~4.7 (when b = 0.5) and A3 = 2.2~2.5 (when b = 0). The final depths for the different values of strength criterion parameter b can be derived from Eqs. 12-58, 12-59 and 12-60. They are shown in Fig. 12.15. 3.0 2.5

z max (m)

2.0

b=0.0 b=0.15 b=0.5 b=1.0 test data

1.5 1.0 0.5 0.0 200

400

600

800

1000

1200

V0 (m/s) Fig. 12.15. Final depth vs initial impact velocity of long rod

When the impact velocity is V0 = 300m / s , the final depths Zmax = 0.236m for b = 1 are close to the test data Zmax = 0.23m (Forrestal and Tzou, 1997). When the impact velocity is V0 = 700m/s, Zmax = 0.915m for b = 0.5 are close to the test data Zmax = 0.9m. When the initial impact velocity is V0 = 1100m/s, Zmax = 2.02m for b = 0.15 are close to the test data Zmax = 2.06m. The penetration depths of the rod are situated within the area of 0 < b < 1. Fig. 12.16 shows the relationship between the rod mass and the final penetration depths when b = 1.0. The rod penetrates more deeply if its mass is heavier. The effect of the mass on the finial depth is more obvious when the initial impact velocity of the rod is higher. One reason why tungsten alloy rods (Rosenberg, 1997) are usually applied in modern arms is that their densities are higher.

346

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

2.5

V0=1100m/s V0=700m/s V0=300m/s

zmax (m )

2.0

1.5

1.0

0.5

0.0

1.5

1.8

2.1

2.4

2.7

M (Kg) Fig. 12.16. Final depth vs mass of the rod

Summary The characteristics line theory for spatial axisymmetric plastic problem is very important in the plasticity and engineering. The unified characteristics line field theory of spatial axisymmetric problem and its applications are described in this chapter. The effects of the intermediate principle stress σ2 and the SD effect of materials are taken into account in the unified characteristics field theory. A series of characteristics line field for spatial axisymmetric problem suitable for different kinds of materials can be derived from the new theory, the previous theories are special cases or linear approximation of the unified characteristics line theory. The new theory can be applied to the limit analysis of spatial axisymmetric plastic problems in plasticity and engineering. Based on the cylindrical cavity-expansion theory and the unified strength theory, a unified plastic-damage model is proposed for penetration problems. The proposed model is used to simulate penetration of a long-rod into a concrete target. The spatial axisymmetric characteristics line theory is used for the analysis of quasi-static normal penetration of a long-rod. The results show that: (1) The rod mass has obvious affect on the final penetration depth; (2) By comparison with the available test date, it appears that the proposed procedure is effective for penetration analysis. The test results are situated within the analysis results (0 < b < 1); (3) When the initial impact velocity of a rod is higher than 1500m/ s , the material behaviour and penetration process of rods and targets will change significantly.

Problems

347

Problems Problem 12.1 The characteristyics fields for indentation of a circular head punch are shown in Fig. P12.1. The limit pressures was obtained by using the Tresca yield criterion as follows. p b= σ s (1+ π ) 4 Find the limit pressure of indentation of a circular head punch by using the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1). .

Fig. P12.1. Circular head penestration into half space

Problem 12.2 Find the limit pressure of indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1).

Problem 12.3 The characteristyics fields for indentation of a circular head punch are shown in Fig. P12.2. This problem was studied by Hill (1950) Prager-Hodge (1951) and Levin (1953) by using the Tresca yield criterion. A is a initial situation; b is the indentation of the circular head; c is the deep indentation of the circular head and bar. The limit pressures are:

p b = σ s (1+ π ) and pc = σs (1 + 3π ) . 4 4 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1) .

348

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Fig. P12.2. Circular head penestration into infinit surface

Problem 12.4 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1) .

Problem 12.5 The characteristyics fields of indentation for non-SD materials under a circular head punch with a uniform pressure q shown in Fig. P12.3. The limit pressures was obtained by using the Tresca yield criterion. Find the limit pressure of indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for non-SD materials (α = 1, and b = 0, b = 1/2, b = 1).

Fig. P12.3. Slip field under circular foundation for non-SD materials

Problem 12.6 Find the limit pressure of deep indentation of a circular head punch by using the the unified characteristics line field theory of spatial axisymmetric problem for SD materials (α ≠ 1, and b = 0, b = 1/2, b = 1).

References and Bibliography Bishop RF, Hill R and Mott NF (1945) The theory of indentation and hardness tests. The Proc. of the Phys. Soc. 57(3): 147–159. Chen WF (1975) Limit Analysis and Soil Plasticity. Elsevier, Amsterdam, New York.

References and Bibliography

349

Chen Z, Deng M and Chen EP (2001) Rate-dependent transition from the tensile damage to discrete fracture in dynamic brittle failure. Theoretical and Applied Fracture Mechanics. 35(3): 229–235. Collins IF, Dewhurst P (1975) A slip line field analysis of asymmetrical hot rolling. International Journal of Mechanical Science, (17): 643 . Forrestal, M. J., Tzou, D. Y., 1997. A spherical cavity-expansion penetration model for concrete targets. Int. J. Solids Structures 34, 4127-4146. Heuze FE (1990). An overview of projectile penetration into geological materials, with emphasis on rock. Int. J. Rock Mech. Min. Sci. and Geomech. Abstr. 27 (1), 1–14. Hill R (1950). The mathematical theory of plasticity. Clarendon Press, London. Hopkins HG (1960). Dynamic expansion of spherical cavities in metal. In: Progress in Solid Mechanics, Vol. 1, Chapter III, ed. I. N. Sneddon and R. Hill. North-Holland Publishing Company, Amsterdam, New York. Ishlinsky AYu (1944) Axisymmetrical plasticity problem and Brinell test. Appl. Math. Mech. 8 (in Russian). Johnson W, Sowerby R, Venter RD (1982) Plane strain slip line fields for metal deformation Processes-A source book and Bibliography. Oxford: Pergamon Press,. Kachanov LM (1975) Foundations of the Theory of Plasticity. North-Holland, London,. Kachanov LM (1986) Introduction to continuum damage mechanics. Martinus Nijhoff Publishers, Dordrecht, The Netherlands. Krajcinovic D (1996). Damage Mechanics. Elsevier, Amsterdam. Liu L, Katsabanis PD (1997). Development of a continuum damage model for blasting analysis. Int. Journal of Rock Mech. Min. Sci. 34, 217–231. Lorrain M and Loland KE (1983) Damage theory applied to concrete. Fracture Mechanics of Concrete, Edited by Writtmann. Luk VK and Forrestal MJ (1987) Penetration into semi-infinite reinforced-concrete targets with spherical and ogival nose projectiles. Int. J. Impact Eng. 6 (4): 291–301. Levin E (1953) Indentation pressure of a smooth circular punch. Quarterly. Appl. Math., (13), 133. Mastilovic S and Krajcinovic D (1999). High-velocity expansion of a cavity within a brittle material. Journal of the Mechanics and Physics of Solids 47, 577-610. Rosenberg Z, Dekal E, Hohler V, et al. (1997). Hypervelocity penetration of tungsten alloy rods into ceramic tiles: experiments and 2-D simulations. Int. J. of Impact Engineering 20, 675-683. Shield RT (1955) The Plastic Indentation of a Layer by a Flat Punch. Quarterly. Appl. Math., (13), 27. Simmons JˈHauser F, Dorn JE (1962) Mathematical Theories of Plastic Deformations under Impulsive Loading. Cambridge University Press, London, England. Sokolovsky VV (1960) Statics of Cohesionless Medium. Publ. Books on Phys. Math. Moscow (in Russian). Suh, NP., Lee RS., Rogers CR (1968).. The Yielding of Truncated Solid Cones under Quasi-Static and Dynamic Loading, J. Mech. Phys. Solids 16, 357. Szczepinski W (1979).. Introduction to the Mechanics of Plastic Forming of Metals. Sijthoff and Noordhoff, Netherlands,. Whittaker KT, Singh RH and Sun D (1992). Rock fracture mechanics principles, design and applications. Elsevier, Amsterdam. Wijk AG (1999). High-velocity projectile penetration into thick armor targets. Int. J. Impact Eng. 22, 45-54. Xu Y, Keer LM, Luk VK (1997) Elastic-cracked model for penetration into unreinforced concrete targets with ogival nose projectiles. Int. J. Solids Structures 34(12), 1479–1491. Yu MH, He LN, Song LY (1985) Twin shear stress theory and its generalization, Scientia Sinica (Science in China), English Edition, Series A, 28(11): 1113–1120. Yu MH, He LN (1991) A new Model and Theory on Yield and Failure of Materials Under Complex Stress State, Mechanical Behaviors of Materials̚6, Pergamon Press, Vol. 3: 841–846. Yu MH (1992) New System of Strength Theory. Xi’an Jiaotong Universitry Press, Xi’an (in Chinese). Yu MH (1994) Unified strength theory for geomaterials and its applications. Chinese J. Geot. Eng. 16(2): 1–10, (in Chinese, English Abstract).

350

12 Unified Characteristics Line Theory for Spatial Axisymmetric Problem

Yu MH, Yang SY, et al (1997). Unified Plane-strain slip Line field theory system. Chinese J. Civil Engineering, 30(2): 14̚26 (in Chinese, English Abstract) . Yu MH (1998) Twin Shear Theory and its Application. Science Press, Beijing 892 pp. (in Chinese). Yu MH, Li JC and Zhang YQ (2001) Unified characteristics line theory of spatial axisymmetric plastic problem. Science in China (Series E), English edn. 44(2), 207–215; Chinese edn. 44(4), 323–331. Yu MH (2002a) Concrete Strength Theory and Its Applications. Higher Education Press, Beijing (in Chinese). Yu MH (2002b) Advances of strength theories of materials under complex stress state in the 20th Century. Applied Mechanics Reviews, 55(3): 169-258. Zhao DW, Xu JZ, Yang H., et al (1998) Application of Twin Shear Stress Yield criterion in axisymmetric Indentation of a Semi-Infinite Medium. In : Strength Theory Science Press, New York, Beijing, 1079-1084. Zukas JA, Nicholas T, Swift HF, et al. (1982). Impact Dynamics. Wiley, New York. Ȼɟɪɟɡɚɧɥɟɜ ȼȽ (1952) Ɉɫɟɫɢɦɦɟɬɪɢɱɧɚɹ Ɂɚɞɚɱɚ Ɍɟɨɪɢɢ ɉɪɟɞɟɥɶɧɨɝɨ Ɋɚɜɧɨɜɟɫɢɹ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. Ɇɨɫɤɜɚ: Ƚɨɫ. ɂɡɞ. Ɍɟɯ. Ɍɟɨ. Ʌɢɬɟɪɚɬɭɪɵ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1942) ɋɬɚɬɢɤɚ ɋɵɩɭɱɟɣ ɋɪɟɞɵ. ɂɡɞ. Ⱥɇ ɋɋɋɊ, Ɇɨɫɤɜɚ (in Russia) ɋɨɤɨɥɨɜɫɤɢɣ BB (1960) ɋɬɚɬɢɤɚ ɋɵɩɭɟɣ ɋɪɟɞɵ (Third ed.).Ƚɨɫ. ɂɡɞ. Ɏɢɡ-Ɇɚɬ. Ʌɢɬɟɪɚɬɭɪɵ. Ɇɨɫɤɜɚ (in Russia)

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

13.1 Introduction Estimation of the crack-tip plastic zone under small-scale yielding ( SSY ) is one of the important topics in elastic-plastic fracture mechanics. Literatures show that researchers have endeavored in finding the shape and size of mode-I, -II and -III crack-tip plastic zone under SSY. Dugdale (1960) and Barenblatt (1962) independently introduced their model representing a yield-strip or cohesive-strip zone around a crack-tip. It is called Dugdale yield-strip model or cohesive model. On the other hand, Irwin (1960) suggested an approximation method by increasing the effective length of a crack based on the anti-plane elastic-perfectly-plastic solution as well as Hult and McClintock (1957). It is known as the Irwin’s plastic-zone correction model. The shape and size of yielding zone were derived from the Huber-von Mises criterion. Irwin (1968) further extended his model for plane-strain condition by enhancing the yield stress by a factor of 3 . Broek (1982) presented his estimation using the Tresca criterion. The above-mentioned models are all based on the SSY condition and are constructed with the assumptions in the linear elastic fracture mechanics (LEFM). They yield reasonably good estimations for certain materials such as metals having equal tensile and compressive strength. Recent investigations revealed that the Tresca criterion do not take into account the effect of the intermediate principal stress properly, while the Huber-von Mises criterion only puts in place the average effect of the three principal stresses. In other words, Tresca criterion is only applicable for those materials governed by a shear-stress limit ( Ĳ s = 0.5ı s ), so is the Huber-von Mises criterion for materials governed by another shear-stress limit ( Ĳ s = 0.58ı s ). The twin-shear yield criterion, which is equivalent to a different shear-stress limit ( Ĳ s = 0.67ıs ). It agrees well with the results ( Ĳ s = 0.7ı s ) reported by the British Royal Air Force who conducted multi-axial tests for four groups of nickel alloy at 750° Celsius (Winston, 1984). Later, a unified strength theory (UST) was proposed (Yu et al. 1991, 1992). An influence parameter ‘b’ for the effect of intermediate principal stress and the effect of intermediate principal shear-stress was put in place. The parameter ‘b’ normally varies between 0 and 1. The earlier twin-shear yield criterion is embraced as a special case (b=1). The UST unifies prevailing strength criteria through the variable parameter ‘b’, which actually bears a physical meaning as a material parameter. Adopting specific values of ‘b’ can lead to results equivalent to those

352

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

through Tresca criterion, Huber-von Mises criterion or its varieties. In addition, stretching beyond the normally admissible range (b1) can generate a new series of strength criteria for unconventional materials, which strength envelope may not necessarily be convex. Against this background, estimations of crack-tip plastic zone under SSY are re-investigated using the UST by Qiang in 1998. It provides unified solutions for shapes and sizes of mode-I, mode-II and mode-III crack-tip plastic zone in the K-dominant region. The minimum and maximum crack-tip plastic zones can be deduced through the normally admissible lower-bound (b = 0) and upper-bound (b=1) respectively. Adopting a proper value of the material parameter ‘b’ can lead to accurate solutions. Estimations of the crack-tip plastic zones using different values of ‘b’ are illustrated and compared, including those deductions equivalent to the Tresca and the Huber-von Mises criteria. The influences on the resulting plastic zone due to strength-differential (SD) effect and Poisson’s ratio are also studied. The investigation of the SD effect has practical significance because most materials have unequal tensile and compressive strength. The present approach is also extended to include some non-conventional materials under unsteady state. The definition of ‘conventional material under steady state’ refers to Drucker’s postulate that its failure/yield strength envelope is of convex shape in the stress space (i.e. the ʌ-space). The convexity condition is satisfied when 0 b 1. Beyond this conventionally admissible range (i.e. b < 0 or b > 1), the UST is ready to be applied to a whole spectrum of non-conventional materials, which strength envelope is not necessarily of convex shape. The shape and size of crack-tip plastic zone of those unconventional materials are also presented.

13.2 Unified Strength Theory The UST has been described in detail in Chapter 4. The mathematical modeling and the mathematical formulation are expressed as follows. F = τ 13 + bτ 12 + β ( σ13 + bσ 12 ) = C

when Ĳ 12 + ȕı 12

F ' = τ 13 + bτ 23 + β (σ 13 + bσ 23 ) = C when Ĳ 12 + ȕı 12

≥ Ĳ 23 + ȕı 23

≤ Ĳ 23 + ȕı 23

(13-1)

principal shear stresses and τ ij = (σi − σ j ) / 2 are the σ ij = ( σ i + σ j ) / 2 are the associated normal stresses. σ i (i =1,2,3) are the

where

principal stresses. ȕ is a coefficient which accounts for the effect of the corresponding normal stresses. Both ȕ and C are strength characteristics of a material, which values can be determined from standard experimental procedures for uniaxial tensile and uniaxial compressive tests. The relations are as follows:

13.2 Unified Strength Theory

353

where ıt and ıc are the uniaxial tensile and compressive strength respectively, Į = ı t /ı c is the strength ratio. This ratio is a measure of the strength

differential (SD) effect. Substituting Eq. (13-2) into Eq. (13-1) leads to the alternative expressions in terms of the principal stresses ıi, the tensile strength ıt and the strength ratio Į as follows. σ1 −

1 1+ b

α

1+ b

( b σ2 + σ 3 ) = σ t when

(σ1 + b σ 2 ) − ασ 3 = σ t when

σ2

σ2

≥

≤

σ 1+ασ 3

1+α σ 1 +ασ 3

(13-3)

1+α

Equation (13-3) shows that the UST not only takes into account the effect of the intermediate principal shear stress but also the SD effect. It is a function of the strength ratio Į. It can be seen from the envelope plotted in the diviatoric plane (see Fig. 13.1). It should be noted that the envelopes have symmetrical characteristics at 60°-intervals. For the sake of clarity, envelopes corresponding to different values of ‘b’ are plotted only in the diagonally opposite sector bounded by ș = 0° and ș = 60°. Along the radiation line rt (at ș = 0°), the limiting value is the tensile strength. Along the radiation line rc (at ș = 60°), the limiting value is the compressive strength. The UST criterion is a bi-linear surface approximation for the envelope between the radiation lines rt and rc. For values of ‘b’ ranging between 0 and 1, the shape of the whole envelope (0°ș < 360°) is convex. Outside this range (i.e. b < 0 or b > 1), the shape of the whole envelope become corrugated, and hence it represents those material not obeying the Drucker’s convexity postulate. In this sense, the UST unified the prevailing strength criteria. Its main features are further elaborated below.

354

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

Twin Shear Unified Strength Theory (Yu,1985) σ

1

'

θ θb

rc

rt

rc

0

60

rt

o

rt

rc

Single Shear Strength Theory (Mohr-Coulomb,1900)

b=0

σ

2

b1

Fig. 13.1 Loci of the UST in π -plane having different values of ‘b’

a)

b)

c)

UST consists of two material parameters - b and ȕ (or its equivalent form Į), which enables it to represent the strength envelope in the deviatoric plane for all conventional materials. In other words, it embraces all traditional strength criteria. For example, setting b = 0 and Į = 1 leads to the well-known Tresca criterion, which neglects totally the effect of intermediate principal shear stress and is only meant for materials having equal tensile and compressive strength. Again, setting Į = 1 and b = 1/2 yields segmental linear envelope very close to the smooth envelope by Mises criterion. It is worth noting that setting b = 1 leads to Yu’s twin-shear criterion – an earlier version of the UST. The UST provides admissible lower and upper bounds of the strength envelope for materials obeying the Drucker’s convexity postulate. When b = 0, it sets the lower bounds. Amongst them, Tresca envelope (Į = 1) is the one for materials having equal tensile and compressive strength; Mohr-Coulomb envelope is another one but it is for materials having different tensile and compressive strengths (Į 1). On the other hand when b = 1, it sets the upper bounds. Yu’s twin-shear criterion is one of it. Hence, the UST can be used to find the minimum and maximum yield/failure zone. When the value of ‘b’ is chosen outside the conventionally admissible range (i.e. b < 0 or b > 1), the corresponding strength envelope becomes non-convex shape. It violates the Drucker’s convexity postulate. In this

13.3 Stress fields around crack-tip

355

range, the UST yields strength envelopes for a whole spectrum of non-conventional materials, which do not obey the Drucker’s postulate.

13.3 Stress Fields Around Crack-Tip By virtue of linear elastic fracture mechanics, the 2D stress field in the vicinity of a mode-I crack-tip can be described as follows (Kanninen, 1985). σ x ½ 1 − sin( θ / 2 ) sin( 3θ / 2 ) ½ KI ° ° ° ° σ θ = cos ( / 2 ) ® y¾ ®1 + sin( θ / 2 ) sin( 3θ / 2 ) ¾ 12 r π ( 2 ) ° sin( θ / 2 ) cos( 3θ / 2 ) ° °τ ° ¯ ¿ ¯ xy ¿

(13-4)

For mode-II crack-tip, σ x ½ − sin(θ / 2)[ 2 + cos(θ /2 ) cos( 3θ / 2)]½ K II ° ° ° (13-5) ° cos(θ / 2) ® sin(θ / 2) cos(θ /2 ) sin( 3θ / 2) ¾ ®σ y ¾ = 1 2 °τ ° ( 2π r ) ° cos(θ / 2)[1 − sin(θ /2 ) sin( 3θ / 2)] ° xy ¿ ¯ ¯ ¿

For mode-III crack-tip, τ zx ½ K III − sin( θ / 2 ) ½ ® ¾= ® ¾ τ ¯ zy ¿ ( 2π r )1 2 ¯ cos( θ / 2 ) ¿

(13-6)

in which K I , K II and K III are the stress-intensity factors for mode-I, mode-II and mode-III respectively. ıx, ıy are the normal stresses in x- and y-direction respectively, and Ĳxy, Ĳzx, Ĳzy are the shear stresses in the xy-, zx- and zy-plane respectively. Position vector is expressed in polar coordinates (r,ș) measured from the crack-tip. The stress components in Eqs. (13-4)-(13-6) can be expressed in terms of the corresponding principal stresses ıi. For 2-dimenional plane problems, the principal stresses are: σ1½

¾= σ 2¿

σ3

σ x +σ y

2

2

§ σ x −σ y · 2 ¸ + τ xy ± ¨¨ 2 ¸¹ ©

0 =® ¯ ν ( σ 1+ σ 2 )

for plane stress for plane strain

(13-7a) (13-7b)

in which ν is Poisson’s ratio. Due to symmetry, the following derivations are presented only for the half-plane ( θ ∈ [0,π ] ). By substituting Eqs. (13-4)-(13-6)

356

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

into Eqs (13-7a)-(13-7b) and arranging the resulting stresses in the order such that σ 1 ≥ σ 2 ≥ σ 3 , we have For mode-I (plane-stress case) σ1

½ θ θ KI cos (1 ± sin ) ¾= σ2 ¿ 2 2 2π r σ3 = 0

(13-8)

For mode-I (plane-strain case) σ1

½ ¾= σ2 ¿

2π r

2ν K I

=

σ3

KI

cos

cos

2π r

θ

θ

(1 ± sin

2

2

)

for 0 ≤ ș < 2 sin

−1

(1 − 2 Ȟ )

(13-9)

θ

2

and σ1

=

σ2

=

σ3

=

KI 2π r 2ν K I 2π r KI 2π r

θ

cos

2

θ

2

)

θ

cos cos

(1 + sin

for 2 sin

−1

(1 − 2 Ȟ ) ≤ ș < ʌ (13-10)

2 θ

2

(1 − sin

θ

2

)

For mode-II (plane-stress case)

K II

σ1

=

σ2

=0

σ3

=

2π r

K II 2π r

1 4 − 3 sin 2 θ ) (− sin θ + 2

2

for 0 ≤ ș < 2 sin

(− sin

θ

2

−

1 2

−1

1

(13-11)

3

4 − 3 sin 2 θ )

and σ1 = 0

1

for 2 sin −1 ≤ș 1. The non-convex material may be called the non-conventional materials. The

366

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

shape and size of plastic zone for non-conventional materials (b=−0.1, −0,25, −0.5) are also plotted. Figures 13.12 and 13.13 are for mode-I plane-stress and plane-strain case respectively, while Figs. 13.14 and 13.15 for mode-II plane-stress and plane-strain case respectively. 13.7.1 Mode-I crack-tip plastic zone for non-conventional materials (plane stress)

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY 3

Dimensionless 2πy(σt/KII)

2

2 1

Crack 0

OX

O

-1 -2 -3 -1

0

1

2

3 2

Dimensionless 2πx(σt/KI)

Fig. 13.12 Mode-I crack-tip plastic zone for unconventional materials in plane-stress state ( Į = 1, Ȟ = 1/3 )

13.7 Shape and size of plastic zone for non-conventional materials

2

Dime nsionless 2πy(σt/KI)

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY

2

1

Crack 0

OX

O

-1

-2 -0.8

-0.6

-0.4

-0.2

0.0

0.2

2

0.4

0.6

Dimensionless 2πx(σt/KI)

Fig. 13.13 Mode-I crack-tip plastic zone for unconventional materials in plane-strain state ( Į = 1, Ȟ = 1/3 )

13.7.2 Mode-I crack-tip plastic zone for non-conventional materials (plane stress) UTSS (b= -0.1)

OY

4

UTSS (b= -0.25) UTSS (b= -0.5)

Dimensionless 2πy(σt/KII)

2

3 2 1

Crack

0

OX

O

-1 -2 -3 -4

-6

-4

-2

0

2

4

Dimensionless 2πx(σt/KII)

6

8

10

2

Fig. 13.14 Mode-II crack-tip plastic zone for unconventional materials in plane-stress states ( Į = 1, Ȟ = 1/3 )

367

368

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

UTSS (b= -0.1) UTSS (b= -0.25) UTSS (b= -0.5)

OY

5 4

Dimension less 2πy(σt/KII)

2

3 2

Crack

1 0

OX

O

-1 -2 -3 -4 -5

-8

-6

-4

-2

0

2

4

6

8

10

2

Dimensionless 2πx(σt/KII)

Fig. 13.15 Mode-II crack-tip plastic zone for unconventional materials in plane-strain state

( Į = 1 . 0 , Ȟ = 1/3 )

13.8 Effect of ‘b’ Value Parameter ‘ b’ represents the influence of the intermediate principal shear stress. For the same material, the extents of the influence are not the same under different crack-tip modes. It reflects in the resulting shape and size of the crack-tip plastic zone. On the other hand, various values of ‘b’ also correspond to a spectrum of strength criteria, including the well-known Tresca and Huber-von Mises. In other words, each ‘b’ value represents a strength criterion, which is only valid for a group of materials. What follows are observations of results obtained from different criteria through its equivalent value of ‘b’. • For mode-I: In both plane-stress and plane-strain cases, a general trend is observed that the larger the value of ‘b’, the smaller is the size of the plastic zone. In other words, the greater the influence of the intermediate shears, the smaller the size of the plastic zone. It can be seen from Figs. 13.2 and 13.3 that the Tresca criterion (equivalent to b = 0) leads to the largest zone, while Yu’s earlier full-twin-shear criterion (equivalent to b = 1) yields the smallest zone. The size of plastic zone by the Huber-von

13.7 Shape and size of plastic zone for non-conventional materials

369

Mises criterion is somewhere in-between the Tresca and the Yu’s twin-shear criterion, and is almost the same as that by UST with b = 0.5 . • For mode-II: Similar trend as in mode-I is observed. The larger the value of ‘b’, the smaller is the size of the plastic zone. Figure 13.4 shows the plane-stress case, while Fig. 13.5 shows the plane-strain case. In both cases, Tresca criterion (equivalent to b = 0 ) leads to the largest zone, while Yu’s full-twin-shear criterion (equivalent to b=1 ) yields the smallest zone. The Huber-von Mises criterion yields zone of intermediate sizes. Their shapes look similar. • For mode-III: Similar trend as in mode-I and mode-II is observed, except that the plastic zones are all of circular shape. • For unconventional materials (b < 0 ): Since the same mathematical expressions are used, the same trends are observed. The smaller the value of ‘b’ (more negative), the larger is the size of the plastic zone. Figures. 13.12 and 13.13 show the results for mode-I plane-stress and plane-strain respectively, while Figs 13.14 and 13.15 show the results for mode-II plane-stress and plane-strain respectively.

13.9 Influence of SD Effect Parameter ‘α ’ is the ratio of the uniaxial tensile strength to the uniaxial compressive strength. The ratio is a measure of the effect of strength differentials (SD). Definitely, it influences the sizes of the crack-tip plastic zone. Trends are observed in different crack modes but no common trend is noted. • In mode-I: The weaker-in-tension materials (Į = 0.5) always result in larger plastic zone (if not less) than the equal-strength materials (Į = 1), in both plane-stress and plane-strain cases. The sizes in plane-stress cases are usually bigger than those in plane-strain cases. It can be seen in Figs. 13.4 13.5 and 13.6 for b = 0, 0.5 and 1.0 respectively. • In mode-II: Contrary to the trend in Mode-I, the weaker-in-tension materials ( α = 0.5) always result in smaller plastic zone than the equal-strength materials (Į = 1), in both plane-stress and plane-strain cases. However, the sizes in plane-stress cases maintain the trend being bigger than those in plane-strain cases. It can be seen in Figs. 13.9, 13.10 and 13.11 for b = 0, 0.5 and 1.0 respectively.

370

•

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

In mode-III: The plastic zones are all of circular shape. The weaker-in-tension materials (α = 0.5) always result in smaller plastic zone than the equal-strength materials (α = 1), in both plane-stress and plane-strain cases. Again, the sizes in plane-stress cases are usually bigger than those in plane-strain cases.

13.10 Influence of Poisson’s Ratio Results for plane-stress cases are independent of the Poisson’s ratio. For Mode-I and -II plane-strain cases, the influence of Poisson’s ratio is similar to the trend observed in the variations of ‘b’ values. The larger the Poisson’s ratio, the smaller is the size of the plastic zone. Figure 13.16 shows the effect of Poisson’s ratio on mode-I crack-tip plastic zone, while Fig. 13.17 shows the Mode-II.

ν =1/3 ν =1/4 ν =1/5

OY

1.0 0.8

Dimensionless 2πy(σt/KI)

2

0.6 0.4

Crack

0.2 0.0 0

OX

O

-0.2 -0.4 -0.6 -0.8 -1.0 -0.5

-0.4

-0.3

-0.2

-0.1

0.0

0.1

0.2

0.3

0.4

0.5

2

Dimensionless 2π x(σt/KI)

Fig. 13.16 Effect of Poisson’s ratio on mode-I crack-tip plastic zone in plane-strain state ( Į = 1 .0 , b = 1 .0 )

Summary

2

Dimensionless 2πy(σt/KII)

ν=1/3 ν=1/4 ν=1/5

OY

2

371

1

Crack 0

O

OX

-1

-2

-4

-3

-2

-1

0

1

2

3

2

Dimensionless 2πx(σt/KII)

Fig. 13.17 Effect of Poisson’s ratio on mode-II crack-tip plastic zone in plane-strain state (Į = 1 .0 , b = 1 .0 )

Summary This chapter presents the estimations of crack-tip plastic zone under small-scale yielding (SSY) using the unified strength theory (UST). The UST unifies all prevailing strength criteria through a variable parameter ‘b’. It provides unified solutions for shapes and sizes of mode-I, -II, -III crack-tip plastic zone in the K-dominant region. The minimum and maximum crack-tip plastic zones can be deduced through the conventionally admissible lowerand upper-bound values of ‘b’ in the UST. Adopting a proper value of the material parameter ‘b’ can lead to accurate solutions. Other specific values of ‘b’ can yield solutions equivalent to those through the Tresca criterion, Huber-von Mises criterion or its varieties. In addition, stretching beyond the normally admissible range for the material parameter ‘b’ (1) can generate a new series of strength criteria for unconventional materials, which strength envelope may not necessarily be convex. Estimations of the crack-tip plastic zones using different values of ‘b’ are illustrated and compared. The influences on the resulting plastic zone due to strength-differential (SD) effect and Poisson’s ratio are also investigated. Embracing the SD effect broadens the applicability to most materials, which have unequal tensile and

372

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

compressive strength. It demonstrates the robustness of present method in the estimation of shape and size of the crack-tip plastic zone under SSY. It is seen that: (1) The Yu's unified strength theory is applied to the study of the shape and size of plastic zones of mode I, II, III cracks, and a complete solution of unified closed forms is obtained. The Tresca criterion and the Huber-von Mises criterion are special case and linear approximation of the Yu’s theory. (2) Except for mode III cracks, the boundary curves of mode I, II crack tip plastic zones are composed of two parts, which is resulted from the piece-wise linearity of the Yu's criterion. (3) Generally speaking, the plastic zone obtained by the Yu's theory is smaller than that by the Huber-von Mises and much smaller than that by the Tresca criterion, showing that a bigger τ s /σ s will lead to a smaller plastic zone and weaker ability to resist fracture. (4) Different values of b in Yu's theory will produce a family of different yield criterion which will help obtain a group of crack tip plastic zones applicable to various materials. The value of σ t also exerts certain influence on the tip plastic zone, but only affects the plane strain condition (except for mode III cracks). The results were obtained by analytical solution. The unified strength theory and unified elasto-plastic constitutive model can be also implemented into commercial finite element codes and other FEM codes. The effect of failure criterion on numerical calculations of finite element method (FEM) can be also observed. These problems will be summarized at another book entailed “Computational Plasticity based on the Unified Strength theory”

Problems Problem 13.1. The solution of crack tip problem can be also studied by using the slip field theory. Figure P16.1 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode I under plane strain. Can you given a new solution by using the twin-shear slip field method described in Chapter 8. Problem 13.2. The solution of crack tip problem can be also studied by using the slip field theory. Figure P16.1 shows a slip field with the Tresca yield criterion for Mode I under plane strain condition. Can you given a new solution by using

Problems

373

the unified slip field theory described in Chapter 9.

Fig. P16.1

Mode I

Fig. P16.2

Mode II

Fig. P16.3 Mixed Mode III

Problem 13.3. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.2 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode II under plane strain condition. Can you given a new solution by using the twin-shear slip field method described in Chapter 8. Problem 13.4. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.2 shows a slip field with the Tresca yield criterion (single-shear theory) for Mode II under plane strain condition. Can you given a new solution by using the unified slip field theory described in Chapter 9. Problem 13.5. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.3 shows a kind of slip field with the Tresca yield criterion (single-shear theory) for Mixed Mode I and II under plane strain. Can you given a new solution by using the unified slip field method described in Chapter 9. Problem 13.6. The solution of crack tip problem can be also studied by using the slip field theory. Figure P13.3 shows a kind of slip field with the Tresca yield criterion (single-shear theory) for Mixed Mode I and II under plane strain. Can you given a new solution by using the unified slip field method described in Chapter 9.

374

13 Unified Solution of Plastic Zones at Crack Tip under Small Scale Yielding

References and Bibliography Barenblatt GI (1962) The mathematical theory of equilibrium cracks in brittle fracture. Advances in Applied Mechanics; 7: 55–129. Broek D (1982) Elementary Engineering Fracture Mechanics (3rd ed.) Martinus Nijihoff Publishers, The Hague. Dugdale DS (1960) Yielding of steel sheets containing slits. Journal of the Mechanics and Physics of Solids; 8: 100–108. Fan SC, Yu MH, Yang SY (2001) On the unification of yield criteria. Journal of Appllied Mechanics, 68: 341–343. Flugge S (1958). Encyclopedia of Physics. New York: Springer-Verlag. Hult JAH, McClintock FA (1957) Elastic-plastic stress and strain distributions around sharp notches under repeated shear, In: Proceedings of the Ninth International Congress for Applied Mechanics, University of Brussels, 51–58. Irwin GR (1960) Plastic zone near a crack and fracture toughness. In: Proceedings of the 7th Sagamore Ordnance Materials Conference, New York: Syracuse University Press, 1960: IV-63-78 Irwin GR (1968) Linear fracture mechanics, fracture transition and fracture control. Engineering Fracture Mechanics; 1: 241-257. Kanninen MF, Popelar CH (1985) Advanced Fracture Mechanics. Oxford University Press, New York, 563 pages. Qiang HF, Xu YH, Zhu JH (1998) Unified solutions of mixture type crack tip plastic zone under small scale yielding. In: Strength Theory: Applications, Developments and prospects for the 21st Century, MH Yu and SC Fan (eds), Science Press, Beijing, New York, 823–829. Qiang HF and Lu N (1999) Unified solutions of crack tip plastic zone under small scale yielding, Chin. J. Mech. Engrg., 35(1), 34–38. (in Chinese) Winstone MR (1984) Influence of prestress on the yield surface of the cast nickel super alloy Mar-Mooz at elevated temperature. Mechanical Behavior of Materials, Pergamon Press, Oxford 1984, Vol. 1, 199–205 Yang Wei. Macro-Micro Scope Fracture Mechanics. Beijing: National Defence Industry Press, 1995.(In Chinese) Yu MH (1983) Twin-shear stress yield criterion. Int. Journal of Mechanical Science, 25(1): 71–74. Yu MH (2002) Advances in strength theories for materials under complex stress state in the 20th century. Applied Mechanics Reviews, 55(3): 169–218. Yu MH (1983) Twin-shear stress strength criterion. International Journal of Mechanical Science, 25(1): 71–74. Yu MH, He LN, Song LY (985) Twin-shear stress theory and its generalization. Scientia Sinica (Science in China) Series A, 28: 1174–1183. Yu MH, He LN (1991) A new model and theory on yield and failure of materials under complex stress state. In: Jono M, Inoue T. Mechanical Behavior of Materials-VI. Pergamon Press. Oxford, 841–846. Yu Mao-hong, New System of Strength Theory. Xian: Xian Jiaotong University Press, 1992. (In Chinese) Yu MH (1998) Twin-shear Theory and Its Applications. Science Press, Beijing (in Chinese) Yu Mao-Hong, Advances in strength theories for materials under complex stress state in the 20th Century. Applied Mechanics Reviews, 55 (2002) 169-218. Yu Mao-hong. (2004) Unified Strength Theory and Its Applications. Springer, Berlin.

14 Unified Fracture Criterion for Mixed Mode Crack Initiation and Fatigue Crack Growth

14.1 Introduction Mixed-mode fracture and fatigue crack growth are one of the most commonly used failure forms of material in analyzing practical engineering problems. The research on the mixed fracture criterion and fatigue crack growth is significant in fracture mechanics and engineering. Many research works in this area have been conducted and some criteria for predicating the direction of the crack initiation angle and the critical fracture load of materials have been proposed by energy principles and the stress approach (Khan et al. 2000). Among the criteria of energy principle type, G-criterion (Hussian et al. 1974), S-criterion (Sih 1974) and T-criterion (Theocaris and Andrianopoulos 1982a, 1982b) are original and more important ones. Other fracture criteria are the maximum tangential stress criterion (Erdogan and Sih 1963), maximum shear stress criterion, maximum stress triaxiality criterion (Kong, Schluter and Dahl 1995), maximum octahedral shear stress criterion etc. The plastic zone radius criterion for crack initiation angle was proposed recently by Golos and Wasiluk (2000), Wasiluk and Golos (2000), Kahn and Khraisheh (2004) and Bian and Kim (2004). S-criterion states that the crack initiation takes place along the direction with the minimum strain energy density around a constant radius around crack tip and a crack extension starts in the initiation direction when strain energy density reaches a critical value. The region within this constant radius is assumed and the linear elastic fracture mechanics does not hold in this circular region. In fact, there is not any evidence supporting the assumption that this area is circular region with constant radius, which is an intuitively fixed value only. This region is firstly called core region by Theocaris (Theocaris and Andrianopoulos 1982a, 1982b) using the caustic method, and the various fracture criteria maybe applied with high accuracy defined by the radius of the initial curve of the respective caustic created by the different loading modes. Then Theocaris et al. modified S-criterion in two aspects, firstly, total strain energy is separated into two components: a dilatational component that mainly causes cavity nucleation and development around a crack tip and distortional component that changes the shape of an element; secondly, the Huber-von Mises elastic-plastic boundary as the core region is assumed by using a variable radius for the core region, therefore T-criterion was defined that the crack

376

14 Unified Fracture Criterion for Mixed Mode Crack Initiation

initiation occurs at the direction with maximum dilatational strain energy density along the contour of constant distortional strain energy. Theocaris et al. also performed experiments on polycarbonate (PCBC) specimen to support their criterion (Theocaris et al. 1982c). The investigation mentioned above showed that the introduction (including both size and shape) of core region is very important for definition of various fracture criteria. However, the studies were performed only by using Huber-von Mises yield criterion, because it coincided with distortional energy part in form. Little attention has been paid to investigate the influence of yield criterion on the core region of crack tip. In fact, the Tresca criterion is the lower bound of yield criteria and the twinshear stress criterion (or the maximum principal deviatoric stress criterion) is the upper bound of yield criteria for stable and isotropic ductile material (Yu 1983). The Huber-von Mises yield criterion is a special case mediated between the lower bound and upper bound. A linear Unified strength theory (UST) was proposed by Yu in 1991 and 1992 (see: Yu 2002, 2004). It is obtained by introducing twin-shear element naturally. It has two simple mathematical formulae, piecewise linear yield surfaces and physical significance. Varying the parameter b in the UST derives a family of convex criteria. Based on the UST, a generalized T-criterion for Strength Difference (SD) or non-SD materials is obtained by Qiang, Yu et al. in 2003 and 2004. A new closed form of plastic core region model and its derivatives are obtained by Qiang in 2004. The Tresca-core region is lower bound, and the twin-shear-core region is upper bound, the Huber-von Mises-core region mediated between these two bounds. They are all the special case of the plastic core region responses of the generalized T-criterion. A unified fracture criterion based directly on the unified strength theory was obtained by Yu, Fan, Che et al. in 2003, 2004. In this chapter, a variable radius for the plastic core region based on the UST elastic-plastic boundary is introduced and incorporated in the formulation of the T-criterion, the lower bound and upper bound plastic core region responses of T-criterion is derived. Comparisons of the three particular solutions with respect to the Tresca-core region, the Huber-von Mises-core region and the TS-core region are made mutually. a generalized T-criterion is obtained, called the UT-criterion. At last, a unified fracture criterion for mixed mode crack is described in detail. It is introduced directly from the formulation of the unified strength theory (Fan 2003, Yu, Fan and Che 2003, 2004). The relations of crack initial angle © with DQG unified strength parameter b for mode Ċcrack (©~~b curves), cracked initial angle with various fracture criteria, unified fracture criterion of mixed I-II mode for various α , unified fracture criterion of mixed I-III mode for various α , and the unified fracture criterion of mixed II-III mode for various α are obtained by using the numerical calculation method. A series of relations are illustrated in Figs. 14.17 to 14.25. The unified fracture criterion may be also used for the study of fatigue crack growth.

14.2 Main Idea of T-Criterion

377

14.2 Main Idea of T-Criterion Consider an elastic-perfectly plastic plate under plane stress condition containing an internal crack inclined by an angle ȕ to the direction of the uniaxial loading, as show in Fig. 14.1. The stresses around the crack-tip are: Y

σ0

r β

θ

o X

2a

σ0

Fig. 14.1 Slant crack under remote uniaxial load σx =

σy =

τ xy =

KI ª KI 3θ · 3θ ·º θ§ θ§ θ θ f x (θ ) «cos 2 ¨1 − sin 2 sin 2 ¸ − µ sin 2 ¨ 2 + cos 2 cos 2 ¸» = 2π r ¬ 2π r ¹¼ ¹ © © ª θ§ θ 3θ · 3θ º KI θ θ f y (θ ) (14-1) «cos 2 ¨1 + sin 2 sin 2 ¸ + µ sin 2 cos 2 cos 2 » = 2π r ¬ 2π r ¹ © ¼

KI

KI ª KI 3θ 3θ · º θ θ θ § θ f xy (θ ) « cos 2 sin 2 cos 2 + µ cos 2 ¨ 1 − sin 2 sin 2 ¸ » = 2π r ¬ 2π r © ¹¼

where ıx, ıy. and Ĳxy are the normal stresses and shear stress in x-y plane respectively; K I = σ 0 π a sin2 β , K II = σ 0 π a sin β cos β and µ = K II / K I are stress-intensity factors for mode-I, -II and its notation respectively, σ 0 is uniaxial loading of remote field, 2a is the crack length; f x (θ ) , f y (θ ) and fxy (θ ) are defined as above. Based on T-criterion, the dilatational and distortional parts of the strain energy density are given respectively by:

TV = TD =

1 − 2ν (σ + σ y )2 6E x

1+ν 2 2 (σ x + σ y2 − σ xσ y + 3τ xy ) 3E

(14-2a)

(14-2b)

378

14 Unified Fracture Criterion for Mixed Mode Crack Initiation

where E and ν are the modulus of elasticity and Poisson’s ratio of the material. Using the notation of equation (1), we obtain from Eqs. (14-2a) and (14-2b) respectively

(1 − 2ν ) K I2 ( f x + f y )2 12π Er

(14-3a)

(1+ ν ) K I2 2 ( f x + f y2 − f x f y + 3 f xy2 ) 6π Er

(14-3b)

TV =

TD =

Since the distortional strain energy is constant along the Huber-von Mises elastic plastic boundary, TD,0 can be considered as a material constant, i.e., (1 + ν ) σ s2 . Combining Eqs. (14-3a) and (14-3b), we get boundary of the TD,0 = 3E core region and the dilatational strain energy 2

TV =

KI

( f x2 + f y2 − f x f y + 3 f xy2 )

(14-4)

( f x + f y )2 (1 − 2ν ) σ s2 6E f x2 + f y2 − f x f y + 3 f xy2

(14-5)

r=

2πσ s2

So the T-criterion is defined as TV

θ =θ 0

≥ T V, cr TD = T D , 0

∂ TV ∂θ

θ =θ 0

=0

∂ 2TV ∂θ 2

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close